* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project

# Download Fundamentals of Semiconductors

Scalar field theory wikipedia , lookup

Symmetry in quantum mechanics wikipedia , lookup

Nitrogen-vacancy center wikipedia , lookup

Matter wave wikipedia , lookup

Renormalization wikipedia , lookup

Ferromagnetism wikipedia , lookup

Molecular Hamiltonian wikipedia , lookup

Renormalization group wikipedia , lookup

Franck–Condon principle wikipedia , lookup

Hydrogen atom wikipedia , lookup

Magnetic circular dichroism wikipedia , lookup

Auger electron spectroscopy wikipedia , lookup

Quantum electrodynamics wikipedia , lookup

Atomic orbital wikipedia , lookup

Wave–particle duality wikipedia , lookup

X-ray photoelectron spectroscopy wikipedia , lookup

Atomic theory wikipedia , lookup

Theoretical and experimental justification for the Schrödinger equation wikipedia , lookup

X-ray fluorescence wikipedia , lookup

Graduate Texts in Physics Graduate Texts in Physics Graduate Texts in Physics publishes core learning/teaching material for graduate- and advanced-level undergraduate courses on topics of current and emerging ﬁelds within physics, both pure and applied. These textbooks serve students at the MS- or PhD-level and their instructors as comprehensive sources of principles, deﬁnitions, derivations, experiments and applications (as relevant) for their mastery and teaching, respectively. International in scope and relevance, the textbooks correspond to course syllabi sufﬁciently to serve as required reading. Their didactic style, comprehensiveness and coverage of fundamental material also make them suitable as introductions or references for scientists entering, or requiring timely knowledge of, a research ﬁeld. Series Editors Professor H. Eugene Stanley Boston University Center for Polymer Studies Department of Physics 590 Commonwealth Avenue, Room 204B Boston, MA 02215, USA E-mail: [email protected] Professor William T. Rhodes Georgia Institute of Technology School of Electrical and Computer Engineering Atlanta, GA 30332-0250, USA E-mail: [email protected] Peter Y. Yu Manuel Cardona Fundamentals of Semiconductors Physics and Materials Properties Fourth Edition 123 Professor Dr. Peter Y. Yu Professor Dr., Dres. h.c. Manuel Cardona University of California Department of Physics Berkeley, CA 94720-7300, USA E-mail: [email protected] Max-Planck-Institut für Festkörperforschung Heisenbergstr. 1, 70569 Stuttgart, Germany E-mail: [email protected] ISSN 1868-4513 ISBN 978-3-642-00709-5 DOI 10.1007/978-3-642-00710-1 e-ISSN 1868-4521 e-ISBN 978-3-642-00710-1 Springer Heidelberg Dordrecht London New York Library of Congress Control Number: 2010924732 © Springer-Verlag Berlin Heidelberg 1996, 1999, 2001, 2010 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specif ically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microf ilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to prosecution under the German Copyright Law. The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specif ic statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Printed on acid-free paper Springer is a part of Springer Science+Business Media (springer.com). Preface to the Fourth Edition Since the appearance of our book, Fundamentals of Semiconductors: Physics and Materials Properties, one of the questions we are asked most frequently is this: “is there a solution manual to this book?” In preparing the questions at the end of each chapter we have already tried to guide the readers to derive the answers by themselves using a step-by-step approach. Clearly this strategy did not work for everyone. We recognize that many of the questions in this book are quite challenging and often require reading of research papers to solve them. In response to readers demand we have decided to provide solutions to some of the problems in this new edition. Since working through problems is an important and necessary part of the learning process in physics we will not give the solutions to all the problems. Instead, we hope to use the solutions to a number of selected problems in each chapter as an additional study help to the readers. We like to use these solutions to provide more in depth discussions to topics which may be too specialized for a typical course on semiconductor physics. By leaving enough unsolved problems and adding a few new ones there are still plenty of opportunities for both the instructors to choose problems for assignments and for students to test their understanding of the text. We like to point out that, even if the solution can be found in this manual, there is usually more than one way to solve a given problem. Conscientious students should always ask whether there is a better way to solve a problem than the one we have provided in this manual. This new addition also allows us to update and expand some topics and references. Finally, we hope to have taken care of the few errors still remaining in the third edition. We like to use this opportunity to thank the readers who have identified them to us. Their support has been invaluable in our effort to improve this book. A Russian translation of our book has appeared in 2003. It joins previous translations of the book into Japanese and Chinese, making this book available to a truly international readership. Last, but not least, the homepage of the book has been given a ”face lift”. Readers are encouraged to visit the new website at: http://pauline.berkeley.edu/Book/Fundamentals.html to discover new information and materials which have been added. Peter Y. Yu and M. Cardona Berkeley, CA and Stuttgart, Germany March 2010 Preface to the Third Edition The support for our book has remained high and compliments from readers and colleagues have been most heart-warming. We would like to thank all of you, especially the many students who have continued to send us their comments and suggestions. We are also pleased to report that a Japanese translation appeared in 1999 (more details can be obtained from a link on our Web site: http://pauline.berkeley.edu/textbook). Chinesea) and Russian translations are in preparation. Semiconductor physics and material science have continued to prosper and to break new ground. For example, in the years since the publication of the first edition of this book, the large band gap semiconductor GaN and related alloys, such as the GaInN and AlGaN systems, have all become important materials for light emitting diodes (LED) and laser diodes. The large scale production of bright and energy-efficient white-light LED may one day change the way we light our homes and workplaces. This development may even impact our environment by decreasing the amount of fossil fuel used to produce electricity. In response to this huge rise in interest in the nitrides we have added, in appropriate places throughout the book, new information on GaN and its alloys. New techniques, such as Raman scattering of x-rays, have given detailed information about the vibrational spectra of the nitrides, available only as thin films or as very small single crystals. An example of the progress in semiconductor physics is our understanding of the class of deep defect centers known as the DX centers. During the preparation of the first edition, the physics behind these centers was not universally accepted and not all its predicted properties had been verified experimentally. In the intervening years additional experiments have verified all the remaining theoretical predictions so that these deep centers are now regarded as some of the best understood defects. It is now time to introduce readers to the rich physics behind this important class of defects. The progress in semiconductor physics has been so fast that one problem we face in this new edition is how to balance the new information with the old material. In order to include the new information we had either to expand the size of the book, while increasing its price, or to replace some of the existing material by new sections. We find either approach undesirable. Thus we have come up with the following solution, taking advantage of the Internet in this a The Chinese version was published in 2002 by Lanzhou University Press (see www.onbook.com.cn) VIII Preface to the Third Edition new information age. We assume that most of our readers, possibly all, are “internet-literate” so that they can download information from our Web site. Throughout this new edition we have added the address of Web pages where additional information can be obtained, be this new problems or appendices on new topics. With this solution we have been able to add new information while keeping the size of the book more or less unchanged. We are sure the owners of the older editions will also welcome this solution since they can update their copies at almost no cost. Errors seem to decay exponentially with time. We thought that in the second edition we had already fixed most of the errors in the original edition. Unfortunately, we have become keenly aware of the truth contained in this timeless saying: “to err is human”. It is true that the number of errors discovered by ourselves or reported to us by readers has dropped off greatly since the publication of the second edition. However, many serious errors still remained, such as those in Table 2.25. In addition to correcting these errors in this new edition, we have also made small changes throughout the book to improve the clarity of our discussions on difficult issues. Another improvement we have made in this new edition is to add many more material parameters and a Periodic Table revealing the most common elements used for the growth of semiconductors. We hope this book will be not only a handy source for information on topics in semiconductor physics but also a handbook for looking up material parameters for a wide range of semiconductors. We have made the book easier to use for many readers who are more familiar with the SI system of units. Whenever an equation is different when expressed in the cgs and SI units, we have indicated in red the difference. In most cases this involves the multiplication of the cgs unit equation by (4Â0 )1 where Â0 is the permittivity of free space, or the omission of a factor of (1/c) where c is the speed of light. Last but not least, we are delighted to report that the Nobel Prize in Physics for the year 2000 has been awarded to two semiconductor physicists, Zhores I. Alferov and Herbert Kroemer (“for developing semiconductor heterostructures used in high-speed- and opto-electronics”) and a semiconductor device engineer, Jack S. Kilby (“for his part in the invention of the integrated circuit”). Stuttgart and Berkeley, January 2001 Peter Y. Yu Manuel Cardona Preface to the Second Edition We have so far received many comments and feedback on our book from all quarters including students, instructors and, of course, many friends. We are most grateful to them not only for their compliments but also for their valuable criticism. We also received many requests for an instructor manual and solutions to the problems at the end of each chapter. We realize that semiconductor physics has continued to evolve since the publication of this book and there is a need to continue to update its content. To keep our readers informed of the latest developments we have created a Web Page for this book. Its address (as of the writing of this preface) is: http://pauline.berkeley.edu/textbook. At this point this Web Page displays the following information: 1) Content, outline and an excerpt of the book. 2) Reviews of the book in various magazines and journals. 3) Errata to both first and second printing (most have been corrected in the second edition as of this date). 4) Solutions to selected problems. 5) Additional supplementary problems. The solutions in item (4) are usually incomplete. They are supposed to serve as helpful hints and guides only. The idea is that there will be enough left for the students to do to complete the problem. We hope that these solutions will satisfy the need of both instructors and students. We shall continue to add new materials to the Web Page. For example, a list of more recent references is planned. The readers are urged to visit this Web Page regularly to find out the latest information. Of course, they will be welcomed to use this Web Page to contact us. While the present printing of this book was being prepared, the 1998 International Conference on the Physics of Semiconductors (ICPS) was being held in Jerusalem (Israel). It was the 24th in a biannual series that started in 1950 in Reading (U.K.), shortly after the discovery of the transistor by Shockley, Bardeen and Brattain in 1948. The ICPS conferences are sponsored by the International Union of Pure and Applied Physics (IUPAP). The proceedings of the ICPS’s are an excellent historical record of the progress in the field and the key discoveries that have propelled it. Many of those proceedings appear in our list of references and, for easy identification, we have highlighted in red the corresponding entries at the end of the book. A complete list of all conferences held before 1974, as well as references to their proceedings, can X Preface to the Second Edition be found in the volume devoted to the 1974 conference which was held in Stuttgart [M. H. Pilkuhn, editor (Teubner, Stuttgart, 1974) p. 1351]. The next ICPS is scheduled to take place in Osaka, Japan from Sept. 18 to 22 in the year 2000. The Jerusalem ICPS had an attendance of nearly 800 researchers from 42 different countries. The subjects covered there represent the center of the current interests in a rapidly moving field. Some of them are already introduced in this volume but several are still rapidly developing and do not yet lend themselves to discussion in a general textbook. We mention a few keywords: Fractional quantum Hall effect and composite fermions. Mesoscopic effects, including weak localization. Microcavities, quantum dots, and quantum dot lasers. III–V nitrides and laser applications. Transport and optical processes with femtosecond resolution. Fullerites, C60 -based nanotubes. Device physics: CMOS devices and their future. Students interested in any of these subjects that are not covered here, will have to wait for the proceedings of the 24th ICPS. Several of these topics are also likely to find a place in the next edition of this book. In the present edition we have corrected all errors known to us at this time and added a few references to publications which will help to clarify the subjects under discussion. Stuttgart and Berkeley, November 1998 Peter Y. Yu Manuel Cardona Preface to the First Edition I, who one day was sand but am today a crystal by virtue of a great fire and submitted myself to the demanding rigor of the abrasive cut, today I have the power to conjure the hot flame. Likewise the poet, anxiety and word: sand, fire, crystal, strophe, rhythm. – woe is the poem that does not light a flame David Jou, 1983 (translated from the Catalan original) The evolution of this volume can be traced to the year 1970 when one of us (MC) gave a course on the optical properties of solids at Brown University while the other (PYY) took it as a student. Subsequently the lecture notes were expanded into a one-semester course on semiconductor physics offered at the Physics Department of the University of California at Berkeley. The composition of the students in this course is typically about 50 % from the Physics Department, whereas the rest are mostly from two departments in the School of Engineering (Electrical Engineering and Computer Science; Materials Science and Mineral Engineering). Since the background of the students was rather diverse, the prerequisites for this graduate-level course were kept to a minimum, namely, undergraduate quantum mechanics, electricity and magnetism and solid-state physics. The Physics Department already offers a two-semester graduate-level course on condensed matter physics, therefore it was decided to de-emphasize theoretical techniques and to concentrate on phenomenology. Since many of the students in the class were either growing or using semiconductors in device research, particular emphasis was placed on the relation between physical principles and device applications. However, to avoid competing with several existing courses on solid state electronics, discussions of device design and performance were kept to a minimum. This course has been reasonably successful in “walking this tight-rope”, as shown by the fact that it is offered at semi-regular intervals (about every two years) as a result of demands by the students. One problem encountered in teaching this course was the lack of an adequate textbook. Although semiconductor physics is covered to some extent in all advanced textbooks on condensed matter physics, the treatment rarely provides the level of detail satisfactory to research students. Well-established books on semiconductor physics are often found to be too theoretical by experimentalists and engineers. As a result, an extensive list of reading materials initially replaced the textbook. Moreover, semiconductor physics being a mature field, most of the existing treatises concentrate on the large amount of XII Preface to the First Edition well-established topics and thus do not cover many of the exciting new developments. Soon the students took action to duplicate the lecture notes, which developed into a “course reader” sold by the Physics Department at cost. This volume is approximately “version 4.0” (in software jargon) of these lecture notes. The emphasis of this course at Berkeley has always been on simple physical arguments, sometimes at the expense of rigor and elegance in mathematics. Unfortunately, to keep the promise of using only undergraduate physics and mathematics course materials requires compromise in handling special graduate-level topics such as group theory, second quantization, Green’s functions and Feynman diagrams, etc. In particular, the use of group theory notations, so pervasive in semiconductor physics literature, is almost unavoidable. The solution adopted during the course was to give the students a “five-minute crash course” on these topics when needed. This approach has been carried over to this book. We are fully aware of its shortcomings. This is not too serious a problem in a class since the instructor can adjust the depth of the supplementary materials to satisfy the need of the students. A book lacks such flexibility. The readers are, therefore, urged to skip these “crash courses”, especially if they are already familiar with them, and consult the references for further details according to their background. The choice of topics in this book is influenced by several other factors. Most of the heavier emphasis on optical properties reflects the expertise of the authors. Since there are already excellent books emphasizing transport properties, such as the one by K. H. Seeger, our book will hopefully help to fill a void. One feature that sets this book apart from others on the market is that the materials science aspects of semiconductors are given a more important role. The growth techniques and defect properties of semiconductors are represented early on in the book rather than mentioned in an appendix. This approach recognizes the significance of new growth techniques in the development of semiconductor physics. Most of the physics students who took the course at Berkeley had little or no training in materials science and hence a brief introduction was found desirable. There were some feelings among those physics students that this course was an easier way to learn about materials science! Although the course offered at Berkeley lasted only one semester, the syllabus has since been expanded in the process of our writing this book. As a result it is highly unlikely that the volume can now be covered in one semester. However, some more specialized topics can be omitted without loss of continuity, such as high field transport and hot electron effects, dynamic effective ionic charge, donor–acceptor pair transitions, resonant Raman and Brillouin scattering, and a few more. Homework assignment for the course at Berkeley posed a “problem” (excuse our pun). No teaching assistant was allocated by the department to help with grading of the problem sets. Since the enrollment was typically over thirty students, this represented a considerable burden on the instructor. As a “solution” we provide the students with the answers to most of the questions. Furthermore, many of the questions “lead the student by the hand” through Preface to the First Edition the calculation. Others have hints or references where further details can be found. In this way the students can grade their own solutions. Some of the material not covered in the main text is given in the form of “problems” to be worked out by the student. In the process of writing this book, and also in teaching the course, we have received generous assistance from our friends and colleagues. We are especially indebted to: Elias Burstein; Marvin Cohen; Leo Esaki; Eugene Haller; Conyers Herring; Charles Kittel; Neville Smith; Jan Tauc; and Klaus von Klitzing for sharing their memories of some of the most important developments in the history of semiconductor physics. Their notes have enriched this book by telling us their “side of the story”. Hopefully, future students will be inspired by their examples to expand further the frontiers of this rich and productive field. We are also grateful to Dung-Hai Lee for his enlightening explanation of the Quantum Hall Effect. We have also been fortunate in receiving help from the over one hundred students who have taken the course at Berkeley. Their frank (and anonymous) comments on the questionnaires they filled out at the end of the course have made this book more “user-friendly”. Their suggestions have also influenced the choice of topics. Many postdoctoral fellows and visitors, too numerous to name, have greatly improved the quality of this book by pointing out errors and other weaknesses. Their interest in this book has convinced us to continue in spite of many other demands on our time. The unusually high quality of the printing and the color graphics in this book should be credited to the following people: H. Lotsch, P. Treiber, and C.-D. Bachem of Springer-Verlag, Pauline Yu and Chia-Hua Yu of Berkeley, Sabine Birtel and Tobias Ruf of Stuttgart. Last but not the least, we appreciate the support of our families. Their understanding and encouragement have sustained us through many difficult and challenging moments. PYY acknowledges support from the John S. Guggenheim Memorial Foundation in the form of a fellowship. Stuttgart and Berkeley, October 1995 Peter Y. Yu Manuel Cardona XIII XIV Preface to the First Edition A SEMI-CONDUCTOR Contents 1. 2. Introduction 1 1.1 2 2 2 3 3 4 4 4 5 5 6 7 8 A Survey of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.1 Elemental Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.2 Binary Compounds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.3 Oxides . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.4 Layered Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.5 Organic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.6 Magnetic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.7 Other Miscellaneous Semiconductors . . . . . . . . . . . . . . . . . 1.2 Growth Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Czochralski Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.2 Bridgman Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.3 Chemical Vapor Deposition . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.4 Molecular Beam Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.5 Fabrication of Self-Organized Quantum Dots by the Stranski–Krastanow Growth Method . . . . . . . . . . . 1.2.6 Liquid Phase Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Periodic Table of “Semiconductor-Forming” Elements . . . . . . . . . . . . . . 11 13 14 15 Electronic Band Structures 17 2.1 2.2 2.3 18 20 25 25 2.4 2.5 Quantum Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Translational Symmetry and Brillouin Zones . . . . . . . . . . . . . . . . . A Pedestrian’s Guide to Group Theory . . . . . . . . . . . . . . . . . . . . . 2.3.1 Definitions and Notations . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.2 Symmetry Operations of the Diamond and Zinc-Blende Structures . . . . . . . . . . . . . . . . . . . . . . . . 2.3.3 Representations and Character Tables . . . . . . . . . . . . . . . 2.3.4 Some Applications of Character Tables . . . . . . . . . . . . . . . Empty Lattice or Nearly Free Electron Energy Bands . . . . . . . . . 2.4.1 Nearly Free Electron Band Structure in a Zinc-Blende Crystal . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.2 Nearly Free Electron Energy Bands in Diamond Crystals Band Structure Calculations by Pseudopotential Methods . . . . . . 2.5.1 Pseudopotential Form Factors in Zinc-Blende- and Diamond-Type Semiconductors . . . . 2.5.2 Empirical and Self-Consistent Pseudopotential Methods 30 32 40 48 48 52 58 61 66 XVI Contents 2.6 3. The k·p Method of Band-Structure Calculations . . . . . . . . . . . . . . 2.6.1 Effective Mass of a Nondegenerate Band Using the k·p Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 Band Dispersion near a Degenerate Extremum: Top Valence Bands in Diamondand Zinc-Blende-Type Semiconductors . . . . . . . . . . . . . . . 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.1 Molecular Orbitals and Overlap Parameters . . . . . . . . . . . 2.7.2 Band Structure of Group-IV Elements by the Tight-Binding Method . . . . . . . . . . . . . . . . . . . . . . . 2.7.3 Overlap Parameters and Nearest-Neighbor Distances . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 87 94 96 105 Vibrational Properties of Semiconductors, and Electron–Phonon Interactions 107 3.1 3.2 4. 68 69 71 83 83 Phonon Dispersion Curves of Semiconductors . . . . . . . . . . . . . . . Models for Calculating Phonon Dispersion Curves of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.1 Force Constant Models . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.2 Shell Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.3 Bond Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.4 Bond Charge Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Electron–Phonon Interactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.1 Strain Tensor and Deformation Potentials . . . . . . . . . . . . 3.3.2 Electron–Acoustic-Phonon Interaction at Degenerate Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.3 Piezoelectric Electron–Acoustic-Phonon Interaction . . . . 3.3.4 Electron–Optical-Phonon Deformation Potential Interactions . . . . . . . . . . . . . . . . . 3.3.5 Fröhlich Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.6 Interaction Between Electrons and Large-Wavevector Phonons: Intervalley Electron–Phonon Interaction . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 135 137 158 Electronic Properties of Defects 159 4.1 4.2 160 161 162 166 171 4.3 Classification of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Shallow or Hydrogenic Impurities . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Effective Mass Approximation . . . . . . . . . . . . . . . . . . . . . 4.2.2 Hydrogenic or Shallow Donors . . . . . . . . . . . . . . . . . . . . 4.2.3 Donors Associated with Anisotropic Conduction Bands 4.2.4 Acceptor Levels in Diamondand Zinc-Blende-Type Semiconductors . . . . . . . . . . . . . . Deep Centers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110 114 114 114 115 117 121 122 127 130 131 133 174 180 Contents 4.3.1 Green’s Function Method for Calculating Defect Energy Levels . . . . . . . . . . . . . . . 4.3.2 An Application of the Green’s Function Method: Linear Combination of Atomic Orbitals . . . . . . . . . . . . . 4.3.3 Another Application of the Green’s Function Method: Nitrogen in GaP and GaAsP Alloys . . . . . . . . . . . . . . . . 4.3.4 Final Note on Deep Centers . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5. 6. 183 188 192 197 198 202 Electrical Transport 203 5.1 5.2 203 206 206 207 Quasi-Classical Approach . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Carrier Mobility for a Nondegenerate Electron Gas . . . . . . . . . . 5.2.1 Relaxation Time Approximation . . . . . . . . . . . . . . . . . . . 5.2.2 Nondegenerate Electron Gas in a Parabolic Band . . . . . 5.2.3 Dependence of Scattering and Relaxation Times on Electron Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.4 Momentum Relaxation Times . . . . . . . . . . . . . . . . . . . . . 5.2.5 Temperature Dependence of Mobilities . . . . . . . . . . . . . 5.3 Modulation Doping . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 High-Field Transport and Hot Carrier Effects . . . . . . . . . . . . . . . 5.4.1 Velocity Saturation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.2 Negative Differential Resistance . . . . . . . . . . . . . . . . . . . 5.4.3 Gunn Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Magneto-Transport and the Hall Effect . . . . . . . . . . . . . . . . . . . . 5.5.1 Magneto-Conductivity Tensor . . . . . . . . . . . . . . . . . . . . . 5.5.2 Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5.3 Hall Coefficient for Thin Film Samples (van der Pauw Method) . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5.4 Hall Effect for a Distribution of Electron Energies . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 208 209 220 223 225 227 228 230 232 232 234 Optical Properties I 243 6.1 244 6.2 Macroscopic Electrodynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Digression: Units for the Frequency of Electromagnetic Waves . . . . . . . . . . . . . . . . . . . . . . . . 6.1.2 Experimental Determination of Optical Functions . . . . 6.1.3 Kramers–Kronig Relations . . . . . . . . . . . . . . . . . . . . . . . . The Dielectric Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Experimental Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.2 Microscopic Theory of the Dielectric Function . . . . . . . . 6.2.3 Joint Density of States and Van Hove Singularities . . . . 6.2.4 Van Hove Singularities in Âi . . . . . . . . . . . . . . . . . . . . . . . 6.2.5 Direct Absorption Edges . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.6 Indirect Absorption Edges . . . . . . . . . . . . . . . . . . . . . . . . 235 236 237 241 247 247 250 253 253 254 261 262 268 269 XVII XVIII Contents 6.2.7 “Forbidden” Direct Absorption Edges . . . . . . . . . . . . . . Excitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 Exciton Effect at M0 Critical Points . . . . . . . . . . . . . . . . . 6.3.2 Absorption Spectra of Excitons . . . . . . . . . . . . . . . . . . . . 6.3.3 Exciton Effect at M1 Critical Points or Hyperbolic Excitons . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.4 Exciton Effect at M3 Critical Points . . . . . . . . . . . . . . . . . 6.4 Phonon-Polaritons and Lattice Absorption . . . . . . . . . . . . . . . . . . 6.4.1 Phonon-Polaritons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4.2 Lattice Absorption and Reflection . . . . . . . . . . . . . . . . . . 6.4.3 Multiphonon Lattice Absorption . . . . . . . . . . . . . . . . . . . 6.4.4 Dynamic Effective Ionic Charges in Heteropolar Semiconductors . . . . . . . . . . . . . . . . . . . . 6.5 Absorption Associated with Extrinsic Electrons . . . . . . . . . . . . . 6.5.1 Free-Carrier Absorption in Doped Semiconductors . . . . 6.5.2 Absorption by Carriers Bound to Shallow Donors and Acceptors . . . . . . . . . . . . . . . . . . 6.6 Modulation Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.1 Frequency Modulated Reflectance and Thermoreflectance . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.2 Piezoreflectance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.3 Electroreflectance (Franz–Keldysh Effect) . . . . . . . . . . . 6.6.4 Photoreflectance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.5 Reflectance Difference Spectroscopy . . . . . . . . . . . . . . . 6.7 Addendum (Third Edition): Dielectric Function . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 303 305 306 Optical Properties II 345 7.1 345 351 354 356 362 369 375 6.3 7. Emission Spectroscopies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1.1 Band-to-Band Transitions . . . . . . . . . . . . . . . . . . . . . . . . . 7.1.2 Free-to-Bound Transitions . . . . . . . . . . . . . . . . . . . . . . . . 7.1.3 Donor–Acceptor Pair Transitions . . . . . . . . . . . . . . . . . . 7.1.4 Excitons and Bound Excitons . . . . . . . . . . . . . . . . . . . . . 7.1.5 Luminescence Excitation Spectroscopy . . . . . . . . . . . . . . 7.2 Light Scattering Spectroscopies . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.1 Macroscopic Theory of Inelastic Light Scattering by Phonons . . . . . . . . . . . . . 7.2.2 Raman Tensor and Selection Rules . . . . . . . . . . . . . . . . . 7.2.3 Experimental Determination of Raman Spectra . . . . . . 7.2.4 Microscopic Theory of Raman Scattering . . . . . . . . . . . . 7.2.5 A Detour into the World of Feynman Diagrams . . . . . . 7.2.6 Brillouin Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.7 Experimental Determination of Brillouin Spectra . . . . . 7.2.8 Resonant Raman and Brillouin Scattering . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 273 276 279 282 288 291 292 295 298 299 311 315 319 321 322 329 332 333 334 343 375 378 385 394 395 398 400 401 422 426 Contents 8. 9. Photoelectron Spectroscopy 8.1 Photoemission . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.1 Angle-Integrated Photoelectron Spectra of the Valence Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.2 Angle-Resolved Photoelectron Spectra of the Valence Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.3 Core Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Inverse Photoemission . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Surface Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.1 Surface States and Surface Reconstruction . . . . . . . . . . . 8.3.2 Surface Energy Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.3 Fermi Level Pinning and Space Charge Layers . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Effect of Quantum Confinement on Electrons and Phonons in Semiconductors 9.1 Quantum Confinement and Density of States . . . . . . . . . . . . . . . 9.2 Quantum Confinement of Electrons and Holes . . . . . . . . . . . . . . 9.2.1 Semiconductor Materials for Quantum Wells and Superlattices . . . . . . . . . . . . . . . 9.2.2 Classification of Multiple Quantum Wells and Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.3 Confinement of Energy Levels of Electrons and Holes . 9.2.4 Some Experimental Results . . . . . . . . . . . . . . . . . . . . . . . 9.3 Phonons in Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3.1 Phonons in Superlattices: Folded Acoustic and Confined Optic Modes . . . . . . . . . . 9.3.2 Folded Acoustic Modes: Macroscopic Treatment . . . . . . 9.3.3 Confined Optical Modes: Macroscopic Treatment . . . . . 9.3.4 Electrostatic Effects in Polar Crystals: Interface Modes . . . . . . . . . . . . . . . . . . 9.4 Raman Spectra of Phonons in Semiconductor Superlattices . . . . 9.4.1 Raman Scattering by Folded Acoustic Phonons . . . . . . . 9.4.2 Raman Scattering by Confined Optical Phonons . . . . . . 9.4.3 Raman Scattering by Interface Modes . . . . . . . . . . . . . . 9.4.4 Macroscopic Models of Electron–LO Phonon (Fröhlich) Interaction in Multiple Quantum Wells . . . . . 9.5 Electrical Transport: Resonant Tunneling . . . . . . . . . . . . . . . . . . . 9.5.1 Resonant Tunneling Through a Double-Barrier Quantum Well . . . . . . . . . . . 9.5.2 I–V Characteristics of Resonant Tunneling Devices . . . . 9.6 Quantum Hall Effects in Two-Dimensional Electron Gases . . . . 9.6.1 Landau Theory of Diamagnetism in a Three-Dimensional Free Electron Gas . . . . . . . . . . . 9.6.2 Magneto-Conductivity of a Two-Dimensional Electron Gas: Filling Factor . . . . 427 431 440 443 451 456 457 457 458 460 465 468 469 470 473 474 478 479 489 494 494 499 500 502 511 511 516 518 521 525 526 529 533 534 537 XIX XX Contents 9.6.3 9.6.4 The Experiment of von Klitzing, Pepper and Dorda . . . Explanation of the Hall Plateaus in the Integral Quantum Hall Effect . . . . . . . . . . . . . . . . 9.7 Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Appendix A: Pioneers of Semiconductor Physics Remember… Ultra-Pure Germanium: From Applied to Basic Research or an Old Semiconductor Offering New Opportunities By Eugene E. Haller . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Two Pseudopotential Methods: Empirical and Ab Initio By Marvin L. Cohen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Early Stages of Band-Structures Physics and Its Struggles for a Place in the Sun By Conyers Herring . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Cyclotron Resonance and Structure of Conduction and Valence Band Edges in Silicon and Germanium By Charles Kittel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Optical Properties of Amorphous Semiconductors and Solar Cells By Jan Tauc . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Optical Spectroscopy of Shallow Impurity Centers By Elias Burstein . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . On the Prehistory of Angular Resolved Photoemission By Neville V. Smith . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Discovery and Very Basics of the Quantum Hall Effect By Klaus von Klitzing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Birth of the Semiconductor Superlattice By Leo Esaki . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 538 541 545 546 551 553 555 558 560 563 566 569 574 576 578 Appendix B: Solutions to Some of the Problems 583 Appendix C: Recent Development 673 Appendix D: Recent Developments and References 687 References 719 Subject Index 755 1. Introduction CONTENTS 1.1 A Survey of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 1.2 Growth Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 In textbooks on solid-state physics, a semiconductor is usually defined rather loosely as a material with electrical resistivity lying in the range of 102 109 ø cm.1 Alternatively, it can be defined as a material whose energy gap (to be defined more precisely in Chap. 2) for electronic excitations lies between zero and about 4 electron volts (eV). Materials with zero bandgap are metals or semimetals, while those with an energy gap larger than 3 eV are more frequently known as insulators. There are exceptions to these definitions. For example, terms such as semiconducting diamond (whose energy gap is about 6 eV) and semi-insulating GaAs (with a 1.5 eV energy gap) are frequently used. GaN, which is receiving a lot of attention as optoelectronic material in the blue region, has a gap of 3.5 eV. The best-known semiconductor is undoubtedly silicon (Si). However, there are many semiconductors besides silicon. In fact, many minerals found in nature, such as zinc-blende (ZnS) cuprite (Cu2 O) and galena (PbS), to name just a few, are semiconductors. Including the semiconductors synthesized in laboratories, the family of semiconductors forms one of the most versatile class of materials known to man. Semiconductors occur in many different chemical compositions with a large variety of crystal structures. They can be elemental semiconductors, such as Si, carbon in the form of C60 or nanotubes and selenium (Se) or binary compounds such as gallium arsenide (GaAs). Many organic compounds, e. g. polyacetylene (CH)n , are semiconductors. Some semiconductors exhibit magnetic (Cd1x Mnx Te) or ferroelectric (SbSI) behavior. Others become superconductors when doped with sufficient carriers (GeTe and SrTiO3 ). Many of the recently discovered high-Tc superconductors have nonmetallic phases which are semiconductors. For example, La2 CuO4 is a semiconductor (gap 2 eV) but becomes a superconductor when alloyed with Sr to form (La1x Srx )2 CuO4 . 1 ø cm is a “hybrid” SI and cgs resistivity unit commonly used in science and engineering. The SI unit for resistivity should be ø m P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed., DOI 10.1007/978-3-642-00710-1_1, © Springer-Verlag Berlin Heidelberg 2010 2 1. Introduction 1.1 A Survey of Semiconductors The following is a brief survey of several types of the better-known semiconductors. 1.1.1 Elemental Semiconductors The best-known semiconductor is of course the element Si. Together with germanium (Ge), it is the prototype of a large class of semiconductors with similar crystal structures. The crystal structure of Si and Ge is the same as that of diamond and ·-tin (a zero-gap semiconductor also known as “gray” tin). In this structure each atom is surrounded by four nearest neighbor atoms (each atom is said to be four-fold coordinated), forming a tetrahedron. These tetrahedrally bonded semiconductors form the mainstay of the electronics industry and the cornerstone of modern technology. Most of this book will be devoted to the study of the properties of these tetrahedrally bonded semiconductors. Some elements from the groups V and VI of the periodical table, such as phosphorus (P), sulfur (S), selenium (Se) and tellurium (Te), are also semiconductors. The atoms in these crystals can be three-fold (P), two-fold (S, Se, Te) or four-fold coordinated. As a result, these elements can exist in several different crystal structures and they are also good glass-formers. For example, Se has been grown with monoclinic and trigonal crystal structures or as a glass (which can also be considered to be a polymer). 1.1.2 Binary Compounds Compounds formed from elements of the groups III and V of the periodic table (such as GaAs) have properties very similar to their group IV counterparts. In going from the group IV elements to the III–V compounds, the bonding becomes partly ionic due to transfer of electronic charge from the group III atom to the group V atom. The ionicity causes significant changes in the semiconductor properties. It increases the Coulomb interaction between the ions and also the energy of the fundamental gap in the electronic band structure. The ionicity becomes even larger and more important in the II–VI compounds such as ZnS. As a result, most of the II–VI compound semiconductors have bandgaps larger than 1 eV. The exceptions are compounds containing the heavy element mercury (Hg). Mercury telluride (HgTe) is actually a zerobandgap semiconductor (or a semimetal) similar to gray tin. While the large bandgap II–VI compound semiconductors have potential applications for displays and lasers, the smaller bandgap II–VI semiconductors are important materials for the fabrication of infrared detectors. The I–VII compounds (e. g., CuCl) tend to have even larger bandgaps (3 eV) as a result of their higher 1.1 A Survey of Semiconductors ionicity. Many of them are regarded as insulators rather than semiconductors. Also, the increase in the cohesive energy of the crystal due to the Coulomb interaction between the ions favors the rock-salt structure containing six-fold coordinated atoms rather than tetrahedral bonds. Binary compounds formed from group IV and VI elements, such as lead sulfide (PbS), PbTe and tin sulfide (SnS), are also semiconductors. The large ionicity of these compounds also favors six-fold coordinated ions. They are similar to the mercury chalcogenides in that they have very small bandgaps in spite of their large ionicity. These small bandgap IV–VI semiconductors are also important as infrared detectors. GaN, a large bandgap III–V compound, and the mixed crystals Ga1x Inx N are being used for blue light emitting diodes and lasers [1.1]. 1.1.3 Oxides Although most oxides are good insulators, some, such as CuO and Cu2 O, are well-known semiconductors. Since cuprous oxide (Cu2 O) occurs as a mineral (cuprite), it is a classic semiconductor whose properties have been studied extensively. In general, oxide semiconductors are not well understood with regard to their growth processes, so they have limited potential for applications at present. One exception is the II–VI compound zinc oxide (ZnO), which has found application as a transducer and as an ingredient of adhesive tapes and sticking plasters. However, this situation has changed with the discovery of superconductivity in many oxides of copper. The first member of these so-called high-Tc superconductors, discovered by Müller and Bednorz2 , is based on the semiconductor lanthanum copper oxide (La2 CuO4 ), which has a bandgap of about 2 eV. Carriers in the form of holes are introduced into La2 CuO4 when trivalent lanthanum (La) is replaced by divalent barium (Ba) or strontium (Sr) or when an excess of oxygen is present. When sufficient carriers are present the semiconductor transforms into a superconducting metal. So far the highest superconducting transition temperature at ambient pressure (Tc 135 K) found in this family of materials belongs to HgBaCa2 Cu3 O8‰ . HgBaCa2 Cu3 O8‰ reaches a Tc 164 K under high pressure [1.2]. At the time this third edition went into print this record had not yet been broken. 1.1.4 Layered Semiconductors Semiconducting compounds such as lead iodide (PbI2 ), molybdenum disulfide (MoS2 ) and gallium selenide (GaSe) are characterized by their layered crystal structures. The bonding within the layers is typically covalent and much stronger than the van der Waals forces between the layers. These layered semiconductors have been of interest because the behavior of electrons in the layers is quasi-two-dimensional. Also, the interaction between layers can be mod2 For this discovery, Bednorz and Müller received the Physics Nobel Prize in 1987. 3 4 1. Introduction ified by incorporating foreign atoms between the layers in a process known as intercalation. 1.1.5 Organic Semiconductors Many organic compounds such as polyacetylene [(CH2 )n ] and polydiacetylene are semiconductors. Although organic semiconductors are not yet used in any electronic devices, they hold great promise for future applications. The advantage of organic over inorganic semiconductors is that they can be easily tailored to the applications. For example, compounds containing conjugate bonds such as –C=C–C= have large optical nonlinearities and therefore may have important applications in opto-electronics. The bandgaps of these compounds can be changed more easily than those of inorganic semiconductors to suit the application by changing their chemical formulas. Recently new forms of carbon, such as C60 (fullerene), have been found to be semiconductors. One form of carbon consists of sheets of graphite rolled into a tube of some nanometers in diameter known as nanotubes [1.3,4]. These carbon nanotubes and their “cousin”, BN nanotubes, hold great promise as nanoscale electronic circuit elements. They can be metals or semiconductors depending on their pitch. 1.1.6 Magnetic Semiconductors Many compounds containing magnetic ions such as europium (Eu) and manganese (Mn), have interesting semiconducting and magnetic properties. Examples of these magnetic semiconductors include EuS and alloys such as Cd1x Mnx Te. Depending on the amount of the magnetic ion in these alloys, the latter compounds exhibit different magnetic properties such as ferromagnetism and antiferromagnetism. The magnetic alloy semiconductors containing lower concentrations of magnetic ions are known as dilute magnetic semiconductors. These alloys have recently attracted much attention because of their potential applications. Their Faraday rotations can be up to six orders of magnitude larger than those of nonmagnetic semiconductors. As a result, these materials can be used as optical modulators, based on their large magnetooptical effects. The perovskites of the type Mn0.7 Ca0.3 O3 undergo metal–semiconductor transitions which depend strongly on magnetic field, giving rise to the phenomenon of collossal magneto-resistance (CMR) [1.5]. 1.1.7 Other Miscellaneous Semiconductors There are many semiconductors that do not fall into the above categories. For example, SbSI is a semiconductor that exhibits ferroelectricity at low temperatures. Compounds with the general formula I–III–VI2 and II–IV–V2 (such as AgGaS2 , interesting for its nonlinear optical properties, CuInSe2 , useful for solar cells, and ZnSiP2 ) crystallize in the chalcopyrite structure. The bonding in these compounds is also tetrahedral and they can be considered as analogs 1.2 Growth Techniques of the group III–V and II–VI semiconductors with the zinc-blende structure. Compounds formed from the group V and VI elements with formulas such as As2 Se3 are semiconductors in both the crystalline and glassy states. Many of these semiconductors have interesting properties but they have not yet received much attention due to their limited applications. Their existence shows that the field of semiconductor physics still has plenty of room for growth and expansion. 1.2 Growth Techniques One reason why semiconductors have become the choice material for the electronics industry is the existence of highly sophisticated growth techniques. Their industrial applications have, in turn, led to an increased sophistication of these techniques. For example, Ge single crystals are nowadays amongst the purest elemental materials available as a result of years of perfecting their growth techniques (see Appendix by E.E. Haller in p. 555). It is now possible to prepare almost isotopically pure Ge crystals (natural Ge contains five different isotopes). Nearly perfect single crystals of Si can be grown in the form of ingots over twelve inches (30 cm) in diameter. Isotopically pure 28 Si crystals have been shown to have considerably higher thermal conductivity than their natural Si counterparts [1.6]. Dislocation densities in these crystals can be as low as 1000 cm3 , while impurity concentrations can be less than one part per trillion (1012 ). More recent developments in crystal growth techniques have made semiconductors even more versatile. Techniques such as Molecular Beam Epitaxy (MBE) and Metal-Organic Chemical Vapor Deposition (MOCVD) allow crystals to be deposited on a substrate one monolayer at a time with great precision. These techniques have made it possible to synthesize artificial crystal structures known as superlattices and quantum wells (Chap. 9). A recent advance in fabricating low-dimensional nanostructures takes advantage of either alignment of atoms with the substrate or strain between substrate and epilayer to induce the structure to self-organize into superlattices or quantum dots. Although a detailed discussion of all the growth techniques is beyond the scope of this book, a short survey of the most common techniques will provide background information necessary for every semiconductor physicist. The references given for this chapter provide further background material for the interested reader. 1.2.1 Czochralski Method The Czochralski method is the most important method for growing bulk crystals of semiconductors, including Si. The method involves melting the raw ma- 5 6 1. Introduction 2–50 rpm Fig. 1.1. Schematic diagram of a Czochralski furnace for growing Si single crystals Si seed Si single crystal SiO2 crucible Si melt Heater Susceptor (graphite) Inert Gas (Ar) terial in a crucible. A seed crystal is placed in contact with the top, cooler region of the melt and rotated slowly while being gradually pulled from the melt. Additional material is solidified from the melt onto the seed. The most significant development in the Czochralski technique [1.7] (shown schematically in Fig. 1.1) is the discovery of the Dash technique [1.8,9] for growing dislocation-free single crystals of Si even when starting with a dislocated seed. Typical growth speed is a few millimeters per minute, and the rotation ensures that the resultant crystals are cylindrical. Silicon ingots grown by this method now have diameters greater than 30 cm. The crucible material and gas surrounding the melt tend to contribute to the background impurities in the crystals. For example, the most common impurities in bulk Si are carbon (from the graphite crucible) and oxygen. Bulk GaAs and indium phosphide (InP) crystals are commonly grown by the Czochralski method but with the melt isolated from the air by a layer of molten boron oxide to prevent the volatile anion vapor from escaping. This method of growing crystals containing a volatile constituent is known as the Liquid-Encapsulated Czochralski (LEC) Method. As expected, LEC-grown GaAs often contains boron as a contaminant. 1.2.2 Bridgman Method In the Bridgman method a seed crystal is usually kept in contact with a melt, as in the Czochralski method. However, a temperature gradient is created along the length of the crucible so that the temperature around the seed crystal is below the melting point. The crucible can be positioned either horizontally or vertically to control convection flow. As the seed crystal grows, the temperature profile is translated along the crucible by controlling the heaters 1.2 Growth Techniques along the furnace or by slowly moving the ampoule containing the seed crystal within the furnace. 1.2.3 Chemical Vapor Deposition Both the Czochralski and Bridgman techniques are used to grow bulk single crystals. It is less expensive to grow a thin layer of perfect crystal than a large perfect bulk crystal. In most applications devices are fabricated out of a thin layer grown on top of a bulk crystal. The thickness of this layer is about 1 Ìm or less. Economically, it makes sense to use a different technique to grow a thin high quality layer on a lower quality bulk substrate. To ensure that this thin top layer has high crystalline quality, the crystal structure of the thin layer should be similar, if not identical, to the substrate and their lattice parameters as close to each other as possible to minimize strain. In such cases the atoms forming the thin layer will tend to build a single crystal with the same crystallographic orientation as the substrate. The resultant film is said to be deposited epitaxially on the substrate. The deposition of a film on a bulk single crystal of the same chemical composition (for example, a Si film deposited on a bulk Si crystal) is known as homo-epitaxy. When the film is deposited on a substrate of similar structure but different chemical composition (such as a GaAs film on a Si substrate), the growth process is known as hetero-epitaxy. Epitaxial films can be grown from solid, liquid or gas phases. In general, it is easier to precisely control the growth rate in gas phase epitaxy by controlling the amount of gas flow. In Chemical Vapor Deposition (CVD) gases containing the required chemical elements are made to react in the vicinity of the substrate. The semiconductor produced as a result of the reaction is deposited as a thin film on a substrate inside the reactor. The temperature of the substrate is usually an important factor in determining the epitaxy and hence the quality of the resultant film. The most common reaction for producing a Si film in this way is given by SiH4 (silane) heat Si + 2H2↑ . ↓ substrate (1.1) Highly pure Si can be produced in this way because the reaction by-product H2 is a gas and can be easily removed. Another advantage of this technique is that dopants, such as P and As, can be introduced very precisely in the form of gases such as phosphine (PH3 ) and arsine (AsH3 ). III–V compound semiconductors can also be grown by CVD by using gaseous metal-organic compounds like trimethyl gallium [Ga(CH3 )3 ] as sources. For example, GaAs films can be grown by the reaction Ga(CH3 )3 AsH3 → 3CH4 ↑ GaAs. (1.2) 7 8 1. Introduction Pressure Gauge Pump (a) Filter GaAs RF heater Purified H2 AsH3 + H2 Ga(CH3)3 + H2 (b) PH3 + H2 (c) Subflow N2+H2 Stainless steel chamber Substrate Rotating susceptor Heater Vacuum pump Conical quartz tube Subflow N 2+H 2 Main flow TMG+NH3 +H2 IR Radiation Thermometer Main Flow TMG+NH3 +H2 Substrate Susceptor Quartz nozzle Exhaust Fig. 1.2. (a) Schematic diagram of a MOCVD apparatus [1.10]. (b) Details of twoflow MOCVD machine introduced by Nakamura and co-workers for growing GaN. (c) Schematic diagram of the gas flows near the substrate surface [1.11] This method of growing epitaxial films from metal-organic gases is known as Metal-Organic Chemical Vapor Deposition (MOCVD), and a suitable growth apparatus is shown schematically in Fig. 1.2a. A recent modification introduced for growing GaN is shown in Fig. 1.2b. Figure 1.2c shows the details of interaction between the two gas flows near the substrate [1.11]. 1.2.4 Molecular Beam Epitaxy In CVD the gases are let into the reactor at relatively high pressure (typically higher than 1 torr). As a result, the reactor may contain a high concentration of contaminants in the form of residual gases. This problem can be avoided by growing the sample under UltraHigh Vacuum (UHV) conditions. (Pressures below 107 torr are considered high vacuum, and a base pressure 1.2 Growth Techniques 10 mm Nozzle Alumina insulators Thermocouple Ta radiation collector Ta radiation shields Heater Fig. 1.3. Schematic diagram of an effusion (Knudsen) cell [1.10] around 1011 torr is UHV. See Sect. 8.1 for further discussion of UHV conditions and the definition of torr.) The reactants can be introduced in the form of molecular beams. A molecular beam is created by heating a source material until it vaporizes in a cell with a very small orifice. Such a cell is known as an effusion (or Knudsen) cell and is shown schematically in Fig. 1.3. As the vapor escapes from the cell through the small nozzle, its molecules (or atoms) form a well-collimated beam, since the UHV environment outside the cell allows the escaping molecules (or atoms) to travel ballistically for meters without collision. Typically several molecular beams containing the necessary elements for forming the semiconductor and for doping the sample are aimed at the substrate, where the film grows epitaxially. Hence this growth technique is known as Molecular Beam Epitaxy (MBE). Figure 1.4 shows the construction of a typical MBE system. In principle, it is difficult to control the concentration of reactants arriving at the substrate, and hence the crystal stoichiometry, in MBE growth. The technique works because its UHV environment makes it possible to utilize electrons and ions as probes to monitor the surface and film quality during growth. The ion-based probe is usually mass spectrometry. Some of the electron based techniques are Auger Electron Spectroscopy (AES), Low Energy-Electron Diffraction (LEED), Reflection High-Energy Electron Diffraction (RHEED), and X-ray and Ultraviolet Photoemission Spectroscopy (XPS and UPS). These techniques will be discussed in more detail in Chap. 8. The one most commonly used in MBE systems is RHEED. A typical RHEED system consists of an electron gun producing a highenergy (10–15 keV) beam aimed at a very large angle of incidence (grazing incidence) to the substrate surface (see Fig. 1.4). The reflected electron diffraction pattern is displayed on a phosphor screen (labeled RHEED screen in Fig. 1.4) on the opposite side. This diffraction pattern can be used to establish the surface geometry and morphology. In addition, the intensity of the zerothorder diffraction beam (or specular beam) has been found to show damped 9 1. Introduction View port MBE sources Water-cooled thermal isolators UHV pump RHEED screen Shutters Electron gun Substrate stage UHV pump Beam monitoring ion gauge Rough pump Sample exchange mechanism Sample entry lock Fig. 1.4. Schematic diagram of a typical MBE system [1.10] Ga on Al on Intensity 10 Al off Ga off 0 5 10 Time [s] 15 20 Fig. 1.5. Oscillations in the intensity of the specularly reflected electron beam in the RHEED pattern during the growth of a GaAs or AlAs film on a GaAs(001) substrate. One period of oscillation corresponds precisely to the growth of a single layer of GaAs or AlAs [1.10] 1.2 Growth Techniques oscillations (known as RHEED oscillations) that allow the film growth rate to be monitored in situ. Figure 1.5 shows an example of RHEED oscillations measured during the growth of a GaAs/AlAs quantum well. Quantum wells are synthetic structures containing a very thin layer (thickness less than 10 nm) of semiconductor sandwiched between two thin layers of another semiconductor with a larger bandgap (see Chap. 9 for further discussion). Each oscillation in Fig. 1.5 corresponds to the growth of a single molecular layer of GaAs or AlAs. To understand how such perfectly stoichiometric layers can be grown, we note that the Ga or Al atoms attach to a GaAs substrate much more readily than the As atoms. Since arsenic is quite volatile at elevated temperatures, any arsenic atoms not reacted with Ga or Al atoms on the substrate will not be deposited on a heated substrate. By controlling the molecular beams with shutters and monitoring the growth via RHEED oscillations, it is possible to grow a thin film literally one monolayer at a time. The MBE technique is used for the growth of high-quality quantum wells. The only drawback of this technique in commercial applications is its slow throughput and high cost (a typical MBE system costs a least US $ 500 000). As a result, the MBE technique is utilized to study the conditions for growing high-quality films in the laboratory but large-scale commercial production of the films uses the MOCVD method. 1.2.5 Fabrication of Self-Organized Quantum Dots by the Stranski–Krastanow Growth Method The epitaxial growth of a thin film A on a substrate B can occur in one of three main growth modes: (1) monolayer or two-dimensional growth; (2) three-dimensional growth or Volmer–Weber mode and (3) Stranski– Krastanow mode [1.12]. In mode (1) the atoms of A are attracted to the substrate more strongly than to each other. As a result the atoms first aggregate to form monolayer islands which then expand and coalesce to form the first monolayer. In mode (2) the atoms of A are attracted more strongly to each other than to the substrate. Thus they will first aggregate to form islands and as deposition continues these islands will grow and finally form a continuous film. In case of mode (3) the atoms of A will first grow two-dimensionally to form either a single monolayer or a small number of monolayers thin film. However, when growth proceeds further the additional atoms of A start to form three-dimensional islands on top of the thin film as in the Volmer–Weber mode. The continuous thin film is often referred to as the wetting layer. One important factor which controls the growth of an epitaxial film is the lattice mismatch between the epitaxial layer A and the substrate B. Let us assume that the lattice mismatch between A and B is not too large, say only around 1% of their lattice constants. There are at least two possible ways for a thin film of A to grow on B. The first possibility is for atoms of A to line up on top of the corresponding atoms of B and to take on the lattice con- 11 12 1. Introduction stant of B. In this case the film A is strained but pseudomorphic (a pseudomorph is an altered crystal form whose outward appearance is the same of another crystal species). In the second possibility the atoms of A retain their bulk lattice constant and therefore are out of registry with the substrate atoms. To minimize this mismatch between the two kinds of atoms, the thin film A will develop a kind of lattice defect known as a dislocation (see also Chap. 4) [1.13]. For example, if the lattice constant of A is smaller than B then the mismatch can be compensated by periodically inserting an extra plane of atoms of A into the film A to bring its atoms into alignment with the substrate atoms again. This kind of dislocation is known as a misfit dislocation. Since the lattice mismatch between A and B occurs in two directions lying within the surface, these dislocations form a two-dimensional network. The competition between these two growth modes for lattice-mismatched systems was studied by Frank and van der Merwe in 1949 [1.14]. The trade-off is between the strain energy in the strained pseudomorphic film and the energy required to form misfit dislocations in the unstrained film. The strain energy increases with the volume of the film while the dislocation energy depends only on the area of the film. As a result pseudomorphic growth dominates when the film thickness is small. However, as the film thickness increases it will become energetically more favorable for dislocations to form. One may expect this “cross-over” to occur at some critical layer thickness. The calculation of this critical thickness [1.13] is beyond the scope of this book. The above consideration may suggest that the Stranski–Krastanow growth mode is undesirable for achieving an epitaxial film of uniform thickness. Recently it was found that this growth mode is a convenient and inexpensive way to produce nanometer structures known as quantum dots [1.15]. In this case the lattice constant of the epi-layer A has to be larger than that of the substrate B. The atoms of A can relax the tensile strain by “buckling” to form islands. The principle behind this island formation is similar to the buckling of a bi-metallic bar with increase in temperature, an effect used in making temperature sensors and thermostats. Since these quantum dots are formed spontaneously and can also be formed coherently, their formation is an example of a phenomenon in crystal growth known as self-organization. Figure 1.6 shows a plane-view transmission electro-microscope (TEM) image of a single sheet of InAs (film A with lattice constant 6.06 Å) quantum dots grown on GaAs substrate (B with lattice constant 5.64 Å). Figure 1.7 shows the cross-sectional TEM image of a 25 layers thick stack of InGaAs quantum dots (the thicker part of the dark regions) grown on a GaAs substrate. Notice that the quantum dots are connected within the layers by thin dark regions representing the wetting layers. The various layers are separated by GaAs represented by the lighter regions. The quantum dots in Fig. 1.7 are aligned on top of each other to form arrays by the tensile strain which is transmitted through the thin GaAs layers. The coherence is gradually lost as the layers get farther from the substrate. In addition to quantum dot arrays, monolayer superlattices, such as GaP/InP, can also be grown by self-organization. 1.2 Growth Techniques Fig. 1.6. A plane-view transmission electromicroscope (TEM) image of a single sheet of InAs quantum dots grown on a [100]-oriented GaAs substrate. Reproduced from [1.15] Fig. 1.7. A cross-sectional TEM image of a 25-layer thick stack of InGaAs quantum dots (the thicker dark regions) grown on GaAs substrate (lighter area near the bottom of the picture). The lighter regions surrounding the InGaAs layers are also GaAs. Reproduced from [1.15] 1.2.6 Liquid Phase Epitaxy Semiconductor films can also be grown epitaxially on a substrate from the liquid phase. This Liquid Phase Epitaxy (LPE) growth technique has been very successful in growing GaAs laser diodes. Usually a group III metal, such as Ga or In, is utilized as the solvent for As. When the solvent is cooled in contact with a GaAs substrate it becomes supersaturated with As and nucleation of 13 14 1. Introduction Graphite Slider Thermocouple GaAs substrate Ga melt with As, Al and dopants Fig. 1.8. Setup for LPE crystal growth GaAs starts on the substrate. By using a slider containing several different solutes (as shown in Fig. 1.8), successive epitaxial layers (or epilayers in short) of different compositions and/or different dopants can be grown. The advantage of LPE is that the equipment required is inexpensive and easy to set up. However, it is difficult to achieve the level of control over the growth conditions possible with the MBE technique. In summary, different techniques are employed to grow bulk single crystals and thin epilayers of semiconductors. The Czochralski or Bridgman techniques are used to grow bulk crystals. When feasible, the LPE method is prefered for growing thin films because of its low cost and fast growth rate. When epilayers of thickness less than 100 nm are required, it is necessary to utilize the MOCVD or MBE techniques. In recent years optical mirror furnaces have become very popular for the growth of oxide semiconductors [1.16]. SUMMARY In this chapter we have introduced the wide class of materials referred to as semiconductors and we have mentioned the large range of structural and physical properties they can have. Most of the semiconductors used in science and modern technology are single crystals, with a very high degree of perfection and purity. They are grown as bulk three-dimensional crystals or as thin, two-dimensional epitaxial layers on bulk crystals which serve as substrates. Among the techniques for growing bulk crystals that we have briefly discussed are the Czochralski and Bridgman methods. Epitaxial techniques for growing two-dimensional samples introduced in this chapter include chemical vapor deposition, molecular beam epitaxy, and liquid phase epitaxy. Self-organized two-dimensional lattices of quantum dots can also be grown with epitaxial techniques. Summary Periodic Table of “Semiconductor-Forming” Elements I II III IV VI V VII 0 VIII H1 2 He2 1s 1s 4 3 5 Be2 2s 2s 2p Na11 12 Mg 2 3s2 3p K19 20 Ca 2 Li 2s 3s B 2 13 Al 3s 4s Sc2 21 4s 29 Cu 10 4s 3d 37 Rb 5s Ag47 10 5s4d Cs55 6s Au79 10 6s5d 4s 3d 31 30 Zn Ga2 2 10 4s 3d 38 4s 4p Y39 Sr 2 5s24d 5s 48 Cd 5s2 6s Si14 3s2 3p2 Ti 22 4s2 3d2 32 Ge 2 2 4s 4p Zr40 5s2 4d2 5s 5p 5s 5p 80 Hg 10 Tl2 81 2 6s 5d 2s 2p 50 In2 491 Sn 2 2 La 57-71 Series Ba56 2 6 C 2 2 6s 6p Hf2 722 6s 5d 4f14 82 Pb 2 2 6s 6p 7 N 2 3 8 O 4 2 2s 2p 2s 2p P15 S16 3s2 3p3 V 3s2 3p4 23 4s 23d 3 33 As 4s2 4p3 Nb414 5s 4d 51 Sb 2 3 5s 5p Ta2 733 6s 5d Bi 83 6s2 6p3 Cr2 244 4s 3d 34 Se 2 4 4s 4p Mo425 5s4d 52 Te2 5s 5p4 W 74 6s25d4 Po84 6s2 6p4 F2 9 5 10 Ne 2 6 2s 2p 2s 2p Cl17 Ar18 3s2 3p5 3s2 3p6 27 25 Ni 28 Fe2 266 Co Mn 2 5 4s 23d7 4s 23d8 4s 3d 4s 3d Br35 Kr36 4s2 4p5 4s2 4p6 Tc436 Ru447 Rh458 Pd1046 5s4d 5s 4d 5s 4d 4d I 53 Xe54 5s2 5p5 5s2 5p6 Re75 Os76 Ir77 Pt 789 9 6s25d5 6s25d6 5d At85 6s 2 6p5 Elements which crystallize as Semiconductors Elements forming Binary III-V Semiconductors Elements forming Binary III-VI Semiconductors Elements forming Binary II-VI Semiconductors Elements forming Binary I-VII Semiconductors Elements forming Binary IV-VI Semiconductors Elements forming I-III-VI2 Chalcopyrite Semiconductors Elements forming II-VI-V2 Chalcopyrite Semiconductors 6s 5d 86 Rn 6 2 6s 6p 15 2. Electronic Band Structures CONTENTS 2.1 2.2 2.3 2.4 2.5 2.6 2.7 Quantum Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18 Translational Symmetry and Brillouin Zones . . . . . . . . . . . . . . . . . . . . . . 20 A Pedestrian’s Guide to Group Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . 25 Empty Lattice or Nearly Free Electron Energy Bands . . . . . . . . . . . . 48 Band Structure Calculations by Pseudopotential Methods . . . . . . . . 58 The k·p Method of Band-Structure Calculations . . . . . . . . . . . . . . . . . . 68 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 83 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 96 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 The property which distinguishes semiconductors from other materials concerns the behavior of their electrons, in particular the existence of gaps in their electronic excitation spectra. The microscopic behavior of electrons in a solid is most conveniently specified in terms of the electronic band structure. The purpose of this chapter is to study the band structure of the most common semiconductors, namely, Si, Ge, and related III–V compounds. We will begin with a quick introduction to the quantum mechanics of electrons in a crystalline solid. The properties of electrons in a solid containing 1023 atoms/cm3 are very complicated. To simplify the formidable task of solving the wave equations for the electrons, it is necessary to utilize the translational and rotational symmetries of the solid. Group theory is the tool that facilitates this task. However, not everyone working with semiconductors has a training in group theory, so in this chapter we will discuss some basic concepts and notations of group theory. Our approach is to introduce the ideas and results of group theory when applied to semiconductors without presenting the rigorous proofs. We will put particular emphasis on notations that are often found in books and research articles on semiconductors. In a sense, band structure diagrams are like maps and the group theory notations are like symbols on the map. Once the meaning of these symbols is understood, the band structure diagrams can be used to find the way in exploring the electronic properties of semiconductors. We will also examine several popular methods of band structure computation for semiconductors. All band structure computation techniques involve approximations which tend to emphasize some aspects of the electronic propP.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed., DOI 10.1007/978-3-642-00710-1_2, © Springer-Verlag Berlin Heidelberg 2010 18 2. Electronic Band Structures erties in semiconductors while, at the same time, de-emphasizing other aspects. Therefore, our purpose in studying the different computational methods is to understand their advantages and limitations. In so doing we will gain insight into the many different facets of electronic properties in semiconductors. We note also that within the past two decades, highly sophisticated techniques labeled “ab initio” have been developed successfully to calculate many properties of solids, including semiconductors. These techniques involve very few assumptions and often no adjustable parameters. They have been applied to calculate the total energy of crystals including all the interactions between the electrons and with the nuclei. By minimization of this energy as a function of atomic spacing, equilibrium lattice constants have been predicted. Other properties such as the elastic constants and vibrational frequencies can also be calculated. Extensions of these techniques to calculate excited-state properties have led to predictions of optical and photoemission spectra in good agreement with experimental results. It is beyond the scope of the present book to go into these powerful techniques. Interested readers can consult articles in [2.1]. 2.1 Quantum Mechanics The Hamiltonian describing a perfect crystal can be written as p2 Pj2 Zj Zj e2 1 i 2mi 2Mj 2 4Â0 |Rj Rj | i j j, i j, j Zj e2 1 e2 4Â0 |ri Rj | 2 4Â0 |ri ri | (2.1) i, i in the cgs system of units. (As mentioned in the preface to this edition, we have printed in red symbols which must be added to the cgs expression to convert them into Si units. Â0 represents the permittivity of vacuum). In this expression ri denotes the position of the ith electron, Rj is the position of the jth nucleus, Zj is the atomic number of the nucleus, pi and Pj are the momentum operators of the electrons and nuclei, respectively, and e is the electronic charge. means that the summation is only over pairs of indices which are not identical. Obviously, the many-particle Hamiltonian in (2.1) cannot be solved without a large number of simplifications. The first approximation is to separate electrons into two groups: valence electrons and core electrons. The core electrons are those in the filled orbitals, e. g. the 1s2 , 2s2 , and 2p6 electrons in the case of Si. These core electrons are mostly localized around the nuclei, so they can be “lumped” together with the nuclei to form the so-called ion cores. As a result of this approximation the indices j and j in (2.1) will, from now on, denote the ion cores while the electron indices i and i will label only the valence 2.1 Quantum Mechanics electrons. These are electrons in incompletely filled shells and in the case of Si include the 3s and 3p electrons. The next approximation invoked is the Born–Oppenheimer or adiabatic approximation. The ions are much heavier than the electrons, so they move much more slowly. The frequencies of ionic vibrations in solids are typically less than 1013 s1 . To estimate the electron response time, we note that the energy required to excite electrons in a semiconductor is given by its fundamental bandgap, which, in most semiconductors, is of the order of 1 eV. Therefore, the frequencies of electronic motion in semiconductors are of the order of 1015 s1 (a table containing the conversion factor from eV to various other units can be found in the inside cover of this book). As a result, electrons can respond to ionic motion almost instantaneously or, in other words, to the electrons the ions are essentially stationary. On the other hand, ions cannot follow the motion of the electrons and they see only a time-averaged adiabatic electronic potential. With the Born-Oppenheimer approximation the Hamiltonian in (2.1) can be expressed as the sum of three terms: ions (Rj ) e (ri , Rj0 ) eion (ri , ‰Rj ), (2.2) where ion (Rj ) is the Hamiltonian describing the ionic motion under the influence of the ionic potentials plus the time-averaged adiabatic electronic potentials. e (ri , Rj0 ) is the Hamiltonian for the electrons with the ions frozen in their equilibrium positions Rj0 , and eion (ri , ‰Rj ) describes the change in the electronic energy as a result of the displacements ‰Rj of the ions from their equilibrium positions. eion is known as the electron–phonon interaction and is responsible for electrical resistance in reasonably pure semiconductors at room temperature. The vibrational properties of the ion cores and electronphonon interactions will be discussed in the next chapter. In this chapter we will be mainly interested in the electronic Hamiltonian e . The electronic Hamiltonian e is given by p2 Z j e2 1 e2 i . (2.3) e 2mi 2 4Â0 |ri ri | 4Â0 |ri Rj0 | i i, i i, j Diagonalizing this Hamiltonian when there are 1023 electrons/cm3 in a semiconductor is a formidable job. We will make a very drastic approximation known as the mean-field approximation. Without going into the justifications, which are discussed in many standard textbooks on solid-state physics, we will assume that every electron experiences the same average potential V(r). Thus the Schrödinger equations describing the motion of each electron will be identical and given by 1e ºn (r) p2 V(r) ºn (r) En ºn (r), 2m (2.4) where 1e , ºn (r) and En denote, respectively, the one-electron Hamiltonian, and the wavefunction and energy of an electron in an eigenstate labeled by n. 19 20 2. Electronic Band Structures We should remember that each eigenstate can only accommodate up to two electrons of opposite spin (Pauli’s exclusion principle). The calculation of the electronic energies En involves two steps. The first step is the determination of the one-electron potential V(r). Later in this chapter we will discuss the various ways to calculate or determine V(r). In one method V(r) can be calculated from first principles with the atomic numbers and positions as the only input parameters. In simpler, so-called semi-empirical approaches, the potential is expressed in terms of parameters which are determined by fitting experimental results. After the potential is known, it takes still a complicated calculation to solve (2.4). It is often convenient to utilize the symmetry of the crystal to simplify this calculation. Here by “symmetry” we mean geometrical transformations which leave the crystal unchanged. 2.2 Translational Symmetry and Brillouin Zones The most important symmetry of a crystal is its invariance under specific translations. In addition to such translational symmetry most crystals possess some rotational and reflection symmetries. It turns out that most semiconductors have high degrees of rotational symmetry which are very useful in reducing the complexity of calculating their energy band structures. In this and the next sections we will study the use of symmetry to simplify the classification of electronic states. Readers familiar with the application of group theory to solids can omit these two sections. When a particle moves in a periodic potential its wavefunctions can be expressed in a form known as Bloch functions. To understand what Bloch functions are, we will assume that (2.4) is one-dimensional and V(x) is a periodic function with the translational period equal to R. We will define a translation operator TR as an operator whose effect on any function f (x) is given by TR f (x) f (x R). (2.5) Next we introduce a function ºk (x) defined by ºk (x) exp (ikx)uk (x), (2.6) where uk (x) is a periodic function with the same periodicity as V, that is, uk (x nR) uk (x) for all integers n. When ºk (x) so defined is multiplied by exp [iˆt], it represents a plane wave whose amplitude is modulated by the periodic function uk (x). ºk (x) is known as a Bloch function. By definition, when x changes to x R, ºk (x) must change in the following way TR ºk (x) ºk (x R) exp (ikR)ºk (x). (2.7) It follows from (2.7) that ºk (x) is an eigenfunction of TR with the eigenvalue exp (ikR). Since the Hamiltonian 1e is invariant under translation by R, 1e commutes with TR . Thus it follows from quantum mechanics that the 2.2 Translational Symmetry and Brillouin Zones eigenfunctions of 1e can be expressed also as eigenfunctions of TR . We therefore conclude that an eigenfunction º(x) of 1e can be expressed as a sum of Bloch functions: Ak ºk (x) Ak exp (ikx)uk (x), (2.8) º(x) k k where the Ak are constants. Thus the one-electron wavefunctions can be indexed by constants k, which are the wave vectors of the plane waves forming the “backbone” of the Bloch function. A plot of the electron energies in (2.4) versus k is known as the electronic band structure of the crystal. The band structure plot in which k is allowed to vary over all possible values is known as the extended zone scheme. From (2.6) we see that the choice of k in indexing a wave function is not unique. Both k and k (2n/R), where n is any integer, will satisfy (2.6). This is a consequence of the translation symmetry of the crystal. Thus another way of choosing k is to replace k by k k (2n/R), where n is an integer chosen to limit k to the interval [/R, /R]. The region of k-space defined by [/R, /R] is known as the first Brillouin zone. A more general definition of Brillouin zones in three dimensions will be given later and can also be found in standard textbooks [2.2]. The band structure plot resulting from restricting the wave vector k to the first Brillouin zone is known as the reduced zone scheme. In this scheme the wave functions are indexed by an integer n (known as the band index) and a wave vector k restricted to the first Brillouin zone. In Fig. 2.1 the band structure of a “nearly free” electron (i. e., V → 0) moving in a one-dimensional lattice with lattice constant a is shown in both schemes for comparison. Band structures are plotted more compactly in the reduced zone scheme. In addition, when electrons make a transition from one state to another under the influence of a translationally invariant operator, k is conserved in the process within the reduced zone scheme (the proof of this (a) (b) E −2π a −π a 0 π a 2π a k E −π a 0 π a k Fig. 2.1. The band structure of a free particle shown in (a) the extended zone scheme and (b) the reduced zone scheme 21 22 2. Electronic Band Structures statement will be presented when matrix elements of operators in crystals are discussed, Sect. 2.3), whereas in the extended zone scheme k is conserved only to a multiple of (i. e. modulo) 2/R. Hence, the reduced zone scheme is almost invariably used in the literature. The above results, obtained in one dimension, can be easily generalized to three dimensions. The translational symmetries of the crystal are now expressed in terms of a set of primitive lattice vectors: a1 , a2 , and a3 . We can imagine that a crystal is formed by taking a minimal set of atoms (known as a basis set) and then translating this set by multiples of the primitive lattice vectors and their linear combinations. In this book we will be mostly concerned with the diamond and zinc-blende crystal structures, which are shown in Fig. 2.2a. In both crystal structures the basis set consists of two atoms. The ba- (a) Zn C S z (b) z (c) L a2 a1 a X Λ ∆ Γ K a3 Σ K y x y x Fig. 2.2. (a) The crystal structure of diamond and zinc-blende (ZnS). (b) the fcc lattice showing a set of primitive lattice vectors. (c) The reciprocal lattice of the fcc lattice shown with the first Brillouin zone. Special high-symmetry points are denoted by °, X, and L, while high-symmetry lines joining some of these points are labeled as § and ¢ 2.2 Translational Symmetry and Brillouin Zones sis set in diamond consists of two carbon atoms while in zinc-blende the two atoms are zinc and sulfur. The lattice of points formed by translating a point by multiples of the primitive lattice vectors and their linear combinations is known as the direct lattice. Such lattices for the diamond and zinc-blende structures, which are basically the same, are said to be face-centered cubic (fcc) see Fig. 2.2b with a set of primitive lattice vectors. In general, the choice of primitive lattice vectors for a given direct lattice is not unique. The primitive lattice vectors shown in Fig. 2.2b are a1 (0, a/2, a/2), a2 (a/2, 0, a/2), and a3 (a/2, a/2, 0), where a is the length of the side of the smallest cube in the fcc lattice. This smallest cube in the direct lattice is also known as the unit cube or the crystallographic unit cell. For a given direct lattice we can define a reciprocal lattice in terms of three primitive reciprocal lattice vectors: b1 , b2 , and b3 , which are related to the direct lattice vectors a1 , a2 , and a3 by bi 2 (aj × ak ) , (a1 × a2 ) · a3 (2.9) where i, j, and k represent a cyclic permutation of the three indices 1, 2, and 3 and (a1 × a2 ) · a3 is the volume of the primitive cell. The set of points generated by translating a point by multiples of the reciprocal lattice vectors is known as the reciprocal lattice. The reason for defining a reciprocal lattice in this way is to represent the wave vector k as a point in reciprocal lattice space. The first Brillouin zone in three dimensions can be defined as the smallest polyhedron confined by planes perpendicularly bisecting the reciprocal lattice vectors. It is easy to see that the region [/R, /R] fits the definition of the first Brillouin zone in one dimension. Since the reciprocal lattice vectors are obtained from the direct lattice vectors via (2.9), the symmetry of the Brillouin zone is determined by the symmetry of the crystal lattice. The reciprocal lattice corresponding to a fcc lattice is shown in Fig. 2.2c. These reciprocal lattice points are said to form a bodycentered cubic (bcc) lattice. The primitive reciprocal lattice vectors b1 , b2 , and b3 as calculated from (2.9) are b1 (2/a) (1, 1, 1), b2 (2/a) (1, 1, 1), and b3 (2/a) (1, 1, 1). 23 24 2. Electronic Band Structures [Incidentally, note that all the reciprocal lattice vectors of the fcc lattice have the form (2/a)(i, j, k), where i, j, and k have to be either all odd or all even]. The first Brillouin zone of the fcc structure is also indicated in Fig. 2.2c. The symmetry of this Brillouin zone can be best visualized by constructing a model out of cardboard. A template for this purpose can be found in Fig. 2.27. In Fig. 2.2c we have labeled some of the high-symmetry points of this Brillouin zone using letters such as X and °. We will conform to the convention of denoting high symmetry points and lines inside the Brillouin zone by Greek letters and points on the surfaces of the Brillouin zone by Roman letters. The center of the Brillouin zone is always denoted by °. The three high-symmetry directions [100], [110], and [111] in the Brillouin zone of the fcc lattice are denoted by: [100] direction : °̇ ¢ Ẋ [111] direction : °̇ § L̇ [110] direction : °̇ ™ K̇ The Brillouin zone of the fcc lattice is highly symmetrical. A careful examination of this Brillouin zone shows that it is unchanged by various rotations, such as a 90˚ rotation about axes parallel to the edges of the body-centered cube in Fig. 2.2c. In addition it is invariant under reflection through certain planes containing the center of the cube. These operations are known as symmetry operations of the Brillouin zone. The symmetry of the Brillouin zone results from the symmetry of the direct lattice and hence it is related to the symmetry of the crystal. This symmetry has at least two important consequences for the electron band structure. First, if two wave vectors k and k in the Brillouin zone can be transformed into each other under a symmetry operation of the Brillouin zone, then the electronic energies at these wave vectors must be identical. Points and axes in reciprocal lattice space which transform into each other under symmetry operations are said to be equivalent. For example, in the Brillouin zone shown in Fig. 2.2c there are eight hexagonal faces containing the point labeled L in the center. These eight faces including the L points are equivalent and can be transformed into one another through rotations by 90˚. Therefore it is necessary to calculate the energies of the electron at only one of the eight equivalent hexagonal faces containing the L point. The second and perhaps more important consequence of the crystal symmetry is that wave functions can be expressed in a form such that they have definite transformation properties under symmetry operations of the crystal. Such wave functions are said to be symmetrized. A well-known example of symmetrized wave functions is provided by the standard wave functions of electrons in atoms, which are usually symmetrized according to their transformation properties under rotations and are classified as s, p, d, f , etc. For example, an s wave function is unchanged by any rotation. The p wave functions are triply degenerate and transform under rotation like the three components of a vector. The d wave functions transform like the five components of a symmetric and traceless second-rank tensor. By classifying the wave functions in this way, some 2.3 A Pedestrian’s Guide to Group Theory matrix elements of operators can be shown to vanish, i. e., selection rules can be deduced. Similarly, wave functions in crystals can be classified according to their transformation properties under symmetry operations of the crystal and selection rules can be deduced for operators acting on these wave functions. The mathematical tool for doing this is group theory. Many excellent textbooks have been written on group theory (see the reference list). It is desirable, but not necessary, to have a good knowledge of group theory in order to study semiconductor physics. Some elementary notions of group theory are sufficient to understand the material covered in this book. The next section contains an introduction to group theoretical concepts and notations. Students familiar with group theory can omit this section. 2.3 A Pedestrian’s Guide to Group Theory Since the purpose of this section is to introduce group theory terminology and notations, no effort will be made to prove many of the statements and theorems mentioned in it. At most we shall illustrate our statements with examples and refer the reader to books on group theory for rigorous proofs. 2.3.1 Definitions and Notations The first step in studying the symmetry properties of any crystal is to determine its symmetry operations. For example: a square is unchanged under reflection about its two diagonals, or under rotation by 90˚ about an axis perpendicular to the square and passing through its center. One can generate other symmetry operations for a square which are combinations of these operations. One may say that it is possible to find an infinite number of symmetry operations for this square. However, many of these symmetry operations can be shown to consist of sequences of a few basic symmetry operations. The mathematical tool for systematically analyzing the symmetry operations of any object is group theory. A group G is defined as a set of elements {a, b, c, . . .} for which an operation ab (which we will refer to as multiplication) between any two elements a and b of the group is defined. This operation must have these four properties: • • • • Closure: The result of the operation ab on any two elements a and b in G must also belong to G. Associativity: for all elements a, b, and c in G (ab)c a(bc). Identity: G must contain an element e known as the identity or unit element such that ae a for all elements a in G. Inverse element: for every element a in G there exists a corresponding element a1 such that a1 a e. Element a1 is known as the inverse of a. 25 26 2. Electronic Band Structures Notice that the order in which one multiplies two elements a and b is important since ab is not necessarily equal to ba in general. If ab ba for all elements in G, multiplication is commutative and G is said to be Abelian. One can easily find many examples of groups. In particular, the set of symmetry operations of a crystal or a molecule can be shown to form a group. As an illustration, we will consider the molecule methane: CH4 . The structure of this molecule is shown in Fig. 2.3. It consists of a carbon atom surrounded by four hydrogen atoms forming the four corners of a regular tetrahedron. To simplify the description of the symmetry operations of the methane molecule, we will introduce the Schönflies notation: C2 : C3 : C4 : C6 : Û: i: Sn : E: rotation by 180˚ (called a two-fold rotation); rotation by 120˚ (called a three-fold rotation); rotation by 90˚ (called a four-fold rotation); rotation by 60˚ (called a six-fold rotation); reflection about a plane; inversion; rotation Cn followed by a reflection through a plane perpendicular to the rotation axis; the identity operation. For brevity, all the above operations are often denoted as rotations. To distinguish between a conventional rotation (such as C3 ) from reflections (such as Û) or rotations followed by reflections (such as S4 ) the latter two are referred to as improper rotations. Notice that the inversion is equal to S2 . This is not the only way to represent symmetry operations. An equally popular system is the international notation. The conversion between these two systems can be found in books on group theory [Ref. 2.3, p. 85]. -[111] H [001] C - H [111] -[111] H H [100] [111] Methane molecule [010] Fig. 2.3. A methane molecule (CH4 ) displaying the bonds (red lines) and the coordinate axes (black arrows). The [001] axis is perpendicular to the paper 2.3 A Pedestrian’s Guide to Group Theory To specify a symmetry operation completely, it is also necessary to define the axis of rotation or the plane of reflection. In specifying planes of reflection we will use the notation (kln) to represent a plane that contains the origin and is perpendicular to the vector (k, l, n). (Readers familiar with crystallography will recognize that this notation is an “imitation” of the Miller indices for denoting lattice planes in cubic crystals). The corresponding simplified notation for the axis containing this vector is [kln]. In Fig. 2.3 we have first chosen the origin at the carbon atom for convenience. Using the coordinate system shown in Fig. 2.3, the four carbon–hydrogen bonds are oriented along the [111], [111], [111], and [111] directions. We will now state without proof (the reader can check these results easily by constructing a balls-and-sticks model of the methane molecule) that the following operations are symmetry operations of the methane molecule: E: the identity; C2 : two-fold rotation about one of the three mutually perpendicular [100], [010] and [001] axes (three C2 operations in total); C3 : rotation by 120˚ in clockwise direction about one of the four C–H bonds (four operations in total); C31 : rotation by 120˚, counterclockwise, about one of the four C–H bonds (four operations in total); Û: reflection with respect to one of these six planes: (110), (110), (101), (101), (011), (011); S4 : a four-fold clockwise rotation about one of the [100], [010], and [001] axes followed by a reflection on the plane perpendicular to the rotation axis (three operations in total); S1 : a four-fold counterclockwise rotation about one of the [100], [010], and 4 [001] axes followed by a reflection on a plane perpendicular to the rotation axis (three operations in total). It can be shown easily that the operations C2 and Û are both the inverse of themselves. The inverse element of C3 is C31 , provided the axis of rotation is the same in the two operations. Similarly, the inverse element of S4 is S1 4 , provided the rotation axes remain the same. If we now define the multiplication of two symmetry elements a and b as a symmetry operation c ab consisting of first applying the operation b to the CH4 molecule followed by the operation a, it can be shown easily that the 24 symmetry operations of CH4 defined above form a group known as Td . Such groups of symmetry operations of a molecule are known as point groups. As the name implies, point groups consist of symmetry operations in which at least one point remains fixed and unchanged in space. Point groups contain two kinds of symmetry operations: proper and improper rotations. An infinite crystal is different from a molecule in that it has translational symmetry. Although in real life crystals never extend to infinity, the problems associated with the finite nature of a crystal can be circumvented by applying the so-called periodic (or Born–von Kármán) boundary conditions to the crystal. Equivalently, one can imagine that the entire space is filled with repli- 27 28 2. Electronic Band Structures cas of the finite crystal. It should be no surprise that the set of all symmetry operations of such an infinite crystal also forms a group. Such groups, which contain both translational and rotational symmetry operations, are known as space groups. There are 230 non-equivalent space groups in three dimensions. Besides their translational invariance, crystals also possess rotational symmetries. Space groups can be divided into two types, depending on whether or not the rotational parts of their symmetry operations are also symmetry operations. Let us first consider the purely translational operations of an infinite crystal. It can be shown that these translational symmetry operations form a group (to be denoted by T). T is known as subgroup of the space group G of the crystal. Let us now denote by R the set of all symmetry operations of G which involve either pure rotations (both proper and improper) only or rotations accompanied by a translation not belonging to T. We will denote the elements of R as ·, ‚, Ù, etc. Such a subset of G is known as a complex. In general R is not a group. For example, if G contains a screw axis or glide plane (these will be defined later, see Fig. 2.4) then R will not form a group and the space group G is said to be nonsymmorphic. If no screw axis or glide planes are present, R is a group (and therefore a subgroup of G): the space group G is then said to be symmorphic. The symmetry properties of symmorphic groups are simpler to analyze since both translational and rotational operations in such space groups form subgroups. In particular, it can be shown that the rotational symmetry operations of a symmorphic space group form point groups similar to those for molecules. However, there are restrictions on the rotational symmetry of a crystal as a result of its translational symmetry. For example, a crystal cannot be invariant under rotation by 72˚ (known as a five-fold rotation). However, a molecule can have this rotational symmetry. Point groups which are compatible with a lattice with translational symmetry are called crystallographic point groups. It can be shown that there are 32 distinct crystallographic point groups in three-dimensional space (see, e. g. [2.4]). Of a total of 230 space groups there are only 73 symmorphic space groups. Thus the simpler, symmorphic space groups are more often the exception rather than the norm. We will now consider how to analyze the rotational symmetries of nonsymmorphic space groups. By definition, a nonsymmorphic space group must contain at least one symmetry operation that involves both translation and rotation such that the rotational operation is not a symmetry operation of G by itself. There are two possibilities for such an operation: the rotation can be either proper or improper. The axis for a proper rotation is called a screw axis while the plane that corresponds to a twofold improper rotation is known as a glide plane. In the case of a screw axis, the crystal is invariant under a rotation about this axis plus a translation along the axis. The crystal is invariant under reflection in a glide plane followed by a translation parallel to the glide plane. Two simple examples of screw axes for a one-dimensional crystal are shown in Figs. 2.4a and b. From Fig. 2.4b it is clear that a simple three-fold rotation about the vertical axis is not a symmetry operation of this hypothet- 2.3 A Pedestrian’s Guide to Group Theory (a) Diad screw axis (b) Triad screw axis ~ (c) Glide reflection A c 2 c a 3 c 3 B Fig. 2.4. Examples of (a) a diad screw axis, (b) a triad screw axis and (c) a glide plane. The crystals in (a) and (c) are assumed to be three dimensional, although only one layer of atoms is shown for the purpose of illustration. If they are two dimensional, the glide operation in (c) becomes equivalent to that of the diad screw in (a). and ⊗ represent arrow pointing towards and away from the reader, respectively. Screw axis such as in (b) are found in the crystal structure of semiconductors like Se and Te [2.5] ical crystal. However, if the crystal is translated by an amount (c/3) along the vertical axis after the three-fold rotation then the crystal is unchanged. the vertical axis is known in this case as a triad screw axis. An example of a diad screw axis is shown in Fig. 2.4a. A glide plane is shown in Fig. 2.4c. The plane labeled A–B in the figure is not a reflection plane. But if after a reflection in the A–B plane we translate the crystal by the amount (a/2) parallel to the A– B plane, the crystal will remain unchanged. This symmetry operation is known as a glide and the A–B plane is a glide plane. Now suppose R is the set of all pure rotational operations of G plus the glide reflection shown in Fig. 2.4c (which we will denote as m). R defined in this way is not a group since mm is a pure translation and therefore not an element of R. To study the rotational symmetries of a space group independent of whether it is symmorphic or nonsymmorphic, we will introduce the concept of a factor group. Let G be the space group and T its subgroup consisting of all purely translational symmetry operations. Let C {·, ‚, . . .} be the complex of all the elements of G not in T. Unlike the elements of the set R defined earlier, the translation operations in the elements of C can belong to T. Next we form the sets T·, T‚, etc. The set T· consisting of operations formed by the product of a translation in T and an operation · not in T is known as a right coset of T. As may be expected, the set ·T is called a left coset of T. Let us first consider the case when G is a symmorphic group. For a symmorphic group we can decompose any symmetry operation · in C into the product of a translation ·t and a rotation ·r : · ·t ·r . Since multiplication is not necessarily commutative, we may worry about the order in which the two operations ·t and ·r occur. It can be shown that T has the property that the right coset Tx is equal to the left coset xT for every element x in G. A subgroup with this property is known as an invariant subgroup. When we multi- 29 30 2. Electronic Band Structures ply · by another translation operation to form an element of the coset T· the resultant operation consists of a new translation but multiplied by the same rotation ·r . This suggests that we can establish a correspondence between the set of cosets {T·, T‚, . . .} and the set of rotational operations R {·r , ‚r , . . .}. When G is symmorphic the set R is a subgroup of G so the set {T·, T‚, . . .} also forms a group. [In order that this set of cosets form a group, we have to define the product of two cosets (T·)(T‚) as T·‚]. This group is known as the factor group of G with respect to T and is usually denoted by G/T. In establishing the factor group G/T we have mapped all the elements of a coset T· into a single rotational operation ·r . Such a mapping of many elements in one set into a single element in another set is known as homomorphism. On the other hand, the mapping between the factor group G/T and the subgroup R of G is one-to-one, and this kind of correspondence is known as isomorphism. This isomorphism between the factor group G/T and the point group R of a symmorphic space group can be extended to a nonsymmorphic space group. The main difference between the two cases is that while the rotational operations ·r , ‚r , etc. are also elements in a symmorphic space group, this is not necessarily true for all rotations in a nonsymmorphic group. If · is a glide or screw then ·r is not an element in G. We will still refer to the group R as the point group of a nonsymmorphic space group because R contains all the information about the rotational symmetries of the space group G. However, special care must be exercised in studying the point groups of nonsymmorphic space groups since they contain elements which are not in the space group. We will next study the symmetry operations of the zinc-blende and diamond crystal structures as examples of a symmorphic and a nonsymmorphic space group, respectively. 2.3.2 Symmetry Operations of the Diamond and Zinc-Blende Structures Figure 2.2a shows the structures of the diamond and zinc-blende crystals. As pointed out in the previous section, both crystal structures consist of a fcc lattice. Associated with every lattice site there are two atoms which are displaced relative to each other by one quarter of the body diagonal along the [111] direction. The volume defined by the primitive lattice vectors and containing these two atoms forms a unit, known as the primitive cell, which is repeated at each lattice site. One simple way to construct these crystal structures is to start with two fcc sublattices, each containing only one atom located on every lattice site. Then one sublattice is displaced by one quarter of the body diagonal along the [111] direction with respect to the remaining sublattice. In the resulting crystal structure each atom is surrounded by four nearest neighbors forming a tetrahedron. The space group of the zinc-blende structure is symmorphic and is denoted by Td2 (or F43m in international notation). Its translational symmetry operations are defined in terms of the three primitive lattice vectors shown in Fig. 2.2b. Its point group has 24 elements. These 24 elements are identical to the elements of the point group of a tetrahedron 2.3 A Pedestrian’s Guide to Group Theory (or the methane molecule discussed in the last section and shown in Fig. 2.3) which is denoted by Td . The point group symmetry operations of the zinc-blende crystal are defined with respect to the three mutually perpendicular crystallographic axes with the origin placed at one of the two atoms in the primitive unit cell. With this choice of coordinates, the 24 operations are enumerated below (they are essentially identical to those of the methane molecule): E: eight C3 operations: identity clockwise and counterclockwise rotations of 120˚ about the [111], [111], [111], and [111] axes, respectively; three C2 operations: rotations of 180˚ about the [100], [010], and [001] axes, respectively; six S4 operations: clockwise and counterclockwise improper rotations of 90˚ about the [100], [010], and [001] axes, respectively; six Û operations: reflections with respect to the (110), (110), (101), (101), (011), and (011) planes, respectively. The diamond structure is the same as the zinc-blende structure except that the two atoms in the primitive unit cell are identical. If we choose the origin at the midpoint of these two identical atoms, we find that the crystal structure is invariant under inversion with respect to this origin. However, for the purpose of studying the point group operations, it is more convenient to choose the origin at an atom, as in the case of the zinc-blende structure. The crystal is no longer invariant under inversion with respect to this new choice of origin, but is unchanged under inversion plus a translation by the vector (a/4)[1, 1, 1], where a is the length of the unit cube. This can be visualized by drawing the carbon atoms in the diamond structure along the [111] direction as shown in Fig. 2.5. The space group of the diamond structure is nonsymmorphic: it contains three glide planes. For example, the plane defined by x (a/8) is a glide plane since diamond is invariant under a translation by (a/4)[0, 1, 1] followed by a reflection on this plane. In place of the three glide planes defined by x (a/8), y (a/8), and z (a/8), it is possible to use the “glide-like” operations: T(1/4, 1/4, 1/4)Ûx : T(1/4, 1/4, 1/4)Ûy : reflection on the x 0 plane followed by a translation of the crystal by the vector a(1/4, 1/4, 1/4); reflection on the y 0 plane followed by a translation of the crystal by the vector a(1/4, 1/4, 1/4); and a 3 4 [111] a 3 Fig. 2.5. Arrangement of atoms along the [111] direction of the diamond crystal. Notice that the crystal is invariant under inversion either with respect to the midpoint between the atoms or with respect to one of the atoms followed by an appropriate translation along the [111] axis 31 32 2. Electronic Band Structures Ca F Fig. 2.6. Schematic crystal structure of CaF2 (fluorite) T(1/4, 1/4, 1/4)Ûz : reflection on the z 0 plane followed by a translation of the crystal by the vector a(1/4, 1/4, 1/4). The factor group of the diamond lattice is isomorphic to the point group generated from the group Td by adding the inversion operation. This point group has 48 elements and is denoted as Oh . While Td is the point group of a tetrahedron, Oh is the point group of a cube. The space group of the diamond crystal is denoted by O7h (or Fd3m in international notation). The CaF2 (fluorite) structure shown in Fig. 2.6 is related to the diamond structure. This is the crystal structure of a family of semiconductors with the formula Mg2 X, where X Ge, Si, and Sn. The lattice of CaF2 is fcc as in diamond, but CaF2 has three sublattices. The two fluorine sublattices are symmetrically displaced by one quarter of the body diagonal from the Ca sublattices, so there is inversion symmetry about each Ca atom. The space group of CaF2 is symmorphic and its point group is also Oh , like diamond. This space group is denoted by O5h (or Fm3m). It is clear that there is a one-to-one correspondence between the elements of the point group of CaF2 and those of the factor group of diamond. 2.3.3 Representations and Character Tables The effect of a symmetry operation, such as a rotation, on a coordinate system (x, y, z) can be represented by a transformation matrix. For example, under a four-fold rotation about the x axis the axes x, y, and z are transformed into x , y , and z with x x, y z and z y. This transformation can be represented by the matrix M: ⎛ ⎞ 1 0 0 M ⎝0 0 1⎠. 0 1 0 Similarly a three-fold rotation about the [111] axis will transform the axes x, y, and z into x z, y x, and z y. This transformation can be represented by ⎛ ⎞ 0 0 1 ⎝1 0 0⎠. 0 1 0 2.3 A Pedestrian’s Guide to Group Theory In the rest of this chapter we will use the abbreviated notation (xyz) → (xzy) to denote the transformation matrix for the four-fold rotation and (xyz) → (zxy) for the three-fold rotation. All the symmetry operations in a point group can be represented by transformation matrices similar to M. It is easy to prove that the set of such transformation matrices corresponding to a group of symmetry operations is also a group. This group of matrices is said to form a representation of the group. There are actually an infinite number of such groups of matrices for a given group. The correspondence between a group and its representation is not, in general, an isomorphism but rather a homomorphism. A representation of a group G is defined as any group of matrices onto which G is homomorphic. Since representations of a group are not unique, we will be interested only in those of their properties that are common to all the representations of this group. One way to generate a representation for a group is to choose some function f (x, y, z) and then generate a set of functions {fi } by applying the symmetry operations Oi of the group to f (x, y, z) so that fi Oi [f ].1 By definition a group has to satisfy the closure requirement. This means that when the operation O is applied to fi the resultant function O[fi ] can be expressed as a linear combination of the functions fi : O[fi ] fj aji . (2.10a) j The coefficients aji form a square matrix, which will be referred to as a transformation matrix. The set of transformation matrices of the form {aji } corresponding to all the operations in the group now forms a representation of the group. The functions {fi } used to generate this representation are said to form a set of basis functions for this representation. Clearly the choice of basis functions for generating a given representation is not unique. If one uses the above method to generate a representation, then the dimension of the resulting transformation matrices will always be equal to the number of elements in the group (known as the order of a group). Some of the matrices will, however, be equal. Also many of the elements in these matrices will be zero. If the matrices in a given representation for all the operations in a group can be expressed in the following block form: ⎛ ⎞ 0 0 ... 0 ⎜ · 0 0 ... 0⎟ ⎜ ⎟ 0 0 ... 0⎟ ⎜ ⎜ ⎟ 0 ... 0⎟ ⎜0 0 0 ‚ (2.10b) ⎜ ⎟, Á ... 0⎟ ⎜0 0 0 ⎜ ⎟ ... 0⎟ ⎜0 0 0 ⎝0 0 0 ... 0⎠ 0 0 0 0 0 ... Ù In our applications {fi } will usually be a set of degenerate eigenfunctions corresponding to a given eigenvalue. 1 33 34 2. Electronic Band Structures where ·, ‚, . . ., Ù are square matrices, obviously the symmetry operations in this group can also be represented by the smaller matrices · and ‚, etc. While the matrices ·i and ‚i for an operation i may not necessarily have the same dimension, the matrices ·i for all the operations i in the group must have the same dimension. A representation of the form of (2.10b) is said to be reducible otherwise the representation may be irreducible. As pointed out earlier, the choice of matrices to form a representation for a given group is not unique. Given one set of transformation matrices {Ai }, we can generate another set {Ai } by a similarity transformation: Ai TAi T 1 , where T is an arbitrary nonsingular matrix with the same dimensionality as Ai . The transformed set of matrices {Ai } will also form a representation. The two sets of matrices {Ai } and {Ai } are then said to be equivalent. Often the matrices of a representation may not appear to have the form given by (2.10b) and hence be regarded as irreducible. However, if by applying similarity transformation it is possible to express these matrices in the form of (2.10b) then this representation is also called reducible. Otherwise it is called irreducible. Two axes of rotation or two reflection planes which transform into each other under a symmetry operation of a point group are said to be equivalent. It can be shown that the matrices of a representation which correspond to such equivalent rotations have identical traces (the trace of a matrix is the sum of the diagonal elements). Although the choice of irreducible representations for a group is not unique, the set of traces of these irreducible representations is unique since unitary transformations preserve the trace. This suggests that the set of all equivalent irreducible representations of a given group can be specified uniquely by their traces. For this reason the traces of the matrices in a representation are called its characters. The representations obviously contain more information than their characters; however, to utilize the symmetry of a given group it often suffices to determine the number of inequivalent irreducible representations and their characters. The determination of the characters of an irreducible representation is simplified by these properties of a group: • • Elements in a group can be grouped into classes. A set of elements T in a group is said to form a class if for any element a in the group, aT Ta. In a given representation all the elements in a class have the same character. The number of inequivalent irreducible representations of a group is equal to the number of classes. These two properties suggest that if the elements of a group can be divided into j classes the characters of its j irreducible representations can be tabulated to form a table with j columns and j rows, which is known as a character table. Assume that a group has N elements and these elements are divided into j classes denoted by C1 , C2 , . . . , Cj . The number of elements in each class will be denoted by N1 , N2 , . . . , Nj . The identity operation E forms a class with only one element and, by convention, it is labeled C1 . This group also has j inequivalent irreducible representations (from now on the set of irreducible 2.3 A Pedestrian’s Guide to Group Theory Table 2.1. The character table of a group Classes Representations R1 R2 · · Rj {E} {N2 C2 } ¯1 (E) ¯2 (E) · · ¯j (E) ¯1 (2) ¯2 (2) · · ¯j (2) · · · · · · · · · · · · · · · · · · {Nj Cj } ¯1 (j) ¯2 (j) · · ¯j (j) representations of a group will be understood to contain only inequivalent ones), which will be denoted by R1 , R2 , . . . , Rj . The character of Ck in Ri will be denoted by ¯i (k). Since the identity operation E leaves any basis function invariant, its representations always consist of unit matrices (that is, diagonal matrices with unity as the diagonal elements). As a result, the character ¯i (E) is equal to the dimension of the representation Ri . Thus the character table of this group will have the form of Table 2.1. In principle, the character table for the point group of a crystal can be calculated from the transformation matrices using a suitable set of basis functions. In practice, the character table can be obtained, in most cases, by inspection using the following two orthogonality relations: ¯i (Ck )∗ ¯j (Ck )Nk h‰ij (2.11) ¯i (Ck )∗ ¯i (Cl ) (h/Nl )‰kl , (2.12) k i where ∗ denotes the complex conjugate of a character, h is the order of the group, Nk is the number of elements of class Ck , and ‰ij is the Kronecker delta. As an illustration of the procedure used to obtain character tables we will consider two examples. EXAMPLE 1 Character Table of the Point Group Td As we showed in Sect. 2.3.1, the point group Td consists of 24 elements representing the proper and improper rotational symmetry operations of a tetrahedral methane molecule. In Sect. 2.3.2 we showed that this group is also the point group of the zinc-blende crystal. The 24 elements of this group can be divided into five classes {E}, {8C3 }, {3C2 }, {6S4 } and {6Û} 35 36 2. Electronic Band Structures by noting that: • • rotations by the same angle with respect to equivalent axes belong to the same class and reflections on equivalent planes also belong to the same class. Since the number of irreducible representations is equal to the number of classes, Td has five irreducible representations, which are usually denoted by A1 , A2 , E, T1 and T2 . Notice that the capital letter E has been used in the literature to denote a large number of entities varying from energy, electric field, the identity operation in group theory to an irreducible representation in the Td group! To avoid confusion we will always specify what E stands for. The next step is to construct the 5×5 character table using (2.11) and (2.12). First, we note again that the character of the class containing the identity operation {E} is equal to the dimension of the representation. Substituting this result into (2.12) we find |¯i (E)|2 h. (2.13) i Since the number of classes is usually small, this equation can often be solved by inspection. For Td it is easily shown that the only possible combination of five squares which add up to 24 is: 2 × 12 22 2 × 32 . This result means that the group Td has two irreducible representations of dimension one (denoted by A1 and A2 ), one irreducible representation of dimension two (denoted by E), and two irreducible representations of dimension three (denoted by T1 and T2 ). Next we note that a scalar will be invariant under all operations, so there is always a trivial identity representation whose characters are all unity. By convention this representation is labeled by the subscript 1, A1 in the present case. So without much effort we have already determined one row and one column of the character table for Td (Table 2.2). The remaining characters can also be determined by inspection with the application of (2.12). For the classes other than {E} the characters can be either positive or negative. The sign can be determined by inspection with some practice. For example, for the class {6Û} the only combination of sums of squares satisfying (2.12) is 4 × 12 02 24/6 4. Applying (2.12) to the characters of {E} and {6Û} it can be easily seen that A2 (6Û) 1, E(6Û) 0 Table 2.2. Determining the character table for the Td group by inspection A1 A2 E T1 T2 {E} {3C2 } {6S4 } {6Û} {8C3 } 1 1 2 3 3 1 · · · · 1 · · · · 1 · · · · 1 · · · · 2.3 A Pedestrian’s Guide to Group Theory Table 2.3. Character table and basis functions of the Td group {E} A1 A2 E T1 T2 1 1 2 3 3 {3C2 } {6S4 } {6Û} {8C3 } 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 Basis functions xyz x4 (y2 z2 ) y4 (z2 x2 ) z4 (x2 y2 ) {(x2 y2 ), z2 12 (x2 y2 )} {x(y2 z2 ), y(z2 x2 ), z(x2 y2 )} {x, y, z} while the two remaining characters for T1 and T2 contain 1 and 1. The final result for the character table of Td is given in Table 2.3. It is instructive to examine some possible basis functions for the irreducible representations of Td . One choice of basis functions for the A1 representation is a constant, as we have mentioned earlier. Another possibility would be the function xyz, which is also invariant under all symmetry operations of Td . A2 is very similar to A1 except that under the operations S4 and Û the character of A2 is 1 rather than 1. This implies that the basis function for A2 must change sign under interchange of any two coordinate axes, such as interchanging x and y. One choice of basis function for A2 is x4 (y2 z2 )y4 (z2 x2 )z4 (x2 y2 ). Similarly, the three-dimensional representations T1 and T2 differ only in the sign of their characters under interchange of any two coordinates. It can be shown that the three components x, y, and z of a vector transform as T2 . A corresponding set of basis functions for the T1 representation would be x(y2 z2 ), y(z2 x2 ), and z(x2 y2 ). The reader should verify these results by calculating the characters directly from the basis functions (Problem 2.2). At the beginning of this chapter we pointed out the importance of notation in group theory. The notation we have used so far to label the irreducible representations of the Td group: A1 , E, T1 , etc. is more commonly found in literature on molecular physics. We now introduce another notation used frequently in articles on semiconductor physics. The wave functions of a crystal with wave vector k at the center of the Brillouin zone (° point) always transform in the way specified by the irreducible representations of the point group of the crystal. Hence the Bloch functions at ° of a zinc-blende crystal can be classified according to these irreducible representations. In semiconductor physics literature it is customary to use ° plus a subscript i to label these irreducible representations of Td . Unfortunately there are two different conventions in the choice of the subscript i for labeling the same irreducible representation. One of these conventions is due to Koster (more commonly used in recent research articles) while the other was proposed by Bouckaert, Smoluchowski and Wigner (BSW) and tends to be found in older articles. The correspondence between the different notations for the Td point group is shown in Table 2.4. 37 38 2. Electronic Band Structures Table 2.4. Commonly used notations for the irreducible representations of the Td point group Koster notationa BSW notation Molecular notation °1 °2 °3 °4 °5 °1 °2 °12 °15 °25 A1 A2 E T2 T1 a Note that °4 and °5 are sometimes reversed in the literature. We recommend the student to check it whenever he encounters this notation [2.4]. EXAMPLE 2 Character Table of Oh We mentioned earlier in this section that the factor group of the diamond structure is Oh and that it is isomorphic to the point group derived from the Td group by including the inversion operation i. It has therefore 48 elements: the 24 symmetry operations of Td plus those of Td followed by i. These include all 48 symmetry operations of a cube. From the properties of the group Td , one can deduce that Oh has ten classes: {E}: identity; {3C2 }: C2 rotation about each of the three equivalent [100] axes; {6S4 }: two four-fold improper rotations about each of the three equivalent [100] axes; {6Ûd }: reflection on each of the six equivalent (110) planes; {8C3 }: two C3 rotations about each of the four equivalent [111] axes; inversion; {i}: {3Ûh }: reflection on each of the three equivalent (100) planes; {6C4 }: two C4 rotations about each of the three equivalent [100] axes; {6C2 }: C2 rotation about each of the six equivalent [110] axes; {8S6 }: two three-fold improper rotations about each of the four equivalent [111] axes. The first five classes are the same as those of Td while the remaining five are obtained from the first five by multiplication with the inversion. Correspondingly, there are ten irreducible representations. Five of them correspond to even transformations under those operations obtained from the Td group operation followed by inversion, while the other five correspond to odd ones. Similarly, the basis functions of the irreducible representations of Oh are either even or odd under those operations. In the terminology of quantum mechanics, these basis functions are said to have even or odd parity. The characters for the Oh group are listed in Table 2.5, while a set of basis functions for its irreducible representations is given in Table 2.6. Table 2.5 has been purposedly presented in a way to show the similarity between the “unprimed” representations in the Oh group and those of the Td group. For example, a scalar 2.3 A Pedestrian’s Guide to Group Theory Table 2.5. Character table of the Oh group presented in a way to highlight the similarity with Table 2.3 for the Td group. BSW notation {E} °1 °2 °12 °25 °15 °1 °2 °12 °25 °15 1 1 2 3 3 1 1 2 3 3 {C2 } {S4 } {Ûd } {C3 } 1 1 2 1 1 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 1 1 1 0 0 {i} 1 1 2 3 3 1 1 2 3 3 {Ûh } {C4 } {C2 } {S6 } 1 1 2 1 1 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 1 1 1 0 0 Table 2.6. Basis functions for the irreducible representations of the Oh group Representation Basis functions °1 °2 °12 °25 °15 °1 °2 °12 °25 °15 1 x4 (y2 z2 ) y4 (z2 x2 ) z4 (x2 y2 ) {[z2 (x2 y2 )/2], x2 y2 } {x(y2 z2 ), y(z2 x2 ), z(x2 y2 )} {x, y, z} xzy[x4 (y2 z2 ) y4 (z2 x2 ) z4 (x2 y2 )] xyz {xyz[z2 (x2 y2 )/2], xyz(x2 y2 )} {xy, yz, zx} {yz(y2 z2 ), zx(z2 x2 ), xy(x2 y2 )} : : : : : : : : : : still belongs to the °1 representation while a vector belongs to the °15 representation in the Oh group. However, the relation between the “primed” and “unprimed” representations is not so clear. For example, a pseudo-scalar belongs to the °2 representation, while a pseudo-vector belongs to the °15 representation. Furthermore, some of the primed representations, e. g. °15 and °25 , are even while others are odd under inversion. When Table 2.5 is rearranged into Table 2.7, the correlations between the first five representations and the remaining five become clear. Note that sometimes a hybrid of the K and BSW notations is used: the primes are omitted and replaced by , superscripts to denote the parity. The student will find this notation in Chaps. 6 and 7. 39 40 2. Electronic Band Structures Table 2.7. Character table of the Oh group rearranged to show the relationship between the even and odd parity representations. Both the Koster (K) and BSW notations are given [2.6] K BSW °1 °2 °3 °4 °5 °1 °2 °3 °4 °5 °1 °2 °12 °15 °25 °1 °2 °12 °15 °25 {E} 1 1 2 3 3 1 1 2 3 3 {C2 } {C4 } {C2 } {C3 } 1 1 2 1 1 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 1 1 1 0 0 {i} 1 1 2 3 3 1 1 2 3 3 {Ûh } {S4 } {Ûd } {S6 } 1 1 2 1 1 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 1 1 1 0 0 2.3.4 Some Applications of Character Tables We will now describe some of the applications of character tables. Further applications will be found throughout this book. a) Decomposition of Representation into Irreducible Components A problem one often faces is this: when given a group G and a representation Ù, how does one determine whether Ù is reducible? If Ù is reducible then how can it be decomposed into its irreducible components? These questions can be answered with the help of the character table of G. Suppose ¯Ù (i) is the character of the given representation Ù corresponding to the class {i}. If Ù is an irreducible representation, the set of characters ¯Ù (i) must be equal to the characters of one of the irreducible representations of G. If this is not the case then Ù is reducible. Suppose Ù is reducible into two irreducible representations · and ‚ and ¯· (i) and ¯‚ (i) are the characters of · and ‚, respectively. By definition ¯· (i) and ¯‚ (i) must satisfy ¯Ù (i) ¯· (i) ¯‚ (i) (2.14) for all classes {i} in the group G. The representation Ù is said to be the direct sum of the two irreducible representations · and ‚. The direct sum will be represented by the symbol ⊕ as in Ù · ⊕ ‚. When the dimension of a reducible representation is not very large, it can often be reduced into a direct sum of irreducible representations by inspection. As an example, let us consider the group Td with its character table given in Table 2.3 and a second-rank tensor {Tij } with components Txx , Txy , Txz , Tyx , Tyy , Tyz , Tzx , Tzy , and Tzz . Using these components as basis functions we can generate a nine-dimensional representation of Td , which we will denote as °. Obviously ° must be reducible since no irreducible representation in Td has 2.3 A Pedestrian’s Guide to Group Theory dimensions larger than three. The way to decompose ° into irreducible representations of Td is to first determine the characters of ° for all the classes in Td . In principle this can be accomplished by applying the symmetry operations of Td to the nine basis functions to produce the 9 × 9 matrices forming the representation °. A simpler and more direct approach is possible for this second-rank tensor. We note that a vector with three components x, y, and z forms a set of basis functions for the three-dimensional irreducible representation T2 of Td . Therefore, the 3 × 3 transformation matrices of a vector form a T2 representation. By taking the matrix product of two such 3 × 3 transformation matrices we obtain a set of 9 × 9 matrices forming a representation for °. This suggests that the characters of ° are equal to the squares of the characters for T2 : {E} {3C2 } {6S4 } {6Û} {8C3 } ¯° : 9 1 1 1 0 When the matrices of a representation Ù are equal to the matrix product of the matrices of two representations · and ‚, Ù is said to be the direct product of · and ‚. Direct products are represented by the symbol ⊗ as in ° T2 ⊗ T2 . (2.15) After determining the characters of °, the next step is to find the irreducible representations of Td whose characters will add up to those of °. The systematic way of doing this is to apply the orthogonality relation (2.11). It is left as an exercise (Problem 2.3) to show that T2 ⊗ T2 T1 ⊕ T2 ⊕ E ⊕ A1 (2.16) With practice this result can also be derived quickly by inspection. In the present example, one starts by writing down various combinations of representations with total dimensions equal to nine. Next one eliminates those combinations whose characters for the other classes do not add up to ¯° . Very soon it is found that the only direct sum with characters equal to that of ° for all five classes of Td is the one in (2.16). Once we realize that ° can be decomposed into the direct sum of these four irreducible representations, we can use the basis functions for these representations given in Table 2.3 as a guide to deduce the correct linear combinations of the nine components of the second-rank tensor which transform according to these four irreducible representations: A1 : E: T1 : T2 : Txx Tyy Tzz {Txx Tyy , Tzz (Txx Tyy )/2} {(Txy Tyx )/2, (Tzx Txz )/2, (Tyz Tzy )/2} {(Txy Tyx )/2, (Txz Tzx )/2, (Tyz Tzy )/2}. b) Symmetrization of Long Wavelength Vibrations in Zinc-Blende and Diamond Crystals The process we have described above is known as the symmetrization of the nine components of the second-rank tensor. This method can also be applied 41 42 2. Electronic Band Structures to symmetrize wave functions. When a Hamiltonian is invariant under the symmetry operations of a group, its wave functions can be symmetrized so as to belong to irreducible representations of this group. Just as atomic wave functions are labeled s, p, and d according to their symmetry under rotation, it is convenient to label the electronic and vibrational wave functions of a crystal at the point k in reciprocal space by the irreducible representations of the group of symmetry operations appropriate for k. We will now explain this statement with an example drawn from the vibrational modes of zinc-blende and diamond crystals. Although we will not discuss lattice vibrations in semiconductors until the next chapter, it is easier to demonstrate their symmetry properties than those of electrons. First, we can argue that vibrations of atoms in a crystal can be described by waves based on its translational symmetry, just as its electrons can be described by Bloch functions. For example, sound is a form of such vibration. Thus atomic motions in a crystal can be characterized by their displacement vectors (in real space) plus their wave vectors k (in reciprocal lattice space). The symmetry of a vibration is therefore determined by the effects of symmetry operations of the crystal on both vectors. Due to the discrete location of atoms in a crystal, a wave with wave vector equal to k or k plus a reciprocal lattice vector are indistinguishable (this point will be discussed further in Chap. 3). Thus an operation which transforms k into another wave vector k differing from k by a reciprocal lattice vector also belongs to the group of symmetry operations of k. This group is known as the group of the wave vector k. In particular, the group of the ° point or zone center is always the same as the point group of the crystal. A long wavelength (that is, k near the Brillouin zone center) vibration in a crystal involves nearly uniform displacements of identical atoms in different unit cells. For a zinc-blende crystal with two atoms per primitive unit cell, a zone-center vibrational mode can be specified by two vectors representing the displacements of these two atoms. We have already pointed out that the three components of a vector transform under the symmetry operations of Td according to the T2 , also called °4 representation (see Tables 2.3 and 2.4). To discuss properties in the zinc-blende crystal we will switch to the Koster notation. For brevity we will refer to the vector as “belonging” to the °4 representation. Two vectors, one associated with each atom in the primitive cell, give rise to a six-dimensional representation. Since irreducible representations in Td have at most three dimensions, this representation is reducible. To reduce it one can calculate its characters by applying the symmetry operations of Td to the two vectors. An alternative method is to consider the two atoms as the basis of a two-dimensional representation R. The characters of R are obtained by counting the number of atoms which are unchanged by the symmetry operations of Td (since each atom satisfying this condition contributes one unity diagonal element to the representation matrix). The two atoms in the zinc-blende lattice are not interchanged by the operations of Td , therefore all the characters of R are simply two. Thus R is reducible to two °1 representations. The representations of the two displacement vectors in the unit cell 2.3 A Pedestrian’s Guide to Group Theory of the zinc-blende crystal are equal to the direct product of R and °4 , which is equal to 2°4 . These two °4 representations correspond to the acoustic and optical phonon modes (see Chap. 3 for further details). In the acoustic mode the two atoms in the primitive cell move in phase while in the optical mode they move 180˚ out of phase. As pointed out in Sect. 2.3.2, the factor group of the diamond crystal is isomorphic to the point group Oh . We should remember that the origin has been chosen to be one of the carbon atoms. The space group operation which corresponds to inversion in Oh is inversion about the origin plus a translation by (a/4)(1, 1, 1) (for brevity this operation will be denoted here by i ). From Table 2.6 one finds that a vector belongs to the °15 representation of the Oh point group. As in the case of the zinc-blende crystal, we can obtain the characters of the six-dimensional representation by determining the characters of R and then calculating the direct product of R and °15 . The characters of R now depend on whether the symmetry operations include i . For all symmetry operations which already exist for the zinc-blende structure and therefore do not involve i , the characters are equal to two, as in the zinc-blende crystal. For all other operations, the two atoms inside the primitive unit cell are interchanged by i , so their characters are zero. By inspection of Table 2.5 one concludes that R reduces to °1 ⊕ °2 . Thus the displacement vectors of the two atoms in the primitive unit cell of diamond transform as °15 and °25 . The displacement vectors of the acoustic phonon change sign (the parity is said to be odd) under i and therefore have symmetry °15 . On the other hand the optical phonon parity is even and has symmetry °25 . The effects of i on the long-wavelength acoustic and optical phonons propagating along the body diagonal of the diamond crystal are shown in Fig. 2.7. c) Symmetrization of Nearly Free Electron Wave Functions in Zinc-Blende Crystals As an example of application of character tables in symmetrizing electronic wave functions, we will consider a nearly free electron in a zinc-blende crystal. By nearly free we mean that the electron is moving inside a crystal with a vanishingly small periodic potential of Td symmetry, so that its energy E and wave function º are essentially those of a free particle: º(x, y, z) exp [i(kx x ky y kz z)] (2.17) E 2 k2 /2m. (2.18) and However, because of the periodic lattice, its wave vector k can be restricted to the first Brillouin zone in the reduced zone scheme. We will assume that the crystal has the zinc-blende structure and that k (2/a)(1, 1, 1), where a is the length of an edge of the unit cube in the zinc-blende lattice. By applying the C3 symmetry operations of zinc-blende we can show that all the eight points (2/a)(±1, ±1, ±1) in the Brillouin zone are equivalent. Furthermore, from the definition of the primitive reciprocal lattice vectors given in Sect. 2.2 all eight points differ from the zone center by 43 44 2. Electronic Band Structures (a) Acoustic phonon Before inversion (111) Center of inversion After inversion (111) After translation a by (1,1,1) 4 (111) () (b) Optical phonon Center of inversion Before inversion (111) After inversion (111) After translation a (1,1,1) by 4 a √3 4 () ( ) (111) a √3 Fig. 2.7. Schematic diagrams of the transformation of (a) the acoustic phonon and (b) the zone-center optical phonon in diamond under inversion plus translation by (a/4)(1, 1, 1) where a is the size of the unit cube of diamond a primitive reciprocal lattice vector. Hence all eight points will map onto the zone center in the reduced zone scheme. The group of the wave vector k (2/a)(1, 1, 1) is therefore Td . To simplify the notation we will represent the electronic wave functions exp [i(kx x ky y kz z)] as {kx ky kz }. The eight wave functions {111}, {111}, {111}, {111}, {111}, {111}, {111} and {111} are degenerate but the degeneracy will be lifted by perturbations such as a nonzero crystal potential. Our goal now is to form symmetrized linear combinations of these eight wave functions with the aid of the character table of Td in Table 2.3. We note first that these eight wave functions form the basis functions of an eight-dimensional representation. Obviously this representation is reducible. Unlike the cases given in (a) and (b), there are no shortcuts in determining the characters of this eight-dimensional representation. Since characters are the sums of the diagonal elements, they can be deduced by determining the number of wave functions unchanged by the symmetry operations. The characters calculated in this way are given in Table 2.8. 2.3 A Pedestrian’s Guide to Group Theory Table 2.8. Characters of the representations formed by the nearly free electron wave functions with wave vectors equal to (2/a)(1, 1, 1) and (2/a)(2, 0, 0) in a zinc-blende crystal Class E 3C2 6S4 6Û 8C3 Transformation xyz xyz xzy yxz yzx Characters [111] [200] 8 0 0 4 2 6 2 0 2 0 Table 2.9. Symmetrized nearly free electron wave functions in a zinc-blende crystal with wave vectors equal to (2/a)(±1, ±1, ±1) Representation °1 °1 °4 °4 Wave function √ (1/ 8)({111} √ {111} {111} {111} {111} {111} {111} {111}) ( 8) cos (2x/a) cos (2y/a) cos (2z/a) √ ( 8) sin (2x/a) sin (2y/a) sin (2z/a) √ ( 8){sin (2x/a) sin (2y/a) cos (2z/a); sin (2x/a) cos (2y/a) sin (2z/a); cos (2x/a) sin (2y/a) sin (2z/a)} √ ( 8){sin (2x/a) cos (2y/a) cos (2z/a); cos (2x/a) sin (2y/a) cos (2z/a); cos (2x/a) cos (2y/a) sin (2z/a)}. By using the orthogonality relations or the method of “inspection”, we found from Table 2.3 (using Table 2.4 to convert to the Koster notation) that the only combination of irreducible representations giving rise to the set of characters in Table 2.8 is the direct sum 2°1 ⊕ 2°4 . Thus the eight {(±)1(±)1(±)1} free electron wave functions can be expressed as two wave functions belonging to the one-dimensional °1 representation and two wave functions belonging to the three-dimensional °4 representation. The proper linear combinations of wave functions which transform according to these irreducible representations can be obtained systematically by using projection operators (see any one of the references on group theory for further details). In many simple cases this can be done by inspection also. The proper linear combinations of the [111] wave functions can be shown to be (see Problem 2.4) those in Table 2.9. Similarly one can show that the six degenerate {(±)200}, {0(±)20} and {00(±)2} wave functions form a six-dimensional representation whose characters are given in Table 2.8. Using these characters one can decompose this six- 45 46 2. Electronic Band Structures Table 2.10. Symmetrized nearly free electron wave functions in a zinc-blende crystal with wave vectors equal to (2/a)(±2, 0, 0), (2/a)(0, ±2, 0), and (2/a)(0, 0, ±2) Representation Wave function °1 cos (4x/a) cos (4y/a) cos (4z/a) °3 cos (4y/a) cos (4z/a); cos (4x/a) (1/2)[cos (4y/a) cos (4z/a)] °4 sin (4x/a); sin (4y/a); sin (4z/a) dimensional representation into the direct sum °1 ⊕ °3 ⊕ °4 . The symmetrized wave functions are given in Table 2.10, while the proof is left as an exercise (Problem 2.4). d) Selection Rules In atomic physics one learns that optical transitions obey selection rules such as: in an electric-dipole transition the orbital angular momentum can change only by ±1. These selection rules result from restrictions imposed on matrix elements of the electric-dipole operator [see (6.29,30)] by the rotational symmetry of the atomic potential. One may expect similar selection rules to result from the symmetry of potentials in crystals. To see how such selection rules can be derived, we will consider the following example. Let p be the electron momentum operator and æ1 be a wave function in a zinc-blende-type crystal with the point group Td . Since p is a vector its three components px , py , and pz belong to the irreducible representation T2 (°15 or °4 according to Table 2.4). Let us assume that æ1 is a triply degenerate wave function belonging to T2 also. Operating with p on æ1 results in a set of nine wave functions, which we will label æ3 . These nine wave functions generate a nine-dimensional reducible representation which can be reduced to the direct sum T1 ⊕ T2 ⊕ E ⊕ A1 as shown in (2.16). Next we form the matrix element M æ2 |p|æ1 æ2 |æ3 between æ3 and another wave function æ2 . Suppose æ2 belongs to an irreducible representation B which is not one of the irreducible representations in the direct sum T1 ⊕ T2 ⊕ E ⊕ A1 of the wave function æ3 . From the orthogonality of the basis functions for different irreducible representations one concludes that the matrix element M is zero. In general, it can be proved that the matrix element between an operator p and two wave functions æ1 and æ2 can differ from zero only when the direct product of the representations of p and æ1 contains an irreducible representation of æ2 . This important group theoretical result is known as the matrix-element theorem. When applied to atoms the matrix-element theorem leads to the familiar selection rules for electric-dipole transitions. For instance, if æ1 and æ2 are atomic wave functions they will have definite parities under inversion, and the parity of their direct product is simply the product of their parities. The electric-dipole operator has odd parity so its matrix element is zero between two states of the same parity according to the matrix-element theorem. If æ1 and æ2 both have 2.3 A Pedestrian’s Guide to Group Theory s symmetry then their direct product also has s symmetry. Since the dipole operator has p-symmetry its matrix element between two s states is zero. On the other hand if one of these two wave functions has p symmetry its direct product will contain a component with p symmetry, and the electric-dipole transition will be nonzero. Thus, application of the matrix-element theorem leads to selection rules for optical transitions in systems with spherical symmetry. Using the matrix-element theorem we can also obtain very general selection rules for optical transitions in zinc-blende-type and diamond-type crystals. In Chap. 6 we will show that electric-dipole transitions in a crystal are determined by the matrix element of the electron momentum operator p. In a zincblende-type crystal p belongs to the °4 irreducible representations. To derive the selection rules for optical transitions involving zone-center wave functions we need to know the direct product between °4 and all the irreducible representations of Td . The results are summarized in Table 2.11. From this table we can easily determine whether or not electric-dipole transitions between any two bands at the zone center of the zinc-blende crystal are allowed. For example, dipole transitions from a °4 valence band to conduction bands with °1 , °3 , °4 , and °5 symmetries are all allowed. Using Table 2.11 one can derive selection rules for optical excitation of phonons by photons in the infrared (to be discussed further in Chap. 6). The ground state of the crystal with no phonons should have °1 symmetry. In zinc-blende crystals only °4 optical phonons can be directly excited by an infrared photon via an electric-dipole transition. Such phonons are said to be infrared-active. On the other hand the °25 optical phonon of the diamond structure is not infrared-active because of the parity selection rule (Ge, Si, and diamond are highly transparent in the infrared!). The ionic momentum operator has symmetry °15 for the Oh group and odd parity under the operation i of the diamond crystal. Hence electric-dipole transitions can only connect states with opposite parity. Selection rules for higher order optical processes, such as Raman scattering can also be obtained from Table 2.11. As will be shown in Chap. 7, Raman scattering involves the excitation of a phonon via two optical transitions. If both optical transitions are of the electric-dipole type in a zinc-blende crystal, the excited phonon must belong to one of the irreducible representations of the direct product °4 ⊗ °4 °4 ⊕ °5 ⊕ °3 ⊕ °1 . Phonons which can be excited optically in Raman scattering are said to be Raman-active. Thus the °4 optical phonon in the zinc-blende crystal is Raman-active in addition to being Table 2.11. Direct products of the °4 representation with all the representations of Td Direct product Direct sum °4 ⊗ °1 °4 ⊗ °2 °4 ⊗ °3 °4 ⊗ °4 °4 ⊗ °5 °4 °5 °4 ⊕ ° 5 °4 ⊕ ° 5 ⊕ ° 3 ⊕ °1 °4 ⊕ ° 5 ⊕ ° 3 ⊕ °2 47 48 2. Electronic Band Structures infrared-active. Similarly, the symmetries of Raman-active phonons in crystals with the Oh point group can be shown to be °25 , °12 , and °1 (see Chap. 7 for further details). Hence the °25 optical phonon of the diamond structure, while not infrared-active, is Raman-active. In crystals with inversion symmetry (said to be centrosymmetric), an infrared-active phonon must be odd while a Raman-active phonon must be even under inversion, therefore a phonon cannot be both infrared-active and Raman-active in such crystals. 2.4 Empty Lattice or Nearly Free Electron Energy Bands We now apply the group theoretical notations to the electron energy band structure of the diamond- and zinc-blende-type semiconductors. Since the electrons move in the presence of a crystal potential, their wave functions can be symmetrized to reflect the crystal symmetry, i. e., written in a form such that they belong to irreducible representations of the space group of the crystal. However, in order to highlight the symmetry properties of the electron wave function, we will assume that the crystal potential is vanishingly small. In this empty lattice or nearly free electron model, the energy and wave functions of the electron are those of a free particle as given by (2.18) and (2.17), respectively. The electron energy band is simply a parabola when plotted in the extended zone scheme. This parabola looks much more complicated when replotted in the reduced zone scheme. It looks especially intimidating when the wave functions are labeled according to the irreducible representations of the point group of the crystal. Such complications have resulted from using the crystal symmetry which was supposed to simplify the problem! The simplification, however, occurs when we consider the band structure of electrons in a non-empty lattice in the remaining sections of this chapter. In this section we will use group theory to analyze the symmetry properties of nearly free electron band structures in both zinc-blende- and diamond-type crystals. 2.4.1 Nearly Free Electron Band Structure in a Zinc-Blende Crystal Figure 2.8 shows the energy band of a nearly free electron plotted in the reduced zone scheme for wave vectors along the [111] and [100] directions only. To analyze this band diagram we will consider the symmetry and wave functions at a few special high-symmetry points in reciprocal space. k (0, 0, 0) As pointed out in Sect. 2.3.4, the group of the k vector at the ° point is always isomorphic to the point group of the lattice. Since the wave function is a constant for k 0, it has the symmetry °1 . 2.4 Empty Lattice or Nearly Free Electron Energy Bands Energy [200] Γ1+Γ3+Γ4 Λ1+Λ3 [ 32 12 12 ] Λ2+Λ3 L1+L2+2L3 2∆1+∆3+∆4 [111] 2Γ1+2Γ4 [011] X1+X3+X5 Λ1 ∆1 [100] X1+X3 [ 12 12 12 ] Λ1 2L1 L ∆1 Γ1 Γ [000] X Wave vector k Fig. 2.8. Band structure of nearly free electrons in a zinc-blende-type crystal in the reduced zone scheme. The numbers in square brackets denote corresponding reciprocal lattice vectors in the extended zone scheme in units of (2/a), a being the size of the unit cube. Note: To conform to notations used in the literature, we will use instead of ⊕ to represent the direct sum of two representations in all figures k (b, b, b), b (/a) In the eight equivalent [111] directions the bands are labeled §, according to the Brillouin zone notations in Fig. 2.2c. The wave functions for k 0 are classified according to the group of the wave vector k. The group of a wave vector along the [111] direction inside the Brillouin zone is C3v and contains six elements divided into three classes: {E}: identity; {C3 , C31 }: two three-fold rotations about the [111] direction; {m1 , m2 , m3 }: three reflections in the three equivalent (110) planes containing the [111] axis. The characters and basis functions for the irreducible representations of § are summarized in Table 2.12. The free-electron wave function given by exp [(i˙/a)(x y z)], where 0 ˙ 1, is invariant under all the symmetry operations of the group of § so it belongs to the §1 representation. We can also obtain this symmetry of the electron wave function by using the so-called compatibility relations. The symmetry of the endpoints of an axis in the Brillouin zone is higher than or equal to that of a point on the axis. Therefore the group of a point on an axis 49 50 2. Electronic Band Structures Table 2.12. Characters and basis functions of the irreducible representations of the group of § (C3v) in a zinc-blende-type crystal {E} {2C3 } §1 §2 1 1 1 1 1 1 §3 2 1 0 {3m} Basis functions 1 or x y z xy(x y) yz(y z) zx(z x) {(x y); 2 (z 1 [x y])} 3 2 is either equal to or constitutes a subgroup of the group of the endpoints. In the latter case, a representation belonging to the group of the endpoints of an axis can be reduced to irreducible representations of the group of the axis. The procedure for this reduction is the same as that described in Sect. 2.3.4. The difference is that only symmetry operations common to both groups need be considered now. When a representation of the group of an axis is contained in a representation of one of the group’s endpoints, the two representations are said to be compatible. For points lying on the [111] axis of a zinc-blende-type crystal, the group of § is a subgroup of ° but is identical to the group of L. From the character tables for ° and § it is clear that °1 is compatible with §1 only. Thus when the band starts out at the zone center with symmetry °1 , the symmetry of the band along the [111] direction must be §1 . This case illustrates a rather trivial application of the compatibility relations. Compatibility relations provide very useful consistency checks on band-structure calculations. Further applications of the compatibility relations can be found in Problem 2.6 at the end of this chapter. k (/a)(1, 1, 1) In the zinc-blende structure the symmetry operations in the group of the L point are identical to those of the § axis. So the §1 representation is compatible with the L1 representation only. For free electrons the wave function is doubly degenerate at (/a)(1, 1, 1) since (/a)(1, 1, 1) and (/a)(1, 1, 1) differ by (2/a)(1, 1, 1), a reciprocal lattice vector of the zinc-blende structure. Using the compatibility relations one can show that the next higher energy band along the § axis also has §1 symmetry. k (2/a)(1, 1, 1) The point k (2/a)(1, 1, 1) is equivalent to ° since it differs from ° by a reciprocal lattice vector. As shown in Sect. 2.3.4, the eight degenerate wave functions of the form exp [(i2/a)(±x ± y ± z)] can be symmetrized into two wave functions with °1 symmetry and two sets of three wave functions with °4 symmetry. The symmetries of the higher energy bands in the [111] direction are given in Fig. 2.8. They can be deduced using Table 2.12 and checked by the compatibility relations. The reader is urged to verify this as an exercise. 2.4 Empty Lattice or Nearly Free Electron Energy Bands Table 2.13. Symmetry operations and classes of the group of ¢ (C2v) in the zinc-blende structure Class Symmetry operations {E} {C42 } {md } {md } xyz xyz xyz xzy Table 2.14. Characters of the irreducible representations of the group of ¢ (C2v) {E} ¢1 ¢2 ¢3 ¢4 1 1 1 1 {C42 } {m d } 1 1 1 1 1 1 1 1 {m d } 1 1 1 1 k (c, 0, 0), c (2/a) Wave vectors in the [100] and equivalent directions are denoted by ¢. The group of ¢ (C2v ) contains four elements divided into the four classes listed in Table 2.13. The irreducible representations and characters of the group of ¢ are summarized in Table 2.14. The symmetry of the wave function in the [100] direction is ¢1 since this is the only representation compatible with °1 . The ¢ axis ends at the X point on the surface of the Brillouin zone. k (2/a)(1, 0, 0) The group of X contains twice as many symmetry operations as the group of ¢ since the wave vectors (2/a)(1, 0, 0) and (2/a)(1, 0, 0) differ by the reciprocal lattice vector (2/a)(2, 0, 0). The eight elements of the group of X (D2d ) are divided into five classes: {E}: {C42 (x)}: {2C42 (y, z)}: {2S4 }: {2md }: identity; two-fold rotation about the x axis; two-fold rotations about the y and z axes; two four-fold improper rotations about the x axis; two mirror reflections on the [011] and [011] planes. The irreducible representations of the group of X and their characters are given in Table 2.15. The wave functions at the X point with k (2/a)(±1, 0, 0) are doubly degenerate in the nearly-free electron model. From the compatibility relations it can be found that these wave functions belong to either the X1 or X3 representations. 51 52 2. Electronic Band Structures Table 2.15. Characters of the irreducible representations of the group of X (D2d) in the zinc-blende structure {E} X1 X2 X3 X4 X5 1 1 1 1 2 {C42 (x)} 1 1 1 1 2 {2C42 (y, z)} 1 1 1 1 0 {2S4 } 1 1 1 1 0 {2m d } 1 1 1 1 0 k (2/a)(0, 0, 2) The points k (2/a)(±2, 0, 0), (2/a)(0, ±2, 0), and (2/a)(0, 0, ±2) differ from the zone center by reciprocal lattice vectors. As already shown in example (c) in Sect. 2.3.4, the six degenerate wave functions exp [±i4x/a]; exp [±i4y/a]; and exp [±i4z/a] can be symmetrized to transform like the °1 , °3 , and °4 irreducible representations. 2.4.2 Nearly Free Electron Energy Bands in Diamond Crystals Obviously, the band structure of a free electron is the same whether it is in a zinc-blende or a diamond crystal. Therefore, in order to obtain the symmetrized wave functions specific to the diamond structure, we have to assume first that the diamond crystal potential is nonzero and symmetrize the electron wave functions accordingly. Afterwards the crystal potential is made to approach zero. The band structure of nearly free electrons in a diamond-type crystal obtained in this way is shown in Fig. 2.9. It serves as an important guide to the band structure of Si (shown in Fig. 2.10 for comparison) calculated by more sophisticated techniques to be discussed later in this chapter. The symmetries of the bands in diamond are very similar to those of zincblende because both crystals have a fcc lattice and tetrahedral symmetry. However, there are also important differences resulting from the existence of glide planes in the diamond structure as discussed in Sect. 2.3.2. We pointed out in that section that, if we choose the origin at one of the carbon atoms in diamond, the crystal is invariant under all the symmetry operations of the point group Td plus three “glide-like” operations: T(1/4, 1/4, 1/4)Ûx , T(1/4, 1/4, 1/4)Ûy , and T(1/4, 1/4, 1/4)Ûz (for brevity, we will now denote these three operations as TÛx , TÛy , and TÛz , respectively). However, the factor group of the space group of diamond is isomorphic to the point group Oh . In symmetrizing the electronic wave functions in the diamond structure, one has to consider the effect of TÛx on the Bloch functions. In this subsection we shall pay special attention to the electron wave functions at the points °, L, and X of the Brillouin zone of the diamond crystal. 2.4 Empty Lattice or Nearly Free Electron Energy Bands Energy Γ2'+Γ25'+Γ12' [200] Λ1+Λ3 [ 32 12 12 ] Λ1+Λ3 L1+L2'+L3+L3' [111] ∆1+∆2'+∆5 [011] X4+X1 Λ1 Γ1+Γ2'+Γ25'+Γ15 ∆'2 [100] X1 [ 12 12 12 ] Λ1 L1+L2' ∆1 Γ1 Γ [000] L X Wavevector k Fig. 2.9. Band structure of nearly free electrons for a diamond-type crystal in the reduced zone scheme 6 Γ2' L3 4 2 L1 Energy [eV] 0 ∆5 Λ3 ∆2 ' Λ1 Γ15 Λ3 Γ25' ∆1 ∆5 –2 Λ1 –4 ∆2 ' –6 –8 –10 X4 X1 L1 ∆1 L2' Λ1 –12 L Si X1 L3' Λ Γ1 Γ ∆ X Wavevector k U,K Σ Γ Fig. 2.10. Electronic band structure of Si calculated by the pseudopotential technique. The solid and the dotted lines represent calculations with a nonlocal and a local pseudopotential, respectively. [Ref. 2.8, p. 81] 53 54 2. Electronic Band Structures k (0, 0, 0) From (2.8) the Bloch functions at the zone center can be written as u(r), where u has the periodicity of the lattice. We define C as a set formed from the group Td plus all the operations obtained by multiplying each element of Td by TÛx . C defined this way is not a group because operations involving the glide, such as (TÛx )2 T(0, 1/2, 1/2) are not a member of C [for brevity, we will denote the operation T(0, 1/2, 1/2) by Q]. Let us now generate a set {Cu} consisting of 48 functions by applying the operations of C to u(r). For any two symmetry operations, a and b of C we define the operation multiplication between the corresponding two elements au and bu in {Cu} as (au)(bu) (ab)u. The set of operations in {Cu}, defined by their effect on the function u, can be easily shown to form a group. In particular, Qu(r) u(r) because u(r) has the translational symmetry of the crystal and hence Qu is now an element of {Cu}. In this group, it is convenient to introduce the element i u where i T(1/4, 1/4, 1/4)i was introduced in Sect. 2.3.4 (i is the inversion operation with respect to the origin). As pointed out in Sect. 2.3.4, the diamond crystal is not invariant under inversion with respect to one of the carbon atoms; it is however invariant under the combined operation of inversion followed by the translation T(1/4, 1/4, 1/4). One can show that the 48 operations in {Cu} are isomorphic to the Oh group. The character table of the group of wave functions of ° is given in Table 2.16. It can be compared with the character table for the Oh group (Table 2.5). Note that the classes are listed in different orders in Tables 2.5 and 2.16. In Table 2.16 the five classes of symmetry operations in the point group Td are listed first. The remaining five classes are obtained by multiplying the Td operations by i . The effects of i on the symmetry of wave functions at different highsymmetry points of the diamond crystal are not the same. For example, points along § are not invariant under i , so their symmetries are the same as in the zinc-blende crystal. On the other hand, the L point is invariant under i , therefore the wave functions at L have definite parity under i . Table 2.16. Characters of the irreducible representations of the group of ° in the diamond structure. The notation is that of Koster (BSW notation in parentheses) {E} °1 (°1 ) °2 (°2 ) °3 (°12 ) °4 (°15 ) °5 (°25 ) °1 (°1) °2 (°2) °3 (°12 ) °4 (°15 ) °5 (°25 ) 1 1 2 3 3 1 1 2 3 3 {C2 } {S4 } {Ûd } {C3 } 1 1 2 1 1 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 1 1 1 0 0 {i } 1 1 2 3 3 1 1 2 3 3 {i C2 } {i S4 } {i Ûd } {i C3 } 1 1 2 1 1 1 1 2 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 1 1 1 1 1 0 0 1 1 1 0 0 2.4 Empty Lattice or Nearly Free Electron Energy Bands k (/a)(1, 1, 1) The group of the L point in the diamond structure is isomorphic to the group of L in the fcc Bravais lattice (that is, a crystal formed by putting only one atom at each lattice point of a fcc lattice). The characters and basis functions for the irreducible representations in the group of L (D3d ) are shown in Table 2.17. k (2/a)(1, 1, 1) It has been pointed out already in the case of the zinc-blende crystal that k (2/a)(1, 1, 1) is equivalent to °. This is, of course, also true for the diamond crystal. From the eight symmetrized wave functions for the zinc-blende crystal given in Table 2.9 it can be shown readily that, for the diamond crystal, the eight equivalent (111) wave functions are symmetrized to transform according to the irreducible representations in Table 2.18. The symmetry of the wave functions in the diamond structure along the [001] directions are quite different from those of zinc-blende. We will first consider the X point since it presents an especially interesting case. Table 2.17. Characters and basis functions for the irreducible representations of the group of L in the diamond structure {E} {2C3 } {3C2 } {i } {2i C3 } {3i C2 } L1 L2 L3 L1 L2 L3 1 1 2 1 1 2 1 1 1 1 1 1 1 1 0 1 1 0 1 1 2 1 1 2 1 1 1 1 1 1 1 1 0 1 1 0 Basis functions 1 xy(x2 y2 ) yz(y2 z2 ) zx(z2 x2 ) {z2 1/2(x2 y2 ); (x2 y2 )} (x y)(y z)(z x) xyz {(x z); (y 1/2[x z])} Table 2.18. Symmetrized nearly free electron wave functions in the diamond crystal with wave vectors equal to (2/a)(±1, ±1, ±1). The origin of coordinates has been taken to coincide with an atomic site. Representation Wave function °1 (°1) cos (2x/a) cos (2y/a) cos (2z/a) sin (2x/a) sin (2y/a) sin (2z/a) °2 (°2') cos (2x/a) cos (2y/a) cos (2z/a) sin (2x/a) sin (2y/a) sin (2z/a) °5 (°25') sin (2x/a) cos (2y/a) cos (2z/a) cos (2x/a) sin (2y/a) sin (2z/a); plus two cyclic permutations °4 (°15) sin (2x/a) cos (2y/a) cos (2z/a) cos (2x/a) sin (2y/a) sin (2z/a); plus two cyclic permutations 55 56 2. Electronic Band Structures k (2/a)(0, 0, 1) A very special property of the wave functions at the X point of the diamond structure is that all relevant irreducible representations of the group of the X point are doubly degenerate, but they do not have definite parity under i . To understand this peculiar property, let us first enumerate all the symmetry operations of the group of the X point. We will start with the eight symmetry operations of the group of the point (2/a)(0, 0, 1) in the Brillouin zone of the zinc-blende structure: {E, C42 (z), 2C42 (x, y), 2S4 , 2md }. Next we will consider the combined effect of these operations and the operation TÛz on a wave function at the X point: ˇ exp (i2z/a)u(r). (2.19) At first we may expect that we can construct a group for the X point by taking the above eight elements and adding to them their products with the operation TÛz . This should result in a set of sixteen elements. It turns out that these sixteen elements do not form a group because translation and rotation do not necessarily commute. For example, consider the combined effect of C42 (x)TÛz on a vector (x, y, z): Ûz (x, y, z) → (x, y, z) T(1/4,1/4,1/4) → (x 1/4a, y 1/4a, z 1/4a) C42 (x) → (x 1/4a, y 1/4a, z 1/4a). If we interchange the order of C42 (x) and TÛz we find that [TÛz C42 (x)](x, y, z) (x 1/4a, y 1/4a, z 1/4a), (2.20a) so the operation C42 does not commute with TÛz . In particular, [TÛz C42 (x)]ˇ T(0, 1/2, 1/2)[C42 ]TÛz ˇ Q[C42 ]TÛz ˇ. {Eˇ, C42 (z)ˇ, . . . , 2md ˇ, TÛz ˇ, . . . , TÛz 2md ˇ} (2.20b) forms a In order that the set group, the operation Q has to be included also. Taking the 16 operations mentioned above and their products with Q, a group with 32 elements is obtained. This group can be divided into 14 classes: C1 C2 C3 C4 C5 C6 C7 C8 C9 C10 C11 {E} {C42 (x), C42 (y), QC42 (x), QC42 (y)} {C42 (z)} {QTÛz Ûx , TÛz Ûy } 1 {TÛz S4 , TÛz S1 4 , QTÛz S4 , QTÛz S4 } {TÛz , QTÛz } {TÛz C42 (x), TÛz C42 (y), QTÛz C42 (x), QTÛz C42 (y)} {TÛz C42 (z), QTÛz C42 (z)} {Ûx , Ûy } 1 {S4 , S1 4 , QS4 , QS4 } {QÛx , QÛy } 2.4 Empty Lattice or Nearly Free Electron Energy Bands C12 {QTÛz Ûy , TÛz Ûx } C13 {QC42 (z)} C14 {Q} The characters of the corresponding 14 irreducible representations are given in Table 2.19. However, not all of these representations are acceptable for wave functions at the X point of the Brillouin zone in the diamond crystal. Since (a/2)(0, 1, 1) is a lattice vector of the fcc lattice the operation Q will leave the periodic part of the X-point wave function invariant. The sinusoidal envelope exp (i2z/a) of the Bloch function changes sign under the translation Q, so overall the X-point wave functions must be odd under Q. Of the 14 irreducible representations only four are odd under the translation Q (or C14 ). These are labeled X1 , X2 , X3 , and X4 in Table 2.19. The interesting point is that these four representations are all doubly degenerate. This degeneracy results from the glide reflection and the fact that the two atoms in the unit cell of the diamond structure are identical. The degeneracy in the X1 and X2 states is lifted in the zinc-blende structure, where the two atoms in the primitive cell are different (see Problem 2.8). Some examples of symmetrized wave functions at the X point are k (2/a)(0, 0, 1): X1 : {cos (2z/a); sin (2z/a)} k (2/a)(±1, ±1, 0): X1 : {cos (2x/a) cos (2y/a); sin (2x/a)sin (2y/a)} X4 : {sin (2x/a) cos (2y/a); cos (2x/a)sin (2y/a)} k (Í/a)(0, 0, 1) where 0 Í 2. Table 2.19. Irreducible representations and characters of the group of symmetry operations on the wave functions at the X point (2/a)(0, 0, 1) of the Brillouin zone of the diamond structure [Ref. 2.7, p. 162] C1 M1 M2 M3 M4 M5 M1 M2 M3 M4 M5 X1 X2 X3 X4 a 1 1 1 1 2 1 1 1 1 2 2 2 2 2 4C 2 1 1 1 1 0 1 1 1 1 0 0 0 0 0 C3 1 1 1 1 2 1 1 1 1 2 2 2 2 2 2C 4 4C 5 2C 6 4C 7 2C 8 2C 9 4C 10 2C 11 2C 12 1 1 1 1 0 1 1 1 1 0 0 0 2 2 1 1 1 1 0 1 1 1 1 0 0 0 0 0 1 1 1 1 2 1 1 1 1 2 0 0 0 0 An error in [2.7] has been corrected. 1 1 1 1 0 1 1 1 1 0 0 0 0 0 1 1 1 1 2 1 1 1 1 2 0 0 0 0 1 1 1 1 0 1 1 1 1 0 2 2 0 0 1 1 1 1 0 1 1 1 1 0 0 0 0 0 1 1 1 1 0 1 1 1 1 0 2 2 0 0 1 1 1 1 0 1 1 1 1 0 0 0 2 2a C13 1 1 1 1 2 1 1 1 1 2 2 2 2 2 C14 1 1 1 1 2 1 1 1 1 2 2 2 2 2 57 58 2. Electronic Band Structures We will denote the Bloch function along the ¢ direction as „ exp (iÍz/a)u(r) as in (2.19). It is invariant under the following space group operations of the diamond structure: {E, Ûx , Cx2 (z), Ûy , TÛz C42 (x), TÛz S4 , TÛz C42 (y), TÛz S1 4 }, which can be divided into 5 classes: C1 C2 C3 C4 C5 {E} {C42 (z)} {TÛz S4 , TÛz S1 4 } {Ûx , Ûy } {TÛz C42 (x), TÛz C42 (y)} The representations generated by these operations acting on „ are isomorphic with the group of ¢ for a cubic lattice. The corresponding characters are shown in Table 2.20. Table 2.20. Irreducible representations and characters of the group of symmetry operations on the wave functions at the ¢ point of the Brillouin zone of the diamond structure [Ref. 2.7, p. 158] ¢1 ¢2 ¢2 ¢1 ¢5 C1 C2 1 1 1 1 2 1 1 1 1 2 2C 3 2C 4 2C 5 1 1 1 1 0 1 1 1 1 0 1 1 1 1 0 2.5 Band Structure Calculations by Pseudopotential Methods In Fig. 2.10 we have shown the electronic band structure of Si. It has been calculated with a sophisticated method known as the pseudopotential technique, which will be discussed in this section. Comparing these results with the nearly free electron band structure in Fig. 2.9 we notice that there are many similarities between the two. The nearly free electron band structure is basically a parabola redrawn in the reduced zone scheme. In the other case the band structure is computed by large-scale numerical calculations using supercomputers. The question is now: why do the two band structures, obtained by completely different methods, look so similar qualitatively? The answer to this question lies in the concept of pseudopotentials. The electronic configuration of a Si atom is 1s2 2s2 2p6 3s2 3p2 . When Si atoms form a crystal we can divide their electrons into core electrons and valence electrons as pointed out in Sect. 2.1. In crystalline Si the 1s, 2s, and 2p 2.5 Band Structure Calculations by Pseudopotential Methods orbitals are completely occupied and form the core shells. The outer 3s and 3p shells are only partially filled. Electrons in these shells are called valence electrons because they are involved in bonding with neighboring Si atoms. The crystal structure of Si at ambient pressure is similar to that of diamond. The tetrahedral arrangement of bonds between a Si atom and its four nearest neighbors can be understood if one of the electrons in the 3s shell is “promoted” to the 3p shell so that the four valence electrons form hybridized sp3 orbitals. This sp3 hybridization is well known from the bonding of carbon atoms and is responsible for the tetrahedral structure found in many organic molecules. But carbon atoms are more versatile than silicon atoms in that they can form double and triple bonds also. As a result, carbon atoms are crucial to all known forms of life while silicon atoms are important only to the highest form of life, namely human beings. It is these valence electrons in the outermost shells of a Si atom that are nearly free. These electrons are not affected by the full nuclear charge as a result of screening of the nucleus by the filled core shells. In the core region the valence electron wave functions must be orthogonal to those of the core. Thus the true wave functions may have strong spatial oscillations near the core, which make it difficult to solve the wave equation. One way to overcome this difficulty is to divide the wave functions into a smooth part (the pseudo-wave function) and an oscillatory part. The kinetic energy from the latter provides an “effective repulsion” for the valence electrons near the core (alternatively one can regard the valence electrons as being expelled from the core due to Pauli’s exclusion principle). Thus we can approximate the strong true potential by a weaker “effective potential” or pseudopotential for the valence electrons. Since the “smooth” parts of the valence electron wave functions have little weight in the core region, they are not very sensitive to the shape of the pseudopotential there. Figure 2.11 shows qualitatively how the pseudopotential in Si varies with distance r from the nucleus. At large values of r the pseudopotential approaches the unscreened Coulomb potential of the Si4 ion. This concept of replacing the true potential with a pseudopotential can be justified mathematically. It can V(r) ~ 1/2 -Bond length r Core region Ion potential ~ –1/r Fig. 2.11. Schematic plot of the atomic pseudopotential of Si in real space [Ref. 2.8, p. 17]. The solid curve in which V(r) → 0 in the core region is said to be a “soft core” pseudopotential. The broken curve in which V(r) → constant is a “hard core” pseudopotential 59 60 2. Electronic Band Structures be shown to reproduce correctly both the conduction and valence band states while eliminating the cumbersome, and in many cases irrelevant, core states [Ref. 2.8, p. 16]. Using the pseudopotential concept, the one-electron Schrödinger equation (2.4) can be replaced by the pseudo-wave-equation p2 V(ri ) „k (ri ) Ek „k (ri ), 2m (2.21) where „ is the pseudo-wave-function. This function is a good approximation to the true wave function outside the core region and therefore can be used to calculate the physical properties of the semiconductors which are dependent on the valence and conduction electrons only. Since pseudopotentials are weak perturbations on the free-electron band structure, a good starting point for diagonalizing (2.21) is to expand „k as a sum of plane waves: „k ag |k g, (2.22) g where the vectors g are the reciprocal lattice vectors and | k represents a plane wave with wave vector k. The coefficients ag and the eigenvalues Ek can be determined by solving the secular equation det | [(2 k2 /2m) Ek ]‰k, kg k | V(r) | k g | 0, The matrix elements of the pseudopotential V(r) are given by 1 1 k | V(r) | k g exp (ig · R) V(r)exp [ig · r]dr, N ø R (2.23) (2.24) ø where R is a direct lattice vector and ø the volume of a primitive cell. As a result of summation over all the lattice vectors inside the bracket, the pseudopotential matrix element is zero unless g is a reciprocal lattice vector. In other words, the matrix elements of the pseudopotential are determined by Fourier components of the pseudopotential (Vg ) defined by 1 (2.25) V(r)exp [ig · r]dr, Vg ø ø where g is a reciprocal lattice vector. If there is only one atom per primitive cell these Fourier components of the pseudopotential are known as the pseudopotential form factors. When there are several different atoms in the primitive cell, it is convenient to define for each kind of atom a pseudopotential form factor and a structure factor which depends only on the positions of one particular kind of atom in the primitive cell. For example, let there be two kinds of atoms · and ‚ in the crystal and let their positions inside the primitive cell be denoted by r·i and 2.5 Band Structure Calculations by Pseudopotential Methods r‚i . The structure factor Sg· of atom · is defined as 1 Sg· exp (ig · r·i ), N· (2.26) i where N· is the number of · atoms in the primitive cell. The structure factor of atom ‚ is defined similarly. The pseudopotential form factor Vg· for atom · can be defined as in (2.25) except that V is now the potential of one · atom and the integration is performed over ø· , which is the volume corresponding to one · atom. The pseudopotential V(r) can be expressed in terms of the structure and form factors by V(r) (Vg· Sg· Vg‚ Sg‚ ) exp (ig · r). (2.27) g From (2.24) we conclude that the pseudopotential mixes the free-electron states whose k’s differ by a reciprocal lattice vector. If these states are degenerate, the degeneracy may be split by the pseudopotential provided the corresponding form factor is nonzero. For example, consider the free-electron states with k (2/a)(±1, ±1, ±1) at the ° point in the diamond structure. The k’s of these eight-fold degenerate states differ by reciprocal lattice vectors (2/a)(2, 0, 0), (2/a)(2, 2, 0), and (2/a)(2, 2, 2). These eight states are degenerate when the electron is free. With the introduction of the pseudopotential, they become coupled and their degeneracy is partly lifted, producing energy gaps (compare Figs. 2.9 and 2.10). When an energy gap opens up at the Fermi level (highest occupied energy level) a semiconductor is obtained. This opening of energy gaps in the nearly-free-electron band structure by the pseudopotential form factors can be explained by Bragg reflection of the freeelectron plane waves by the crystal potential with the formation of standing waves. When the pseudopotential form factors are small, their effect on the band structure is weak so the actual band structure is not too different from the free-electron band structure. This is the reason why the nearly free electron bands drawn in the reduced zone scheme are a good starting point for understanding the band structure of most semiconductors. 2.5.1 Pseudopotential Form Factors in Zinc-Blende- and Diamond-Type Semiconductors The main reason why pseudopotentials are so useful is because only a small number of these form factors are sufficient for calculating a band structure. In semiconductors with the diamond structure, such as Si and Ge, just three pseudopotential form factors are sufficient. In semiconductors with the zincblende structure the number of required pseudopotential form factors doubles to six. To show this we first note that there are two atoms a and b in the unit cell. We will denote the atomic pseudopotentials of these two atoms by Va (r ra ) and Vb (r rb ), where ra and rb are the positions of the two atoms in the unit cell. Substituting these potentials into (2.25) we obtain the Fourier 61 62 2. Electronic Band Structures components of the crystal pseudopotential 1 Vg [Va (r ra ) Vb (r rb )] exp [ig · r]dr ø 1 [Va (r) exp (ig · ra ) Vb (r) exp (ig · rb )] ø × exp [ig · r]dr. (2.28) (2.29) Without loss of generality we can take the midpoint between the two atoms in the unit cell as the origin, so that ra (a/8)(1, 1, 1) s and rb (a/8)(1, 1, 1) s. We can now write Va (r) exp (ig · ra ) Vb (r) exp (ig · rb ) (Va Vb ) cos (g · s) i(Va Vb ) sin (g · s). (2.30) Next we define the symmetric and antisymmetric components of the pseudopotential form factor by 1 s (Va Vb ) exp (ig · r)dr (2.31) Vg ø and 1 a (Va Vb ) exp (ig · r)dr. (2.32) Vg ø Substituting the results in (2.30–32) back into (2.29) we arrive at Vg Vgs cos (g · s) iVga sin (g · s). (2.33) By symmetrizing the pseudopotential form factors in this way, it is clear that the antisymmetric form factors Vga vanish in the diamond structure. The factor cos (g · s) is just the structure factor of diamond defined in (2.26). In the III–V semiconductor, where the difference in the potentials of the anion and cation is small, Vga is expected to be smaller than Vgs and furthermore Vgs should be almost the same as in their neighboring group–IV semiconductors. For example, consider the pseudopotential form factors in Ge and the III–V semiconductor GaAs formed from its neighbors in the periodic table. In the diamond and zinc-blende structures, the reciprocal lattice vectors in order of increasing magnitude are (in units of 2/a): g0 g3 g4 g8 g11 (0, 0, 0); (1, 1, 1), (2, 0, 0), (2, 2, 0), (3, 1, 1), (1, 1, 1), (2, 0, 0), (2, 2, 0), (3, 1, 1), ..., ..., ..., ..., (1, 1, 1); ( 0, 0, 2); ( 0, 2, 2); (3, 1, 1). We can neglect pseudopotential form factors with g2 11(2/a)2 because typically Vg decreases as g2 for large g. Figure 2.12 shows a schematic plot of a pseudopotential as a function of the magnitude of g (g is assumed to be spherically symmetrical as in the case of a free atom). 2.5 Band Structure Calculations by Pseudopotential Methods V(q) V(r) ~ ∫ V(q) eiqrdq ~(1/2 Bond length)–1 q ~-12 q Fig. 2.12. Schematic plot of a pseudopotential form factor in reciprocal space [Ref. 2.8, p. 21] V(q = g) for typical g's –2/3 EF Screened ion limit for metals The pseudopotential form factor V0 corresponding to g0 is a constant potential, which merely shifts the entire energy scale: it can therefore be set equal to zero or any other convenient value (see Fig. 2.12). The pseudopotential form factors for all the equivalent reciprocal lattice vectors with the form (±1, ±1, ±1) and magnitude 3(2/a) are equal by symmetry and will be denoted by V3 . The structure factor corresponding to g4 is zero because cos (g · s) 0 for g (2/a)(2, 0, 0). Thus we conclude that there are only three s important pseudopotential form factors for Ge: V3s , V8s and V11 . In GaAs, a V8 vanishes because sin (g · s) 0, so only six pseudopotential form facs a tors are required: V3s , V8s , V11 , V3a , V4a , and V11 . The pseudopotential form factors of Ge, GaAs, and a few other semiconductors are listed in Table 2.21. One should keep in mind that the sign of the antisymmetric form factors depends on whether the anion or cation is designated as atom a. The sign of the antisymmetric form factors in Table 2.21 are all positive because the cation has been chosen to be atom a and the anion (which has a more negative atomic pseudopotential) to be atom b. Note also that the magnitude of the form factor V3s is the largest and furthermore it is negative in sign, as shown schematically in Fig. 2.12. In the III–V and II–VI compounds, V3s is comparable to the corresponding V3s in the group-IV semiconductors Table 2.21. Pseudopotential form factors of several group-IV, III–V and II–VI semiconductors (in units of Rydbergs = 13.6 eV) [2.9,10]. Note that the sign of V ai depends on the positions chosen for the anion and the cation (see text). Si Ge GaAs GaP InAs InSb ZnSe CdTe V 3s V 8s 0.211 0.269 0.252 0.249 0.27 0.25 0.23 0.245 0.04 0.038 0 0.017 0.02 0.01 0.01 0.015 s V 11 V 3a V 4a a V 11 0.08 0.035 0.08 0.083 0.041 0.044 0.06 0.073 0 0 0.068 0.081 0.078 0.049 0.18 0.089 0 0 0.066 0.055 0.038 0.038 0.12 0.084 0 0 0.012 0.003 0.036 0.01 0.03 0.006 63 2. Electronic Band Structures and always larger than V3a in magnitude. Nevertheless, as the ionicity increases in going from the III–V semiconductors to the II–VI semiconductors, the antisymmetric pseudopotential form factors become larger. Some band structures of diamond- and zinc-blende-type semiconductors calculated by the pseudopotential method are shown in Figs. 2.13–15. These band structure calculations include the effect of spin–orbit coupling, which will be discussed in Sect. 2.6. As a result of this coupling, the irreducible representations of the electron wave functions must include the effects of symmetry operations on the spin wave function. (For example, a rotation by 2 will change the sign of the wave function of a spin-1/2 particle). The notations used in Figs. 2.13–15, including this feature, are known as the double group notations and will be discussed in Sect. 2.6. The effect of ionicity on the band structures of the compound semiconductors can be seen by comparing the band structure of Ge with those of GaAs and ZnSe as shown in Figs. 2.13–15. Some of the differences in the three band structures result from spin–orbit coupling. Otherwise most of these differences can be explained by the increase in the antisymmetric components of the pseudopotential form factors as the ionicity increases along the sequence Ge, GaAs, ZnSe. One consequence of this increase in ionicity is that the energy gap between the top of the valence band and the bottom of the conduc- L4++L5+ 4 2 Γ8– L6+ L4–+L5– –2 Γ8– Γ6– Γ– 6 L6+ Γ7– 0 Energy [eV] 64 L6– Γ7+ –4 X5 Γ8+ Γ7– Ge Γ8+ Γ7+ X5 –6 L + 6 –8 X5 –10 L – 6 Γ6+ –12 L Λ Γ Γ6+ ∆ X U,K Wavevector k Σ Γ Fig. 2.13. Electronic band structure of Ge calculated by the pseudopotential technique. The energy at the top of the filled valence bands has been taken to be zero. Note that, unlike in Fig. 2.10, the double group symmetry notation is used [Ref. 2.8, p. 92] 2.5 Band Structure Calculations by Pseudopotential Methods 6 L4,5 4 2 Γ8 L6 Γ7 Γ6 L6 Energy [eV] Γ6 Γ8 Γ7 –2 L6 GaAs X6 Γ8 0 L 4,5 Γ8 Γ7 X7 Γ7 X7 X6 –4 –6 –8 L6 X7 –10 –12 X6 L6 Γ6 Γ6 Γ X K Σ Γ ∆ Wavevector k Fig. 2.14. Electronic band structure of GaAs calculated by the pseudopotential technique. The energy scale and notation (double group) are similar to those for Fig. 2.13 [Ref. 2.8, p. 103] Λ L Γ8 L4,5 8 Γ8 L6 6 X7 Γ7 4 2 L6 Energy [eV] 0 L4,5 –2 L6 Γ7 X6 Γ6 Γ8 Γ6 ZnSe Γ8 X7 Γ7 –4 X6 –6 L6 X7 Γ7 –8 –10 L6 –12 L X6 Γ6 Γ X K Γ Γ6 Wavevector k Fig. 2.15. Electronic band structure of ZnSe calculated by the pseudopotential technique. The energy scale and notation (double group) are similar to those for Fig. 2.14 [Ref. 2.8, p. 113] 65 66 2. Electronic Band Structures tion band at ° increases monotonically in going from Ge to ZnSe. Another consequence is that some of the doubly degenerate states in Ge at the X point of the Brillouin zone are split in the III–V and II–VI compounds, as pointed out in Sect. 2.4.2. For example, the lowest energy X1 conduction band state in Ge is split into two spin doublets of X6 and X7 symmetry (X1 and X3 without spin–orbit coupling) in GaAs and ZnSe. The explicit dependence of this splitting on the antisymmetric pseudopotential form factors is calculated in Problem 2.8. 2.5.2 Empirical and Self-Consistent Pseudopotential Methods There are two approaches to calculating pseudopotential form factors. Since the number of relevant pseudopotential form factors is small, they can be determined by fitting a small number of experimental data, such as the position of peaks in optical reflectivity spectra (Chap. 6) or features in the photoelectron spectra (Chap. 8). This approach is known as the Empirical Pseudopotential Method (EPM). The flow diagram for calculating the band structure with the EPM is as follows: Vg ↓ V(r) Vg exp (ig · r) g ↓ H (p2 /2m) V(r) Solve H„k (r) Ek „k (r) to obtain „k (r) and Ek ↓ Calculate reflectivity, density of states, etc., and compare with experiments ↓ Alter Vg if agreement between theory and experiment is not satisfactory. The disadvantage of the EPM is that it requires experimental inputs. However, this is not a major disadvantage since atomic pseudopotential form factors are often “transferable” in the sense that once they are determined in one compound they can be used (sometimes after suitable interpolation) in other compounds containing the same atom. For example, the atomic pseudopotential form factors for Ga determined empirically from GaAs can be used to calculate the band structure of other Ga compounds such as GaSb and GaP. With the availability of high-speed computers, however, it is possible to determine the pseudopotential form factors from first principles without any experimental input. These first-principles pseudopotential methods are known as self-consistent or ab initio pseudopotential methods. These meth- 2.5 Band Structure Calculations by Pseudopotential Methods ods use atomic pseudopotentials and a model for the crystal structure (from which an ionic potential Vion can be constructed) as the starting point of the calculation. After the wave functions have been obtained the contribution of the valence electrons to the potential is calculated. It is then used to evaluate the total one-electron potential, which is compared with the starting potential. Self-consistency is achieved when the calculated one-electron potential agrees with the starting potential. The flow diagram for such a calculation is shown below. The exchange and correlation term Vxc , which takes into account the many-body effects, is usually calculated with approximations such as the Local Density Approximation (LDA)2 . In this approximation, Vxc is assumed to be a function of the local charge density only. The LDA gives good results for the ground state properties such as the cohesive energies and charge density of the valence electrons. However, it gives poor results for the excitation energies. For instance, it typically underestimates the fundamental energy gap by about 1 eV. Thus it predicts semiconductors like Ge to be semimetals. The band structures shown in Figs. 2.10 and 2.13–15 have been calculated with the EPM since this method gives better overall agreement with experiments. This shortcoming of the LDA can be overcome by many-body techniques such as the quasiparticle approach [2.13]. Choose V(r) ↓ Solve (H V)„ E„ ↓ Calculate charge density Ú „∗ „ ↓ Solve ∇2 VHartree 4Ú 1 4Â0 ↓ Calculate Vxc f [Ú(r)] ↓ Vsc VHartree Vxc ↓ Model structure Vion → V Vsc Vion ( ) In recent years the ab initio pseudopotential method has been refined so as to be able to handle semicore electrons such as the 3d electrons of the copper halides. The pseudopotentials used are very smooth near the core (ultrasoft pseudopotentials) and reduce the number of plane waves required for the expansion of the wavefunctions to converge. The method is particularly useful for CuCl and diamond [2.14]. 2 For his development of the local density functional method of calculating electronic structures W. Kohn was awarded the Nobel prize for Chemistry in 1998 [2.11, 12]. 67 68 2. Electronic Band Structures 2.6 The k·p Method of Band-Structure Calculations The pseudopotential method is not the only method of band structure calculation which requires a small number of input parameters obtainable from experimental results. In the empirical pseudopotential method the inputs are usually energy gaps. In optical experiments one typically determines both energy gaps and oscillator strengths of the transitions. Thus it can be an advantage if the optical matrix elements can also be used as inputs in the band structure calculation. In the k·p method the band structure over the entire Brillouin zone can be extrapolated from the zone center energy gaps and optical matrix elements. The k · p method is, therefore, particularly convenient for interpreting optical spectra. In addition, using this method one can obtain analytic expressions for band dispersion and effective masses around high-symmetry points. The k · p method can be derived from the one-electron Schrödinger equation given in (2.4). Using the Bloch theorem the solutions of (2.4) are expressed, in the reduced zone scheme, as ºnk exp (ik · r)unk (r), (2.34) where n is the band index, k lies within the first Brillouin zone, and unk has the periodicity of the lattice. When ºnk is substituted into (2.4) we obtain an equation in unk of the form3 p2 k · p 2 k2 V 2m m 2m unk Enk unk . At k0 (0, 0, 0), (2.35) reduces to p2 V un0 En0 un0 (n 1, 2, 3, . . .). 2m (2.35) (2.36) Similar equations can also be obtained for k equal to any point k0 . Equation (2.36) is much easier to solve than (2.4) since the functions un0 are periodic. The solutions of (2.36) form a complete and orthonormal set of basis functions. Once En0 and un0 are known, we can treat the terms k · p/m and 2 k2 /(2m) as perturbations in (2.35) using either degenerate or nondegenerate perturbation theory. This method for calculating the band dispersion is known as the k · p method. Since the perturbation terms are proportional to k, the method works best for small values of k [2.15]. In general, the method can be applied to calculate the band dispersion near any point k0 by expanding (2.35) around k0 provided the wave functions (or the matrix elements of p between these wave functions) and the energies at k0 are known. Furthermore, by using a sufficiently large number of un0 to approximate a complete set of basis 3 Equation (2.35) is rigorously valid only if V is a local potential, i.e., it depends only on one spatial coordinate r. This is not strictly true in the case of pseudopotential [2.8] 2.6 The k·p Method of Band-Structure Calculations functions, (2.35) can be diagonalized with the help of computers to calculate the band structure over the entire Brillouin zone [2.16]. Only a limited number of energy gaps and matrix elements of p determined experimentally are used as input in the calculation. As examples of application of the k · p method we will derive the band dispersion and effective mass for a nondegenerate band and for a three-fold degenerate (or nearly degenerate) p-like band. The nondegenerate band case is applicable to the conduction band minimum in direct-bandgap semiconductors with the zinc-blende and wurtzite structures (examples of the latter semiconductor are CdS and CdSe). The nearly degenerate band is a model for the top valence bands in many semiconductors with the diamond, zinc-blende, or wurtzite structures. 2.6.1 Effective Mass of a Nondegenerate Band Using the k·p Method Let us assume that the band structure has an extremum at the energy En0 and the band is nondegenerate at this energy. Using standard nondegenerate perturbation theory, the eigenfunctions unk and eigenvalues Enk at a neighboring point k can be expanded to second order in k in terms of the unperturbed wave functions un0 and energies En0 by treating the terms involving k in (2.35) as perturbations. un0 | k · p | un 0 unk un0 un 0 (2.37) m En0 En 0 n n and Enk En0 2 k2 2 |un0 | k · p | un 0 |2 . 2 2m m En0 En 0 (2.38) n n The linear terms in k vanish because En0 has been assumed to be an extremum. It is conventional to express the energy Enk , for small values of k, as 2 k2 , (2.39) 2m∗ where m∗ is defined as the effective mass of the band. Comparing (2.38) and (2.39) we obtain an expression for this effective mass: Enk En0 1 1 2 |un0 | k · p | un 0 |2 2 2 . ∗ m m m k En0 En 0 (2.40) n n Formula (2.40) can be used to calculate the effective mass of a nondengenerate band. Also it shows that an electron in a solid has a mass different from that of a free electron because of coupling between electronic states in different bands via the k · p term. The effect of neighboring bands on the effective mass of a band depends on two factors. 69 70 2. Electronic Band Structures • • A wave function un 0 can couple to un0 only if the matrix element un 0 | p | un0 is nonzero. In Sect 2.3.4 we pointed out that, using the matrix element theorem and group theory, it is possible to enumerate all the symmetries un 0 can have. For example, p has °4 symmetry in the zinc-blende structure. If the conduction band has °1 symmetry, as in GaAs, its effective mass will be determined only by coupling with bands having °4 symmetry. On the other hand a valence band with °4 symmetry can be coupled via p to bands with °1 , °3 , °4 , and °5 symmetries. The energy separation En 0 En0 between the two bands n and n determines the relative importance of the contribution of n to the effective mass of n. Furthermore, bands with energies less than En0 will contribute a positive term to 1/m∗ , making m∗ smaller than the free electron mass. Conversely, bands with energies higher than En0 tend to increase m∗ or even cause m∗ to become negative as in the case of the top valence bands in the diamond- and zinc-blende-type semiconductors. These two simple results can be used to understand the trend in the conduction band effective mass m∗c in many of the group-III–V and II–VI semiconductors with direct bandgaps. In these semiconductors the lowest conduction band at the zone center has °1 symmetry. From the above considerations, its effective mass will be determined mainly by its coupling, via the k · p term, to the nearest bands with °4 symmetry. They include both valence and conduction bands. As we will show in the next section, the conduction bands in the group-IV, III–V, and II–VI semiconductors have antibonding character, while the valence bands have bonding character. What this means is that in the diamond-type structure the °2 (or °2 ) conduction band and its nearest °15 (or °4 ) conduction band both have odd parity and the momentum matrix element between them vanishes because of the parity selection rule. In III–V semiconductors, the antisymmetric pseudopotential breaks the inversion symmetry. As a result, the momentum matrix element between the °1 conduction band and its nearest °4 conduction band in III–V semiconductors is nonzero, but still much smaller than its momentum matrix element with the top °4 valence bands [2.17]. The separation between the °1 conduction band and the °4 valence band is just the direct band gap E0 , so m∗c can be approximated by 1 1 2 |°1c | k · p | °4v |2 . m∗c m m2 E0 k2 (2.41) It is customary to represent the three °4 wave functions as | X , | Y , and | Z. From the Td symmetry it can be shown that the only nonzero elements of °1c | k · p | °4v are X | px | °1 Y | py | °1 Z | pz | °1 iP. (2.42) Without loss of generality we can assume that the wave functions | X , | Y , | Z, and | °1 are all real. Since the operator p is equal to i∇ the matrix element in (2.42) is purely imaginary and P is real. With these results (2.41) simplifies to 2.6 The k·p Method of Band-Structure Calculations 2P2 m ≈ 1 . m∗c mE0 (2.43) It turns out that the matrix element P2 is more or less constant for most group-IV, III–V and II–VI semiconductors, with 2P2 /m ≈ 20 eV. The reason is that the values of P2 for these semiconductors are very close to those calculated for nearly free electron wave functions: P 2/a0 (see Problem 2.9). Since E0 is typically less than 2 eV, 2P2 /(mE0 ) 1 and (2.43) further simplifies to m 2P2 ≈ . m∗c mE0 (2.44) In Table 2.22 we compare the values of m∗c calculated from (2.44) with those determined experimentally for several group-IV, III–V, and II–VI semiconductors. The values of E0 are from experiment. Equation (2.44) can be extended to estimate the increase in m∗c away from the band minimum (non-parabolicity) which can be qualitatively described by an increase in E0 . See problem 6.15. Table 2.22. Experimental values of the °1 conduction band effective masses in diamondand zinc-blende-type semicondutors compared with the values calculated from (2.44) using the values of E0 obtained from experiment [2.18] Ge GaN 0.89 3.44 E0 [eV] 0.041 0.17 m∗c /m (exp ) m∗c /m ((2.44)) 0.04 0.17 GaAs GaSb InP InAs ZnS ZnSe ZnTe CdTe 1.55 0.067 0.078 0.81 1.34 0.047 0.073 0.04 0.067 0.45 0.026 0.023 3.80 0.20 0.16 2.82 0.134 0.14 2.39 0.124 0.12 1.59 0.093 0.08 2.6.2 Band Dispersion near a Degenerate Extremum: Top Valence Bands in Diamond- and Zinc-Blende-Type Semiconductors To apply the k · p method to calculate the band dispersion near a degenerate band extremum we consider the highest energy °25 (°4 ) valence bands at the zone center of semiconductors with the diamond (zinc-blende) structure. As pointed out in the previous section, these valence band wave functions are p-like, and they will be represented by the eigenstates | X , | Y , and | Z. The electron spin is 1/2, so the spin states will be denoted by · and ‚ to correspond to spin-up and spin-down states, respectively. In atomic physics it is well-known that the electron spin can be coupled to the orbital angular momentum via the spin–orbit interaction. The spin–orbit coupling is a relativistic effect (inversely proportional to c2 ) which scales with the atomic number of the atom. Thus for semiconductors containing heavier elements, such as Ge, Ga, As, and Sb, one expects the spin–orbit coupling to be significant and 71 72 2. Electronic Band Structures has to include it in the unperturbed Hamiltonian, in particular for states near k 0. The Hamiltonian for the spin–orbit interaction is given by Hso (∇ V × p) · Û , 4c2 m2 where the components of Û are the Pauli spin matrices: 0 1 0 i 1 0 ; Ûy ; Ûz . Ûx 1 0 i 0 0 1 (2.45a) (2.45b) (In crystals with the diamond structure the “vector” ∇ V × p is an example of a pseudovector with symmetry °15 ). The Hamiltonian Hso operates on the spin wave functions so the symmetry of Hso should depend also on the symmetry properties of the spin matrices. As is known from quantum mechanics, spin behaves differently than classical properties of particles such as the orbital angular momentum. For example, a spatial wave function is invariant under a rotation of 2 about any axis. However, under the same rotation the spin wave functions of a spin-1/2 particle will change sign. Let us denote a rotation of 2 about a unit vector n̂ as Ê (Problem 2.10). For a spinless particle Ê is equal to the identity operation. For a spin-1/2 particle Ê is an additional symmetry operation in the point group of its spin-dependent wave function. Thus, if G is the point group of a crystal neglecting spin, then the corresponding point group including spin effects will contain G plus ÊG and is therefore twice as large as G. Groups containing symmetry operations of spin wave functions are known as double groups. It is beyond the scope of this book to treat double groups in detail. Interested readers should refer to references listed for this chapter at the end of the book [Refs. 2.4, p. 103; 2.5; 2.7, p. 258]. Although many band diagrams in this book use the double group notation (for example, Figs. 2.13–15), in most cases it is sufficient to know only the irreducible representations for the double group at the zone center (° point) of zinc-blende-type crystals. Since the single group of ° in zinc-blende-type crystals contains 24 elements, one expects the double group to contain 48 elements. However, the number of classes in a double group is not necessarily twice that of the corresponding “single group”. The reason is that a class C in the single group may or may not belong to the same class as ÊC in the double group. For example, two sets of operations Ci and ÊCi belong to the same class if the point group contains a two-fold rotation about an axis perpendicular to n̂i (the rotation axis of Ci ). In the case of the group of ° of a zinc-blende-type crystal, elements in {3C2 } and {3ÊC2 } belong to the same class in the double group. This is also true for the elements in {6Û} and {6ÊÛ}. As a result, the 48 elements in the double group of ° in zinc-blende-type crystals are divided into eight classes. These eight classes and the eight irreducible representations of the double group of ° are listed in Table 2.23. Instead of using Table 2.23 to symmetrize the p-like valence band wave functions in zinc-blende-type crystals including spin–orbit coupling, we will utilize their similarity to the atomic p wave functions. We recall that, in atomic physics, the orbital electronic wave functions are classified as s, p, d, etc., ac- 2.6 The k·p Method of Band-Structure Calculations Table 2.23. Character table of the double group of the point ° in zinc-blende-type semiconductors {E} °1 °2 °3 °4 °5 °6 °7 °8 1 1 2 3 3 2 2 4 {3C2 / ^ } 3EC 2 1 1 2 1 1 0 0 0 {6S4 } {6Û/ ^ 6EÛ} {8C3 } ^ {E} ^ } {6ES 4 1 1 0 1 √1 √2 2 0 1 1 0 1 1 0 0 0 1 1 1 0 0 1 1 1 1 1 2 3 3 2 2 4 1 1 0 1 √1 √ 2 2 0 ^ } {8EC 3 1 1 1 0 0 1 1 1 cording to the orbital angular momentum l. The p states correspond to l 1 and are triply degenerate. The three degenerate states can be chosen to be eigenstates of lz , the z component of l. The eigenvalues of lz are known as the magnetic quantum numbers (usually denoted as ml ). For the p states ml 1, 0, 1. The wave functions of the orbital angular momentum operator are known as spherical harmonics. The spherical harmonics corresponding to the l 1 states can be represented as (except for a trivial factor of (x2 y2 z2 )1/2 ): ⎧ √ ⎨ | 1 1 (x iy)/ 2, (2.46) | lml | 1 0 z, √ ⎩ | 11 (x iy)/ 2. The spin-orbit interaction in atomic physics is usually expressed in terms of l and the spin s as Hso Ïl · s (2.47) The constant Ï is referred to as the spin–orbit coupling. The eigenfunctions of (2.47) are eigenstates of the total angular momentum j l s and its z component jz . For l 1 and s 1/2 the eigenvalues of j can take on two possible values: j l s 3/2 and j l s 1/2. The eigenvalues of jz (denoted by mz ) can take on the 2j 1 values j, j 1, . . . , j 1, j. The eigenfunctions of j and jz can be expressed as linear combinations of the eigenfunctions of the orbital angular momentum and spin (· = spin-up, ‚ = spin-down): 3/2, 3/2 | 1, 1· 3/2, 1/2 (1/√3)(| 1, 1‚ √2 | 1, 0·) (2.48) 3/2, 1/2 (1/√3)(| 1, 1· √2 | 1, 0‚) 3/2, 3/2 | 1, 1‚ | jmj √ √ | 1/2, 1/2 (1/ 3)(| 1, 0· 2 | 1, 1‚) √ √ | 1/2, 1/2 (1/ 3)(| 1, 0‚ 2 | 1, 1·) (2.49) 73 74 2. Electronic Band Structures The spin–orbit interaction in (2.47) splits the j 3/2 states in (2.48) from the j 1/2 states in (2.49). This splitting ¢0 is known as the spin–orbit splitting of the valence band at °, and in the case of the j 3/2 and j 1/2 states ¢0 3Ï/2. Using the atomic physics results as a guideline we can similarly symmetrize the six electronic states | X ·, | X ‚, | Y ·, | Y ‚, | Z·, and | Z‚ in the diamond- and zinc-blende-type semiconductors. First, we make use of the similarity between the p-like °4 states and the atomic p states to define three “(l 1)-like” states in the zinc-blende-type crystals: √ | 1, 1 (| X i | Y ) 2, | 1, 0 |Z, √ | 1, 1 (| X i | Y ) 2. (2.50) Next we define (j 3/2)-like and (j 1/2)-like states in the diamond- and zinc-blende-type crystals by substituting the expressions in (2.50) into (2.48) and (2.49). From now on we will refer to these (j 3/2)-like and (j 1/2)-like states as the j 3/2 states and j 1/2 states in the case of semiconductors. From the characters of the double group of ° in Table 2.23, one easily concludes that the four-fold degenerate j 3/2 states belong to the °8 representation, since this is the only four-dimensional representation. The two-fold degenerate j 1/2 states must belong to either the °6 or °7 representations. A way to decide between these two representations is to calculate the character of the representation matrix generated by j 1/2 states under an S4 operation. Using the result of Problem 2.10 it can be shown that the j 1/2 states belong to the °7 representation. As in the atomic case, the °8 and °7 states are split by the spin–orbit Hamiltonian in (2.45a). Typically, the magnitude of the spin– orbit splitting ¢0 in a semiconductor is comparable to the ¢0 of its constituent atoms. For example, semiconductors containing heavier atoms, such as InSb and GaSb, have ¢0 ≈ 1 eV, which is as large as or larger than the bandgap. When the anion and cation in the compound semiconductor have different ¢0 the anion contribution tends to be weighted more, reflecting its larger influence on the p-like valence bands. In semiconductors containing lighter atoms, such as Si and AlP, ¢0 (≈ 0.05 eV) is negligible for many purposes. The values of ¢0 in some diamond- and zinc-blende-type semiconductors are given in Table 2.24. The values of ¢0 in Table 2.24 are all positive, and as a result the j 3/2 (°8 ) valence band has higher energy than the j 1/2 (°7 ) valence band states (Figs. 2.13–15). In some zinc-blende-type crystals, such as CuCl, where there is a large contribution to the valence bands from the core d-electrons, ¢0 can be negative, leading to a reversal in the ordering of the °8 and °7 valence bands. In Sect. 2.3.4d it was shown that the operator p couples a state with °4 symmetry to states with °1 , °3 , °4 , and °5 symmetries. By examining the band structure of several semiconductors calculated by the pseudopotential method (Figs. 2.10, 2.13–15) we find that the bands which have the above symmetries and are close to the °4 valence bands are typically the lowest 2.6 The k·p Method of Band-Structure Calculations Table 2.24. Valence band parameters A and B in units of (2/2m) and |C |2 in units of (2/2m)2. The spin–orbit splitting of the valence bands ¢0 is given in units of eV. The averaged experimental [exp] and theoretical [th, obtained from A, B, C 2 with (2.69a,b)] values of the effective masses of the heavy hole (hh), light hole (lh) and spin–orbit split-off hole (so) valence bands [(2.59), p. 268] are in units of the free electron mass. [2.16, 18] A B | C |2 ¢0 [eV] Cb Si e Ge SiC c GaNd GaP e GaAs GaSb InP e InAs InSb ZnS ZnSe ZnTe CdTe 2.5 4.28 13.38 2.8 5.05 4.05 6.9 13.3 5.15 20.4 36.41 2.54 2.75 3.8 4.14 0.2 0.68 8.5 1.016 1.2 0.98 4.4 8.8 1.9 16.6 32.5 1.5 1.0 1.44 2.18 4.6 24 173 5.8 34 16 43 230 21 167 43 7.5 14.0 30.3 0.013a 0.044 0.295 0.014 0.017 0.08 0.341 0.75 0.11 0.38 0.81 0.07 0.43 0.93 0.92 m hh /m 0 exp 0.54 0.34 0.57 0.53 0.8 0.58 0.4 0.42 th 0.66e 0.50 0.43 0.6 0.5 e 0.51 0.73 0.98 0.44 0.4 0.48 m lh /m 0 exp 0.15 0.043 0.18 0.08 0.05 0.12 0.026 0.016 1.09 th 0.29e 0.15 0.041 0.25 0.13e 0.16 0.08 0.04 0.11 0.026 0.013 m so /m 0 exp 0.23 0.095 0.15 0.12 0.14 th 0.39b 0.24 0.1 0.36 0.2 0.25 0.17 0.15 0.2 0.10 0.12 0.145 a See: J. Serrano, M. Cardona, and T. Ruf, Solid State Commun. 113, 411 (2000) See: M. Willatzen, M. Cardona, N. E. Christensen, Linear Muffin-tin-orbital and k · p calculation of band structure of semiconducting diamond. Phys. Rev. B50, 18054 (1994) c See: M. Willatzen, M. Cardona, N. E. Christensen: Relativistic electronic structure of 3CSiC. Phys. Rev. B51, 13150 (1995). d See [1.1]. e The theoretical values of mhh /mo and mlh /mo in these materials are calculated with the equations in Problem 4.4 on p. 201 since the assumption of small warping of the valence bands is not valid for them. b conduction bands with symmetries °1 and °4 . For the conduction band °1c we have already shown that the only significant momentum matrix elements are X | px | °1 Y | py | °1 Z | pz | °1 iP, see (2.42). One can also use symmetry arguments to show that the nonzero matrix elements of p between the °4 valence bands and the °4 conduction band states are X | py | °4c (z) Y | pz | °4c (x) Z | px | °4c (y) iQ, X | pz | °4c (y) Y | px | °4c (z) Z | py | °4c (x) iQ (2.51) (details of the proof are left for Problem 2.11). The °4v valence bands together with the °1c and °4c conduction bands now form a set of 14 unperturbed wave functions which are coupled together by the k · p term of (2.35). The resultant 14×14 determinant can be diagonalized either with the help of computers or by using approximations. Löwdin’s perturbation method is most commonly used to obtain analytic expressions 75 76 2. Electronic Band Structures for the dispersion of the valence bands. In this method the 14×14 matrix is divided into two parts: the wave functions of interest and their mutual interactions are treated exactly while the interaction between this group of wave functions and the remaining wave functions is treated by perturbation theory. For example, in the present case the six °4v valence bands (including spin degeneracy) are of interest and their mutual coupling via the k · p and spin–orbit interactions will be treated exactly. The coupling between these valence band states and the conduction bands will be treated as a perturbation by defining an effective matrix element between any two valence band wave function as Hik Hkj Hij Hij . (2.52) Ei Ek k the °4 valence bands Within this approximation the 14×14 matrix reduces to a 6×6 matrix of the form {Hij }, where i and j run from 1 to 6. To simplify the notation we will number the six °4v valence band wave functions as º1 | 3/2, 3/2 º2 º3 º4 º5 º6 | 3/2, | 3/2, | 3/2, | 1/2, | 1/2, 1/2 1/2 3/2 1/2 1/2 and the doubly degenerate °1c and six-fold degenerate °4c conduction band wave functions as º7 to º14 . The calculation of all the matrix elements Hij is left for Problem 2.14a. Here we will calculate only the matrix element H11 as an example. According to (2.52) the effective matrix element H11 is given by 2 k2 p · k º1 H11 º1 2m m 2 2 k2 k · p 1 . º1 ºj (2.53) (E1 Ej ) 2m m j To simplify the notation again we introduce the following symbols: E0 , energy separation between °1c and the j 3/2 valence bands; and E0 , energy separation between °4c and the j 3/2 valence bands. Using these symbols we can express H11 as 2 2 2 k · p k · p 1 k º1 º1 °1c H11 º1 2m m m E0 2 k · p °4c 1 . º1 (2.54) E m 0 In principle, the term k · p/m can give rise to a term linear in k in the band dispersion. In the diamond-type semiconductors this term vanishes ex- 2.6 The k·p Method of Band-Structure Calculations actly because of the parity selection rule. In zinc-blende-type crystals the linear k · p term can be shown to be zero within the basis used. While the k linear term is strictly zero in diamond-type crystals because of the parity selection rule, this is not true in crystals without a center of inversion symmetry. In zinc-blende- and wurtzite-type crystals, it has been demonstrated [2.19, 20] that both the conduction and valence bands can possess small k-linear terms. However, these k-linear terms do not come from the k · p term alone, instead they involve also spin-dependent terms which have been neglected here. Since the k linear terms are relatively unimportant for the valence bands of most semiconductors they will not be considered further here. To simplify the notation we define 2 P2 ; m2 E0 2 Q2 ; M m2 E0 N L M; L 2 P2 ; m2 (E0 ¢0 ) 2 Q2 . M 2 m (E0 ¢0 ) L With these definitions, the term 2 k · p 1 °1c º1 E0 m in (2.54) can easily be shown to be equal to 2 k · p 1 1 2 2 °1c º1 E0 2 L(kx ky ) m (2.55) while 2 k · p 1 °4c º1 E m 0 is given by 2 k · p 1 1 2 2 2 °4c º1 E 2 M(kx ky 2kz ). m 0 (2.56) The result is H11 2 k2 1 N(k2x k2y ) Mk2z . 2m 2 (2.57) 77 78 2. Electronic Band Structures Similarly we can show that the remaining matrix elements are N H12 √ (kx kz iky kz ) 3 1 H13 √ [(L M)(k2x k2y ) 2iNkx ky ] 2 3 H14 0 1 √ H12 H15 2 √ H16 2H13 1 2 k2 1 (M 2L)k2 (L M)(k2x k2y ) 2m 3 2 0 H22 H23 H13 H24 1 H25 √ (H22 H11 ) 2 3 H26 H 2 12 H33 H22 H34 H12 ∗ H35 (H26 ) H36 H25 H44 H11 √ ∗ H45 2(H13 ) ∗ H46 (H15 ) 1 2 k2 (2M L )k2 ¢0 2m 3 0 H55 H56 H55 . H66 The matrix {Hij } is Hermitian, i. e., Hij [Hji ]∗ . This 6×6 matrix can be diagonalized numerically without further simplification. Readers with access to a personal computer and a matrix diagonalization program are encouraged to 2.6 The k·p Method of Band-Structure Calculations calculate the valence band structure of GaAs by diagonalizing this 6×6 matrix {Hij } (Problem 2.14b). The matrix {Hij } can be diagonalized analytically with some approximations. We will now restrict k to values small enough that the matrix elements which couple the J 3/2 and J 1/2 bands, such as H15 , H16 , and H25 , are negligible compared with the spin–orbit coupling. With this assumption, and limiting the expansion of the eigenvalue to terms of the order of k2 only, the 6×6 matrix reduces to a 4×4 and a 2×2 matrix. The 2×2 matrix gives the energy of the doubly degenerate j 1/2 °7 band as 2 k2 1 (2M L )k2 ¢0 2m 3 2 2 2Q2 k 2 P2 ¢0 1 . 2m 3 m(E0 ¢0 ) m(E0 ¢0 ) Eso H55 (2.58) Thus, within the above approximation, the constant energy surface for the j 1/2 split-off valence band is spherical and the band dispersion parabolic. In analogy with the conduction band we can define an effective mass mv,so for the split-off valence band given by 2 m 1 mv, so 3 P2 2Q2 m(E0 ¢0 ) m(E0 ¢0 ) . (2.59) The dispersion of the j 3/2 bands is obtained by diagonalizing the 4×4 matrix H H12 H13 0 11 (H )∗ H22 0 H13 12 ∗ . (H ) 0 H H 22 12 13 0 (H )∗ (H )∗ H 13 12 11 The secular equation for this matrix reduces to two identical equations of the form (H11 E)(H22 E) |H12 |2 |H13 |2 (2.60) and their solutions are 2 E± 12 (H11 H22 ) ± 12 [(H11 H22 ) 4(H11 H22 |H12 |2 |H13 |2 )] 2 . 1 (2.61) Substituting the matrix elements Hij as defined earlier into (2.61) E± can be expressed as 1 E± Ak2 ± [B2 k4 C2 (k2x k2y k2y k2z k2z k2x )] 2 , (2.62) an equation first derived by Dresselhaus et al. [2.21]. The constants A, B, and C in (2.62) are related to the electron momentum matrix elements and energy 79 80 2. Electronic Band Structures gaps by 2 P2 2Q2 2m A1 2 3 mE0 mE0 2 P2 Q2 2m B 2 3 mE0 mE0 2 16P2 Q2 2m C . 2 3mE0 mE0 (2.63) (2.64) (2.65) Equations (2.63–65) show that it is more convenient to define the constants A, B, and C in units of 2 /2m. Note that in the literature [2.17] the definitions of A, B, and C may contain a small additional term R, which is the matrix element of the electron momentum operator between the °4v valence band and a higher energy °3c conduction band. Inclusion of R is particularly important for large bandgap materials such as diamond [2.22] The dispersion of the °8 (J 3/2) bands near the zone center is given by (2.62); this equation has been derived after much simplification and is valid only for energies small compared to the spin–orbit splitting. We note that both A and B are negative since the dominant term in both (2.63) and (2.64) is 2P2 /(3mE0 ), which is 1. As a result, the effective masses of these bands, and of the splitt-off valence band in (2.59), are negative. In many cases we have to consider the properties of a semiconductor in which a few electrons are missing from an otherwise filled valence band. Instead of working with electrons with negative masses, it is more convenient to introduce the idea of a hole. A filled valence band with one electron missing can be regarded as a band (known as a hole band) containing one hole. If the energy of the missing electron in the valence band is E (assuming that E 0 is the top of the valence band) then the energy of the corresponding hole is E and is positive. With this definition the effective mass of a hole in the valence band is opposite to that of the corresponding missing electron and is positive also. The hole mass of the split-off valence band mso mv,so is positive with this definition (Table 2.24). Since the valence band represented by E has a smaller dispersion and hence larger mass, it is generally referred to as the heavy hole band, while the band represented by E is known as the light hole band. From now on the energies of these two hole bands will be written as Ehh and Elh with the corresponding hole energies defined as 1 Ehh Ak2 [B2 k4 C2 (k2x k2y k2y k2z k2z k2x )] 2 , 1 2 Elh Ak2 [B2 k4 C2 (k2x k2y k2y k2z k2z k2x )] . (2.66a) (2.66b) Constant energy surfaces represented by (2.66a) and (2.66b) are shown in Fig. 2.16. The shapes of these constant energy surfaces are referred to as “warped” spheres. The warping occurs along the [100] and [111] directions because of the cubic symmetry of the zinc-blende crystal. In fact one can argue that these warped spheres are the only possible shapes for constant energy surfaces described by 2.6 The k·p Method of Band-Structure Calculations (010) heavy hole Fig. 2.16. Constant energy surfaces of the J 3/2(°8 ) bands in diamond- and zincblende-type semiconductors (100) light hole a second-order equation in cubic crystals. Assuming that odd-order terms in k are either zero or negligible, the lowest order terms even in k consistent with the 1 cubic symmetry are k2 and [·k4 ‚(k2x k2y k2y k2z k2z k2x )] 2 . If we neglect higher order terms, the most general expression for the k dependence of the energy of the °8 (j 3/2) component of a °4 state in a cubic crystal is of the form of (2.62), where A, B, and C are linearly independent parameters related to the electron momentum matrix elements. One may notice from the definitions of the coefficients A, B, and C in (2.63–65) that C can be expressed in terms of A and B. This is a result of neglecting in our model the coupling between the °4v bands and higher conduction bands (such as °3c ), for the inclusion of the lowest °3c state see Problem 2.15d. The hole band dispersions along the [100] and [111] directions are parabolic, but the hole effective masses are different along the two directions: k(100) k(111) 1 2 2 (A B), mhh 1 2 2 (A B), mlh ⎡ 1 ⎤ 2 2 1 2 ⎣ |C| ⎦, A B 1 mhh 2 3B2 ⎡ 1 ⎤ 2 2 2 ⎣ |C| 1 ⎦. A B 1 mlh 2 3B2 (2.67a) (2.67b) (2.68a) (2.68b) From the above expressions we see that the warping of the valence bands is caused by the term | C |2 , which is proportional to Q2 . If the term B2 is much larger than | C |2 /3 warping can be neglected and we can obtain the approximate result that mlh ≈ 3m∗c /2 and mso ≈ 3m∗c . Note that Q2 is crucial to mhh . If we put Q2 0 we obtain the incorrect result mhh m0 (even the sign is wrong!). Often, for simplicity, it is expedient to assume that the valence band masses are isotropic. In such cases average heavy and light hole masses m∗hh and m∗lh can be obtained by averaging (2.67) and (2.68) over all possible directions of k (Problem 4.4): 81 82 2. Electronic Band Structures 1 2 | C |2 1 2A 2B 1 , m∗hh 2 15B2 1 2 | C |2 1 2A 2B 1 . m∗lh 2 15B2 (2.69a) (2.69b) In Table 2.24 we have listed what we judge to be reliable values of the constants A, B, and | C |2 for several semiconductors obtained from data in [2.18]. In this table the three valence band effective masses calculated from (2.67–69) using these values of A, B, and | C |2 and experimental energy gaps are compared with the experimentally determined effective masses. We note that the constant energy surfaces for the valence bands as described by (2.62) have inversion symmetry: E(k) E(k), even though the crystal may not have such symmetry. This is a consequence of the electron Hamiltonian we have used being invariant under time reversal (time-reversal symmetry). A Bloch wave traveling with wave vector k is transformed into a Bloch wave with wave vector k under time reversal. If the Hamiltonian is invariant under time reversal, these two Bloch waves will have the same energy. Finally we point out that there is an alternate equivalent approach often used in the literature to represent the valence band dispersion in diamondand zinc-blende-type semiconductors. Using group theory it is possible to derive an effective k · p Hamiltonian which is appropriate for the °4 valence bands. An example of such a Hamiltonian was proposed by Luttinger [2.23]: 2 5 Á1 Á2 ∇ 2 2Á3 (∇ · J)2 HL 2m 2 (2.70) 2(Á3 Á2 )(∇ 2x Jx2 c. p.) , where the parameters Á1 , Á2 , and Á3 are known as the Kohn–Luttinger parameters; J (Jx , Jy , Jz ) is an operator whose effects on the °8 valence bands are identical to those of the angular momentum operator on the J 3/2 atomic states, and c. p. stands for cyclic permutations. This approach facilitates the diagonalization of HL together with additional perturbations applied to the crystal. In Chap. 4 we will see an application of this Hamiltonian to calculate the energies of acceptor states. The first two terms in (2.70) have spherical symmetry while the last represents the effect of the lower, cubic symmetry. It is thus clear that the warping of the valence band is directly proportional to the difference between Á2 and Á3 . The Kohn–Luttinger parameters can be shown to be related to the coefficients A, B, and C in (2.62) by (2 /2m)Á1 A (2.71a) (2 /2m)Á2 B/2 ! "1/2 (2 /2m)Á3 (B2 /4) (C2 /12) (2.71b) The proof of these results is left as an exercise (Problem 2.15). (2.71c) 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors The pseudopotential approach to calculating the band structure of semiconductors discussed in Sect. 2.5 starts with the assumption that electrons are nearly free and their wave functions can be approximated by plane waves. In this section we will approach the problem from the other extreme. We will assume that the electrons are tightly bound to their nuclei as in the atoms. Next we will bring the atoms together. When their separations become comparable to the lattice constants in solids, their wave functions will overlap. We will approximate the electronic wave functions in the solid by linear combinations of the atomic wave functions. This approach is known as the tight-binding approximation or Linear Combination of Atomic Orbitals (LCAO) approach. One may ask: how can two completely opposite approaches such as the pseudopotential method and the tight-binding method both be good starting points for understanding the electronic properties of the same solid? The answer is that in a covalently bonded semiconductor there are really two kinds of electronic states. Electrons in the conduction bands are delocalized and so can be approximated well by nearly free electrons. The valence electrons are concentrated mainly in the bonds and so they retain more of their atomic character. The valence electron wave functions should be very similar to bonding orbitals found in molecules. In addition to being a good approximation for calculating the valence band structure, the LCAO method has the advantage that the band structure can be defined in terms of a small number of overlap parameters. Unlike the pseudopotentials, these overlap parameters have a simple physical interpretation as representing interactions between electrons on adjacent atoms. 2.7.1 Molecular Orbitals and Overlap Parameters To illustrate the tight-binding approach for calculating band structures, we will restrict ourselves again to the case of tetrahedrally bonded semiconductors. The valence electrons in the atoms of these semiconductors are in s and p orbitals. These orbitals in two identical and isolated atoms are shown schematically in Figs. 2.17a, 2.18a, and 2.19a. The pz orbitals are not shown since (a) (b) + A A s ± σ (bonding) B B s +A B– σ (antibonding) Fig. 2.17a,b. Overlap of two s orbitals to form bonding and antibonding Û orbitals 83 84 2. Electronic Band Structures (a) (b) + – ± A – – + – + A B – + px px A σ (bonding) B - + σ (antibonding) B Fig. 2.18a,b. Overlap of two px orbitals along the x axis to form bonding and antibonding Û orbitals (a) (b) A – py ± + + A B – py + A – + B – – B π (bonding) π (antibonding) + Fig. 2.19a,b. Overlap of two py orbitals to form bonding and antibonding orbitals their properties are similar to those of the py orbitals. Figures 2.17b, 2.18b, and 2.19b show schematically what happens to the atomic orbitals when the two atoms are brought together along the x direction until the atomic orbitals overlap to form a diatomic molecule. The interaction between the two atomic orbitals produces two new orbitals. One of the resultant orbitals is symmetric with respect to the interchange of the two atoms and is known as the bonding orbital while the other orbital, which is antisymmetric, is known as the antibonding orbital. In the case of p orbitals there are two ways for them to overlap. When they overlap along the direction of the p orbitals, as shown in Fig. 2.18b, they are said to form Û bonds. When they overlap in a direction perpendicular to the p orbitals they are said to form bonds, as shown in Fig. 2.19b. The interaction between the atomic orbitals changes their energies. Typically the antibonding orbital energy is raised by an amount determined by the interaction Hamiltonian H. The energy of the bonding orbital is decreased by the same amount. The changes in orbital energies are shown schematically in Fig. 2.20a for a homopolar molecule and in Fig. 2.20b for a heteropolar one. In both cases V is the matrix element of the interaction Hamiltonian between the atomic orbitals and is usually referred to as the overlap parameter. For a homopolar molecule containing only s and p valence electrons, there are four nonzero overlap parameters. To derive this result we will denote the atomic orbital on one of the atoms as | · and that on the second atom as | ‚. These 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors (a) homopolar molecule antibonding V Es V bonding (b) heteropolar molecule antibonding √V 2 + (∆E)2 (a) Es (c) Es 2∆E √V 2 + (∆E)2 bonding Fig. 2.20. Effect of orbital overlap on the energy levels in (a) a diatomic homopolar molecule and (b) a diatomic heteropolar molecule. V represents the matrix element of the interaction Hamiltonian orbitals can be expressed as products of a radial wave function and a spherical harmonic Ylm (ı, ˇ) with the atom chosen as the origin. We will denote the vector going from the first atom (designated as A in Fig. 2.21) to the second atom (B) as d. For both orbitals | · and | ‚ we will choose the coordinate axes such that the z axes are parallel to d and the azimuthal angles ˇ are the same (see Fig. 2.21). In these coordinate systems the spherical harmonic wave functions of the two atoms A and B are Ylm (ı, ˇ) and Yl m (ı , ˇ), respectively. The Hamiltonian H has cylindrical symmetry with respect to d and therefore cannot depend on ˇ. Thus the matrix element · | H | ‚ is proportional to the integral of the azimuthal wave functions exp [i(m m)ˇ]. This integral vanishes except when m m . As a result of this selection rule we conclude that x x' rA φ θ A φ rB θ' z z B d y y' Fig. 2.21. Choice of the polar coordinate systems for the two atoms A and B in a diatomic molecule in order that the z axis be parallel to the vector joining the two atoms A and B and the azimuthal angle ˇ be identical for both atoms 85 86 2. Electronic Band Structures there are four nonzero and linearly independent overlap parameters between the s and p electrons: s | H | s VssÛ ; s | H | pz VspÛ ; pz | H | pz VppÛ ; and px | H | px Vpp . We notice that px | H | py 0 and py | H | py px | H | px as a result of symmetry. The overlap parameters are usually labeled Û, and ‰ for (l 2 wave functions), depending on whether m is 0, 1, or 2 (in analogy with the s, p, and d atomic wave functions). The concept of bonding and antibonding orbitals introduced for molecules can be easily extended to crystals if one assumes that the orbitals of each atom in the crystal overlap with those of its nearest neighbors only. This is a reasonable approximation for most solids. The results of orbital overlap in a solid is that the bonding and antibonding orbitals are broadened into bands. Those occupied by electrons form valence bands while the empty ones form conduction bands. Figure 2.22 shows schematically how the s and p orbitals evolve into bands in a tetrahedral semiconductor. In this case the bonding orbitals are filled with electrons and become the valence bands while the antibonding orbitals become the conduction bands. As may be expected, the crystal structure affects the overlap between atomic orbitals. For example, in a tetrahedrally coordinated solid each atom is surrounded by four nearest neighbors. The vectors d linking the central atom to each of its nearest neighbors are different, so it is not convenient to choose the z axis parallel to d. Instead it is more convenient to choose the crystallographic axes as the coordinate axes. The spherical harmonics Ylm (ı, ˇ) of the atomic orbitals are then defined with respect to this fixed coordinate system. In calculating the overlap parameter for any pair of neighboring atoms, one expands the spherical harmonics defined with respect to d in terms of Ylm (ı, ˇ). An example of this expansion is shown schematically in Fig. 2.23. Conduction bands from the p antibonding orbitals p Conduction bands from the s antibonding orbitals s Valence band from p bonding orbitals EF Valence band from s bonding orbitals Fig. 2.22. Evolution of the atomic s and p orbitals into valence and conduction bands in a semiconductor. EF is the Fermi energy 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors z - s py B + - = d Θ y A - + B + + A A s x <s |H| py > Vspσ cosΘ = B 0 sinΘ + z - - py A + py + + B - = Θ + - y B + A A B + + x <py |H| py > = Vppσ cos2Θ + Vppπ sin2Θ Fig. 2.23. Projection of the overlap parameter between an s and a py orbital, and between py orbitals, along the vector d joining the two atoms and perpendicular to d 2.7.2 Band Structure of Group-IV Elements by the Tight-Binding Method After this introduction to the interaction between atomic orbitals we are ready to perform a quantitative calculation of the electronic band structure using the method of Linear Combination of Atomic Orbitals (LCAO). While the method has been utilized by many authors [Ref. 2.25, p. 75], the approach we will describe follows that of Chadi and Cohen [2.25]. The position of an atom in the primitive cell denoted by j will be decomposed into rjl Rj rl , where Rj denotes the position of the jth primitive cell of the Bravais lattice and rl is the position of the atom l within the primitive cell. For the diamond and zinc-blende crystals l 1 and 2 only. Let hl (r) denote the Hamiltonian for the isolated atom l with its nucleus chosen as the origin. The Hamiltonian for the atom located at rjl will be denoted by hl (r rjl ). The wave equation for hl is given by hl ˇml (r rjl ) Eml ˇml (r rjl ), (2.72) where Eml and ˇml are the eigenvalues and eigenfunctions of the state indexed by m. The atomic orbitals ˇml (r rjl ) are known as Löwdin orbitals. They are different from the usual atomic wave functions in that they have been constructed in such a way that wave functions centered at different atoms are 87 88 2. Electronic Band Structures orthogonal to each other. Next we assume that the Hamiltonian for the crystal is equal to the sum of the atomic Hamiltonians and a term int which describes the interaction between the different atoms. We further assume the interaction between the atoms to be weak so that can be diagonalized by perturbation theory. In this approximation the unperturbed Hamiltonian 0 is simply 0 hl (r rjl ) (2.73) j, l and we can construct the unperturbed wave functions as linear combinations of the atomic wave functions. Because of the translational symmetry of the crystal, these unperturbed wave functions can be expressed in the form of Bloch functions: 1 ºmlk √ exp (irjl · k)ˇml (r rjl ), (2.74) N j where N is the number of primitive unit cells in the crystal. The eigenfunctions æk of can then be written as linear combinations of ºmlk : æk Cml ºmlk . (2.75) m, l To calculate the eigenfunctions and eigenvalues of , we operate on æk with the Hamiltonian 0 int . From the orthogonality of the Bloch functions we obtain a set of linear equations in Cml : # $ Hml, m l Ek ‰mm ‰ll Cm l (k) 0, (2.76) m, l where Hml, m l stands for the matrix element ºmlk | | ºm l k and Ek are the eigenvalues of H. To simplify the solution of (2.76) we introduce the following approximations. • • We include only the s2 and p6 electrons in the outermost partially filled atomic shells. We neglect spin–orbit coupling (although it can be included easily). The two atomic orbitals of s symmetry for the two atoms in the unit cell will be denoted by S1 and S2, respectively. Correspondingly, the atomic orbitals with p symmetry will be denoted by: X1, X2, Y1, Y2, Z1 and Z2, respectively. In the following equations the index m will represent the s, px , py , and pz orbitals. When we substitute the wave functions ºmlk defined in (2.74) into (2.76) we obtain N N exp [i(rj l rjl ) · k] Hml, m l (k) N j j × ˇml | (r rjl ) | H | ˇm l (r rj l ) N (2.77) exp [i(Rj rl rl ) · k] j × ˇml (r rjl ) | H | ˇm l (r rjl ). (2.78) 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors Instead of summing j over all the unit cells in the crystal, we will sum over the nearest neighbors only. In the diamond and zinc-blende crystals this means j will be summed over the atom itself plus four nearest neighbors. These atoms will be denoted as j 1, 2, 3, 4, 5. If needed, one can easily include second neighbor or even further interactions. Within the above approximation the collection of matrix elements of the form in (2.77) constitutes an 8 × 8 matrix (note that the dimensions of the matrix depend only on the number of basis functions, not the number of neighbors included). Applying symmetry arguments allows the number of nonzero and linearly independent matrix elements of int to be greatly reduced. As an example, we will consider the matrix element Hs1, s2 . From (2.78) this matrix element is given by Hs1, s2 [exp (ik · d1 ) exp (ik · d2 ) exp (ik · d3 ) exp (ik · d4 )] × S1 | int | S2, (2.79) where we have assumed that atom 1 is located at the origin and d· (· 1 to 4) are the positions of its four nearest neighbors, with d1 (1, 1, 1)(a/4); d2 (1, 1, 1)(a/4); d3 (1, 1, 1)(a/4); and d4 (1, 1, 1)(a/4). The matrix element S1 | int | S2 is basically the same overlap parameter VssÛ as we have defined for molecules. The other matrix elements Hs1, px 2 , and Hpx 1, px 2 , etc., can also be expressed in terms of the overlap parameters VspÛ , VppÛ , and Vpp . For example Hs1, px 2 can be shown to contain four terms involving the four phase factors exp (ik · d· ) and the matrix element S1 | int | X2. However, for each nearest neighbor S1 | int | X2 has to be decomposed into Û and components as shown √ in Fig. 2.23. This decomposition introduces a factor of cos £ ± (1/ 3). The or sign depends on whether the s orbital lies in the direction of the positive or negative lobe of the px orbital. As a result, it is convenient to introduce a new set of four overlap parameters appropriate for the diamond lattice: Vss 4VssÛ , (2.80a) √ Vsp 4VspÛ / 3, (2.80b) Vxx (4VppÛ /3) (8Vpp /3), (2.80c) Vxy (4VppÛ /3) (4Vpp /3), (2.80d) With this√notation the matrix element S1(r) | int | X2(r d1 ) is given by (VspÛ )/ 3 Vsp /4. The remaining three matrix elements are related to S1(r) | int | X2(r d1 ) by symmetry. For example, a two-fold rotation about 89 90 2. Electronic Band Structures the y axis will transform (x, y, z) into (x, y, z), so d1 is transformed into d3 . The s-symmetry wave function | S1 is unchanged while the p-symmetry wave function |X2 is transformed into | X2 under this rotation. As a result, S1(r) | int | X2(r d3 ) S1(r) | int | X2(r d1 ). By applying similar symmetry operations we can show that exp [i(d· · k)]S1 (r) | int | X2(r d· ) 14 Vsp {exp [i(d1 · k)] · exp [i(d2 · k)] exp [id3 · k)] exp [i(d4 · k)]} (2.81) In the zinc-blende structure, because the atoms 1 and 2 are different, S1 | int | X2 is, in principle, different from S2 | int | X1. They are, however, often assumed to be equal [Ref. 2.24, p. 77]. The case of the zinc-blende crystal is left as an exercise in Problem 2.16. Here we will restrict ourselves to the case of the diamond structure. The 8×8 matrix for the eight s and p bands can be expressed as in Table 2.25. Es and Ep represent the energies S1 | 0 | S1 and X1 | H0 | X1, respectively. The four parameters g1 to g4 arise from summing over the factor exp [i(k · d· )] as in (2.81). They are defined by g1 (1/4){exp [i(d1 · k)] exp [i(d2 · k)] exp [i(d3 · k)] exp [i(d4 · k)]}, g2 (1/4){exp [i(d1 · k)] exp [i(d2 · k)] exp [i(d3 · k)] exp [i(d4 · k)]}, g3 (1/4){exp [i(d1 · k)] exp [i(d2 · k)] exp [i(d3 · k)] exp [i(d4 · k)]}, g4 (1/4){exp [i(d1 · k)] exp [i(d2 · k)] exp [i(d3 · k)] exp [i(d4 · k)]}. If k (2/a)(k1 , k2 , k3 ) the gj ’s can also be expressed as g1 cos (k1 /2) cos (k2 /2) cos (k3 /2) (2.82a) i sin (k1 /2) sin (k2 /2) sin (k3 /2),. g2 cos (k1 /2) sin (k2 /2) sin (k3 /2) (2.82b) i sin (k1 /2) cos (k2 /2) cos (k3 /2),. Table 2.25. Matrix for the eight s and p bands in the diamond structure within the tight binding approximation S1 S1 S2 X1 Y1 Z1 X2 Y2 Z2 S2 X1 Y1 Z1 Es Ek Vss g1 0 0 0 Vss g1∗ Es Ek Vsp g2∗ Vsp g3∗ Vsp g4∗ Ep E k 0 0 0 Vsp g2 0 Vsp g3 0 E p Ek 0 0 Vsp g4 0 0 Ep E k Vsp g2∗ 0 Vxx g1∗ Vxy g4∗ Vxy g3∗ ∗ ∗ ∗ 0 Vxy g4 Vxx g1 Vxy g2∗ Vsp g3 ∗ ∗ ∗ 0 Vxy g3 Vxy g2 Vxx g1∗ Vsp g4 X2 Y2 Z2 Vsp g2 0 Vxx g1 Vxy g4 Vxy g3 Ep E k 0 0 Vsp g3 0 Vxy g4 Vxx g1 Vxy g2 0 Ep Ek 0 Vsp g4 0 Vxy g3 Vxy g2 Vxx g1 0 0 Ep Ek 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors g3 sin (k1 /2) cos (k2 /2) sin (k3 /2) (2.82c) i cos (k1 /2) sin (k2 /2) cos (k3 /2),. g4 sin (k1 /2) sin (k2 /2) cos (k3 /2) (2.82d) i cos (k1 /2) cos (k2 /2) sin (k3 /2),. The valence and lowest conduction band energies of the diamond-type crystals can be obtained by diagonalizing the 8×8 matrix of Table 2.25, provided the four parameters Vss , Vsp , Vxx , and Vxy are known. These four parameters can be determined by comparing the calculated band structure with a first principles or empirical band structure calculation. For example Chadi and Cohen [2.25] obtained the tight-binding parameters for C, Si, and Ge by comparison with empirical pseudopotential calculations. Their results are shown in Table 2.26. Note that the signs of Vss etc. are, in part, arbitrary and are determined by the choice of the relative phases of the two overlaping atomic orbitals. The signs in Table 2.26 correspond to the choices shown in Figs. 2.17a and 2.23. The magnitudes of the interaction parameters decrease in the sequence C to Ge. We will show later that this trend can be understood from the increase in the lattice constant along this sequence. When the second-nearest neighbor interactions are included, only Vxx decreases somewhat. Since Vxx is the smallest interaction, the overall band structure is not significantly affected. Table 2.26. Tight-binding interaction parameters (in eV) for C, Si, and Ge obtained by Chadi and Cohen [2.25] when only nearest-neighbor interactions are included Ep Es C Si Ge 7.40 7.20 8.41 Vss 15.2 8.13 6.78 Vsp Vxx Vxy 10.25 5.88 5.31 3.0 3.17 2.62 8.3 7.51 6.82 To gain some insight into the band structure obtained with the tightbinding approach, we will calculate the band energies at the k 0 point. From (2.82a–d) we find g2 g3 g4 0 and g1 1 at k 0. Thus the 8×8 matrix simplifies into a 2×2 matrix for the s electrons and three identical 2×2 matrices for the p levels: Es E(0) Vss (2.83a) Vss Es E(0) and Ep E(0) Vxx . Vxx Ep E(0) (2.83b) These two matrices can be easily diagonalized to yield four energies: Es± (0) Es ± | Vss | (2.84a) 91 2. Electronic Band Structures and Ep± (0) Ep ± | Vxx | (2.84b) As a result of the overlap of the atomic orbitals the two s and p levels of the two atoms inside the primitive cell are split by an amount equal to 2 | Vss | and 2 | Vxx |, respectively. The level Es is raised in energy and its wave function is antisymmetric with respect to the interchange of the two atoms. This state corresponds to the antibonding s state in a diatomic molecule. The level Es corresponds to the bonding s state. From Table 2.5 we expect the antisymmetric antibonding state to have °2 symmetry and the symmetric bonding state to have °1 symmetry. Using a similar analogy, the triply degenerate antisymmetric °15 conduction band states correspond to the antibonding p orbitals while the symmetric °25 valence band states are identified with the bonding p orbitals. In Fig. 2.24 the valence band structure of Si calculated by the tight-binding method is compared with that obtained by the empirical pseudopotential method. Figure 2.24 also compares the valence band density of states obtained by the two methods (We will define density of states of a band in Sect. 4.3.1 and also in Chap. 8, where this concept will be utilized). In this tight-binding calculation one second-nearest-neighbor interaction has been included in addition to the nearest-neighbor interactions. The agreement between the two methods is quite good for the valence bands. Figure 2.25 shows a comparison between the band structure of Ge calculated by the tight-binding method, the empirical pseudopotential method, and the nearly free electron model. While the valence bands are well reproduced by the tight-binding method with the simple sp3 base used here, this is not true for the conduction bands since the 2 Γ25' 0 Energy [eV] → 92 Γ25' L3' L3' Si X4 –2 –4 Γ25' Σ1min K1 –6 –8 –10 L1 X1 L1 0.8 0.4 Density of states [states/eV atom] 0L K3 Γ1 L2' Γ1 Σ1min K1 L2' –12 1.2 K2 X4 Λ Γ Γ1 ∆ X U,K Σ Γ k→ Fig. 2.24. The valence band structure and density of states (see Sect. 4.3.1 for definition) of Si calculated by the tight-binding method (broken curves) and by the empirical pseudopotential method (solid lines) [2.25] Gap Conduction (a) LCAO Bands L2 v→ L1v→ L 3 v→ L1c→ L3c→ L2c→ °1→ °15c→ °2 c→ → ←X4v ™1→ (b) True bands °25v ←X1c ←Xc (c) Free-electron bands –12 –8 –4 0 4 8 12 Band energy [eV] Fig. 2.25. A comparison between the band structure of Ge calculated by (a) the tight-binding method, (b) the empirical pseudopotential method, and (c) the nearly free electron model [Ref. 2.24, p. 79] Valence Lc→ 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors 93 94 2. Electronic Band Structures conduction band electrons are more delocalized. The accuracy of the conduction bands in the tight-binding calculations can be improved by introducting additional overlap parameters. However, there is another shortcoming in the tight-binding model presented here. There are only four conduction bands in this model because we have included only four s and p orbitals. To correct this problem additional orbitals and overlap parameters are required; unfortunately they destroy the simplicity of this model. 2.7.3 Overlap Parameters and Nearest-Neighbor Distances So far we have shown that the advantage of the tight-binding approach is that the valence band structures of semiconductors can be calculated in terms of a small number of atomic energies and overlap parameters. Now we will demonstrate that these overlap parameters in different semiconductors can be expressed as a simple function of the nearest-neighbor distance multiplied by a geometric factor. These results combined make the tight-binding method very powerful for predicting the properties of many compounds (not just semiconductors) with only a small number of parameters [Ref. 2.24, p. 49]. One may expect some relationship between the overlap parameters and the interatomic distance based on the following simple argument. Figures 2.20 and 2.22 show that the atomic energy levels broaden into bands due to overlap of the atomic orbitals. The width of the band is essentially 2V, where V is the relevant overlap parameter. At the same time the electron wave functions become delocalized over a distance given by the nearest-neighbor separation (i. e., the bond length) d as a result of this overlap. Using the uncertainty principle the momentum of the delocalized electron is estimated to be (/d), so the electron kinetic energy is given by 2 2 /(2md2 ). This result suggests that the overlap parameters depend on d as d2 . This simple heuristic argument can be made more rigorous by comparing the band structures calculated by the tight-binding method and by the nearly free electron model. As an example, we will consider the lowest energy valence band in a crystal with the simple cubic structure. This band can be identified with the bonding s orbitals and its dispersion along the [100] direction can be shown to be given by Es 4VssÛ 2VssÛ cos kx (Problem 2.16). Thus the width of this band is equal to 4VssÛ . On the other hand the nearly free electron model gives the band width as 2 2 /(2md2 ). Equating the band widths obtained by these two different methods we get 4VssÛ 2 2 . 2md2 (2.85) In general, all four overlap parameters for the s and p orbitals can be expressed in the form Vll m Ùll m 2 md2 (2.86) 2.7 Tight-Binding or LCAO Approach to the Band Structure of Semiconductors where Ùll m is a factor which depends on the crystal symmetry. From (2.85) we see that ÙssÛ 2 /8 in crystals with the simple cubic structure. Table 2.27 lists the values of Ùll m for the simple cubic and diamond lattices. For the diamond and zinc-blende crystals, Harrison [2.26] has treated the factors Ùll m as adjustable parameters in fitting the energy bands of Si and Ge. He found excellent agreement between the calculated values and the adjusted values for three of the parameters. The only exception is Ùpp , where the fitted value of 0.81 is somewhat lower than the calculated one. Table 2.27. The geometric factor Ù relating the overlap parameters for the s and p bands to the free electron band width 2/(md 2) as shown in (2.86). The last column represents the adjusted values obtained by fitting the energy bands of Si and Ge [Ref. 2.24, p. 49] Simple cubic ÙssÛ 2 /8 1.23 Diamond and zinc–blende 92 /64 1.39 Adjusted values 1.40 ÙspÛ (/2)[(2 /4) 1]1/2 1.90 (92 /32)[1 (16/32 )]1/2 1.88 1.84 ÙppÛ 3 2 /8 3.70 212 /64 3.24 3.24 Ùpp 2 /8 1.23 32 /32 0.93 0.81 Table 2.27 together with (2.86) and the lattice constants are all that is needed to calculate the overlap parameters for computing the valence bands and the lowest conduction bands in many zinc-blende- and diamond-type semiconductors. Even without any detailed calculations,. we can understand qualitatively the symmetries of the conduction and valence bands at the Brillouin zone center of the three group-IV elements Si, Ge, and gray tin (or ·Sn). The lattice constant increases from Si to ·-Sn. This results in a decrease in the overlap parameters | Vss | and | Vxx | (the variation from C to Ge is shown in Table 2.26). The decrease is larger for | Vss | than for | Vxx |. As a result, the ordering of the s and p orbitals changes from Si to ·-Sn in the manner shown in Fig. 2.26. The Fermi level is located by filling the bands with the eight valence electrons available. In this way it is easily seen that the lowest conduction band at zone center in Si is p-like while the corresponding band in Ge is s-like. In this scheme ·-Sn turns out to be a semi-metal because of the lower energies of the bands derived from the s orbitals. It was first shown by Herman [2.27] that relativistic effects are responsible for this in gray tin (and also in HgTe and HgSe. Note, however, that the s-p reversal for HgSe has recently been the object of controversy; see [2.28]). 95 96 2. Electronic Band Structures s (antibonding) p (antibonding) p Si EF (Fermi level) p (bonding) s s (bonding) p (antibonding) p s (antibonding) EF (Fermi level) p (bonding) Ge s s (bonding) p (antibonding) p p (bonding) EF (Fermi level) s (antibonding) α-Sn s s (bonding) Fig. 2.26. Evolution of s and p atomic orbitals into the conduction and valence bands at zone center within the tight-binding approximation for Si, Ge, and ·-Sn. The band ordering for diamond is similar to that of Si. PROBLEMS 2.1 Template of an fcc Brillouin Zone Construct a model of the Brillouin zone of the fcc lattice by pasting a copy of the template shown in Fig. 2.27 on cardboard and cutting along the solid lines. Score along the broken lines. Tape the edges together. 2.2 Group Theory Exercises a) Verify the character table of the Td point group as given in Table 2.3. Problems X U Z W K L Fig. 2.27. Template for constructing a model of the Brillouin zone of the fcc lattice. Paste this sheet on thin cardboard and cut along solid lines. Score along broken lines and tape the joints b) By applying the symmetry operations of Td to the basis functions in Table 2.3 show that the functions transform according to their respective irreducible representations. 2.3 Group Theory Exercises a) By using the character table of Td show that T2 ⊗ T2 T1 ⊕ T2 ⊕ E ⊕ A1 . b) Verify that the symmetrized linear combinations of the matrix elements of a second-rank tensor given in Sect. 2.3.4 transform according to the irreducible representations T1 , T2 , E, and A1 . 2.4 Symmetrized Wave Functions: Transformation Properties Verify that the symmetrized wave functions in Tables 2.9 and 2.10 transform according to their respective irreducible representations. 97 98 2. Electronic Band Structures 2.5 Characters of C3v and C2v Point Groups Deduce by inspection the characters for the C3v and C2v point groups in Tables 2.12 and 2.14, respectively. 2.6 Compatibility Relations Use Tables 2.3, 2.4, 2.12 and 2.14 to verify the following compatibility relations: °1 ¢1 §1 °2 ¢2 §2 °3 ¢1 ⊕ ¢2 §3 °4 ¢1 ⊕ ¢3 ⊕ ¢4 §1 ⊕ §3 °5 ¢2 ⊕ ¢3 ⊕ ¢4 §2 ⊕ §3 . 2.7 Representations of Nonsymmorphic Groups a) Using Tables 2.15 and 2.19 show that the doubly degenerate X1 and X2 states in the diamond crystal split into the X1 ⊕ X3 and X2 ⊕ X4 states, respectively, when the diamond crystal (nonsymmorphic) is transformed into a zinc-blende crystal (symmorphic) by making the two atoms in the primitive cell different. Under the same transformation the X3 and X4 states remain doubly degenerate and become the X5 state in the zinc-blende crystal. b) Some Insight into the Doubly Degenerate Wavefunctions at the X point of the Brillouin Zone in the Diamond Structure. Within the free electron approximation, the wave functions at the X point of the Brillouin Zone can be written as: exp [ik · r] where k (2/a)(±1, 0, 0), (2/a)(0, ±1, 0), or (2/a)(0, 0, ±1). Let us consider the wave functions „1 sin [(2/a)x] and „2 cos [(2/a)x]. Assume that the crystal structure of diamond simply has inversion symmetry I: (x, y, z) → (x, y, z); then by applying this symmetry operation to „1 we obtain „1 . Since the crystal is invariant under I we expect „1 and I„1 to have the same energy. We find that this is trivially satisfied since „1 and I„1 are linearly dependent. Thus we cannot conclude that the states „1 and „2 should be degenerate. Now we take into account that the inversion operation in the diamond lattice is not simply I but rather I : (x, y, z) → (x (a/4), y (a/4), z (a/4)). Applying I to „1 we find that: I „1 sin [(2/a)(x (a/4)] sin [(2/a)(x) (/2)] cos [(2/a)(x)] cos [(2/a)x] „2 . Since „1 and „2 are not linearly independent we have to conclude that „1 and „2 are degenerate from the fact that the crystal is invariant under I . Similarly one can show that all the other plane wave states at the X point are doubly degenerate because of this symmetry operation I . 2.8 Pseudopotential Band Structure Calculation by Hand The purpose of this exercise is to show how pseudopotentials lift degeneracies in the nearly-free-electron band structure and open up energy gaps. Since the pseudopotentials are weak enough to be treated by perturbation theory, rather Problems accurate band energies can be evaluated with a pocket calculator without resorting to a large computer. We will consider only the six lowest energy wave functions at the X point of a zinc-blende-type semiconductor. In the nearly-free-electron model, the electron wave functions are given by exp (ik · r), where k (2/a)(±1, 0, 0) and (2/a)(0, ±1, ±1). For brevity these six wave functions will be denoted by | 100, | 100, | 011, | 011, | 011, and | 01 1. a) Show that these six wave functions can be symmetrized according to the following irreducible representations: √ √ „1 (1/ 2)[| 011 | 01 1] and „2 (1/ 2)[| 011 | 01 1] ↔ X5 „3 (1/2){[| 011 | 01 1] i[| 011 | 011]} ↔ X3 „4 (1/2){[| 011 | 01 1] i[| 011 | 011]} ↔ X1 „5 (1/2){[| 100 | 1 00] i[| 100 | 100]} ↔ X1 „6 (1/2){[| 100 | 1 00] i[| 100 | 100]} ↔ X3 It should be noted that the pseudopotential form factors in Table 2.21 have been defined with the origin chosen to be the midpoint between the two atoms in the primitive cell. In order to conform with this coordinate system, the symmetry operations for the group of X have to be defined differently from those in Sect. 2.3.2. Taking the axes and planes of the point group to intersect at the midpoint some of the symmetry operations must involve a translation. b) Calculate the matrix elements of the pseudopotential between these wave functions. This task can be greatly simplified by using the matrix element theorem. Since the pseudopotential V has the full symmetry of the crystal, it has °1 symmetry. The only states that are coupled by V are then the X3 states „3 and „6 and the X1 states „4 and „5 . Show that the resulting 6×6 matrix {Vij } is s v8 0 0 0 0 0 0 vs 0 0 0 0 8 √ 0 s a a s 0 v8 2v4 0 0 i 2(v3 v3 ) √ 0 0 0 vs8 2va4 i 2(va3 vs3 ) 0 √ a s a 0 0 0 i 2(v3 v3 ) v4 0 √ a s a 0 0 i 2(v3 v3 ) 0 0 v4 c) Diagonalize the secular determinant 2 k2 E ‰ij Vij 0 2m by reducing it to three 2×2 determinants. Show that the resultant energy levels are 42 2 E(X5 ) vs8 , ma2 99 100 2. Electronic Band Structures 62 2 s a v8 3v4 ma2 ⎡ ⎤1/2 2 1 ⎣ 22 2 ± vs8 va4 8(va3 vs3 )2 ⎦ , 2 ma2 1 62 2 E(X3 ) vs8 3va4 2 ma2 ⎡ ⎤1/2 2 2 2 1 2 ± ⎣ vs8 va4 8(va3 vs3 )2 ⎦ . 2 ma2 1 E(X1 ) 2 d) Calculate the energies of the X1 , X3 , and X5 levels in GaAs by substituting into the expression in (c) the pseudopotential form factors for GaAs. Take the lattice parameter a to be 5.642 Å. In Fig. 2.28 these results are compared with the nearly free electron energies and with the energies obtained by the EPM. e) If you want to improve on the present calculation, what are the plane wave states and pseudopotential form factors you should include? Note: Often in the literature, the origin of the coordinates adopted by the authors is not specified.4 The symmetry of the band structure at the X point of the zinc-blende-type crystal depends on the choice of origin and this has Free electron model X1, X3, X5 Empirical pseudopotential model X3 1.0eV X1 } Pseudopotential by hand Conduction band X5 4.3eV X1, X3 X3 X1 2.74eV 4.3eV 4.72 eV 0.74eV X3 4.7eV X1 } X5 5.6eV X3 Valence band 4.6eV X1 Fig. 2.28. The lowest energy bands at the X point of GaAs computed by the nearly free electron model, the EPM, and the perturbation approach of Problem 2.8. The X1 –X3 notation corresponds to ˘ja 0, i. e., to placing the cation at (a/4)(111) and the anion at the origin. 4 We assume, implicitly, that the origin is also the common point of the point group axes which specify the symmetry. Problems caused considerable confusion, see [2.29]. For example, if the origin is chosen at the anion the conduction band with the X1 symmetry is mainly composed of the anion s wave function and cation p wave function. On the other hand, the X3 conduction band state is made up of the cation s wave function and the anion p wave function. In all zinc-blende-type semiconductors with the exception of GaSb [2.30, 31] the X1 state has lower energy than the X3 state. If the origin is chosen at the cation, the signs of ˘ja and, correspondingly, the roles of X1 and X3 are reversed. 2.9 Wave Functions of the L-Point of Zinc-Blende Using the symmetrized k (2/a)(1, 1, 1) wave functions in the nearly free electron model for zinc-blende-type crystals: √ °1 : √8 cos (2x/a) cos (2y/a) cos (2z/a); °4 (x): 8 sin (2x/a) cos (2y/a) cos (2z/a), and similar wave functions for °4 (y) and °4 (z) in Table 2.9, show that the matrix elements of the momentum operator p between the °1 and °4 functions are given by |°1 | px | °4 (x)|2 |°1 | py | °4 (y)|2 |°1 | pz | °4 (z)|2 (2/a)2 while all the other matrix elements of pi such as |°1 | px | °4 (y)|2 are equal to 0. 2.10 Double Group Representations In many quantum mechanics textbooks one can find the following result. The effect of a rotation by an infinitesimal amount ‰ı with respect to an axis defined by the unit vector n̂ on an orbital wave function f (r) can be obtained by applying the operator exp [i‰£n · l/] to f (r). For a spin s 1/2 particle the corresponding operator on the spin wave functions due to rotation by an angle £ is given by exp [i£n̂ · Û /2]. Using this operator,. show that: a) The effect of a 2 rotation on the wave functions · and ‚ of a spin 1/2 particle is to change the sign of · and ‚, and hence the corresponding trace of Ê is 2; b) the traces corresponding to the symmetry operations in Table 2.23 within the basis · and ‚ are {E} {3C2 } {3ÊC2 } 2 0 {6S4 } √ 2 {6Û} {6ÊÛ} {8C3 } {Ê} {6ÊS4 } {8ÊC3 } 0 1 2 √ 2 1 c) The Double Group at the X Point of the Zinc-Blende Structure As an additional exercise on the calculation of double group character table, we shall consider the X point of the zinc-blende structure. 101 102 2. Electronic Band Structures The first step is to decide what are the classes in the double group. In this case we need only to compare the single group and double group classes at the zone center since the classes of X form a subset of these classes. It should not be difficult to see that there are now 7 classes: {E}, {C42 (x), ÊC42 (x)}, {2C42 (y, z), 2ÊC42 (y, z)}, {2S4 }, {2md }, {Ê} and {ÊS4 }. Using the results of Problem 2.10 one can show that the characters of these operations on the two spin wavefunctions are: E C42 (x), ÊC42 (x) 2 2C42 (y, z), 2ÊC42 (y, z) 0 2S4 √ 0 2 2md Ê ÊS4 0 2 √ 2 Using this result we can show that the character table for the double group of the X point in the zinc-blende crystal is: E X1 X2 X3 X4 X5 X6 X7 1 1 1 1 2 2 2 C42 (x), ÊC42 (x) 1 1 1 1 2 0 0 2C42 (y, z), 2ÊC42 (y, z) 1 1 1 1 0 0 0 2S4 1 1 1 1 √0 √2 2 2md 1 1 1 1 0 0 0 Ê ÊS4 1 1 1 1 2 2 2 1 1 1 1 √0 √2 2 Using these characters the reader should show that the X1 , X3 , and X5 representations in the zinc-blende structure (see Problem 2.10) go over to the X6 ⊗ X1 X6 , X6 ⊗ X3 X7 and X6 ⊗ X5 X6 ⊕ X7 representations in the double group (see, for example, the band structure of GaAs in Fig. 2.14). 2.11 The Structure Factor of Bond Charges in Si The intensity of x-ray scattering peaks from a crystal depends on the structure factor S of the crystal. The structure factor of the Si crystal (face centered cubic or fcc lattice), in particular, is discussed in many standard textbooks on solid state physics, such as Kittel’s “Introduction to Solid State Physics” (Chap. 2 in 6th Edition). The basis of the fcc structure is usually taken to be the cubic unit cell with four atoms per unit cube. These four atoms can be chosen to have the locations at (0, 0, 0); (0, 1/2, 1/2); (1/2, 0, 1/2) and (1/2, 1/2, 0) [in units of the size of the cube: a]. The structure factor Sfcc (hkl) for a wave vector (h, k, l) in reciprocal space then vanishes if the integers h, k and l contain a mixture of even and odd numbers. In the case of the Si crystal there are now 8 atoms per unit cube since there are two interpenetrating fcc sublattices displaced from each other by the distance (1/4, 1/4, 1/4). As a result, the structure factor of the Si crystal Problems SSi (hkl) is given by: SSi (hkl) Sfcc (hkl)[1 exp (i/2)(k k l)]. This implies that SSi (hkl) will be zero if the sum (h k l) is equal to 2 times an odd integer. When combining the above two conditions one obtains the result that SSi (hkl) will be non-zero only if (1) (k, k, l) contains only even numbers and (2) the sum (h k l) is equal to 4 times an integer. See, for example, Kittel’s “Introduction to Solid State Physics” (Chap. 2 in 6th Edition), Problem 5 at the end of Chap. 2. Based on this result one expects that the diffraction spot corresponding to (2, 2, 2) in the x-ray diffraction pattern of Si will have zero intensity since h k l 6. It has been known since 1959 that the so-called forbidden (2, 2, 2) diffraction spot in diamond has non-zero intensity (see Ref. [3.23] or Kittel’s “Introduction to Solid State Physics”, p. 73 in 3rd Edition). It is now well established that the presence of this forbidden (2, 2, 2) diffraction spot can be explained by the existence of bond charges located approximately mid-way between the atoms in diamond or silicon. What is the structure factor of the bond charges in the Si crystal if one assumes that they are located exactly mid-way between two Si atoms? 2.12 Matrix Elements of p a) Show that all matrix elements of p between the °4 valence bands and the °4 conduction bands of zinc-blende-type semiconductors of the form X | px | °4c (z), Z | py | °4c (z), or X | py | °4c (y), where at least two of the labels x, y, or z are identical, vanish as a result of the requirement that the crystal is invariant under rotation by 180˚ with respect to one of the three equivalent [100] axes. b) As a result of (a), the only nonzero matrix elements of p are of the form X | py | °4c (z). Using the three-fold rotational symmetries of the zinc-blende crystal, show that X | py | °4c (z) Y | pz | °4c (x) Z | px | °4c (y) and X | pz | °4c (y) Y | px | °4c (z) Z | py | °4c (x). c) Finally, use the reflection symmetry with respect to the (110) planes to show that X | py | °4c (z) Y | px | °4c (z). 2.13 Linear Terms in k Show that the k linear term due to the k · p interaction is zero in the zincblende crystal at the °-point. 103 104 2. Electronic Band Structures 2.14 k · p Method a) Use (2.52) to calculate the elements of the 6×6 matrix {Hij }. b) Use a computer and a matrix diagonalization program to calculate the valence band structure of GaAs from these parameters for GaAs: P2 /(m0 ) 13 eV; Q2 /(m0 ) 6 eV; E0 1.519 eV; E0 4.488 eV; ¢ 0.34 eV and ¢0 0.171 eV. 2.15 Valence Bands; k · p Hamiltonian a) Calculate the 4×4 matrix obtained by taking matrix elements of the Luttinger Hamiltonian in (2.70) between the Jz ± 3/2 and ±1/2 states of the J 3/2 manifold. b) Diagonalize this 4×4 matrix to obtain two sets of doubly degenerate levels with energies 2 E± {Á1 k2 ± [4Á22 k4 12(Á23 Á22 )(k2x k2y k2y k2z k2z k2x )]1/2 }. 2m c) By comparing the results in (b) with (2.66) derive (2.71). d) Calculate the contributions of the lowest °3 conduction band term to Á1 , Á2 , and Á3 . Show that it is not negligible for silicon and diamond [2.22]. 2.16 Energy Bands of a Semiconductor in the Tight-Binding Model a) Derive the 8×8 matrix for the s and p band energies in a zinc-blende-type semiconductor using the tight-binding model. b) Show that at k 0 the energies of the s and p bands are given by Es± (0) 12 (Es1 Es2 ) ± 12 [(Es1 Es2 )2 4 | Vss |2 ]1/2 and Ep± (0) 12 (Ep1 Ep2 ) ± 12 [(Ep1 Ep2 )2 4 | Vxx |2 ]1/2 instead of (2.84a) and (2.84b). Es1 and Es2 are the atomic s level energies S1 | 0 | S1 and S2 | 0 | S2, respectively, while Ep1 and Ep2 are the corresponding energies for the atomic p levels. 2.17 Tight Binding Overlap Integrals Evaluate the geometric factors Ùll m in Table 2.27. 2.18 Tight Binding Hamiltonian Given two p orbitals, one located at the origin and the other at the point d(cos £x , cos £y , cos £z ), where d is the distance between the two p orbitals and cos £x , cos £y , and cos £z are the directional cosines of the second p orbital, show that the overlap parameters Vxx and Vxy are given by Vxx VppÛ cos 2 £x Vpp sin 2 £x , Vxy [VppÛ Vpp ] cos £x cos £y . 2.19 Conduction and Light Hole Bands in Small Band Gap Semiconductors Write down the 2 × 2 Hamiltonian matrix which describes the conduction and Problems the light hole band of a narrow gap semiconductor such as InSb. Diagonalize it and discuss the similarity of the resulting expression with the relativistic energy of free electrons and positrons [4.28]. Use that expression to estimate non-parabolicity effects on the conduction band mass. Comments on the Equivalence of the Brillouin Zone Edge Points U and K 3 In these figures the zone-edge points U and K are indicated to be equivalent. This is true strictly only for Bloch waves indexed by these points which lie on the Brillouin Zone (BZ) surface but not for for waves with wave vector along the lines joining them to X nor to °. This is easily seen from the fcc lattice template in Fig. 2.27. Both U and K lie on the hexagonal Brillouin zone face along the [111] direction. However, the line X-U is in general not equivalent to the line XK. For the endpoints U and K which lie on the BZ boundary their Bloch waves become equivalent in the diamond lattice as a result of the three-fold rotation and the “inversion symmetry” operations of the lattice. Also only the line °-K is along the [110] or ™ direction so the label for the horizontal axis °-™-U,K in these figures refers to K only. In the zincblende structure without the “inversion symmetry” U and K are no longer equivalent as can be seen from Fig. 2.14 and 2.15. In Figures 3.2, 3.10 and 3.11 this problem is avoided by not labeling the symmetry points indicated by a broken vertical line in these figures. This symmetry point is really K as we can conclude from the above discussion. We are grateful to Dr. L.C. Andreani of the University of Pavia, Italy for pointing out this ambiguity to us. 2.20 Parity of the s-like Electron Wavefunctions at the L point of Si and Ge In discussing the valence and conduction band structures of diamond-type semiconductors based on the tight-binding approximation, we point out that the valence bands are formed from the bonding orbitals while the conduction bands are formed from the anti-bonding orbitals. Furthermore, we note that the bonding orbitals have even parity under inversion in order that the electron charge density be higher at the center of the bond. On the other hand, the antibonding orbitals have odd parity under inversion. This result explains why the valence bands at the zone center of Si (see Fig. 2.10) and Ge (see Fig. 2.13) have even parity while the conduction bands at the zone center have odd parity. This is not true at the L point of the Brillouin zone. [It should be noted that along many high symmetry directions, such as ¢ and §, inversion is not a symmetry operation since k and k are not identical. However, at the L point k and k are the same in the reduced zone scheme and hence parity is a good quantum number.]. The lowest energy valence band state at the L-point (which arises from the bonding s-orbital) has odd parity (L 6 in Ge and L2 in Si) while the lowest energy conduction band (which arises mainly from the anti-bonding s-orbital) has even parity (L 6 in Ge and L1 in Si) under the special inversion operator I of the diamond lattice. 105 106 2. Electronic Band Structures (a) Calculate the energy and wave functions of these bands at the L point directly by using the nearly-free electron model (use reasonable approximations to simplify the problem as far as possible) and check the parity of the resulting wave functions under the “inversion” operation I . (b) Repeat your calculation by using the tight-binding model and check again the parity of the resulting wave functions under the operation I . (c) Why does the odd parity state have lower energy rather than the even parity state at the L point? Does this result somehow violate the “compatibility relation” in changing a bonding state at k 0 into an anti-bonding state at the L point? SUMMARY A semiconductor sample contains a very large number of atoms. Hence a quantitative quantum mechanical calculation of its physical properties constitutes a rather formidable task. This task can be enormously simplified by bringing into play the symmetry properties of the crystal lattice, i. e., by using group theory. We have shown how wave functions of electrons and vibrational modes (phonons) can be classified according to their behavior under symmetry operations. These classifications involve irreducible representations of the group of symmetry operations. The translational symmetry of crystals led us to Bloch’s theorem and the introduction of Bloch functions for the electrons. We have learnt that their eigenfunctions can be indexed by wave vectors (Bloch vectors) which can be confined to a portion of the reciprocal space called the first Brillouin zone. Similarly, their energy eigenvalues can be represented as functions of wave vectors inside the first Brillouin zone, the so-called electron energy bands. We have reviewed the following main methods for calculating energy bands of semiconductors: the empirical pseudopotential method, the tight-binding or linear combination of atomic orbitals (LCAO) method and the k · p method. We have performed simplified versions of these calculations in order to illustrate the main features of the energy bands in diamond- and zinc-blende-type semiconductors. 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions CONTENTS 3.1 3.2 Phonon Dispersion Curves of Semiconductors . . . . . . . . . . . . . . . . . . . Models for Calculating Phonon Dispersion Curves of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Electron–Phonon Interactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110 114 121 137 158 We will start the discussion of the vibrational properties of semiconductors by reviewing the theory of the dynamics of a crystalline lattice. The Hamiltonian describing a perfect crystal has already been given in (2.1). We note that the electrons have been separated into two groups. The core electrons are assumed to move rigidly with the nucleus to form what has been referred to as the ion. The valence electrons interact with these ions via the pseudopotentials. The part of the Hamiltonian in (2.1) which involves the nuclear motions is given by Hion (R1 , . . . , Rn ) Pj2 j 2Mj 1 Zj Zj e2 Z j e2 , (3.1) 2 4Â0 |Rj Rj | 4Â0 |ri Rj | j, j i, j momentum, where Rj , Pj , Zj and Mj are, respectively, the nuclear positions, charge, and mass, ri is the position of the electron and means summation over pairs of indices j and j where j is not equal to j . The appearance of the electronic coordinates in this Hamiltonian makes it difficult to solve for the nuclear motion since electronic motion is coupled to ionic motion. As pointed out already in Sect. 2.1, one way to separate the two is by introducing the Born–Oppenheimer or adiabatic approximation. In this approximation the electrons are assumed to follow the ionic motion adiabatically. As a result we can solve the electronic part of the Hamiltonian H in (2.1) to obtain the energies of the electrons as functions of the ion positions. On the other hand, the ions cannot follow the electronic motion and therefore they see only a time-averaged adiabatic electronic potential. Hence the Hamiltonian for the ions can be written as Hion Pj2 j 2Mj Ee (R1 , . . . , Rn ), P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed., DOI 10.1007/978-3-642-00710-1_3, © Springer-Verlag Berlin Heidelberg 2010 (3.2) 108 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions where Ee (R1 , . . . , Rn ), which represents the total energy of the valence electrons with ions held stationary at positions R1 , . . . , Rn , is treated as the interaction between ions via the electrons. With the help of supercomputers, it is now possible to calculate Ee (R1 , . . . , Rn ) and then solve ab initio for the motion of the ions. Since much of the work on lattice dynamics was carried out before supercomputers were available, these early investigations had to rely on a phenomenological approach. In this approach typically an equation of motion for the ions is obtained by expanding Hion as a function of their displacements ‰Rj from their equilibrium positions Rj0 : Hion H0 (R10 , . . . , Rn0 ) H (‰R10 , . . . , ‰Rn0 ). (3.3) In (3.3), H0 (R10 , . . . , Rn0 ) is the Hamiltonian of the crystal with all the nuclei at their equilibrium positions and H (‰R10 , . . . , ‰Rn0 ) is the change in Hion due to displacements of the nuclei by small amounts ‰R10 , . . . , ‰Rn0 from the equilibrium positions. To diagonalize H , one expands Hion around R10 , . . . , Rn0 . Since the Rj0 are the equilibrium positions of the ions, the first-order terms in ‰Rj vanish. In addition, when all the ‰Rj are identical, the crystal is uniformly displaced and not distorted. Thus the lowest order terms in the expansion of Hion relevant to the vibration of the crystal are second order in ‰(Rj Rk ). If we keep only the terms quadratic in H , the motions of the nuclei are described by a collection of simple harmonic ocillators, and hence this approach is known as the harmonic approximation. We will restrict our treatment of the lattice dynamics of semiconductors to the harmonic approximation only. One important limitation of this approach is that we cannot explain some phenomena, for example, thermal expansion. In particular, it is now well established that the coefficient of linear expansion in many diamond- and zinc-blende-type semiconductors changes sign twice when their temperature is increased from liquid helium temperature to room temperature [3.1]. To simplify the notations we will denote the displacement from equilibrium of the ion k in the unit cell l by ukl . Within the harmonic approximation H can be expressed as 2 1 1 dukl H (ukl ) Mk ukl · º(kl, k l ) · uk l . (3.4) 2 dt 2 kl In this equation H (ukl ) represents the change in the ion Hamiltonian induced by a displacement of the ion (kl) while all the other atoms are kept in their equilibrium position. The matrix º(kl, k l ) contains the force constants describing the interaction between the ions denoted by (kl) amd (k l ). For example, the force on ion (kl) due to the displacement uk l of the (k l ) ion is given by º(kl, k l ) · uk l . The force constants contain two parts. The first part is the direct ion–ion interaction due to their Coulomb repulsion, the second is an indirect interaction mediated by the valence electrons. The motion of one ion causes the electron distribution to change. This rearrangement of the electrons produces a force on the neighboring ions. In Sect. 3.2 we will consider the various models for calculating the force constants. At this point we will 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions summarize the procedures for obtaining the phonon dispersion curves assuming the force constants are known. The determination of the lattice dynamics described by the Hamiltonian in (3.4) can be carried out in two steps. First we will treat the Hamiltonian classically and solve the equation of motion. In this classical approximation (3.4) describes the energy of a collection of particles executing small-amplitude oscillations. As is well known in classical physics, these oscillations can be expressed in terms of normal modes which are independent of each other [3.2]. In the second step we quantize the energies of these normal modes. Each quantum of lattice vibration is called a phonon. The procedures for determining the quantized energy levels of one-dimensional simple harmonic oscillators can be found in most quantum mechanics textbooks, so we will not repeat them here. Instead we will concentrate on the determination of the normal modes of vibrations described by (3.4). Since º(kl, k l ) possesses translational symmetry, we expect that the atomic displacements which diagonalize (3.4) can be expressed in terms of plane waves similar to the Bloch functions for electrons in a crystal [as defined by (2.6) in Sect. 2.2]. If ukl is the displacement of the kth ion in the lth unit cell specified by the lattice vector Rl , it can be related to the displacement uk0 of a corresponding ion in the unit cell located at the origin by a Bloch wave of the form ukl (q, ˆ) uk0 exp i(q · Rl ˆt), (3.5) where q and ˆ are, respectively, the wave vector and frequency of the wave. There is, however, one important difference between phonon and electron Bloch waves. While an electron can be anywhere in the crystal, ion positions, in the classical approximation, are discrete. Since the Rl in (3.5) are lattice vectors, two waves whose wave vectors differ by a reciprocal lattice vector are equivalent. In terms of Brillouin zones introduced in Sect. 2.2, this result can be stated as: the phonon frequencies in the first Brillouin zone are identical to those in the other Brillouin zones. Thus the frequency versus wave vector plots for lattice vibrations in crystals (or phonon dispersion curves) are always presented in the reduced zone scheme. Another important consequence of (3.5) is that the degrees of freedom or the number of independent waves is equal to three times the number of atoms in the crystal. By substituting (3.5) for ukl into (3.4) and using the resultant expression in the classical Hamilton equation [3.2] we obtain the equation for uk0 : Mk ˆ2 uk0 º(km, k 0) exp(iq · Rm )uk 0 . (3.6) k, m Introducing a mass-modified Fourier transform of º as Dkk (q) º(mk, 0k ) (Mk Mk )1/2 exp iq · Rm , (3.7) m (3.6) can be written as Dkk (q) ˆ2 ‰kk uk 0 0. k (3.8) 109 110 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions Dkk (q) is known as the dynamical matrix. The vibrational frequencies ˆ are found by solving the secular equation | Dkk (q) ˆ2 ‰kk | 0. (3.9) The vibrational amplitudes uk0 are obtained by substituting the solutions of (3.9) into (3.8). Readers should refer to textbooks on linear algebra or classical mechanics for further details of procedures for diagonalizing the matrix in (3.8). The main differences between the above classical treatment and a quantum mechanical calculation are: (1) in the quantum case the energy levels of a vibrational mode of frequency ˆ are quantized as [n (1/2)] ˆ and (2) the creation and annihilation operators for a quantum of vibration (or phonon) are expressed in terms of the vibration amplitudes uk0 . The organization of the rest of this chapter is as follows: in the next section we discuss qualitative features of phonon dispersion curves in diamondand zinc-blende-type semiconductors, in Sect. 3.2 we study models for computing these dispersion curves from (3.9), while the last section concentrates on interactions between electrons and phonons. Within the harmonic approximation (3.4) the phonons have an infinite lifetime. Inclusion of higher order, anharmonic terms results in a finite lifetime which can be calculated by ab initio techniques [3.3]. 3.1 Phonon Dispersion Curves of Semiconductors Phonon dispersion curves in crystals along high-symmetry directions of the Brillouin zone can be measured quite precisely by inelastic neutron scattering1 and more recently by high resolution inelastic x-ray scattering. Figures 3.1– 3.3 show the dispersion curves of Si, GaAs, and GaN. These results can be regarded as representatives of semiconductors with the diamond-, zincblende-, and wurtzite-type lattices, respectively. In the diamond- and zincblende-type lattices there are two atoms per primitive unit cell, and hence there are six phonon branches. These are divided into three acoustic phonon branches (the three lower energy curves) and three optical phonon curves. Along high-symmetry directions (such as the [100] and [111] directions in Si and GaAs) the phonons can be classified as transverse or longitudinal according to whether their displacements are perpendicular or parallel to the direction of the wave vector q. In a solid the long wavelength transverse acoustic (abbreviated as TA) phonons are shear sound waves while the longitudinal acoustic (LA) phonons correspond to compressional sound waves. The velocities of these sound waves are determined by the shear and bulk elastic moduli, respectively. Since it is 1 B.N. Brockhouse and C.G. Shull were awarded the Nobel Prize in 1994 for their development of neutron scattering spectroscopy, Brockhouse and Iyengar first measured the phonon dispersion in Ge by inelastic neutron scattering [Phys. Rev. 111, 747 (1958)]. 3.1 Phonon Dispersion Curves of Semiconductors ∆ 2' 15 Frequency [THz] ∆5 L3' Σ1 X4 Γ25' Σ2 L1 Σ3 X1 10 L 2' Σ1 ∆1 Σ3 5 Σ4 X3 ∆5 L3 Γ L Λ ∆ X Γ Σ Fig. 3.1. Phonon dispersion curves in Si along high-symmetry axes. The circles are data points from [3.4]. The continuous curves are calculated with the adiabatic bond charge model of Weber [3.5] 10 Γ ∆ Σ X 1 Frequency [THz] 3,4 1 3 6 4 1 5 8 Γ Λ 1 3 3 2 1 1 1 1 3,4 1 2 1 1 X Z W 2 2 3 1 3 1 1 4 1 5 1 3 1 1 1 2 3 5 2 L 2 1 Q L 3 1 1 5 3 2 3 2 4 0 Fig. 3.2. Phonon dispersion curves in GaAs along high-symmetry axes [3.6]. The experimental data points were measured at 12 K. The continuous lines were calculated with an 11-parameter rigid-ion model. The numbers next to the phonon branches label the corresponding irreducible representations usually easier to shear than to compress a crystal, the TA phonons travel with lower velocities than the LA phonons. Two special features of the TA phonons in the diamond- and zinc-blende-type semiconductors are: (1) their dispersion curves are relatively flat near the zone edge; and (2) their energies are much lower than the LA phonon energy near the zone edge. We will later show that these features are related to the covalent nature of bonds in these crystals. In Si the transverse optical (TO) phonons and the longitudinal optical (LO) phonons are degenerate at the zone center. In GaAs and other zincblende-type semiconductors, the LO phonon has higher energy than the TO 111 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions 800 Γ K Γ M E1(LO) A A1(LO) 700 B1 600 −1 Energy (cm ) 112 E2 500 A1(TO) 400 E1(TO) B1 300 200 E2 100 0 0 0.1 0.2 0.3 0.4 0.5 0.4 0.3 0.2 0.1 0 0.1 0.2 0.3 0.4 0.5 qx (r.l.u.) 3 1/2 qy (r.l.u.) qz (r.l.u.) Fig. 3.3. Phonon dispersion along high symmetry directions in the wurtzite structure semiconductor GaN [3.7]. The experimental points have been obtained by Raman scattering (open circles) and by high resolution inelastic x-ray scattering (closed circles). The continuous curves are obtained by an ab initio calculation phonons near the zone center. Exactly at the zone center, the TO and LO phonons in the zinc-blende crystals must also be degenerate because of the cubic symmetry of the zinc-blende structure. This degeneracy and dispersion of the zonecenter optical phonons in zinc-blende crystals will be taken up again in Sect. 6.4 when we study the interaction between the TO phonons and infrared radiation. At wave vectors near but not exactly at the zone center, the LO phonon frequency in GaAs and other zinc-blende crystals is higher than that of the TO phonons. The reason lies in the partially ionic nature of the bonding in zincblende crystals. For example, in GaAs the As atoms contribute more electrons to the bond than the Ga atoms. As a result, the electrons in the covalent bond spend, on average, somewhat more time near the As atoms than near the Ga atoms, so the As atoms are slightly negatively charged while the Ga atoms are slightly positively charged. Let us assume that a long-wavelength TO phonon propagating along the [111] direction is excited. The positive and negative ions lie on separate planes perpendicular to the [111] axis. In a TO mode the planes of positive and negative ions essentially slide pass each other. The situation is similar to sliding the two plates of a parallel-plate capacitor relative to each other while keeping their separation constant. The energy of the capacitor is not changed by such motion. On the other hand, the energy of the charged capacitor is increased when the two plates are pulled apart because there is an additional restoring force due to the Coulomb attraction between the positively and negatively charged plates. Similarly, an additional Coulombic restoring force is present in long-wavelength LO phonon modes but not in the TO phonon modes. The analogy between the optical phonons and the displacements of the capacitor plates is shown in Fig. 3.4. This additional restoring force (F) aris- 3.1 Phonon Dispersion Curves of Semiconductors + + + + + + Zinc-blende crystal along <111> axis + + + F F - - Displacement Parallel plate capacitor Displacement <111> + + + + - Fig. 3.4. Comparison between the displacement of atoms in an ionic crystal during a longwavelength longitudinal optical vibration and in an infinite parallel plate capacitor. F represents the restoring force which results from displacements of the charges shown ing from the displacement of the ions increases the frequencies of the longwavelength LO phonons above those of the corresponding TO phonons. In Sect. 6.4.4 we shall show explicitly that there is a longitudinal electric field which depends on the atomic displacements in a LO phonon but not in a TO phonon. This longitudinal electric field results in an additional interaction between LO phonons and electrons (Sect. 3.3.5). In Si the two atoms in the unit cell are identical so the bonding is purely covalent and the two atoms do not carry charge. As a result there is no additional restoring force associated with LO phonons and the zone-center optical phonons are degenerate.2 Vibrational modes in a crystal can be symmetrized according to the space group symmetry of the crystal just like the electronic states. A phonon mode is defined by the displacements of the atoms inside the unit cell. Thus the symmetry of the phonon must belong to the direct product of the representation of a vector and the respresentation generated by a permutation of the positions of equivalent atoms in the unit cell. The symmetry of the longwavelength phonons in Si and GaAs has already been considered in Sect. 2.3.2a. An example of how to determine the symmetries of long-wavelength phonons in another cubic crystal, Cu2 O with six atoms per primitive unit cell, can be found in Problem 3.1. The corresponding phonons in a non-cubic crystal structure, such as the wurtzite structure, can be found in Problem 3.7b. 2 Note, however, that if more than two atoms of the same kind are present within each primitive cell, infrared active modes and LO–TO splittings are possible. See the case of selenium and tellurium [3.8] 113 114 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions 3.2 Models for Calculating Phonon Dispersion Curves of Semiconductors To calculate the phonon dispersion curves from (3.9) it is necessary to know the force constants. In most calculations these force constants are obtained by first modeling the interactions between ions in terms of a number of parameters and then fitting some experimental quantities, such as sound velocity, zone-center phonon frequencies, bulk modulus, etc., by adjusting these parameters. Even after the force constants are known, numerical computations are necessary in solving (3.9) to obtain the phonon frequencies. Hence we can discuss only qualitatively the features of various models proposed for semiconductors. 3.2.1 Force Constant Models The Born–von Kármán model [Ref. 3.9, p. 55] represents the first attempt to calculate the phonon dispersion in semiconductors such as diamond and Si. The atoms are assumed to be hard spheres connected by springs. The spring constants º(kl, k l ) are determined by fitting experimental results. Born [3.10] tried to fit the experimental results for C and Si with only two spring constants: · and ‚ which determine the restoring force on each atom due to its own displacement and the displacements of its nearest neighbors. This simple model was applied by Hsieh [3.11] to calculate the phonon dispersion in Si. The calculated curve failed to fit the experimental dispersion curve at short wavelengths. The Si lattice turned out to be unstable under shear stress in this simple model. The flattening of the TA phonon dispersion near the zone edge cannot be explained without introducing long-range interatomic interactions. Herman [3.12] showed later that by extending interactions to the fifthnearest neighbors and by using as many as 15 force constants, a good fit to the phonon dispersion curves of Ge could be achieved. This model is not easy to understand from a physical point of view since some of the distantneighbor force constants were found to be larger than their nearer-neighbor ones. 3.2.2 Shell Model One can argue that a model in which the atoms are regarded as point masses connected by springs will be a poor approximation for semiconductors. After all, the valence electrons in covalent semiconductors such as Ge and Si are not rigidly attached to the ions. In a model proposed by Cochran [3.13] each atom is assumed to consist of a rigid ion core surrounded by a shell of valence electrons (shown schematically in Fig. 3.5) that can move relative to the cores. This is the basis of the shell model. 3.2 Models for Calculating Phonon Dispersion Curves of Semiconductors k2 k1 Core 1 Shell 1 Core 2 Shell 2 Fig. 3.5. Typical interactions between two deformable atoms in the shell model In the shell model the interactions between the two atoms inside the unit cell of Si are represented schematically by springs, as shown in Fig. 3.5. One important feature introduced by the shell model is that long-range Coulomb interaction between atoms can be included. This is achieved by assigning charges to the shells so that dipole moments are produced when the shells are displaced relative to the ions. By using the interaction between the induced dipoles to simulate the long-range interaction, the short-range interaction can be limited to the nearest neighbors. With the shell model Cochran [3.13] was able to fit the phonon dispersion in Ge with five adjustable parameters. Dolling and Cowley [3.14] were able to fit the phonon dispersion curves of Si using an 11-parameter shell model. In this model the short-range interactions have been extended to the next-nearest neighbors. Similar 11-parameter shell models have been successfully used to fit the phonon dispersion curves even in III–V compounds. With 14-parameters the agreement between theory and experiment is quite good. The main criticism of the shell model is that the valence electron distributions in the diamond- and zinc-blende-type semiconductors are quite different from spherical shells. As a result, the parameters determined from the shell model have no obvious physical meaning and have limited applications beyond fitting the phonon dispersion curves. Phillips [3.15] has pointed out that the most serious problems of the shell model appear when applying it to covalent solids. The shell model artificially divides the valence charges between the two atoms involved in the covalent bond. In reality the valence electrons are “time-shared” between the two atoms in that they all spend part of their time on each atom. 3.2.3 Bond Models It is well known that valence electrons in diamond- and zinc-blende-type semiconductors form highly directed bonds. These valence electrons are important for explaining cohesion in these semiconductors so they must also play an important role in determining the vibrational frequencies. The vibrational properties of molecules formed from covalent bonds have been extensively studied by chemists. These vibrational modes are usually analyzed in terms of valence force fields for stretching the bonds and for changing the angles between bonds (bond bending). The force constants can be determined in a straightforward manner from these valence force fields since the displacements of the ions are related to the bond coordinates. One advantage of this approach is 115 116 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions that the force constants for bond stretching and bond bending are often characteristics of the bonds and can be transferred from one molecule to another containing the same bonds. To see what kind of parameters are involved in this valence force field method (VFFM) of calculating lattice dynamics let us consider a crystal with two atoms, A and B, per unit cell. The potential energy of the valence bonds about the equilibrium positions can be expanded phenomenologically in terms of the valence bond coordinates as ⎡ 1 V ⎣ Û(‰rij )2 Ì(‰rik )2 k£ r02 (‰£ijk )2 2 i, j BAB i, k k£ r02 (‰£jkl )2 kr£ r0 (‰£ijk )(‰rij ) ABA BAB kr£ r0 (‰£jkl )(‰rjk ) ... . (3.10) ABA The first two terms in (3.10) correspond to bond stretching forces: j and k denote, respectively, the nearest and next-nearest neighbors of an atom i. The remaining terms give rise to bond bending forces. The bond motions for these terms are shown in Fig. 3.6. This method of calculating phonon dispersion works best when only a small number of valence force fields are sufficient to explain the phonon dispersion. In ionic crystals it is necessary to introduce additional long-range forces due to Coulomb interactions in order to reproduce the LO–TO phonon splittings near the zone center. Musgrave and Pople [3.16] first applied this method to study the lattice dynamics of diamond. They included only two kinds of valence force fields in the potential energy: bond stretching and bond bending about a common apex atom. The model requires five parameters, which translates into six force constants involving the nearest and next-nearest neighbors. The model does not reproduce well the elastic constants nor the zone-center optical phonon fre(i) B δΘ ijk B (k) A (j) B B A(l) δΘ ijl (j) (k) A kΘ r 02(δΘ ijk )2 A B krΘr0(δΘ ijk )(δr ij ) A k'Θ r 02(δΘ jkl )2 A δΘ jkl B k'rΘr0(δΘ jkl )(δr jk) Fig. 3.6. Bond-bending configurations for a crystal with two atoms, A and B, per unit cell 3.2 Models for Calculating Phonon Dispersion Curves of Semiconductors quencies. Subsequent work showed that better results could be achieved by introducing additional parameters involving the change of two bond angles with a common bond. In ionic crystals the number of adjustable parameters is increased to eight to include the Coulomb interactions. Thus the number of adjustable parameters in the VFFM necessary for a good fit to the experimental results is comparable to that of the shell model, and there is no major advantage of one method over the other. The phonon dispersion curve in a wurtzite-type semiconductor, CdS, has been calculated by Nusimovici and Birman [3.17] using the VFFM with eight adjustable parameters. Since the experimental phonon dispersion curves of CdS were not known at that time,3 these parameters were adjusted to fit the experimental zone center optical phonon energies. A simplified version of the VFFM has been introduced by Keating [3.22]. There are only two parameters, · and ‚, in this model for covalent semiconductors, with an additional charge parameter for ionic compounds. The Keating parameter · is equivalent to the bond-stretching term Û in (3.10) while ‚ is equivalent to the bond-bending term k£ . Because of its simplicity and the clear physical meaning of its parameters, the Keating model has been widely used to study the elastic and static properties of covalent semiconductors [3.23a, 24]. The phonon dispersion curves calculated from the Keating model show reasonably good agreement with experimental results except for the problematic TA branch. If the parameters · and ‚ are determined from the elastic constants, the zone-edge (X-point) TA phonon energies tend to be too high and cannot reproduce the flat dispersion in the experimental curves (see Fig. 3.1). 3.2.4 Bond Charge Models To understand the motivation for the bond charge model, let us return to the Hamiltonian for the ions given in (3.2). The force constants can be obtained, in principle, by differentiating the total energy Ee with respect to the ion coordinates (this is known as the frozen phonon approximation) [3.21]. However, this approach is very computation intensive and requires the use of supercomputers. On the other hand, with some insight and approximations, phonon dispersion curves of diamond- and zinc-blende-type semiconductors can be calculated without supercomputers. The most difficult part of this calculation is how to handle the Coulomb interaction between ions and electrons. This interaction causes the effective charge of an ion seen by other ions to be reduced, an effect known as screening. A simple way to introduce screening effects is to calculate the dielectric function Â (for a definition see Sect. 6.1) and then divide the ionic potential by Â. There are several approaches to approximating the screening of the ions by the valence electrons. One obvious simplification is to assume that the valence electrons are free so that the dielectric function of the semiconductor can be 3 Neutron scattering cannot be performed on compounds containing 113 Cd because of its very large thermal neutron absorption cross section. Phonon dispersion curves in isotopically enriched 114 CdS [3.18], 114 CdTe [3.19], and 116 CdSe [3.20] have however been reported. 117 118 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions replaced by that of a metal. Using this approach, Martin [3.23b] found that the Coulomb repulsion between the ions is very strongly screened: the silicon lattice becomes unstable against a long-wavelength shear distortion. The TA modes have imaginary energies as a result. One way to avoid this problem is to localize some of the valence electrons so that not all of them can contribute to the screening of the ions. To handle these localized valence electrons Martin used the idea of bond charges introduced by Phillips [3.15]. X-ray scattering measurements had already suggested that there was a pile-up of charges along bonds in Si and diamond crystals which could not be explained by a spherical charge distribution such as in a shell model. This pile-up of charge in the covalent bond is known as the bond charge and is well known in the formation of covalent molecules. Experimentally, Göttlicher and Wolfel [3.25] observed a diffraction peak in the X-ray spectra of diamond corresponding to the (2,2,2) reciprocal lattice vector. This diffraction peak is forbidden by Bragg’s diffraction law in a crystal with the diamond structure (see Problem 2.11). Those authors noted that this forbidden diffraction peak could be explained by assuming that approximately 0.4 of an electronic charge was located at the middle of each bond. More recently, the distribution of the bond charge in Si has been mapped out by Yang and Coppens [3.26] also using X-ray diffraction. Their experimental results are shown in Fig. 3.7a and are in excellent agreement with the theoretical charge distribution in Fig. 3.7b calculated by Chelikowsky and Cohen [3.27]. Martin [3.23b] introduced the bond charges into the lattice dynamics calculation of semiconductors in a very simple phenomenological manner. He assumed that bond charges of magnitude Zb e are located exactly midway between two adjacent atoms. As a first approximation he postulated that Zb e was given by 2e Zb e , (3.11) Â where 2e represents the two electrons involved in the covalent bond and the dielectric constant Â results from the screening of the bond charge by the re(a) Experiment (silicon) (b) Theory 24 20 24 16 12 16 12 12 8 8 4 4 Bond Bond Fig. 3.7. Valence charge distribution in Si showing the constant charge density contours (a) determined experimentally from X-ray diffraction [3.26] and (b) calculated with the empirical pseudopotential method [3.27]. The numbers in the figure are in units of electrons per unit cell volume 3.2 Models for Calculating Phonon Dispersion Curves of Semiconductors Fig. 3.8. Schematic diagram of the bond charge model proposed by Martin [3.23b] for Si. Zb represents the bond charge Zb 2 Zb 2 Zb 2 Zb 2 Si(1) Si(2) Zb Zb 2 Zb 2 maining valence electrons. For simplicity Â was assumed to be given by the dielectric constant for small wave vectors and at low frequencies (see Sect. 6.1 for further discussion of the wavevector and frequency dependence of Â). For diamond, at least, this approximation worked rather well. The dielectric constant of diamond is equal to 5.7, so Zb e is equal to 0.35e in reasonable agreement with the value of 0.4e needed to fit the phonon dispersion curves [3.25]. This simple model for the Si crystal is shown schematically in Fig. 3.8. Each Si ion has a charge of 4e. The four valence electrons from each Si atom are divided into localized bond charges and nearly free electrons. Each Si atom contributes four Zb /2 electron to the four bonds it forms with its four nearest neighbors. These bond charges are localized, and therefore do not contribute to screening of the Si ions. The remaining (4 2Zb ) valence electrons from each Si atom are assumed to be free and can screen the ions. The forces which determine the phonon frequencies are: • • • • Coulomb repulsion between the bond charges; Coulomb attraction between the bond charges and the ions; Coulomb repulsion between the ions; a non-Coulombic force between the ions to be approximated by a spring. Using this approach Martin was able to calculate the phonon dispersions and elastic constants of Si with no other adjustable parameters. A further refinement of the bond charge models of Phillips and Martin was the adiabatic bond charge model (ABCM) proposed by Weber [3.5]. This model combines the features found in the bond charge model, in the shell model and in the Keating model. The ABCM uses the bond charge model of Martin as its starting point. A conceptual improvement in the ABCM is to treat the bond charges not as rigidly located in the middle of the bonds, as Martin did, but instead to allow the bond charges to follow the motion of the ions adiabatically as in the shell model. As a result of their Coulomb attraction to the ions, the bond charges are unstable against any small perturbation which moves them closer to one ion than to another. To stabilize the bond charges, Weber introduced two additional types of forces: (1) short range re- 119 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions 2Z Fig. 3.9. Schematic diagram of the adiabatic bond charge model of Weber [3.5]. See text for explanations of the symbols 2Z β φ ′′i–bc –Z BC φ ′′i–i Ion pulsive forces between the bond charges and the ions and (2) bond-bending forces as in the Keating model. The various interactions between nearestneighbor ions and bond charges in the ABCM are shown schematically in Fig. 3.9. There are four adjustable parameters in the model: • • • • ˇii , the potential of central forces between ions; ˇibc , the potential of central forces between ions and bond charges; Z2 /Â, representing the Coulomb interaction between the bond charges; ‚, the bond-bending parameter in the Keating model. Some of these parameters can be determined from the elastic constants or long-wavelength phonon dispersion curves while others have to be deduced from the zone-edge phonon energies. The phonon dispersion curves of the group-IV elements calculated with the ABCM are in good agreement with experiment. As an example, Figs. 3.1, 3.10 and 3.11 show, respectively, comparisons between the experimental results and the calculated phonon dispersion curves in Si, ·-Sn (or gray tin), and diamond. The phonon dispersion curves of diamond pose a special problem for the ABCM since, unlike the other groupIV elements, the zone-edge TA phonon energies in diamond are quite high. ∆5 6 Frequency [THz] 120 X4 Σ2 ∆ 2' 4 Γ25' Σ1 ∆ X3 X X4 W2 W1 L 2' X1 Λ1 Σ3 Γ L1 Σ1 2 ∆5 L3' Λ1 Σ3 X1 ∆1 Λ3 W2 Σ4 Λ3 Σ Γ Λ L3 L L K W X3 X Fig. 3.10. Phonon dispersion curves of ·-Sn. The solid lines were calculated with the ABCM of Weber; the broken lines are calculated by a valence force field model while the solid circles are experimental points. (From [3.5]) 3.3 Electron–Phonon Interactions ∆ 2' 40 X1 Frequency [THz] ' L2 Σ2 ∆5 X4 30 Γ 25 Σ1 ∆1 W2 W1 X3 L1 Σ1 W2 X3 20 X1 L3' Σ3 Σ3 ' X4 Σ4 ∆5 L3 10 Γ ∆ X Σ Γ Λ L L K W X Fig. 3.11. Phonon dispersion curves of diamond. The solid lines were calculated with the ABCM of Weber while the circles represent experimental points. (From [3.5]) In addition, there are features in the optical phonon branches which cannot be reproduced by a four-parameter ABCM. To obtain a satisfactory fit to the experimental data in diamond, Weber introduced, in an ad hoc manner, an additional adjustable parameter in the bond-bending term. A comparison between the experimental phonon dispersion curves in diamond and the results calculated from this five-parameter ACBM is shown in Fig. 3.11. A minor but interesting feature which is not obvious in this figure is that the maximum energy of the optical phonon branch occurs along the [100] direction instead of at ° as in Si and Ge. A more recent comparison between experimental lattice dynamical results and a first-principles calculation can be found in [3.28]. 3.3 Electron–Phonon Interactions In Sect. 2.1 we pointed out that, within the Born–Oppenheimer approximation, we can decompose the Hamiltonian of a crystal into three terms: Hion (Rj ), He (ri , Rj0 ), and Heion (ri , ‰Rj ). The first two terms deal separately with the motions of the ions and the electrons. In Chap. 2 and in Sect. 3.2 we discussed how to solve those two Hamiltonians to obtain, respectively, the electronic band structure and the phonon dispersion curves. We will now consider the third term, which describes the interaction between the electron and the ionic motion, i.e., the electron–phonon interaction. Within the spirit of the Born–Oppenheimer approximation we will assume that the electrons can 121 122 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions respond instantaneously to the ionic motion so that the electron–phonon interaction Hamiltonian can be expressed as a Taylor series expansion of the electronic Hamiltonian He (ri , Rj ): He · ‰Rj . . . . Heion (ri , ‰Rj ) (3.12) Rj Rj0 j Usually the electronic Hamiltonian He (ri , Rj ) is not known, and therefore approximations are needed to calculate the electron–phonon interaction. For simplicity, we shall consider in detail mostly the long-wavelength phonons in diamond- and zinc-blende-type crystals with two atoms per unit cell. As discussed in Sect. 3.1 there are four kinds of long-wavelength (i.e., k near °) phonons: TA, LA, TO, and LO phonons. Their interactions with electrons will be treated separately. Interaction between electrons and large wave-vector phonons will be discussed at the end of this section. 3.3.1 Strain Tensor and Deformation Potentials Let us assume that the electronic energies of a non-degenerate band Enk (where n is the band index and k the wave vector) are known so that the expectation value of (He /Rj ) can be approximated by He Enk · ‰R ≈ · ‰Rj . (3.13) j Rj Rj 0 Rj Rj 0 The constant (Enk /Rj ) represents simply the shift of the electronic band energy caused by a static displacement of the atoms. In the case of the longwavelength acoustic phonons, the atomic displacements can correspond to a deformation of the crystal (deformation potential theorem). Such deformations will change the electronic energies at different points in the Brillouin zone; the parameters which describe these changes in the electronic energies induced by static distortions of the lattice are known as deformation potentials. Thus the coefficient Enk /Rj is related to the deformation potentials of the crystal. We shall now express the electron–phonon interactions in a semiconductor explicitly in terms of deformation potentials. Within the limit of zero wave vector or infinite wavelength, an acoustic phonon becomes a uniform translation of the crystal. Obviously such translations will not alter the electronic band structure, hence, if all ‰Rj ’s are identical, the change in Enk is zero. Thus we have to assume that an acoustic phonon has a nonzero but small wave vector in order to couple to electrons and consider the gradient of the atomic displacements: dij (‰Ri ) . Rj (3.14) dij is a second-rank tensor which can be decomposed into the sum of a symmetric tensor eij and an antisymmetric one fij : 3.3 Electron–Phonon Interactions eij 1 2 fij 1 2 and ‰Rj ‰Ri Rj Ri ‰Rj ‰Ri Rj Ri (3.15a) . (3.15b) The antisymmetric tensor fij describes a rotation of the crystal and does not change the electron energies. However, the symmetric tensor eij describes a strain induced in the crystal by the atomic displacements and is known as the strain tensor. Such strains in a crystal can shift the electronic energies. This suggests that we can derive the electron–phonon interactions for longwavelength acoustic phonons by expanding He (ri , Rj ) in terms of the strain tensor eij . As a symmetric second-rank tensor, eij contains six independent elements. One can interpret these elements as corresponding to different ways in which the crystal can be deformed. One question which arises is: how many linearly independent deformation potentials are needed to describe all the possible changes in the energy of a given electronic state induced by strain? This question can be answered in general by applying group theory. The answer depends on the space group of the crystal, and the wave vector and symmetry (in terms of the irreducible representations of the group of the wave vector) of the particular electronic state being considered. As an illustration of the principles involved, we will discuss the specific cases of electrons and acoustic phonons in diamond- and zinc-blende-type crystals. Since electron and phonon properties are invariant under symmetry operations of a crystal, we expect the electron–phonon interaction to remain unchanged also. Thus the first step is to symmetrize the strain tensor and the electronic state in terms of the irreducible representations of the crystal. The symmetrization of electron states has already been discussed in Chap. 2. To symmetrize the strain tensor, we note that a second-rank tensor can be constructed from the tensor product of two vectors. A vector has °4 symmetry in zinc-blende crystals, so a second-rank tensor can be decomposed into these irreducible representations (see also Problem 2.3): °4 ⊗ °4 °1 ⊕ °3 ⊕ °4 ⊕ °5 . (3.16) To decompose the symmetric tensor eij according to the irreducible representations in (3.16), we can either use projection operators, as described in any of the references on group theory given for Chap. 2, or use the method of inspection. From the form of the basis functions for the Td group given in Table 2.3 (see Sect. 2.3.3) we can guess that the three diagonal elements of a second-rank tensor transform as °1 ⊕ °3 while the six off-diagonal elements transform as °4 ⊕ °5 . If we form symmetric and antisymmetric combinations of the off-diagonal elements, the symmetric combination belongs to a representation which has a character equal to 1 under the symmetry operation involving 123 124 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions the reflection Û [under this reflection about the (110) plane xy → yx, xz → yz, and yz → xz], while the antisymmetric combination leads to the character of 1 under the same operation. From Table 2.3 we see that the off-diagonal elements of a symmetric tensor (like the strain tensor) should belong to the °4 representation while those of an antisymmetric tensor (like the one describing a rotation, a pseudovector) belong to the °5 representation. Thus the elements of the (symmetric) strain tensor can be combined into these irreducible representations: °1 : e11 e22 e33 ; °3 : e11 e22 , e33 (e11 e22 ) 2; and °4 : e12 , e23 , e31 . Given any strain tensor eij in matrix form we can always decompose it into the sum of three matrices: ⎡ ⎤ e e22 e33 0 0 1 ⎣ 11 ⎦, [eij (°1 )] 0 e11 e22 e33 0 3 0 0 e11 e22 e33 ⎡ ⎤ 2e (e22 e33 ) 0 0 1 ⎣ 11 ⎦, [eij (°3 )] 0 2e22 (e33 e11 ) 0 3 0 0 2e33 (e11 e22 ) ⎡ ⎤ 0 e12 e13 [eij (°4 )] ⎣ e12 0 e23 ⎦ . e13 e23 0 Note that the matrix with °1 symmetry has a nonzero trace while the other two matrices are traceless. Using the definition of the strain tensor components in (3.15a), it can be shown that the trace (e11 e22 e33 ) of the strain tensor is equal to the fractional volume change (‰V/V) or volume dilation associated with a strain pattern. On the other hand, a traceless strain matrix describes a shear of the medium. In a zinc-blende crystal, eij (°3 ) corresponds to the shear component of the strain produced by a uniaxial stress applied along a [100] direction of the crystal while eij (°4 ) corresponds to a [111] uniaxial stress. The proof of these results is left for Problem 3.2 at the end of this chapter. Let us consider a long wavelength acoustic vibration described by a plane wave with frequency ˆ and wave vector q: ‰R ‰R0 sin(q · r ˆt). (3.17) The strain tensor eij associated with this phonon, according to the definition in (3.15a), is given by eij 12 [qi ‰R0j qj ‰R0i ] cos(q · r ˆt). (3.18) In a longitudinal mode, the displacement ‰R is parallel to the direction of propagation q. Thus the nonzero strain tensor components for LA phonons are simply (in the limit of both q and ˆ approaching zero) 3.3 Electron–Phonon Interactions eii qi ‰R0i . (3.19) The strain tensor associated with a long-wavelength LA is therefore a diagonal tensor. An examination of the trace of this tensor shows that the LA phonon always produces an oscillatory dilation (‰V/V) with amplitude equal to q · ‰R0 plus a shear. This is consistent with our expectation that an acoustic wave causes periodic expansion and compression of a medium. A small uniform expansion of the crystal by ‰V will shift the energy of an electronic band extremum Enk by an amount ‰Enk ank (‰V/V), (3.20) where ank is known as the volume deformation potential of the energy level Enk . In principle, this deformation potential can be determined by measuring the shift in Enk induced by hydrostatic pressure. In practice, there are very few experimental techniques capable of measuring the volume deformation potential directly. Often optical measurements on samples under hydrostatic pressure are applied to determine the volume deformation potentials. In these optical experiments, usually only energy differences between two band extrema are measured. As a result, only relative volume deformation potentials between two band extrema are derived from such optical experiments while absolute ones are required in (3.20). For non-degenerate bands, we can neglect the effect of the shear strain associated with LA and write down the electron–LA phonon interaction Hamiltonian HeLA for small phonon wave vectors q as HeLA ank (q · ‰R), (3.21) where ‰R can be expressed in terms of phonon creation and annihilation operators c q and cq by using the standard result obtained from quantum mechanics [Ref. 3.29, p. 107] 1/2 ‰R eq c q exp[i(q · rj ˆt)] 2NVÚˆ (3.22) q cq exp[i(q · rj ˆt)] , where N is the number of unit cells in the crystal, V and Ú are, respectively, the volume of the primitive cell and the density, and eq is the phonon polarization unit vector. The Hamiltonian HeLA in (3.21) is valid for a nondegenerate band extremum such as the °1 conduction band minimum in GaAs and other zinc-blende semiconductors. The values of the volume deformation potentials a(°1c ) for the conduction band and the relative volume deformation potentials a(°1c ) a(°15v ) in these semiconductors are listed in Table 3.1. As pointed out earlier, only the relative volume deformation potentials a(°1c ) a(°15v ) between the conduction and valence bands are measured in an optical experiment under hydrostatic stress. In cases where the absolute deformation potentials for the conduction band are known [3.31] one finds that the °1 conduction band deformation potential is typically about ten times 125 126 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions Table 3.1. Deformation potentials for the conduction and valence band extrema in diamond and zinc-blende semiconductors (in eV). a denotes the volume deformation potential for the lowest energy °1c conduction band minimum or the highest energy °15v valence band maximum (zinc-blende notation). b and d are the shear deformation potentials for the °15v valence band maximum. •d and •u denote deformation potentials at zone boundaries. Most of the data are taken from [3.30] •u •d Si Ge GaP GaAs GaSb InP InAs InSb ZnS ZnSe ZnTe CdTe ≈5 12.3b a 6.5a a(°1c ) a 8.77 16.3b 13 14.5b 8.6 7 a(°1c) a(°15v ) b d 10 12 9.3 9 8.3 6.4 6.0 7.7 4.0 5.4 5.8 3.4 2.2 2.3 1.8 2.0 1.8 2.0 1.8 2.0 0.62 1.2 1.8 1.2 5.1 5.0 4.5 5.4 4.6 5.0 3.6 5.0 3.7 4.3 4.6 5.4 a [100] valleys; [111] valleys, D.N. Mirlin, V.F. Sapega, I.Ya. Karlik, R. Katilius: Hot luminescence investigation of L-valley spliting in GaAs. Solid State Commun. 61, 799–805 (1987) b larger than that of the °15 (or °25 ) valence bands. The relative volume deformation potentials of the conduction and valence bands at the zone center in diamondand zinc-blende-type semiconductors can be calculated quite easily within the tight-binding approximation. This is left as an exercise (Problem 3.9). However, the calculation of the absolute deformation potentials is not trivial [3.32]. One thing to notice about HeLA is the explicit and implicit dependence of its matrix element on q. From (3.22) the LA phonon displacement ‰R is pro1 portional to ˆ 2 . Since ˆ is linear with q for acoustic phonons (in the limit of long wavelength) and HeLA depends on q · ‰R in (3.21), HeLA varies explic1 itly with q as q 2 . On the other hand, in (3.22) ‰R is expressed in terms of the phonon creation and annihilation operators, whose matrix elements depend on the phonon occupation number. The probability that a phonon state with energy ˆ is excited at a temperature T is known as its occupation number. Phonons are bosons and their phonon occupation number Nph (ˆ) is given by the Bose–Einstein distribution function Nph (ˆ) {exp[ˆ/(kB T)] 1}1 , where kB is the Boltzmann constant. The magnitudes squared of the matrix elements of the phonon creation and annihilation operators are Nph (ˆ) 1 and Nph (ˆ), respectively. For kB T ˆ, Nph (ˆ) ≈ kB T/(ˆ) 1. As a result, the phonon occupation term in the matrix element (squared) of HeLA depends on q as q1 . Hence, the explicit and implicit dependences of the matrix element (squared) of HeLA on q cancel each other. These results will be used in Chap. 5 in calculating the mobility of electrons as a function of temperature. 3.3 Electron–Phonon Interactions 3.3.2 Electron–Acoustic-Phonon Interaction at Degenerate Bands In the previous section we concentrated on LA phonons because they always produce a change in the volume of the crystal which affects all energy bands. One can easily prove this based on the matrix-element theorem (see Sect. 2.3.4). A volume dilation does not change the symmetry of the crystal so the Hamiltonian in (3.21) must belong to the identity representation. When acting on an electronic band at the zone center (i. e., °), HeLA must contain a term belonging to the °1 representation. If the electron symmetry is °i , then °i ⊗ °1 °i and therefore the matrix element of °i | HeLA | °i is nonzero. Compared to their dilation component the shear components of LA phonons are usually less important. On the other hand transverse acoustic (TA) phonons contain only shear waves. To first order, a shear strain does not affect the energy of a nondegenerate band in a cubic crystal. Shear strains, however, lower the symmetry of a cubic crystal. As a result, the most important effect of a shear strain on a cubic crystal is to lift some of the degeneracy of energy bands at high symmetry points of the Brillouin zone. Again the matrix-element theorem can be applied to predict whether a particular shear strain of symmetry, say °s , will split the degeneracy of a state of symmetry °i . In this section we will consider the effect of strain and acoustic phonons on two important cases of degenerate bands in diamond- and zinc-blende-type semiconductors. These are the degenerate heavy and light hole bands and the degenerate conduction band minima in Si and Ge. a) Degenerate Heavy and Light Hole Bands at ° In the previous section we showed that any strain tensor in a zinc-blende crystal can be decomposed into three separate irreducible tensors transforming as °1 , °3 , and °4 . This result suggests that we require three deformation potentials to describe the effect of a general strain on a general band extremum at °. In the case of the degenerate °15 valence bands, it is convenient to regard these six (including spin) bands as transforming like the eigenstates of a J 3/2 and a J 1/2 angular momentum operator (see Sect. 2.6.2). The hole–strain interaction Hamiltonian can be derived by symmetrizing the angular momentum operator J through multiplication by the appropriate components of the strain tensor (method of invariants). The procedure for doing this can be derived from group theory and has been described in detail by Kane [3.33] and by Pikus and Bir [3.34, 35]. The Pikus and Bir effective strain Hamiltonian for the J 3/2 valence bands in the zinc-blende semiconductors is given by (see also the discussion in Problem 3.8) HPB a(exx eyy ezz ) b (J 2 x J 2 /3)exx c.p. 2d 1 √ (Jx Jy Jy Jx )exy c.p. , 3 2 (3.23) where a, b, and d are the three deformation potentials corresponding to strain tensors with symmetries °1 , °3 , and °4 , respectively, and c.p. stands for 127 128 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions cyclic permutation. It is no coincidence that HPB is very similar to the Kohn– Luttinger Hamiltonian in (2.70). After all, both of them have been deduced based on the symmetry of the zinc-blende crystal, and the strain tensor eij has the same symmetry as ki kj or ∇i ∇j . The deformation potentials b and d determine the splitting of the four-fold degenerate J 3/2 valence bands at ° under [100] and [111] uniaxial stress, respectively. Although (3.23) has been derived for a static uniform strain, it is reasonable to assume that this Hamiltonian and the deformation potentials are valid also for long-wavelength acoustic phonons. By applying static uniaxial stress to the diamond- and zinc-blende-type semiconductors listed in Table 3.1, their shear deformation potentials can be determined. In particular, it can be shown (see Problem 3.8) that the splittings ‰E of the J 3/2 valence bands under a uniaxial compressive stress of magnitude X along the [100] or [111] directions are given by ‰E 2b(S11 S12 )X, [100] stress, √ (1/ 3)dS44 X, [111] stress, (3.24a) (3.24b) where S11 , S12 and S44 are components of the fourth-rank compliance tensor Sijkl , which relates the strain tensor eij to the stress tensor Xkl . The definitions of the stress tensor and of the compliance tensor can be found in Problem 3.2. The shear deformation potentials (in the absence of spin–orbit interaction) can be calculated within the tight-binding approximation as shown in Problems 3.10–13. b) Degenerate Conduction Band Minima along ¢ in Si and at L in Ge The second example of the interaction between phonons and degenerate electron bands is that of the degenerate conduction band minima in Si and Ge. In general, we expect that a shear strain will deform a crystal and lift some of the degeneracies in the conduction band as in the case of the degenerate valence bands discussed in the previous section. For example, Fig. 2.10 shows that the lowest conduction band minimum in Si occurs at a point [kx0 , 0, 0] along the [100] direction of the Brillouin zone. The symmetry of that band in the group of the wave vector k along the [100] direction is ¢1 . While this state is nondegenerate for a given k, there are five other k vectors (in the [100], [010], [010], [001] and [001] directions) which are equivalent to the [100] wave vector by symmetry, so that the ¢1 conduction band minimum is six-fold degenerate as a result of degeneracy in reciprocal space. A uniaxial stress applied along the [100] direction will make the [100] and [100] directions different from the remaining four equivalent directions. Thus, from symmetry arguments one expects that a [100]-oriented uniaxial stress will split the six equivalent conduction band minima in Si into a doublet and a quadruplet. On the other hand a uniaxial stress applied along the [111] direction will affect all six minima in the same way and leave the degeneracy unchanged. To derive the strain Hamiltonian we have to consider the symmetries of the strain tensor, and the wave function of the band and of the equivalent 3.3 Electron–Phonon Interactions wave vectors k. For example, in the case of Si, the wave function of the conduction band has symmetry ¢1 while the six equivalent k vectors form a sixfold reducible representation. If the wave function of the band for each given k is nondegenerate, the form of the strain Hamiltonian is much simpler. Since this is the case for the conduction band minima in both Si and Ge, this is the only case we will consider here. Treatment of the more difficult case of degenerate bands can be found in, for example, the article by Kane [3.33]. The strain Hamiltonian for the nondegenerate band was first derived by Herring and Vogt [3.37] by generalizing the definition of the volume deformation potential in (3.20) into 6 ‰Enk •j ej , (3.25) j1 where the •j are the deformation potentials and the ej are the components of the strain tensor. To simplify the notation this second-rank strain tensor has been contracted into a six-component array (see Problem 3.3 for a discussion of this contracted notation). In a general crystal without considering symmetry, six deformation potentials are required to describe the strain-induced energy shift of a nondegenerate electronic state at a point k. This number is greatly reduced by symmetry considerations. For example, the strain tensor of a diamond crystal can be decomposed into three tensors belonging to the irreducible representations °1 (°1 ), °12 (°3 ) and °25 (°5 ) (Tables 2.5 and 2.7; note that because of the inversion symmetry of the diamond lattice, all its secondrank tensors must be even under the inversion operation). As a result, we need no more than three deformation potentials to describe the strain-induced energy shift of a given nondegenerate electronic state in the diamond crystal. The number is further reduced to two for k pointing along high symmetry directions such as [100] and [111]. As pointed out in Sect. 3.3.1 and in Problem 3.4, the traceless strain tensors with °3 and °4 symmetries in the zinc-blende crystal correspond to the shear components of the strains produced by uniaxial stress applied along the [100] and [111] directions, respectively. Since all the equivalent [100] valleys in Si appear symmetrical with respect to a [111] uniaxial stress, their degeneracy cannot be split by such a stress. On the other hand, a [100] stress will split the [100] valley from the [010] and [001] valleys. As a result, only two deformation potentials are required to describe the strain effect on the [100] conduction valleys in Si. Herring and Vogt [3.37] have expressed this result as a strain Hamiltonian of the form HHV •d (Tr{e}) •u (k̂ · e · k̂), (3.26) where Tr{e} is the trace of the strain tensor e, and k̂ is a unit vector along the direction of one of the equivalent [100] conduction band minima in reciprocal space. In (3.26) •u is a shear deformation potential associated with a uniaxial strain along the [100] direction and •d •u is the volume deformation potential (the reader is urged to verify this). Sometimes the deformation potentials •d and •u are also denoted by E1 and E2 following the notation introduced by Brooks [3.38]. 129 130 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions It is straightforward to show that the above arguments for Si can also be applied to derive a strain Hamiltonian for the L6 conduction band minima in Ge which occur along the four equivalent [111], [111], [111], and [111] directions. In this case a [001] uniaxial stress will not split the equivalent [111] valleys just as a [111] uniaxial strain will not split the [100] valleys. Instead a [111] stress will split the [111] valley (which will form a singlet) from the other three valleys, which remain degenerate (triplet). The result can be expressed in terms of a strain Hamiltonian similar to HHV in (3.26). However, the shear deformation potential •u is now the shear deformation potential for a [111] uniaxial strain rather than a [100] strain (readers should check this also) and k̂ is a unit vector along one of the equivalent [111] directions. Table 3.2 summarizes the relationship between the deformation potentials •j and the deformation potentials •d and •u in cubic semiconductors for k along high-symmetry directions. For equivalent valleys along the [110] directions, we note that three deformation potentials (•d , •u , and •p ) are required. The proof of this result, which does not follow from (3.26), is left as an exercise in Problem 3.14. The values of the deformation potentials for the conduction band valleys in Si and Ge are given in Table 3.1. The electron–acousticphonon interaction Hamiltonians for Si and Ge are obtained by substituting (3.18), the strain tensor associated with an acoustic phonon, into (3.26). Table 3.2. Relation between the deformation potentials •j and the deformation potentials •d , •u and •p in cubic semiconductors at high symmetry points [3.37] Direction of k : •1 •2 •3 •4 •5 •6 100 111 110 •d •u •d •d 0 0 0 •d (1/3)•u •d (1/3)•u •d (1/3)•u (1/3)•u (1/3)•u (1/3)•u •d •u (1/2)•p •d •u (1/2)•p •d • u • p 0 0 (1/2)•p 3.3.3 Piezoelectric Electron–Acoustic-Phonon Interaction In noncentrosymmetric crystals, a stress can induce a macroscopic electric polarization field E. This phenomenon is known as the piezoelectric effect [Ref. 3.39, p. 110]. This phenomenon can also be described as a strain inducing an electric field. The induced field will be proportional to the strain provided it is small. Since the strain tensor e has rank two and the induced electric field is a vector (or tensor of rank one) this constant of proportionality can be expressed as a third-rank electromechanical tensor em . In a medium with dielectric constant Â∞ the strain-induced field can be expressed as 1 (em · e) . (3.27) E (4) Â∞ 4Â0 3.3 Electron–Phonon Interactions This result for a static strain can be extended to the case of an oscillating strain field associated with long-wavelength acoustic phonons. If q and ‰R [defined in (3.17)] are, respectively, the wave vector and atomic displacements associated with the acoustic phonon, the strain tensor corresponding to the acoustic phonon is iq‰R from (3.15a). Substituting this result into (3.27) we obtain the sinusoidal macroscopic piezoelectric field induced by an acoustic phonon: q‰R . (3.28) 4Â0 Â∞ The longitudinal component of this electric field can be expressed in terms of a scalar piezoelectric potential ˇpe Epe (4)iem · ˇpe q · Epe /(iq2 ). (3.29) In the presence of this potential, the energy of an electron will be changed by | e | ˇpe , therefore the piezoelectric electron–phonon Hamiltonian can be written as |e| q · em · (q‰R). (3.30) Hpe | e | ˇpe (4) 4Â0 q2 Â∞ The form of the electromechanical tensors in crystals with the zinc-blende and wurtzite structure can be determined by symmetry (see Problem 3.15). Using (3.30), explicit expressions for Hpe can be deduced for any acoustic phonons. As an example, the calculation of Hpe for acoustic phonons in wurtzite crystals is left as an exercise (see Problem 3.16 and paper by Mahan and Hopfield [3.40]). If we compare the deformation-potential electron– acoustic-phonon interaction in (3.21) with the piezoelectric electron–acousticphonon interaction in (3.30), we notice that (3.30) contains an additional (1/q) dependence. This extra term arises from the Coulomb interaction in the piezoelectric electron–acoustic-phonon interaction. As a result, Hpe becomes stronger for small q or long-wavelength acoustic phonons. This is why Hpe is said to be a long-range interaction while the deformation potential interaction is a short-range interaction: the Fourier transform of a function of long range in q is of short range in r and vice versa. The values of electromechanical tensor components in tetrahedrally coordinated semiconductors can be estimated within empirical models such as the tight-binding model. We will not discuss these calculations here and interested readers should consult [3.41, 42]. Instead, we will list the values of electromechanical tensor components for some typical semiconductors in Table 3.3. Note that the more-ionic wurtzite semiconductors such as ZnO, CdS, and CdSe have electromechanical tensor components that are larger and also different in sign from those of the zinc-blende semiconductors. 3.3.4 Electron–Optical-Phonon Deformation Potential Interactions In crystals with two or more atoms per unit cell, a long-wavelength optical phonon involves relative displacements of atoms within the primitive unit cell. 131 132 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions Table 3.3. Values of the nonzero and linearly independent components of the electromechanical tensor in some zinc-blende and wurtzite-type (labeled as W) semiconductors [4.43, 44]. Note that the electromechanical tensor is defined in terms of the polarization. The cgs unit for polarization is statcoulomb/cm2 . The corresponding SI unit is Coulomb/m2 . The unit of the electromechanical tensor components in this table is 104 statcoulomb/cm2 . One statcoulomb/cm2 is equal to 1/(3 × 105 ) Coulomb/m2 Semiconductor AlAs AlSb GaP GaAs GaSb InP InAs InSb ZnS ZnSe ZnTe CdTe ZnO(W) CdS(W) CdSe(W) (em ) 14 (em ) 33 (em ) 31 (em ) 15 33 14.7 10.4 4.8 7.5 4.8 9.3 6.3 4.14 6.7 2.04 3.0 4.8 3.78 1.2 1.38 2.13 5.1 1.35 0.81 1.02 Unlike acoustic phonons, a long-wavelength optical phonon does not involve a macroscopic strain of the crystal, since there is no macroscopic distortion of the lattice. Instead, optical phonons can be regarded as “microscopic distortions” within the primitive unit cell. Optical phonons can change the energy of an electronic band in two ways, similar to the acoustic phonons. In nonpolar crystals optical phonons alter the electronic energies by changing the bond lengths and/or the bond angles. This electron–optical-phonon interaction is the analog of the deformation potential interaction of acoustic phonons and is known accordingly as the deformation-potential electron–optical-phonon interaction. In polar crystals a long-wavelength longitudinal optical (LO) phonon involves uniform displacements of the charged atoms within the primitive cell. Such relative displacement of oppositely charged atoms generates a macroscopic electric field. This electric field can then interact with electrons in a way similar to the piezoelectric electric field of acoustic phonons. This electron–longitudinal-optical-phonon interaction is known as the Fröhlich interaction. In this section we will first consider the deformation-potential interaction. Let us define the distance between the two atoms inside the primitive unit cell of a diamond- or zinc-blende-type semiconductor as a0 and the relative displacement between these two atoms associated with a zone-center optical phonon as u. As in the case of the acoustic phonons, we will define a phenomenological optical phonon deformation potential to describe the electron–optical-phonon interaction: HeOP Dn, k (u/a0 ), (3.31) where Dn, k is now the optical phonon deformation potential for the energy band indexed by n and k. Since this deformation potential interaction does 3.3 Electron–Phonon Interactions not depend on the phonon wave vector it is also a short-range interaction. In zinc-blende-type (or diamond-type) semiconductors the optical phonon displacement u has symmetry °4 (°25 for diamond structure), so the matrix element of (3.31) between two nondegenerate s-like °1 (or °2 ) conduction band states is zero. Thus there is no deformation-potential interaction between the lowest conduction band electrons and optical phonons in direct bandgap semiconductors such as GaAs and InP. The case of indirect bandgap semiconductors like Si or Ge is more complicated and will be discussed below together with the interaction between optical phonons and the p-like valence bands in diamond- and zinc-blende-type semiconductors. In some crystals, macroscopic strains are symmetry compatible with displacements of atoms involved in zone-center optical phonons. In such crystals an optical phonon may be described in terms of an internal strain [3.45, 46]. For example, the optical phonons in diamond- and zinc-blende-type semiconductors can be represented by a relative displacement of the two atoms within the primitive cell along the [111] body diagonal. (Although a macroscopic [111] shear strain will also produce such relative displacement of the atoms within the primitive cell, this displacement is not uniquely defined by the strain tensor, see Problem 3.11.) In such cases the quantity 2u/a0 is known as the internal strain (see Problem 3.13) and it is possible to deduce the electron– optical phonon interaction by considering the effect of a [111] uniaxial stress. For example, if the spin–orbit couplings in the valence bands of diamond- and zinc-blende-type semiconductors are neglected, the optical phonon deformation potentials for the p-like valence band (usually denoted by d0 ) can be related to that of the splitting of the valence bands under a [111] uniaxial stress. The calculation of d0 within the tight-binding approximation is left as an exercise (Problem 3.12), see [3.30] for more details. For a more general discussion of the calculation of the optical-phonon deformation potentials in tetrahedrally bonded semiconductors, readers are referred to [3.47]. There are relatively few experimental techniques capable of determining the optical-phonon deformation potentials in semiconductors. The value of d0 in Ge and GaAs has been measured to be 36 and 41 eV, respectively, by Raman scattering [3.48]. Other methods available for estimating d0 are based on the temperature dependence of the hole mobilities in p-type samples and of the linewidth of the direct optical transition from the split-off valence band to the conduction band. These measurements involve phenomena to be discussed in Chaps. 5–7. Typically one finds that d0 is of the order of 40 eV in most tetrahedrally coordinated semiconductors (see experimental values compiled in [3.47]). 3.3.5 Fröhlich Interaction In a polar or partly ionic crystal with two atoms per unit cell, the longwavelength longitudinal optical (LO) phonon can induce an oscillating macroscopic polarization, leading to an electric field ELO , see, e.g. [Ref. 3.9, p. 86]) ELO FuLO , (3.32) 133 134 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions where 1 1/2 F 4NÌˆ2LO (Â1 (4Â0 )1/2 . ∞ Â0 ) (3.33) In (3.32, 33) the phonon amplitude uLO is defined as the displacement of the positive ion relative to the negative ion, N is the number of unit cells per unit volume of the crystal, Ì is the reduced mass of the primitive cell defined by Ì1 M11 M21 , (3.34) M1 and M2 are the masses of the two atoms inside the primitive cell, ˆLO is the LO phonon frequency, and Â∞ and Â0 are, respectively, the high- and low-frequency dielectric constants. We will delay the derivation of (3.33) until Chap. 6, when we study the effect of long-wavelength transverse optical (TO) phonons on the infrared optical properties of semiconductors. This effect is due to the fact that the TO phonons associated with the LO phonons in polar crystals produce transverse electric dipole moments which couple to photons. The longitudinal field in (3.32) can be expressed in terms of a scalar potential ˇLO in the same way as for the piezoelectric acoustic phonons in (3.29): ˇLO (F/iq)uLO . (3.35) The interaction between an electron of charge | e | and this macroscopic Coulomb potential is known as the Fröhlich interaction. The Hamiltonian for this interaction is given by the simple expression HFr (e)ˇLO (ieF/q)uLO . (3.36) When combined with an expression for the displacement uLO analogous to (3.22), uLO (/2NÌˆLO )1/2 c (3.37) q exp[i(q · r ˆLO t)] c.c. , the Fröhlich Hamiltonian can be written as HFr (iCF /q) c q exp[i(q · r ˆLO t)] c.c. (3.38) q where the coefficient CF is given by 1/2 2ˆLO 1 –1/2 1 CF e (Â∞ Â0 ) (4Â0) . NV (3.39) Notice the change in the sign of the complex conjugate terms inside the two brackets in (3.37) and (3.38). This is necessary to ensure that the Fröhlich Hamiltonian is Hermitian. While the deformation potentials for optical phonons and acoustic phonons are difficult to calculate, the Fröhlich interaction can be calculated in terms of macroscopic parameters such as Â∞ and Â0 . Note that the Fröhlich interaction depends on the phonon wave vector as q1 . Hence it diverges, in principle, as q decreases to zero. This is not possible in intraband electron– LO-phonon scattering because the LO phonon frequency is nonzero even at q 0. Energy and momentum conservation prevents electrons from undergo- 3.3 Electron–Phonon Interactions Table 3.4. Summary of electron–phonon interactions in Si and GaAs. DP and PZ stand for deformation potential and piezoelectric interactions, respectively. Symbols in parentheses represent the commonly used notations for these interactions Phonon TA LA TO LO Si GaAs Conduction Valence Conduction Valence DP (•u ) DP (•d , •u ) DP (b, d) DP (av , b, d) PZ DP (ac ), PZ DP (b, d), PZ DP (av , b, d), PZ DP (d0 ) DP (d0 ) Fröhlich DP (d0 ) DP (d0 ), Fröhlich ing intraband scattering via q ≡ 0 optical phonons. Nevertheless, depending on the electron band dispersion, q can be quite small, and this scattering mechanism can dominate at temperatures where a significant number of LO phonons are excited (i. e., kB T ≥ ˆLO ). From the above discussion we see that there are many different ways for electrons to interact with long-wavelength phonons. Table 3.4 summarizes these different kinds of interactions in a representative polar (GaAs) and nonpolar (Si) semiconductor for electrons at either the lowest conduction band or the top valence bands. Note that while a TA phonon involves only shear strain and no volume dilation, an LA phonon can produce both. 3.3.6 Interaction Between Electrons and Large-Wavevector Phonons: Intervalley Electron–Phonon Interaction So far we have considered the interaction between electrons and zone-center phonons. Interactions between electrons and zone-edge or near zone-edge phonons has been found to play an important role in optical absorption at indirect energy gaps and in phenomena involving hot electrons (Chap. 5). For example, a zone-edge phonon can scatter an electron from a band minimum at the zone center to a band minimum at the zone edge. This kind of electron– phonon scattering is known as intervalley scattering. In Chap. 5 we will show that intervalley scattering is responsible for the Gunn effect [5.33]. For indirect bandgap semiconductors, such as Si, where the conduction band minimum occurs at a point either inside the Brillouin zone or at the zone edge, there are several equivalent conduction band valleys. In these cases electrons can be scattered from one valley to another via a large wave-vector phonon. There are several qualitative differences between the interaction of electrons with zone-center phonons and with zone-edge phonons. Zone-edge phonons cannot generate long-range electric fields [remember the q1 dependence in (3.35)] so they have no analog of the Fröhlich or piezoelectric interaction. Intervalley electron–phonon interactions are always short-range and usually approximately independent of phonon wave vector. Whereas the en- 135 136 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions ergy difference between zone-center acoustic and optical phonon modes can be quite large, this difference may be insignificant for zone-edge phonons. We can express the intervalley electron-phonon Hamiltonian as He u, (3.40) R where e, u, q, and b respresent, respectively, the phonon polarization vector, amplitude, wave vector, and branch number. In practice, this Hamiltonian is often expressed in terms of its matrix element between two electronic states: Hiv ebq · Dij u ni , ki | Hiv | nj , kj , (3.41) with Dij known as the intervalley deformation potential. i and j denote, respectively, the initial and final valleys in the scattering, n and k are the electron band index and wave vector, respectively. The electron wave vectors ki and kj are related to q by wave vector conservation: kj ki q. Notice that in (3.41) the intervalley deformation potential has the dimension of energy per unit length instead of energy. Table 3.5 lists intervalley deformation potentials (in units of eV/Å) of some zinc-blende semiconductors calculated by Zollner et al. [3.49]. Often more than one zone-edge phonon can participate in intervalley scattering. Possible selection rules can be deduced from group theory. For example, in scattering an electron from the °1c valley to the L1c valley in GaAs, the LA and LO phonons at the L point of the Brillouin zone are allowed because they both have L1 symmetry. On the other hand, the transverse phonons at the L point have L3 symmetry and are not allowed. Intervalley scattering plays an important role in determining the mobility of electrons in indirect bandgap semiconductors such as Si, in the relaxation of hot electrons in a direct bandgap semiconductor like GaAs, and in the optical absorption at indirect bandgaps. However, most of these phenomena involve scattering of electrons by several different phonon modes so it is difficult to deduce the values of the symmetry-allowed intervalley deformation potentials for the individual zone-edge phonons. The determination of intervalley deformation potentials from experiments will be made clear in Chap. 5 and 6, where these phenomena are discussed. Table 3.5. Calculated intervalley deformation potentials for the conduction bands in a few ° . (From [3.49]) representative zinc-blende semiconductors (in eV/A) °–X 1 °–X 3 °–L Semiconductor LA LO LA LO LA LO GaP GaAs GaSb InP InAs InSb 1.5 0 0 2.3 3.2 0 0 4.1 4.5 0 0 4.9 0 4.7 2.5 0 0 3.3 1.2 0 0 3.7 2.8 0 1.2 4.1 2.8 1.6 2.5 4.3 1.0 0.6 2.7 3.0 1.4 1.1 Problems PROBLEMS 3.1 Symmetry of Zone-Center Phonons in Cu2 O Figure 3.12 shows the crystal structure of cuprite (Cu2 O), which was one of the earliest minerals known to be a semiconductor. There are two molecules, i. e., six atoms, in the unit cell. The space group is O4h . This is a nonsymmorphic group which is homomorphic to the point group Oh . The crystal has inversion symmetry with respect to the copper atoms. When considering the point group symmetry it is more convenient to take an oxygen atom as the origin. The point group symmetry is clearly tetrahedral in this case. With the oxygen atom as the origin, the inversion operation has to be followed by a translation of the crystal by (a/2) [1, 1, 1], where a is the size of the unit cube. Thus the factor group of Cu2 O is isomorphic to the factor group of Si except for the fact that the inversion operation in Si has to be followed by (a/4) [1, 1, 1]. There are ten classes in the group. Five of them do not involve the inversion operation while the other five do. Since there are six atoms per primitive unit cell we expect fifteen optical phonon branches and three acoustic branches. a) The permutation of the six atoms in the primitive unit cell of Cu2 O by its symmetry operations defines a representation G. Determine the characters of G. This can be done by counting the number of atoms which are left unchanged by the symmetry operations of the group since each unchanged atom will contribute one to the trace of the transformation matrix. b) Using the character table for the irreducible representations of the group of ° in the diamond structure (Table 2.16) show that G can be decomposed into the direct sum of these irreducible representations: G 2°1 ⊕ °1 ⊕ °5 . c) Show, by combining G with the °4 representation (that of a vector), that the 18 zone-center phonon modes in Cu2 O have the symmetries °1 ⊕ °3 ⊕ 3°4 ⊕ °5 ⊕ °5 . Of the three sets of triply degenerate °4 phonons, one set corresponds to the acoustic phonons while the other two are the infrared-active optical modes. The °5 mode is Raman-active (see Chap. 7 for a discussion of Raman scattering). Optical phonons which are neither infrared-active nor O–2 Cu+ Fig. 3.12. Crystal structure of Cu2 O (cuprite). (From [3.50]) 137 138 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions Raman-active are said to be silent. The °1 and °3 modes in Cu2 O are examples of silent modes. 3.2 Stress Tensor In (3.15a) the strain tensor eij was defined. Strain can be induced in a solid by the application of stress. Stress can be defined as the force per unit area applied to a face of an elementary cube within a solid. Since both the direction of the force and orientation of the face to which the force is applied are important, it takes nine components to specify the stress completely: F(X)x , F(Y)x , F(Z)x , . . . , F(Z)z . Here F(X)y denotes a force F per unit area applied along the x axis to a face whose normal is along the y axis. It is understood that these forces are applied in pairs so that a force F(X)y will be balanced by another force F(X)y , producing no acceleration of a solid in equilibrium. In addition, the off-diagonal components are equal: F(X)y F(Y)x , F(X)z F(Z)x , and F(Y)z F(Z)y , so that there is also no net torque. As a result of these restrictions the stress components form a symmetric secondrank tensor X, known as the stress tensor, defined by Xyz F(Y)z and so on. a) Show that a hydrostatic pressure P is specified by the diagonal stress tensor ⎛ ⎞ P 0 0 X⎝ 0 P 0 ⎠. 0 0 P Note that our sign convention for stress is that tensile stresses are positive while compressive stresses are negative. b) Show that a tensile uniaxial stress X applied along the [100] direction is represented by the tensor ⎛ ⎞ X 0 0 X ⎝ 0 0 0⎠. 0 0 0 c) Show that a tensile uniaxial stress X applied along the [111] direction is represented by the tensor ⎛ ⎞ 1 1 1 X (X/3) ⎝ 1 1 1 ⎠ . 1 1 1 3.3 Elastic Compliance Tensor in Diamond- and Zinc-Blende-Type Crystals In linear elasticity theory the strain induced in a medium is proportional to the applied stress. The constants of proportionality can be expressed as a fourthrank tensor known as the compliance tensor (Sijkl ), which is defined by eij Sijkl Xkl . Problems Using the symmetry operations of a zinc-blende crystal, show that the nonzero and linearly independent components of the compliance tensor of a zincblende crystal are Sxxxx Syyyy Szzzz , Sxxyy Sxxzz Syyzz Syyxx Szzxx Szzyy , Sxyxy Syxyx Sxzxz Szxzx Syzyz Szyzy . Since both the strain and stress tensors are symmetric tensors, each can be described by six matrix elements rather than nine. One often finds in the literature a contracted notation in which the strain and stress tensors are represented by a six-component array [Ref. 3.39, p. 134]. For example the strain tensor is written as e (e1 , e2 , e3 , e4 , e5 , e6 ). The numbering of 1 to 6 in this six-dimensional array is related to the 3×3 matrix by the convention ⎛ ⎞ e1 e6 /2 e5 /2 e ⎝ e6 /2 e2 e4 /2 ⎠ . e5 /2 e4 /2 e3 One advantage of this contracted notation is that fourth-rank tensors, such as the compliance tensor, can be expressed as a 6×6 matrix. For example, Sijkl in a zinc-blende-type crystal has the compact form ⎛ ⎞ S11 S12 S12 0 0 0 0 0 ⎟ ⎜ S12 S11 S12 0 ⎜ ⎟ 0 0 ⎟ ⎜ S12 S12 S11 0 ⎜ ⎟. 0 0 S44 0 0 ⎟ ⎜ 0 ⎝ 0 0 0 0 S44 0 ⎠ 0 0 0 0 0 S44 with Smn 2Sijkl when either m or n 4, 5 or 6. Smn 4Sijkl when both m and n 4, 5 or 6. 3.4 Strain Tensors for Hydrostatic and Uniaxial Stresses a) A hydrostatic pressure P is applied to a zinc-blende crystal of volume V. Show that the fractional change in volume is given by ‰V 3P(S11 2S12 ). V The negative sign implies that the volume decreases for P 0. The bulk modulus of a medium is defined as B dP/d(lnV), so for a zinc-blende crystal B [3(S11 2S12 )]1 . 139 140 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions b) A tensile uniaxial stress X is applied along the [100] axis of a zinc-blendetype crystal. Show that the resultant strain tensor is equal to ⎛ ⎞ S11 X 0 0 ⎝ 0 S12 X 0 ⎠ 0 0 S12 X and that this matrix can be expressed as the sum of a diagonal matrix and a traceless shear strain tensor ⎛ ⎞ ⎛ ⎞ 1 0 0 2 0 0 [(S11 2S12 )X/3] ⎝ 0 1 0 ⎠ [(S11 S12 )X/3] ⎝ 0 1 0 ⎠ . 0 0 1 0 0 1 Notice that the fractional change in volume of the crystal is equal to (S11 2S12 )X under this uniaxial stress. c) Show that the strain tensor corresponding to a tensile uniaxial stress applied along the [111] direction of a zinc-blende-type crystal is given by ⎛ ⎞ S 2S12 S44 /2 S44 /2 X ⎝ 11 S44 /2 S11 2S12 S44 /2 ⎠ 3 S44 /2 S44 /2 S11 2S12 Decompose this tensor into the sum of a multiple of a unit tensor and a traceless tensor as in part (b). Show that the fractional volume change is also equal to (S11 2S12 )X under a [111] stress. d) Determine the strain tensor for a uniaxial stress applied along the [110] direction of a zinc-blende-type crystal. 3.5 Elastic Stiffness Tensor In Problem 3.3 the second-rank strain tensor was expressed in terms of the stress tensor via a fourth-rank compliance tensor. Inversely, the stress tensor can be expressed in terms of the strain tensor by another fourth-rank tensor Cijkl known as the stiffness tensor: Cijkl ekl . Xij k, l Show that in zinc-blende-type crystals the stiffness tensor, when written in the compact form introduced in Problem 3.3, is given by [Ref. 3.39, p. 140] ⎛ ⎞ C11 C12 C12 0 0 0 0 0 0 ⎟ ⎜ C12 C11 C12 ⎜ ⎟ 0 0 0 ⎟ ⎜ C12 C12 C11 ⎜ ⎟, 0 0 C44 0 0 ⎟ ⎜ 0 ⎝ 0 0 0 0 C44 0 ⎠ 0 0 0 0 0 C44 where C44 (1/S44 ), C11 C12 (S11 S12 )1 , and C11 2C12 (S11 2S12 )1 . Table 3.6 lists the stiffness constants of some semiconductors. Problems Table 3.6a. Stiffness constants C11 , C12 , and C44 in some diamond- and zinc-blende-type semiconductor (in 1012 dyne/cm2 ). [Note that stiffness constants and pressure have the same units: dyne/cm2 (cgs units) or pascal (abbreviated as Pa in SI units). 10 dyne/cm2 is equal to 1011 Pa or 100 GPa (Gigapascal)]. Reproduced from Madelung et al. [3.43]. The values in italics are theoretical values. See A.F. Wright, Elastic Properties of zincblende and wurtzite AlN, GaN, and InN. J. Appl. Phys. 82, 2833 (1997) Semiconductor C11 C12 C44 C Si Ge AlN GaN GaP GaAs GaSb InN InP InAs InSb ZnS ZnSe ZnTe CdTe 10.76 1.66 1.285 3.04 2.93 1.412 1.181 0.885 1.87 1.022 0.833 0.672 1.046 0.81 0.713 0.535 1.25 0.639 0.483 1.6 1.59 0.625 0.532 0.404 1.25 0.576 0.453 0.367 0.653 0.488 0.407 0.368 5.76 0.796 0.680 1.93 1.55 0.705 0.594 0.433 0.86 0.46 0.396 0.302 0.461 0.441 0.312 0.199 Table 3.6b. Stiffness constants C11 , C12 , C13 , C33 , C44 , and C66 in some wurtzite-type semiconductors (units in 1012 dynes/cm2 ). Semiconductor C11 C12 C13 C33 C44 C66 AlN GaN InN CdS CdSe 4.11 3.9 1.90 0.858 0.74 1.49 1.45 1.04 0.533 0.452 0.99 1.06 1.21 0.462 0.393 3.89 3.98 1.82 0.937 0.836 1.25 1.05 0.1 0.149 0.132 0.163 0.145 3.6 Elastic Waves in Zinc-Blende-Type Crystals Let u be the displacement induced by an elastic wave traveling in a continuum. The equation governing u as a function of time t is obtained from Newton’s equation of motion: Ú 2 u ∇ · X, t2 where Ú is the density of the crystal and X the stress tensor. a) Use the results of Problem 3.5 to express the stress tensor in terms of the strain tensor. Next, by using the definition of the strain tensor e ∇u, show that the wave equations governing the propagation of elastic waves in a zinc- 141 142 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions blende-type crystal are 2 ux 2 ux Ú 2 C11 2 C44 t x 2 uy 2 uy Ú 2 C11 2 C44 t y 2 uz 2 uz Ú 2 C11 2 C44 t z 2 ux 2 u x 2 y z2 2 u y 2 uy 2 x z2 2 uz 2 u z x2 y2 (C12 C44 ) (C12 C44 ) (C12 C44 ) 2 uy 2 uz xy xz 2 ux 2 uz xy yz 2 uy 2 ux zy xz , , , b) Assume that a longitudinal (sound) wave propagating along the [100] axis is represented by a solution to the above wave equations of the form ux u0 exp[i(kx ˆt)] and uy uz 0, where k and ˆ are, respectively, the wave vector and frequency of the acoustic wave. Show that the resultant sound wave has a velocity ˘l ˆ/k (C11 /Ú)1/2 . Repeat this calculation for a transverse shear wave propagating along the [100] direction by assuming a solution of the form uy u0 exp[i(kx ˆt)], ux uz 0; and show that the transverse wave has a velocity ˘t (C44 /Ú)1/2 . c) Repeat the calculations in (b) for waves propagating along the [111] direction and show that ˘l [(C11 2C12 4C44 )/3Ú]1/2 and ˘t [(C11 C12 C44 )/3Ú]1/2 . d) For waves propagating along the [110] direction, the transverse waves polarized along the [001] and [110] directions have different velocities. Show that the elastic waves have the following velocities along the [110] direction: ˘l [(C11 C12 2C44 )/2Ú]1/2 ; ˘t (C44 /Ú)1/2 when polarized along [001] and ˘t [(C11 C12 )/2Ú]1/2 when polarized along [110]. The two quantized transverse waves are referred to as the fast (usually ˘t ) and slow (usually ˘t ) TA phonons. e) Discuss the eigenvectors (and the corresponding symmetries) of the TA and LA phonons propagating along [100], [111], and [110] directions of k-space. 3.7 Elastic Waves and Optical Phonons in Wurtzite-Type Crystals The wurtzite crystal structure shown in Fig. 3.13 is a variation of the zincblende structure. The bonding between nearest neighbors is also tetrahedral. The relationship between these two structures can be visualized most easily by viewing the zinc-blende structure along the [111] direction. In this direction the zinc-blende structure can be considered as consisting of layers of atoms arranged in regular hexagons stacked together. This hexagonal symmetry of the atoms within the layers is, of course, the origin of the C3 rotational symmetry of the zinc-blende crystal. Within each layer the atoms are identical and Problems C axis A(Zn) B(S) B(Zn) A(S) A(Zn) Fig. 3.13. Crystal structure of ZnS in the wurtzite form the layers alternate between Zn and S. In the zinc-blende crystal the stacking order of the Zn and S atomic layers is the sequence A(S)A(Zn)B(S)B(Zn)C(S)C(Zn)A(S)A(Zn)B(S)B(Zn) . . . as shown in Fig. 3.14a. If the stacking order of the layers is changed to A(S)A(Zn)B(S)B(Zn)A(S)A(Zn)B(S)B(Zn)A(S)A(Zn) . . . as shown in Fig. 3.14b the wurtzite structure is obtained. The arrangement of the tetrahedra is said to be “staggered” in the zinc-blende structure and “eclipsed” in the wurtzite structure. The reason for these descriptions becomes clear in Fig. 3.14. The Bravais lattice of the wurtzite structure is hexagonal, with the axis perpendicular to the hexagons usually labeled as the c axis. (a) (b) A (Zn) B (S) A (Zn) B (Zn) B (Zn) C (S) A (S) C (Zn) A (Zn) A (S) B (S) B (S) A (Zn) Fig. 3.14. Arrangement of atoms (a) along the [111] direction of the zinc-blende structure, showing the “staggered” stacking sequence, and (b) along the c axis of the wurtzite structure with the “eclipsed” geometry 143 144 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions The cohesive energy of the wurtzite structure is very close to that of the zincblende structure. As a result some group-II–VI semiconductors, such as ZnS and CdS, and also GaN, can crystallize in both zinc-blende and wurtzite structures. 4 The space group of the wurtzite structure is C6˘ . This group is nonsymmorphic with a screw axis along the c axis. It is homomorphic to the point group C6˘ . As in the latter there are 12 symmetry operations which are divided into 6 classes. To enumerate these symmetry operations it is most convenient to choose the origin in the center of one of the isosceles triangles formed by three neighboring atoms, such as the point labeled O in the following ﬁgure. In this ﬁgure the ﬁlled circles and the open circles represent the atoms in the two adjacent planes of the hcp structure. We shall also choose as our coordinate system the x and y axis as shown in the ﬁgure while the z-axis is along the c-axis. The reasons for our choice will become clear when we consider the symmetry operations. a) Show that the space group of wurtzite contains the following symmetry elements divided into the following classes: {E}: {C2 }: identity; a two-fold rotation about the c-axis followed by a translation by the vector (0, 0, c/2). In other words this is a screw axis operation; {C3 , C3⫺1 }: three-fold rotations about the c-axis; {C6 , C6⫺1 }: a six-fold rotation about the c-axis followed by a translation by the vector (0, 0, c/2). In other words this is also a screw axis operation. Note that this operation is a symmetry operation mainly because of our choice of the origin. This operation is not a symmetry operation if we simply choose the origin at one of the atoms; {3Ûd }: reﬂection in the yz-plane plus two other reﬂection planes obtained from the yz-plane by three-fold rotations about the c-axis; {3Ûd }: reﬂection in the plane denoted by AA in the ﬁgure followed by a translation by the vector (0, 0, c/2) plus two other glide planes obtained from AA by three-fold rotations about the c-axis. b) Using the symmetry properties of the wurtzite crystal show that its stiffness tensor is given by (the c axis has been chosen to be the z axis) ⎛ ⎞ C11 C12 C13 0 0 0 0 0 0 ⎜ C12 C11 C13 ⎟ ⎜ ⎟ 0 0 0 ⎜ C13 C13 C33 ⎟ ⎜ ⎟. 0 0 C44 0 0 ⎜ 0 ⎟ ⎝ 0 ⎠ 0 0 0 C44 0 0 0 0 0 0 (C11 ⫺ C12 )/2 Problems c) Show that the wave equations for acoustic phonons in wurtzite crystals are given by Ú Ú 2 ux (C11 C12 ) 2 ux (C11 C12 ) 2 uy 2 ux 2 ux C C 44 11 t2 x2 2 y2 z2 2 xy 2 uz (C13 C44 ) , xz 2 uy 2 uy 2 uy (C11 C12 ) 2 uy (C11 C12 ) 2 ux C11 2 C44 2 2 2 t y 2 x z 2 xy 2 uz , (C13 C44 ) yz 2 uz 2 uz Ú 2 C33 2 C44 t z 2 u z 2 uz x2 y2 (C13 C44 ) 2 uy 2 ux zy xz . d) Assume a solution for an acoustic wave in the wurtzite crystal of the form u(t) (u1 , u2 , u3 ) exp[i(q · r ˆt)]. Because of the hexagonal symmetry about the c axis, the y axis can be chosen, without loss of generality, such that the wave vector q lies in the yz plane. Show that the three components of the amplitudes satisfy the equations Úˆ2 u1 12 (C11 C12 )(q sin £)2 u1 C44 (q cos £)2 u1 , Úˆ2 u2 C11 (q sin £)2 u2 C44 (q cos £)2 u2 (C13 C44 )q2 sin £ cos £ u3 , Úˆ2 u3 C33 (q cos £)2 u3 C44 (q sin £)2 u3 (C13 C44 )q2 sin £ cos £ u2 , where £ is the angle between q and the c axis. Note that u1 is decoupled from u2 and u3 , so it is always possible to obtain a transverse acoustic wave perpendicular to the plane containing q and the c axis. This TA wave is usually referred to as TA2 . e) Show that for £ 0˚ the longitudinal and transverse acoustic waves have velocities ˘l (C33 /Ú)1/2 and ˘t (C44 /Ú)1/2 , respectively. f) For £ 90˚ there are two transverse acoustic waves: one polarized along the c axis (TA1 ) and one polarized along the x axis (TA2 ). Show that the longitudinal wave has velocity ˘l (C11 /Ú)1/2 while the velocities for the two transverse waves are (C44 /Ú)1/2 for TA2 and [(C11 C12 )/2Ú]1/2 for TA1 . g) Assume a Bloch function has the form: æk (r) uk (r) exp(ik · r) where uk (r) has the full periodicity of the lattice. By applying the symmetry operations of wurtzite to this wave function show that the corresponding character table is given by [see I. Rashba, Soviet Physics-Solid State, 1, 386 (1959)]: 145 146 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions °1 °2 °3 °4 °5 °6 {E} {C2 } {2C3 } {2C6 } {3Ûd } {3Ûd } 1 1 1 1 2 2 Ë Ë Ë Ë 2Ë 2Ë 1 1 1 1 1 1 Ë Ë Ë Ë Ë Ë Ë Ë Ë Ë 0 0 1 1 1 1 0 0 where Ë exp[ikz c/2] is the phase factor arising from the translation by the vector (0, 0, c/2) in the screw and glide operations. In the particular case of k 0 then Ë 1 and we find that the character table of the wurtzite structure is identical to that of the point group C6v . In the following table we show the correspondence between the two groups for this case: Point Group Space Group A1 A2 B1 B2 E1 E2 °1 °2 °3 °4 °5 °6 {E} {C2 } {2C3 } {2C6 } {3Ûd } {3Ûd } 1 1 1 1 2 2 1 1 1 1 2 2 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 0 0 1 1 1 1 0 0 h) Show that the long wavelength acoustic phonons in the wurtzite structure have the symmetries: °1 (or A1 ) plus °5 (or E1 ). The direction of the displacement of the atoms for the °1 representation is parallel to the c-axis while the displacements are perpendicular to the c-axis for the two-fold degenerate representation °5 . i) Show that the nine zone-center optical phonons in the wurtzite structure belong to the irreducible representations: °1 ⊕ 2°3 ⊕ °5 ⊕ 2°6 or A1 , 2B1 , E1 and 2E2 . 3.8 Pikus–Bir Strain Hamiltonians There are two forms of the Pikus–Bir strain Hamiltonian [3.34, 35] for the valence bands in the zinc-blende-type semiconductors (similar results can be obtained for diamond-type crystals) depending on whether spin–orbit interaction is included or not. If spin–orbit interaction is neglected, the p-like °4 valence band wave functions labeled |X , |Y , and |Z (Sect. 2.6.1) at the zone center are degenerate. From symmetry we can show that a uniaxial stress along the [100] direction will split the band labeled |X off from the other two bands. Thus a [100] stress will split the three bands into a singlet and a doublet. If spin–orbit interaction is included and assumed to be much larger than Problems any strain-induced effect, the valence bands at the zone center will be split into a four-fold degenerate °8 (or J 3/2) state and a doubly degenerate °7 (J 1/2) state (Sect. 2.6.2). For a sufficiently small stress we can neglect the effect of strain on the spin–orbit interaction. Since strain is not expected to affect the spin degeneracy of the electrons (Kramers degeneracy) we expect that a uniaxial stress will split the J 3/2 states into two doublets. The strain Hamiltonian HPB in (3.23) is valid in this limit of large spin-orbit interaction and care should be exercised in using it to analyze experimental results. For theoretical considerations, one may want to simplify the problem by “turning off” the spin–orbit interaction. In this case the total angular momentum operator J in (3.23) can be replaced by the orbital angular momentum operator L. However, the deformation potentials b and d should also be changed to b∗ and d∗ since the expression for the strain-induced splitting will be different in the two cases. In Problems 3.11 and 3.12 we will perform theoretical calculations of b∗ and d∗ . a) Use the results of Problem 3.4 to show that the Pikus–Bir strain Hamiltonian (3.23) reduces to HPB (X) a(S11 2S12 )X b(S11 S12 )X[Jx2 (J 2 /3)] for a stress X applied along the [100] direction. b) Show similarly that the strain Hamiltonian is given by √ HPB (X) a(S11 2S12 )X (dS44 X/3 3)[(Jx Jy Jy Jx ) c.p.] for a stress X applied along the [111] axis. c) Use the result of parts (a) and (b) to show that the four-fold degenerate J 3/2 valence bands will be split into two doubly degenerate bands with the splitting ‰E given by 2b(S11 S12 )X, [100] stress, √ ‰E (d/ 3)S44 X, [111] stress. d) Let us rewrite the Pikus–Bir strain Hamiltonian in the absence of spin–orbit interaction as HPB a(exx eyy ezz ) 3b∗ [(L2x L2 /3)exx c.p.] 6d∗ 1 (Lx Ly Ly Lx )exy c.p. , √ 3 2 (3.41) where b∗ and d∗ are equal to b and d in the absence of spin–orbit interaction. The prefactors of the b∗ and d∗ terms in (3.41) have been chosen to agree with those in (3.77) of [3.36]. Show that the stress-induced splittings are given by 3b∗ (S11 S12 )X, [100] stress, √ ‰E ( 3/2)d∗ S44 X, [111] stress. 147 148 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions Show that if the spin–orbit splitting implicit in the Hamiltonian of (3.23) does not depend an strain, b b∗ and d d∗ . Explain the origin of the difference of those prefactors in (3.23) and (3.41). Now include spin–orbit coupling and assume that the J 3/2 and J 1/2 states are separated by ¢. Use the Pikus– Bir Hamiltonian involving L to calculate the stress-induced splitting of these levels to second order in X for stress parallel to both [100] and [111]. 3.9 Calculation of Volume Deformation Potentials Using the Tight-Binding Model The calculation of the absolute volume deformation potential of a band edge in a finite solid is a difficult task because in a finite solid the band edges are dependent on surface properties (for example, see discussion in [3.32]). This difficulty does not appear when calculating the relative volume deformation potentials between two bands, such as between an s-like antibonding conduction band and a p-like bonding valence band. In this case the deformation potential can be calculated easily with the tight-binding model. Assume that the zone-center °2 conduction and °25 valence band edges in a diamond-type semiconductor are given by (2.84a) and (2.84b), respectively. Furthermore, assume that the overlap parameters Vss and Vxx both depend on the nearest neighbor distance d as d2 . Show that the relative deformation potential ac av is given by (2/3)(| Vss | | Vxx |). Use the empirical values of Vss and Vxx for Si and Ge given in Table 2.26 to calculate the theoretical values of ac av for Si and Ge. Compare these values with the experimental values for Si and Ge given in Table 3.1 under a(°1c ) a(°15v ) Calculation of the Shear Deformation Potential b∗ for the °15 Valence Bands Using the Tight-Binding Model The shear deformation potentials b∗ and d∗ for the °15 (or °25 ) valence bands in zinc-blende (or diamond) type semiconductors can also be calculated using the tight-binding model. This problem involves the calculation of the shear deformation potential b∗ , leaving the calculation of d∗ to the next problem. Assume a stress X is applied along the [100] crystallographic axis. According to Problem 3.4b, the strain induced in the crystal can be decomposed into a multiple of a unit matrix plus a traceless matrix of the form 3.10 ⎛ 2 ·⎝0 0 0 1 0 ⎞ 0 0 ⎠, 1 where · (X/3)(S11 S12 ). The effect of this shear strain is to lower the cubic symmetry of the crystal to tetragonal symmetry by making the x direction inequivalent to the y and z directions. As a result, we expect that the originally triply degenerate °15 wave functions |X , |Y , and |Z will split into a doublet and a singlet. To calculate this splitting it is necessary to evaluate the overlap parameters Vxx and Vyy ( Vzz ) in the presence of the shear strain. Problems a) Suppose that the locations of the four nearest neighbors of an atom located at the origin in the unstrained lattice are d1 (1, 1, 1)a/4; d2 (1, 1, 1)a/4; d3 (1, 1, 1)a/4; and d4 (1, 1, 1)a/4. Show that in the strained lattice these four nearest-neighbor locations are changed to d1 (1 2·, 1 ·, 1 ·)a/4; d2 (1 2·, 1 ·, 1 ·)a/4; d3 (1 2·, 1 ·, 1 ·)a/4; and d4 (1 2·, 1 ·, 1 ·)a/4. Show that, to first order in ·, the bond lengths are unchanged by the strain but the bond angles are changed. b) Use the results of Problem 2.16 to show that the overlap parameters in the strained lattice are 4 8 VppÛ (1 4·) Vpp (1 2·) Vxx 3 3 and 4 8 VppÛ (1 2·) Vpp (1 ·). Vyy 3 3 c) Calculate the energy of the bonding orbitals with p-symmetry at zonecenter in the strained lattice. Show that the splitting between the doublet with py and pz symmetries and the singlet with px symmetry is given by 8·(VppÛ Vpp ). d) By combining the result of part (c) with those of Problem 3.9d show that 2 8 b (VppÛ Vpp ) Vxy . 9 3 Substitute the values of Vxy for Si and Ge given in Table 2.26 into the above expression to evaluate the theoretical values of b∗ for Si and Ge. You will find that the calculated values are larger than the experimental values by about a factor of two but the signs agree. The agreement between theory and experiment can be improved by including an additional higher energy s orbital in the tight-binding model (the resultant model is referred to as the sp3 s∗ model). See [3.30] for more details. 149 150 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions Calculation of the Shear Deformation Potential d∗ for the °15 Valence Bands Using the Tight-Binding Model The calculation of the shear deformation potential d∗ is complicated by the following considerations. Let us assume that a uniaxial stress is applied along the [111] axis of a diamond or zinc-blende crystal. As shown in Problem 3.4c, the resultant strain tensor can be decomposed into a multiple of a unit tensor and the traceless shear strain tensor (of °15 symmetry) ⎛ ⎞ 0 1 1 · ⎝ 1 0 1 ⎠ , where · S44 X/6. 1 1 0 3.11 This strain tensor describes a trigonal distortion of the cubic lattice along the [111] direction. The symmetry of this distortion is the same as that of a displacement of the two sublattices in the diamond or zinc-blende lattice along the body diagonal. As a result, it is possible to “mix” these two types of distortions. The displacement of the two neighboring atoms in the diamond or zinc-blende crystals along the body diagonal corresponds to the zone-center (°15 ) optical phonon. A macroscopic °15 shear strain along the [111] direction can, therefore, change the nearest-neighbor distance along the [111] direction in addition to producing a trigonal distortion in the cubic lattice. To specify the change in the nearest-neighbor distance it is necessary to define an internal strain parameters ˙ in terms of the relative displacement u between the two sublattices. The internal strain parameter will be defined in Problem 3.13. In this problem we will assume that the [111] stress does not produce an internal strain (i. e., ˙ 0). The resultant deformation potential will be denoted by d so as to distinguish it from the deformation potential d for the case when the internal strain is not zero. From symmetry considerations, it is clear that the effect of a [111] stress on the p orbitals will be different from that of a [100] stress. While a [100] stress makes the px orbital different from the py and pz orbitals, a [111] stress should affect the three orbitals in exactly the same way. Instead, a [111] stress will mix the three orbitals and produce a new set of three orbitals which should be symmetrized according to the trigonal symmetry (C3v point group). Such a set of three orthogonal and symmetrized orbitals is given by √ |X1 [|X1 |Y1]/ 2, √ |Y1 [|X1 |Y1 2|Z1]/ 6, √ |Z1 [|X1 |Y1 |Z1]/ 3. Similarly symmetrized p orbitals are defined for the second atom within the primitive cell. Under [111] stress the orbitals |Z1 and |Z2 which are parallel to the stress direction (and of §1 symmetry) will split from the other two sets of two orbitals (of §3 symmetry) which are perpendicular to the stress direction. Problems a) Show that under a [111] shear strain the locations of the four nearest neighbors in the diamond and zinc-blende lattice are changed to d1 {(a/4) (a·/2)}(1, 1, 1); d2 (a/4)(1 2·, 1, 1); d3 (a/4)(1, 1 2·, 1); d4 (a/4)(1, 1, 1 2·). b) Based on the result of (a), show that the effects of the [111] stress are: (1) to change the lengths of the nearest-neighbor distance by the amount (to first order in ·) (‰d1 )/d1 2·; (‰d2 )/d2 (‰d3 )/d3 (‰d4 )/d4 2·/3 and (2) to change the orientations of the three bonds d2 , d3 , and d4 . The directional cosines of the bond d2 in the strained lattice are given by d2 {3[1 (4·/3)]}1/2 (1 2·, 1, 1) with similar results for d3 and d4 . c) Assuming that the overlap parameters VppÛ and Vpp both depend on bond distance d as d2 , show that, to first order in ·, the [111] shear strain does not change the matrix elements X1 | int | X2, Y1 | int | Y2, etc. On the other hand (use the results of Problem 2.16), the matrix elements X1 | int | Y2, X1 | int | Z2, etc., in the strained lattice are all changed to (8·/9)(VppÛ Vpp ). Vxy Thus a [111] shear strain couples the wave function |X1 with |Y2 and |Z2, |Y1 with |X2 and |Z2, and so on. The new 6×6 matrix for the six p orbitals of the two atoms within the primitive cell is now given by X1 Y1 Z1 X2 Y2 Z2 X1 Y1 Z1 X2 Y2 Z2 Ep1 Ek 0 0 Vxx Vxy Vxy 0 Ep1 Ek 0 Vxy Vxx Vxy 0 0 Ep1 Ek Vxy Vxy Vxx Vxx Vxy Vxy Ep2 Ek 0 0 Vxy Vxx Vxy 0 Ep2 Ek 0 Vxy Vxy Vxx 0 0 Ep2 Ek where Ep1 and Ep2 are the energies of the p orbitals of the two atoms in the primitive cell. d) Assume that the two atoms in the primitive cell are identical (thus the results we will obtain from now on are only valid for the diamond structure) 151 152 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions and diagonalize the 6×6 matrix in part (c) to obtain the eigenfunctions and energies in the [111]-strained lattice. The more general results for the case when the two atoms are different are given in [3.30]. Hint: Since the Hamiltonian is symmetric with respect to interchange of the atoms in the primitive cell, define linear combinations of the wave functions √ √ |X [|X1 |X2]/ 2; |X [|X1 |X2]/ 2, √ √ |Y [|Y1 |Y2]/ 2; |Y [|Y1 |Y2]/ 2, √ √ |Z [|Z1 |Z2]/ 2; |Z [|Z1 |Z2]/ 2. Show that the 6×6 matrix decomposes into two 3×3 matrices: X Y Z X Y Z Ep Ek Vxx Vxy Vxy 0 0 0 Ep Ek Vxx Vxy 0 0 0 Vxy Vxy Ep Ek Vxx 0 0 0 Vxy Vxy Vxy 0 0 0 Ep Ek Vxx 0 0 0 Vxy Ep Ek Vxx Vxy 0 0 0 Vxy Vxy Ep Ek Vxx Note that the wave functions with the () subscript are antisymmetric (symmetric) under interchange of the two atoms inside the primitive cell so they correspond to the antibonding (bonding) orbitals. The two resultant 3×3 matrices can be diagonalized by a transformation to two new sets of symmetrized wave functions, one for the bonding orbitals and one for the antibonding orbitals. The set of eigenfunctions for the antibonding orbitals is given by √ |X [|X |Y ]/ 2, √ |Y [|X |Y 2|Z ]/ 6, √ |Z [|X |Y |Z ]/ 3. The corresponding energies are given by Z | int |Z Ep Vxx 2Vxy and X | int |X Y | int |Y Ep Vxx Vxy . The energies for the bonding orbitals are given by Z | int |Z Ep Vxx 2Vxy and X | int |X Y | int |Y Ep Vxx Vxy . Problems These results show that a [111] uniaxial stress splits both the antibonding (°15 conduction band) and bonding (°25 valence band) orbitals into a doublet and a singlet with an energy splitting equal to 3Vxy . e) Using the results in part (d) and in Problem 3.8d, show that the deformation potential d is given by d (8/35/2 )(VppÛ Vpp ) (2/33/2 )Vxy in the tight-binding model. The values of d obtained this way for Si and Ge are, respectively, 2.9 eV and 2.6 eV. These theoretical values of d are not only quite different but also have signs opposite to those of the experimental values of d since we have neglected the internal strains, which are usually not equal to zero in stressed crystals. 3.12 Calculation of the Optical Deformation Potential d0 for the °15 Valence Bands Using the Tight-Binding Model As pointed out in Problem 3.11, a relative displacement u between the two sublattice in the diamond and zinc-blende crystals corresponds to the zonecenter optical phonon with °15 symmetry. The deformation potential describing the electron–optical-phonon interaction is denoted by d0 and is defined by ‰E111 d0 u , a where √ ‰E111 is the shift in energy of the singlet component ([|X |Y |Z]/ 3) of the p orbital induced by the sublattice displacement u. d0 can also be calculated within the tight-binding model in a way very similar to that adopted in Problem 3.11. a) Assuming that the relative displacement of the two sublattices is given by u (a·/4)(1, 1, 1), show that the locations of the four nearest neighbors in the diamond or zinc-blende lattice are changed to d1 (a/4)(1 ·)(1, 1, 1); d2 (a/4)(1 ·, 1 ·, 1 ·); d3 (a/4)(1 ·, 1 ·, 1 ·); and d4 (a/4)(1 ·, 1 ·, 1 ·). b) Based on the result of (a), show that the effects of the relative displacement u are: (1) to change the lengths of the nearest-neighbor distances by the amount (to lowest order in ·) (‰d1 )/d1 ·; (‰d2 )/d2 (‰d3 )/d3 (‰d4 )/d4 ·/3 153 154 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions and (2) to change the orientations of the three bonds d2 , d3 , and d4 . The directional cosines of the bond d2 are given by d2 {3[1 (·/3)]}1/2 (1 ·, 1 ·, 1 ·) with similar results for d3 and d4 . c) As in the case of Problem 3.11c, show that, to first order in ·, the sublattice displacement does not change the matrix elements X1 | int | X2, Y1 | int | Y2, etc. On the other hand the matrix elements X1 | int | Y2, X1 | int | Z2, etc., are all equal to Vxy (16·/9)(VppÛ Vpp ). Set up the 6×6 matrix for calculating the energies of the p orbitals in the displaced sublattices as in Problem 3.11. d) Diagonalize the 6×6 matrix in part (c) and show that the splitting between the doublet and singlet in the displaced sublattices is given by 16· (VppÛ Vpp ) 4·Vxy . 3 The optical phonon deformation potential is then given by ‰E 32 d0 √ Vxy 16d . 3 3 Note that d0 is much larger than d . 3.13 Internal Strain and the Deformation Potential d In Problems 3.11 and 3.12 the tight-binding model is used to calculate the deformation potentials for the diamond- and zinc-blende-type crystals in two extreme cases. In Problem 3.11 the crystal is assumed to be a continuum and the displacements of the atoms are described by the macroscopic strain tensor. In Problem 3.12 the atomic structure of the crystal is taken into account. The fact that the crystal is constructed from two sets of atoms located at two sublattices suggests that one can displace the two sublattices relative to each other in a way such that the symmetry of the primitive cell of the crystal is unchanged. For the diamond and zinc-blende structures this is the case when the two atoms within the primitive cell are displaced relative to each other along the body diagonal of the fcc lattice. Such microscopic relative displacements of the sublattices in a crystal cannot be described by the macroscopic strain tensor and are known as an internal strain. By definition internal strain can only occur in crystals with more than one atom per primitive cell. The number of possible internal strain patterns for a given crystal structure can be determined by group theory and crystal symmetry [3.46]. In the diamond and zinc-blende structure the only possible internal strain is the relative displacement of the two atoms in the primitive cell along the [111] axis (or equivalent ones, e.g., [111]) described above. As noted in Problem 3.12, this displacement pattern is identical to that of the zone-center optical phonon in these structures. This is no coincidence. Anastassakis and Cardona [3.46] have shown that internal strains can be regarded as “frozen” Raman-active optical phonons. Problems It was pointed out by Kleinman [3.45] that under a [111] strain the bond length between the two atoms inside the primitive cell of Si is undetermined due to the possibility of an internal strain. Assume the [111] strain is given by the strain tensor ⎛ ⎞ 0 1 1 ·⎝1 0 1⎠. 1 1 0 The internal strain is specified by choosing one atom as the origin and describing the displacement u of its nearest neighbor atom at (a/4)(1, 1, 1) as u (a·/2)(˙, ˙, ˙), where ˙ is the internal strain parameter mentioned in Problem 3.11. For ˙ 0, there is no internal strain and the change in the bond length is specified completely by the macroscopic strain tensor as in Problem 3.11. For ˙ 1 the internal strain exactly cancels the change in the bond length induced by the [111] strain so that the bond length in the strained crystal is unchanged. a) Show that for a [111] shear strain with an internal strain parameter ˙ the shear deformation potential d is given by d d (1/4)˙d0 . b) The value of ˙ has recently been deduced from experimental results for Si (0.58), Ge (0.56) [3.51] and a few zinc-blende semiconductors such as GaAs (0.65) [3.52]. Since d0 16d and the value of ˙ is fairly close to 1, the deformation potential d is determined mainly by d0 . Calculate the value of d for Si using the value of d0 obtained in Problem 3.12 and compare it with the experimental value of d(5.1 eV) in Table 3.1. 3.14 Stress Induced Splitting of [110] Valleys Consider a nondegenerate electronic state with wave vector k[110] in a cubic crystal. There are six equivalent valleys along the [110], [110], [101], [101], [011], and [011] directions (it is not necessary to consider the six opposite directions). Show from symmetry arguments that: a) A [100] uniaxial strain will split these six valleys into a doublet {[011] and [011] valleys} and a quadruplet {the remaining four valleys} (this splitting is described by the shear deformation potential •u in Table 3.2); b) A [111] uniaxial strain will split the six valleys into two triplets: {[110], [011], and [101] valleys} and {[101], [110], and [011]} (this splitting is described by the shear deformation potential •p in Table 3.2). c) Explain, using group theory, why the deformation potentials •u given in Table 3.2 are, in general, different for [100] and for [111] strain. Explain why two different shear deformation potentials •u and •p are needed for k along [110]. 155 156 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions 3.15 Electromechanical Tensors in Zinc-Blende- and Wurtzite-Type Semiconductors a) Use the symmetry properties of the zinc-blende crystal described in Chap. 2 to show that the nonzero and linearly independent components of its electromechanical tensor em are (em )14 (em )25 (em )36 . b) Use the symmetry properties of the wurtzite crystal described in Problem 3.7 to show that its electromechanical tensor has the form ⎛ ⎞ 0 0 0 0 (em )15 0 ⎝ 0 0 0 (em )15 0 0⎠. (em )31 (em )31 (em )33 0 0 0 3.16 Piezoelectric Electron–Phonon Interactions in Wurtzite-Type Semiconductors a) Combine the results in Problems 3.7 and 3.15 to calculate the electric field induced by a phonon displacement u, E em · (∇u)/Â∞ , for all three acoustic modes. In particular show that for the TA1 and LA phonons E is given by Ex 0, Ey iq (em )15 sin £ uz (em )15 cos £ u⊥ Â∞ , and Ez iq (em )31 sin £ u⊥ (em )33 cos £ uz Â∞ , where £ is the angle between the phonon wave vector q and the c axis of the wurtzite crystal, uz is the projection of u on the c axis, and u⊥ is the component of u perpendicular to the c axis. b) Substituting the results of part (a) into (3.29) and (3.30), show that the piezoelectric electron–phonon interaction in wurtzite crystals is given by [3.40] Hpe (4| e |/Â∞ )[(em )15 sin £(uz sin £ u⊥ cos £) (em )31 sin £ cos £ u⊥ (em )33 cos2 £ uz ]. 3.17 Dependence of Phonons Frequencies on Volume: Grüneisen Parameters In the harmonic approximation, the phonon frequencies are independent of strain. In nature, however, external strains result in small changes in the frequencies of phonons (anharmonic effects). The simplest of these effects are represented by the so-called mode Grüneisen parameters Áˆ d ln ˆ/d ln V, where V is the crystal volume. Each phonon frequency has a specific mode Grüneisen parameter Áˆ . a) The Áˆ of optical phonons of tetrahedral semiconductors are ∼1. Give a qualitative explanation. Problems b) The thermal expansion is a manifestation of anharmonicity. Derive the following expression for the linear thermal expansion coefficient · (1/3)(d ln V/dT): · ÁC/3B, (3.42) where C is the specific heat, B the bulk modulus (p. 131) and Á an average Grüneisen parameter of all phonon frequencies. c) The Áˆ of TA modes near the edge of the BZ is often negative [3.53]. Discuss the effect of a negative Áˆ on · [3.54]. 3.18 Phonons in Selenium and Tellurium Selenium and tellurium have three equal atoms per unit cell, hence 6 optical and 3 acoustic phonon branches. Discuss the eigenvectors of the optical phonons at the center of the BZ, their symmetries and degeneracies [2.5]. 3.19 Biaxial Strains Nowadays there is much interest in the growth of epitaxial layers of one material on a substrate of different lattice constant (see, for example, Section 1.2.5). Depending on the lattice mismatch between the epilayer and the substrate, the epilayer can experience either a tensile or compressive strain. The characteristic of this strain is that the corresponding stress is two-dimensional and lies within the plane of the epilayer. Such strain is known as a biaxial strain as distinct from a unaxial strain. Assume that an epilayer of diamond- or zincblende-type crystal is grown epitaxially along the [001] axis on a substrate of similar crystal structure. The difference in the two lattice constants is given by: ¢a a0 a where a and a0 are the lattice constants of the epilayer and substrate, respectively. Along the [001] axis we can usually assume that there is no stress on the epilayer. (a) Show that the strain tensor of the resultant biaxial strain is given by: ⎛ ⎞ exx 0 0 ⎝ 0 eyy 0 ⎠ with exx eyy ¢a0 /a0 and ezz 2C12 exx C11 0 0 ezz where C11 and C12 are the components of the fourth rank stiffness tensor defined in Problem 3.5. (b) Show that a biaxial strain is equivalent ⎛ to a sum of two ⎞ strains: (1) a hyexx 0 0 drostatic strain described by the tensor: ⎝ 0 exx 0 ⎠ and (2) a uniaxial 0 0 ⎛ exx ⎞ 0 0 0 ⎠. strain along the [001] axis described by the tensor: ⎝ 0 0 0 0 0 ezz exx Note that: if the biaxial strain is compressive then the hydrostatic strain is also compressive. However, the corresponding uniaxial strain is tensile. 157 158 3. Vibrational Properties of Semiconductors, and Electron-Phonon Interactions SUMMARY Although the atoms in semiconductors are not stationary, their motion is so slow compared to that of electrons that they were regarded as static in Chap. 2. In this chapter we have analyzed the motion of atoms in semiconductors in terms of simple harmonic oscillations. Instead of calculating from first principles the force constants for these quantized oscillators or phonons, we have studied models based on which these force constants can be deduced from experimental results. The usefulness of these models is judged by the minimum number of parameters they require to describe experimental phonon dispersion curves. The more successful models typically treat the interaction between the electrons and ions in a realistic manner. The shell model assumes that the valence electrons are localized in deformable shells surrounding the ions. Bond models regard the solid as a very large molecule in which atoms are connected by bonds. Interactions between atoms are expressed in terms of bond stretching and bond bending force constants. In covalent semiconductors charges are known to pile up in regions between adjacent atoms, giving rise to bond charges. So far, models based on bond charges have been most successful in fitting experimental results. In this chapter we have also studied the different ways electrons can be affected by phonons, i. e., electron–phonon interactions. These interactions have a significant effect on the optical and transport properties of electrons in semiconductors. We showed how long-wavelength acoustic phonons can change the energy of electrons via their strain field. These interactions can be described in terms of deformation potentials. Optical phonons can be regarded as giving rise to “internal strain” and their interactions with electrons can likewise be described by optical-phonon deformation potentials. In polar semiconductors both long-wavelength acoustic and optical phonons can generate electric fields through the charges associated with the moving ions. These fields can interact very strongly with electrons, giving rise to piezoelectric electron–phonon interactions for acoustic phonons and the Fröhlich interaction for optical phonons. Electrons located at band extrema near or at zone boundaries can be scattered from one valley to another equivalent valley via intervalley electron–phonon interactions. 4. Electronic Properties of Defects CONTENTS 4.1 Classification of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Shallow or Hydrogenic Impurities . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Deep Centers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 160 161 180 198 202 One reason why semiconductors are so useful for device applications is that their electrical properties can be modified significantly by the incorporation of small amounts of impurities or other kinds of defects. However, while one type of defect can make a semiconductor useful for fabricating a device, another type can have undesirable effects which render the device useless. The quantity of defects necessary to change the properties of a semiconductor is often considerably less than one defect atom per million host atoms. As a result, our ability to control the defects in a semiconducting material often determines whether it can be used in device applications. To control the amount and nature of defects in a material typically involves developing a process for growing a relatively defect-free sample. Then the desired amounts of defects are introduced either during the growth process or after growth. There is extensive literature devoted to the study of defects in semiconductors. It would take more than a whole book to review all the properties of defects, so in this chapter we will limit ourselves to the study of the electronic properties of defects. We shall begin by classifying the different kinds of defects found in semiconductors. Next we will separate defects into two broad categories. Impurities whose electronic energies can be calculated by means of the “effective mass approximation” are referred to as shallow impurities, while defects whose energies cannot be calculated with that approximation are known as deep centers. One method capable of calculating the energy levels of deep centers is the Green’s function method. As simple illustrations of this method we will study deep centers in tetrahedrally bonded semiconductors. P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed., DOI 10.1007/978-3-642-00710-1_4, © Springer-Verlag Berlin Heidelberg 2010 160 4. Electronic Properties of Defects 4.1 Classification of Defects In general, defects are classified into point defects and line defects. As the name implies, point defects usually involve isolated atoms in localized regions of a host crystal. Line defects, on the other hand, involve rows of atoms, and typical examples of line defects are dislocations. In addition to point and line defects, there are defects which are composed of a small number of point defects. These are referred to as complexes. Line defects are always detrimental to devices. Hence semiconductor wafers used in fabricating devices have to be as free of such defects as possible. The surface which terminates a threedimensional crystal can also be considered as a two-dimensional “defect”. However, the electronic states introduced by such surfaces are usually called “surface states” rather than defect states. In this chapter we shall not consider surface states or dislocations. Instead we will concentrate on the properties of point defects and complexes only, since they tend to determine the properties of semiconductor devices. For a brief discussion of surface states and their energies see Sect. 8.3. Point defects are often further classified into the following kinds with special nomenclature and notations: Vacancy: the vacancy created by a missing atom A is denoted by VA . Interstitial: an atom A occupying an interstitial site is denoted by IA . Substitutional: an atom C replacing a host atom A is denoted by CA . Antisite: a special kind of substitutional defect in which a host atom B occupies the site of another host atom A. Frenkel defect pair: a complex VA –IA formed by an atom A displaced from a lattice site to a nearby interstitial site. Vacancies and antisite defects are intrinsic or native defects since they do not involve foreign atoms. Their concentrations cannot be determined by chemical analysis or mass spectrometry. Defects involving foreign atoms (i. e., impurities) are referred to as extrinsic defects. Many important defects are electrically active. Defects which can contribute free electrons to the host crystal are known as donors, while defects which can contribute holes (i. e., remove free electrons) are known as acceptors. Examples of donors in Si are substitutional group-V atoms such as P, As, and Sb or interstitial monovalent atoms such as Li and Na. The group-V atoms have one more valence electron than the Si atoms they replace. Furthermore, this extra electron is loosely bound to the group-V atom in Si so that it can be easily excited into the conduction band of the host Si crystal. Substitutional group-VI atoms such as S, Se, and Te in Si can contribute up to two conduction electrons so they are known as double donors. Examples of acceptors in Si are substitutional group-III atoms such as B, Al, Ga, and In. Substitutional group-II atoms (such as Be and Zn) in Si are double acceptors. When a substitutional impurity atom has the same valence as the host atom, it is referred to as an isoelectronic or isovalent center. Examples of such cen- 4.2 Shallow or Hydrogenic Impurities ters are CSi in Si and NP in GaP. As we will show later (Sect. 4.3.3), isovalent centers can behave as donors or acceptors or remain electrically inactive. A term which is commonly found in the literature but rarely defined is deep center. In the past, some authors have used the term “deep centers” to mean defects whose electronic levels are located near the middle of the bandgap. Now we know that there are many defects with properties similar to those of deep levels but whose energies are not near the center of the gap. As a result, the term has been broadened to apply to any center which cannot be classified as shallow! Thus, to understand deep centers we have to understand first what shallow centers are. In the next section we shall study the properties of shallow or hydrogenic impurities in semiconductors with the diamond and zinc-blende structures. After that we shall study the properties of some deep centers. 4.2 Shallow or Hydrogenic Impurities Let us consider a substitutional donor atom such as PSi in Si. Compared to the Si nucleus, the P nucleus has one extra positive charge, which is balanced by the extra valence electron in the P atom as compared to the Si atom. The attractive potential between this extra valence electron and the P nucleus is not equal to that of an isolated P nucleus since the Coulomb potential of the P nucleus in Si will be screened, not only by the core electrons of the P atom, but also by the remaining four valence electrons of the P atom, and all the valence electrons of neighboring Si atoms. This screening effect allows us to approximate the attractive Coulomb potential seen by the extra valence electron in P by the Coulomb potential of a proton screened by the valence electrons of the Si host. Thus a P impurity in Si behaves effectively like a hydrogen atom embedded in Si, except that the mass of the P nucleus is so much heavier than the mass of the proton that we can assume it to be infinite. In addition, the Coulomb attraction between the electron and the positive charge in this “hydrogen-like” impurity is much weaker than the Coulomb attraction in the hydrogen atom since it is strongly screened by the large number of valence electrons in Si. As a result, the extra valence electron in the P atom is only loosely bound to the P atom when the atom is embedded in Si. This loosely bound electron can be ionized easily by thermal or electrical excitations. For this reason P in Si is known as a donor and the extra valence electron which it can “donate” to the Si conduction band is referred to as the donor electron. In the case of an acceptor impurity atom (such as a B atom replacing a Si atom) in Si, there is a deficiency of a valence electron when the acceptor bonds with its four nearest-neighbor Si atoms. Instead of regarding an acceptor atom as short of a valence electron, we think of it as possessing an extra hole which is loosely bound to a negatively charged B nucleus with an infinite mass. While 161 162 4. Electronic Properties of Defects a donor atom can be compared with a hydrogen atom, an acceptor atom is analogous to a positron bound to a negatively charged muon. To calculate exactly the screened Coulomb potential between the donor electron and the donor ion is very difficult, since it depends on the manybody interactions between the electrons in the impurity atom with the valence electrons of the host. One simple approach to circumventing this problem is to assume that the positive charge on the donor ion is screened by the dielectric constant of the host crystal. With this approximation the Coulomb potential of the donor ion can be expressed as VS |e| , 4Â0 Â0 r (4.1) where Â0 is the dielectric constant of the host crystal. If we assume further that the donor electron is not too localized near the donor ion then we can use the static (i. e., zero-frequency) dielectric constant as Â0 in (4.1). More detailed studies of the dielectric constants of semiconductors will be presented in Chap. 6. Since the donor electron is moving inside a semiconductor, its motion is affected by the crystal potential in addition to the impurity potential (4.1). The Schrödinger equation of the donor electron is given by (H0 U)æ(r) Eæ(r), (4.2) where H0 is the one-electron Hamiltonian of the perfect crystal, U is the potential energy of the electron in the screened Coulomb potential VS U | e | VS (4.3) and æ(r) is the donor electron wave function. In principle, one way to solve (4.2) is to expand æ(r) in terms of the Bloch functions „nk (r) of the perfect crystal, since they form a complete orthonormal set. This approach requires extensive numerical calculations. Since the defect breaks down the translational symmetry of the crystal we cannot take advantage of the Bloch theorem to simplify the problem. The most common approach to solving (4.2) is to utilize the effective mass approximation. This approximation makes use of the known electronic band structure parameters, such as effective masses, of the perfect crystal and is useful not only for calculating defect energy levels but also for studying properties of electrons under any weak external perturbation. We will make a digression to discuss this approximation in the next section. 4.2.1 Effective Mass Approximation There are two approaches to deriving the effective mass approximation. One approach involves introducing the concept of Wannier functions. The other utilizes Bloch functions only. The Wannier functions are Fourier transforms of the Bloch functions, so the two approaches will eventually produce the same 4.2 Shallow or Hydrogenic Impurities results. The Wannier function an (r ; Ri ) is related to the Bloch function „nk (r) by an (r ; Ri ) N 1/2 exp(ik · Ri )„nk (r), (4.4a) „nk (r) N 1/2 k exp(ik · Ri )an (r; Ri ), (4.4b) Ri where Ri is a lattice vector, n the band index, k the wave vector in the reduced zone scheme, and N the number of unit cells in the crystal. While Bloch functions are indexed by the wave vectors in reciprocal lattice space, Wannier functions are indexed by lattice vectors in real space. While Bloch functions are more convenient for representing extended states in crystals, Wannier functions are more appropriate for localized states. We note that Wannier functions are similar to the Löwdin orbitals defined in (2.72) for the tight-binding model (Sect. 2.7.2). For very localized electrons, one can think of Wannier functions as atomic orbitals. In this chapter we will approach the problem of defects by using Wannier functions. An excellent reference for this approach is the classic text by Wannier himself [4.1]. An equally excellent reference for the alternative approach based on Bloch functions is the review article by Kohn [4.2]. Some of the properties of Wannier functions are summarized below • • • an (r; Ri ) is a function of r Ri only. This can be easily shown by noting that an (r; Ri ) an (r s; Ri s) for any vector s. From now on we will represent an (r; Ri ) as an (r Ri ). Wannier functions an (r Ri ) where Ri varies over all the lattice vectors inside the crystal, form a complete and orthonormal set just like the Bloch functions. Wannier functions are eigenfunctions of a “lattice vector operator” Rop defined by Rop an (r Ri ) Ri an (r Ri ). (4.5) The effect of Rop on a wave function æ(r) An (k)„nk (r) n, k can be represented approximately as i An (k) „nk (r). Rop æ(r) ≈ k (4.6) n, k The proof of (4.6) involves expanding æ(r) first in terms of Bloch functions and then in terms of Wannier functions: æ(r) An (k)„nk (r) n, k n, k An (k) Ri (N 1/2 ) exp(ik · Ri ) an (r Ri ). (4.7) 163 164 4. Electronic Properties of Defects Operating on both sides of (4.7) with Rop we obtain An (k) (N 1/2 ) exp(ik · Ri ) Ri an (r Ri ). Rop æ(r) n, k (4.8) Ri Formula (4.8) can be rewritten as 1/2 Rop æ(r) An (k) (N ) i exp(ik · Ri ) an (r Ri ) (4.9) k Ri n, k i An (k)„nk (r) i An (k) „nk (r). (4.10) k k n, k n, k The summation over k on the right hand side of (4.10) can be approximated by an integral over k in the limit that the crystal volume becomes infinite. After integration, the first term on the right hand side of (4.10) involves An (k2 ) „nk2 (r) An (k1 ) „nk1 (r), where k1 and k2 are two equivalent points on opposite surfaces of the Brillouin zone. Because of the periodicity of the Bloch functions An (k)„nk (r), this term vanishes and we obtain (4.6) [4.1]. The ≈ sign in (4.6) is a reminder that this equation is an approximation because the values of k are discrete. The interpretation of (4.6) is as follows: the effect of operating with Rop on any function æ(r) is equivalent to applying the operator (i/k) to the coefficients An (k) of the expansion of æ(r) in terms of Bloch functions. One can show that k and Rop are conjugate operators just like momentum p and r in the sense that R ↔ (i/k) and k ↔ (i/R). (4.11) From now on we will drop the subscript op in Rop and, for simplicity, R will be understood to represent both the lattice vector R and its operator Rop . One should keep in mind that k and R are discrete variables while p and r are truly continuous variables. The correspondences in (4.11) represent approximations which are valid only under the various assumptions discussed above. We will now utilize the result in (4.6) to simplify the Schrödinger equation (4.2). Let us expand the wave function æ(r) in (4.2) as a linear combination of Wannier functions: æ(r) N 1/2 Cn (Ri ) an (r Ri ), (4.12) n, i where n is again the band index and the Cn (Ri ) are coefficients analogous to An (k) in (4.7). Thus the Cn (Ri ) can be regarded as the amplitudes of Wannier functions. We will show later that they are also solutions to a wave equation, so they are known as envelope wave functions. Let the eigenvalues of the unperturbed Hamiltonian H0 (r) in (4.2) be represented as Wn (k). Then (4.11) allows us to convert Wn (k) into an operator on Wannier functions: n, Ri | H0 (r) | n, Rj ↔ ‰nn ‰ij Wn (i/R). (4.13) where | n , Rj denotes the Wannier function an (r Rj ) and the index for R has been dropped, as in (4.11), to simplify the notation. 4.2 Shallow or Hydrogenic Impurities To obtain the operator corresponding to U(r) in (4.2), we will assume that U is a slowly varying function of r, so that the change in U within one lattice constant (a0 ) is small compared with U, i. e. a0 | ∇U(r) | U(r). (4.14) The matrix elements of U between two Wannier functions are given by n, Ri | U(r) | n, Rj a∗n (r Ri ) U(r) an (r Rj ) dr. (4.15) Suppose r lies within the primitive cell indexed by the lattice vector R. Because U is a slowly varying function of r we can expand U about U(R) to just the first order in ∇R U: U(r) U(R) (r R)∇R U(R). (4.16) Substituting (4.16) into (4.15) we obtain n, Ri | U(r) | n, Rj U(R)‰nn ‰ij ∇U(R) a∗n (r Ri )(r R)an (r Rj )dr. (4.17) Using the inequality (4.14), the second term in (4.17) can be neglected compared with the first term, so that (4.17) reduces to n, Ri | U(r) | n, Rj ≈ ‰nn ‰ij U(R). (4.18) Combining (4.13) and (4.18) we obtain n, Ri | H0 U(r) | n, Rj ↔ ‰nn ‰ij [Wn (i/R) U(R)]. (4.19) We should note that while the lattice vectors Ri on the left hand side are discrete, at the right hand side of (4.19) they are treated as continuous variables. To be exact (4.19) should be replaced by a set of difference equations [4.3]. Replacing (4.19) into (4.2) and using (4.12) we arrive at a very useful equation: [Wn (i/R) U(R)]Cn (R) ≈ ECn (R). (4.20) As an illustration of how to apply (4.20) to solve for the energies of a donor electron, we will assume that the lowest conduction band for the semiconductor is isotropic, nondegenerate, and parabolic, with the band minimum located at the zone center. Its energy is thus given by Wn (k) Ec (0) 2 k2 , 2m∗ (4.21) where m∗ is the effective mass of this conduction band and Ec (0) the band edge. Since we consider only one conduction band the band index n will be dropped. We note that both Si and Ge do not satisfy these assumptions since their conduction band minima are degenerate and do not occur at the zone center. However, these assumptions are valid for many semiconductors with 165 166 4. Electronic Properties of Defects the zinc-blende structure, such as GaAs and InP. Substituting the expression for Wn (k) in (4.21) into (4.20) we obtain 2 2m∗ 2 U(R) C(R) ≈ [E Ec (0)]C(R), R2 (4.22) which is equivalent to the Schrödinger equation for a particle with effective mass m∗ moving in a potential U. In other words, the net effect of the crystal potential on the donor electron inside the crystal is to change the electron mass from the value in free space to the effective mass m∗ and also to contribute the factor Â0 in (4.1). As a result this approach is known as the effective mass approximation. We should remember that (4.22) enables only the envelope function C(R) to be calculated. This envelope function has to be multiplied by the Wannier function a(r R) in order to arrive at the final electron wave function æ(r). The effective mass approximation will be used throughout this book in calculating the transport and optical properties of electrons in semiconductors (these topics will be covered in Chaps. 5 and 6, respectively). In order for this approximation to be valid the perturbing potential must be weak (so that no electrons are excited from one band to another) and slowly varying in space (so that R can be regarded as continuous). In the next section we will apply it to calculate the energies and wave functions of shallow donors. 4.2.2 Hydrogenic or Shallow Donors By treating R as a continuous vector in real space rather than as a discrete lattice vector (4.22) can be solved as a differential equation. Equation (4.2) then essentially becomes the Schrödinger equation for a particle moving in a Coulomb potential and the motion of the donor electron becomes equivalent to that of the electron in the hydrogen atom. Donors whose electrons can be described by the solutions of (4.22) are said to be hydrogenic or shallow. The solutions to the Schrödinger equation for the electron in the hydrogen atom are well known. They can be found in many textbooks on quantum mechanics, hence we will not repeat them here. Instead we will state the results. • There are both discrete and continuous eigenvalues. The continuum states of the donor electron are now the delocalized conducting states. Note that in the vicinity of the bandgap these conducting states are not the same as the conduction band states in the absence of the defect potential. Only in the limit that U approaches zero does the donor electron energy E in (4.22) approach the conduction band energy Ec and the wave functions of the donor electron become equal to those of the nearest conduction band electrons. The bound states of the donor electron are classified according to their principal quantum number N, angular momentum L, and spin. In atomic physics these bound states are denoted as 1s, 2s, 2p, etc. Similar 4.2 Shallow or Hydrogenic Impurities notations are used to denote the bound states of shallow impurities. The energies of these bound states are given by the Rydberg series: E Ec (0 ) R/N 2 (N 1, 2, 3, . . .) . (4.23) R is the Rydberg constant for the donor electron and is related to the Rydberg constant for the hydrogen atom [e4 m0 /(22 )] by R • m∗ m0 1 1 e4 m0 , 22 Â20 (4Â0) 2 (4.24) m0 being the free electron mass. A schematic diagram of some of the bound states of a donor atom near a simple parabolic conduction band is shown in Fig. 4.1. The extent of the bound-state electron wave functions in real space is measured in terms of a donor Bohr radius a∗ . It is related to the Bohr radius in the hydrogen atom [2 /(m0 e2 )] by 2 Â0 m0 ∗ a (4.25) (4Â0). m∗ m0 e2 In particular, the wave function of the 1s state is given by 1/2 3/2 1 1 R exp . C1s (R) a∗ a∗ (4.26) In order that R can be considered continuous rather than discrete, we require a∗ a0 . This condition also ensures that it is meaningful to approximate the entire conduction band structure by an effective mass m∗ . The reason is that the extent in R of an envelope function C(R) corresponding to the electron wave function æ(r) scales as a∗ . On the other hand, the extent in k-space of Bloch functions (which are indexed by k) to be summed over in the reciprocal space to construct æ(r) can be small. This is because of an “uncertainty principle” for two variables that are related by Fourier ∞ E Conduction 3S, 3P, 3D 2S, 2P 1S Eg k Valence Fig. 4.1. Schematic diagram of the n1, 2, and 3 bound states of a shallow donor electron near a nondegenerate and parabolic conduction band (corresponding to n ∞). Eg is the bandgap 167 168 4. Electronic Properties of Defects • transformations. For example, if a function f (t) of the time t has an extent ¢t, its Fourier transform g(ˆ) is a function of angular frequency ˆ and has an extent ¢ˆ. Then there is a relation between ¢t and ¢ˆ given by ¢t¢ˆ ≈ 1. Similarly, we expect that ¢k · ¢R ≈ | ¢k |a∗ ≈ 1 or | ¢k | ≤ (1/a∗ ). Hence only conduction band states over a small region of reciprocal space around the band minimum contribute to the defect wave function if a∗ a0 . This justifies the expansion of the conduction band energy in (4.21) to only the quadratic term, which involves the effective mass. We note that while the binding energy of the donor electron decreases as (1/N 2 ), the extent of its wave function increases as N 2 . It is therefore possible for the higher excited states of a donor electron to be well described by the hydrogenic model even if this is not true for its 1s ground state. The relative errors in eigenvalues introduced by using the effective mass approximation are of the order of [a0 /(2a∗ )]2 , where a0 , the lattice constant of the semiconductor, is usually a few angstroms. To obtain an order of magnitude estimate for a∗ and R, let us assume some typical values for Â0 and m∗ in semiconductors, such as Â0 ≈ 10 and m∗ ≈ 0.1m0 . Substituting these values into (4.24) and (4.25) gives an a∗ of about 50 Å and a binding energy of about 14 meV for a donor electron. Since a∗ , as shown by this estimate, is generally much larger than a0 , donor electrons in most semiconductors with conduction band minimum at °, can be described rather well by the effective mass approximation. As pointed out earlier, the function C(R) obtained by solving (4.22) is only the envelope function and not the complete wave function. It has to be multiplied by the Wannier functions to obtain the complete wave function. We shall now consider the donor electron wave function æ(r) in the limit of a very large Bohr radius a∗ . We first express the wave function in terms of Bloch functions. Starting with æ(r) C(Ri )a(r Ri ) (4.27) i we substitute (4.4a) for a(r Ri ) and obtain æ(r) C(Ri )N 1/2 exp(ik · Ri )„k (r). i (4.28) k The Bloch function „k (r) can be expressed in terms of the periodic functions uk (r) using (2.6): „k (r) exp(ik · r)uk (r). (4.29) Substituting (4.29) into (4.28) we arrive at C(Ri )N 1/2 exp[ik · (Ri r)]uk (r). æ(r) i (4.30) k As pointed out earlier, when a∗ is large, the summation over k in (4.30) can be restricted to a small region near the band minimum at the zone center. This allows us to assume the periodic function uk (r) to be independent of k and 4.2 Shallow or Hydrogenic Impurities equal to the function at k 0. Equation (4.30) can therefore be approximated by C(Ri )N 1/2 exp[ik · (Ri r)] æ(r) ≈ u0 (r) i u0 (r) k C(Ri )‰(Ri r) (4.31) i u0 (r)C(r). (4.32) It should be remembered that (4.32) is only an approximate result. However, it provides a very simple picture of the defect wave function. The wave function of a conduction electron is constructed by multiplying u0 , a periodic function, with a plane wave. To construct the donor electron wave function, u0 is multiplied by the envelope function C(r) which is localized around the defect. Figure 4.2 shows a schematic wave function for a donor electron in the 1s state. In Table 4.1 we list the binding energies for the 1s level of donors in several zinc-blende-type semiconductors calculated with (4.23) and (4.24) using the experimentally measured values of m∗ and Â0 . These theoretical binding Ψ(r) C(r) u0(r) –2a –a a 2a r Fig. 4.2. Schematic diagram of a shallow donor electron wave function in real space. u0 (r) is the Bloch function part and C(r) is the envelope function; a is the distance between the lattice sites Table 4.1. Experimental binding energies of the 1s state of shallow donors in some zincblende-type semiconductors (from [Ref. 4.4, p. 224]) compared with the predictions of (4.24) GaAs 5.72 SiGa (5.84); GeGa (5.88) SAs (5.87); SeAs (5.79) InP 7.14 7.14 InSb 0.6 TeSb (0.6) CdTe 11.6 InCd (14); AlCd (14) ZnSe 25.7 AlZn (26.3); GaZn (27.9) FSe (29.3); ClSe (26.9) 169 170 4. Electronic Properties of Defects energies are compared with the experimental values for some of the common donors in each semiconductor. This table shows that the effective mass approximation can predict the shallow donor binding energies rather well. However, there are also a large number of donors whose binding energies do not agree with the prediction of the effective mass theory. For example, Cu in GaAs is a donor with a binding energy of 70 meV. Centers whose binding energy cannot be calculated by the effective mass approximation are referred to as deep centers. They will be discussed in greater detail in the following sections. Given an impurity atom in a host semiconductor, it is not easy to predict whether it will form a shallow or a deep center. The following guidelines have been found to be helpful, although not foolproof. • • If the “core” (the atom minus the outer valence electrons) of the impurity atom resembles the core of the host atom (allowing, of course, for the difference of one nuclear charge), the impurity levels tend to be shallow. For example, consider GeGa in GaAs. The core of the Ge atom is almost identical to the core of the Ga atom, so GeGa is a shallow donor in GaAs. If the impurity atom induces a strongly localized potential, such as a strain field around the impurity atom, the result is most likely a deep center. The part of a defect potential which is localized within one unit cell is known as a central cell correction. Central cell corrections violate the assumption that the defect potential is slowly varying in space in the effective mass approximation and therefore may result in deep centers. In some cases a defect may have both shallow and deep bound states. For example, electrons with s-symmetry envelope wave functions are more likely to behave like deep centers than electrons with p-symmetry envelope functions. The reason is that envelope functions with s-symmetry have nonzero probability densities at the origin (or the defect) and therefore are more sensitive to central cell corrections. The above guidelines are not infallible principles. The problem is that the properties of defects in semiconductors depend on a number of factors, including the charge state of the defect, the band structure, and so on. An illustration of the difficulty in predicting whether an impurity will be shallow or deep is the case of Si in GaAs. While SiGa in GaAs is a perfect example of a hydrogenic donor, Si can also be incorporated as a deep donor known as the DX center, with completely different properties in GaAlAs alloys containing more than about 25 % of Al [4.5] or in pure GaAs under pressure [4.6]. It is now generally accepted that while the lowest electronic levels of SiGa in GaAs are hydrogenic there is an excited deep state which is resonant with the conduction band. Alloying with Al or applying hydrostatic pressure changes the conduction band structure and lowers the resonant deep state into the bandgap. When this deep state becomes lower in energy than the shallow levels a shallow-to-deep instability occurs. It has been suggested [4.7, 8] that this resonant level of Si in GaAs behaves like a deep center because of a large lattice relaxation associated with the impurity. The predicted configuration of this lattice distortion has not yet been confirmed experimentally. However, 4.2 Shallow or Hydrogenic Impurities the theoretical models are now believed to be correct based on the verfications of their other predictions [See Appendix on DX Centers in A4.1 of Appendix C]. 4.2.3 Donors Associated with Anisotropic Conduction Bands Some of the most important semiconductors, such as Si, Ge, GaP, and even diamond, have their lowest conduction band minima near the zone boundaries. In these semiconductors the conduction band effective mass is strongly anisotropic. In addition, the conduction valleys are degenerate as a result of their symmetry. For example, we see in Fig. 2.10 that there are six conduction band minima in Si occurring in the six equivalent [100] directions about 85 % out towards the zone boundary. The impurity central cell corrections produce an interaction between the six degenerate valleys known as the valley–orbit coupling. These complications require a modification of the effective mass appoximation discussed in the last section. We will consider the donors in Si as an example but the technique can also be applied to donors in Ge with slight modifications. Let us first neglect the valley–orbit coupling between the six equivalent conduction band valleys. The electron effective mass for each valley in Si can be written as a second-rank tensor ml 0 0 0 mt 0 , 0 0 mt where ml and mt are, respectively, the effective masses longitudinal and transverse to the [100] axis (these masses have to be permuted when considering the equivalent [010] and [001] directions). For Si the masses have been determined by means of cyclotron resonance experiments to be 0.916m0 and 0.190m0 , respectively. With this effective mass tensor the wave equation (4.22) for the envelope wave function ºj (R) (where the integer j now labels the valley along the [100] axis) becomes 2 2∇ 2t ∇ 2l | e |VS ºj (R) ≈ [E Ec (k0 )]ºj (R), (4.33) 2 mt ml where ∇t and ∇l are, respectively, the components of the operator ∇ projected along directions transverse and longitudinal to the [100] axis and k0 is the location of the conduction band minimum along the [100] axis in reciprocal lattice space. Equation (4.33) can be regarded as the wave equation for an “elliptically deformed hydrogen atom”. If ml is not too different from mt , the solutions of this equation should be quite similar to those of the hydrogen atom and we can still label its eigenstates as 1S, 2S, and 2P, etc. However, the lowering of the symmetry from spherical to cylindrical inherent in (4.33) means that states with the same principal quantum number N and angular momentum L but different magnetic quantum numbers m are no longer degenerate. It can be shown (for example, with time reversal symmetry arguments) 171 4. Electronic Properties of Defects that states with equal and opposite values of m remain degenerate. For example, 2P1 and 2P1 are still degenerate but will have a different energy than 2P0 . If ml is much larger than mt , (4.33) can be solved by using an adiabatic approximation to separate the longitudinal motion from the transverse one. More generally, (4.33) can be solved approximately by a variational technique. Kohn and Luttinger [4.9] solved (4.33) by using trial functions of the form º(x, y, z) exp[a(y2 z2 ) bx2 ]1/2 , (4.34) where the parameters a and b are varied to minimize the energy and the x axis is chosen along the direction ([100] in the present case) of the valley. The results of a variational calculation performed by Faulkner [4.10] for several donors in Si are compared with the experimental results in Fig. 4.3. We see that the agreement between Faulkner’s calculation and experiment is very good for the excited states but rather poor for the 1S ground state. This is expected since the excited states have larger orbits and are therefore less sensitive to central cell corrections. The theoretical 1S ground state energy can be greatly improved by including the valley–orbit coupling. For simplicity, we shall treat the valley–orbit coupling among the 1S ground states of the six equivalent [100] valleys by perturbation theory and neglect their mixing with the excited states. As unperturbed wave functions, we construct six approximate wave functions similar to the donor wave function in (4.32): xj (r) ºj (r)„j (r), (4.35) Li Theory 0.0 –10.0 Energy [meV] 172 5F+ 4F+ - - 6P0 4F0 4P0 4P+3P0 5P 0 5P+- As P Sb Bi S 6P+- 6H 0 5F+3P+ 6F0 2P+ - 2P0 –20.0 –30.0 1S A1 E+T 2 E T2 E T2 E >T2 –40.0 A1 A1 –50.0 A1 Fig. 4.3. Calculated and measured shallow donor energy levels in Si. (From [4.10]) 4.2 Shallow or Hydrogenic Impurities where „j (r) is the Bloch function for the jth (j 1, . . . , 6) conduction band minimum and ºj (r) the corresponding envelope function obtained by solving (4.33). For convenience, the six Bloch wave functions „j (r) are labeled X, X, Y, Y, Z and Z according to the direction of the corresponding conduction band minimum. If we assume that the donor in Si is substitutional (such as AsSi ), the impurity potential has tetrahedral symmetry. The diagonalization of the perturbation Hamiltonian is simplified by symmetrizing the six functions according to the irreducible representations of the Td group. Using the character table for the Td group (Table 2.3) it can be shown (Problem 4.1) that these six Bloch functions form a singlet with A1 symmetry, one doublet with E symmetry, and a triplet with T2 symmetry. Since the impurity potential has only rotational and no translational symmetry, it is customary to use the point group notations for the symmetrized defect wave functions. The appropriate linear combinations are √ A1 : (X X Y Y Z Z) 6; (4.36a) √ (4.36b) E: (X X Y Y) 2, (2Z 2Z X X Y Y) 12; √ √ √ (4.36c) T2 : (X X) 2, (Y Y) 2, (Z Z) 2. In Fig. 4.3 we notice that the totally symmetric A1 state is usually found experimentally to have the lowest energy. A plausible explanation is that the impurity potential is attractive and the A1 state, like the s states in the hydrogen atom, has the highest probability of being near the origin, where attractive central cell corrections are generated. In addition, different donor species exhibit rather large chemical shifts in their ground state energies. This is because the impurity potential is usually not purely Coulombic near the core. There are corrections due to exchange and correlation effects between the donor electron and the core electrons. In addition, the screening of the Coulomb potential (via the dielectric constant Â0 ) is reduced near the core. It is difficult to calculate these corrections from first principles. Once a realistic potential has been determined, the Hamiltonian for the envelope wave function can be diagonalized by numerical methods. Table 4.2 compares the experimental valley– orbit split energy levels for donors in Si with theoretical values computed by Pantelides and Sah [4.11]. The agreement between theory and experiment is very good for P and As but not so satisfactory for Sb. Table 4.2. Experimental substitutional donor binding energies [meV] in Si compared with values computed numerically by solving the effective mass equation including valley–orbit interaction (from [4.11]) A1 E T2 44.3 30.5 31.3 45.5 32.6 33.9 53.1 29.6 29.8 53.7 31.2 32.6 31.7 28.5 27.8 42.7 30.5 32.9 173 174 4. Electronic Properties of Defects 4.2.4 Acceptor Levels in Diamond- and Zinc-Blende-Type Semiconductors The calculation of acceptor binding energies in tetrahedrally coordinated semiconductors presents a special challenge due to two factors. First, the valence bands are degenerate at the Brillouin zone center, and second, as a result of the degeneracy, the valence bands are warped (Sect. 2.6.2). Hence, it is not possible to define a simple effective mass tensor for the valence bands. Several different approaches to solving the acceptor problem have appeared in the literature. Invariably they all involve numerical solutions of a wave equation for the envelope functions. Here we present a derivation of these wave equations without solving them. The purpose is to obtain some insight into the problem without going into the details of the numerical solutions. We will also try to simplify the calculation as much as possible. We start by assuming that the spin–orbit coupling is much larger than the acceptor binding energies so that only the heavy- and light-hole bands need to be considered. The wave equation for the four resultant envelope functions ºi (r) (i 1, . . . , 4) can be cast in the form [4.2] ·‚ e2 Dij ºj (4.37) ºi Eºi . 4Â0Â0 r x· x‚ j ·‚ ·‚ Dij (/x· ) (/x‚ ) is the 4×4 matrix operator obtained from the 4×4 matrix {Hij } in Sect. 2.6.2 by using (4.11) to convert k into (/r). In the absence of the Coulomb potential term, the solutions of (4.37) are four-fold degenerate (symmetry: °8 in zinc-blende structure and °8 in diamond structure). One could also have included in (4.37) the doubly degenerate, spin-orbit split bands (symmetries: °7 in zinc-blende structure and °7 in diamond structure) but except in the case of Si [4.12], their effect on acceptor levels is very small. The spin degeneracy is not lifted by the Coulomb potential so the solutions of (4.37) should remain at least doubly degenerate. The approach adopted by Kohn and Schechter [4.13] was to expand ºi (r) in terms of radial wave functions and spherical harmonics as in the case of the hydrogen atom. For simplicity the expansion was truncated at an angular momentum (l) less than some value l0 , and then a variational technique was used to solve (4.37). With this approach Kohn and Schechter [4.13] obtained a value of 8.9 meV for the ground state acceptor binding energy in Ge as compared to an experimental value of between 10.2 to 11.2 meV. The disadvantage of this technique lies in the difficulty of improving its accuracy. More recently, Baldereschi and Lipari [4.14, 15] have developed a different and more systematic approach to solving this problem. Their starting point is the Luttinger Hamiltonian in (2.70). This Hamiltonian has been constructed to reflect the cubic symmetry of the crystal. Noting that deviations from spherical symmetry in the warped heavy and light hole bands are small in most semiconductors, Baldereschi and Lipari rewrote the Luttinger Hamiltonian using spherical tensors instead of Cartesian tensors. The idea is that all the symmetry operations of a spherically symmetric potential form a group known 4.2 Shallow or Hydrogenic Impurities as the full rotational group. The spherical harmonic functions form a complete orthonormal set of basis functions for the irreducible representations of this group. Symmetrizing the Luttinger Hamiltonian with spherical tensors is, therefore, the systematic way to decompose the Luttinger Hamiltonian into terms with spherical and cubic symmetries. The process involved is left as an exercise in Problems 4.2 and 4.3. The resultant “spherically symmetrized” Luttinger Hamiltonian obtained by Baldereschi and Lipari (HBL ) is given by (4) Á1 p2 3Á3 2Á2 (2) (2) Á3 Á2 (2) HBL ·J × J (2) 4 2m0 45m0 18m0 √ (4) (4) 70 (2) (4.38) × J (2) 0 (2) × J (2) 4 , 5 where (2) and J (2) are second-order spherical tensors. Their definitions plus (4) those of the tensor products (2) · J (2) and [(2) × J (2) ]i can be found in Problems 4.2 and 4.3. Note that both the first and second terms in (4.38) are spherically symmetric. Only the third term proportional to (Á3 Á2 ) has lower, cubic symmetry and gives rise to warping of the valence bands. In most diamond- and zinc-blende-type semiconductors the spherical terms are much larger than the cubic one. This can be seen in Table 4.3, where the values of Á1 , Á2 , and Á3 for a number of tetrahedrally bonded semiconductors are listed. As a result, the Table 4.3. Values of the dimensionless valence band parameters Á1 , Á2 , Á3 , Ì and ‰ for various semiconductors with the diamond and zinc-blende structures. Although most of these values have been reproduced from [4.14] many of the values in this reference have been changed to the most recent valuesa,b . In addition, the values of these parameters now agree with those computed from the parameters A, B and C in Table 2.4 using (2.71a) to (2.71c) C Si Ge SiCc GaNd GaP GaAs GaSb InP InAs InSb ZnS ZnSe ZnTe CdTe a b c Á1 Á2 Á3 Ì ‰ 2.5 4.28 13.38 2.8 5.05 4.05 6.9 13.3 5.15 20.4 36.41 2.54 2.75 3.8 4.14 –0.1 0.339 4.24 0.51 0.59 0.49 2.2 4.4 0.95 8.3 16.24 0.75 0.5 0.72 1.09 0.63 1.446 5.69 0.67 1.78 1.25 2.9 5.7 1.62 9.1 17.34 1.09 0.27 0.47 0.766 0.433 0.52 0.47 0.75 0.8 0.523 0.861 0.928 0.751 0.29 0.26 0.11 0.488 0.24 0.19 0.1 0.1 0.13 0.039 0.03 0.134 1.3 1.62 0.562 0.68 0.153 0.128 Refer to Landolt-Börnstein Tables Vol. 22a. (Springer, Berlin Heidelberg 1987) H. Mayer and U. Rössler: Solid State Commun. 87, 81 (1993) and d Values for the zinc-blende structure. 175 176 4. Electronic Properties of Defects cubic term can be neglected in the first-order approximation and the heavy and light hole bands treated as spherical. To calculate the acceptor binding energy, it is more convenient to simplify first the acceptor Hamiltonian: H HBL | e |2 4Â0 Â0 r (4.39) by • defining two new parameters Ì 2(3Á3 2Á2 )/5Á1 (4.40) and ‰ (Á3 Á2 )/Á1 , • (4.41) where Ì is a measure of the magnitude of the second spherical term in (4.38) while ‰ is proportional to the coefficient of the cubic term, and introducing effective atomic units in which both the effective Bohr radius: Â0 2 Á1 · 4Â0 (4.42) a∗ m0 e2 and the effective Rydberg: e4 m0 1 R 2 2 · (4.43) 2 Â0 Á1 (4Â0 )2 are set equal to unity [this implies e2 2Â0 , 2 2m0 /Á1 ]. With these simplifications, (4.39) becomes (4) Ì 2 ‰ p2 H 2 2 ((2) · J (2) ) 2 (2) × J (2) 4 r 9 9 (2) 70 (2) (2) (4) (2) (4) ×J 0 ×J 4 . 5 (4.44) Except for the last term, which is proportional to ‰, this Hamiltonian has full rotational symmetry. Hence it is important to compare the values of Ì and ‰ for various semiconductors, shown in Table 4.3. We see that, with the exception of Si, SiC and GaN, the spherical parameter Ì is at least four times larger than the cubic parameter ‰. We shall not attempt to diagonalize (4.44) since it is quite complicated, as one may expect. Instead we shall discuss the qualitative features of the solutions. We shall begin with the simplest case by neglecting most of the terms in (4.44). Then we shall introduce one additional term at a time and examine the consequence of each term using perturbation theory. a) “One Spherical Band Approximation” The simplest approximation of (4.44) one can make is to set the terms depending on Ì and ‰ both equal to zero: 4.2 Shallow or Hydrogenic Impurities H p2 2 . 2 r (4.45) Within this approximation the heavy and light hole masses are equal (hence, they are treated as one band). Equation (4.45) becomes analogous to the hydrogenic donor, therefore its solutions are characterized by a principal quantum number N and an angular momentum L. The bound states will be labeled nS, nP, etc. and their energies are given by the Rydberg series (4.23), except that the Rydberg constant (4.24) is now defined by (4.43). b) “Spherical Approximation” Next, the term (2) · J (2) is added as a perturbation to (4.45): H p2 2 Ì 2 (2) · J (2) . 2 r 9 (4.46) The Hamiltonian still has spherical symmetry but now the heavy and light hole bands have different masses (Problem 4.3). The term (2) · J (2) resembles the spin–orbit interaction if we note that the “pseudo-angular momentum” J plays the role of spin except that J 3/2. Using this similarity, a “pseudototal angular momentum” F L J can be defined. F is conserved just as the total angular momentum LS would be conserved if spin–orbit coupling were included (except that now J is the pseudo-angular momentum of the Bloch function while L represents the angular momentum of the impurity envelope function). As in atomic physics, the bound states of the acceptor can be labeled with the spectroscopic notation L 0 : nS3/2 ; L 1 : nP5/2 , nP3/2 , and L 2, and so on. nP1/2 ; In general, only terms with L 2 are significant. Notice that there is only one 1S acceptor state. If we had made the assumption that the heavy and light hole bands can be treated as two separate spherical bands we would, instead, incorrectly obtain two 1S acceptor states. In spite of the analogy with the spin–orbit coupling, the (2) · J (2) term is not trivial to treat by perturbation theory because of the degeneracy of the heavy and light holes. Since (2) and J (2) are second-order spherical tensors, the selection rules for the matrix elements of (2) · J (2) are ¢F 0 and ¢L 0 or ±2. For simplicity we will consider only these lowest energy states: 1S3/2 , 2S3/2 , 2P5/2 , 2P3/2 , and 2P1/2 . Except for the 2P1/2 state, these states are coupled to higher energy levels by the (2) · J (2) term. Baldereschi and Lipari [4.14] assumed that each of these states is coupled with no more than one other state. In this approximation, the envelope wave functions consist of linear combinations of at most two functions: º(S3/2 ) f0 (r) | L 0, J 3/2, F 3/2, Fz g0 (r) | L 2, J 3/2, F 3/2, Fz ; (4.47a) 177 178 4. Electronic Properties of Defects º(P1/2 ) f1 (r) | L 1, J 3/2, F 1/2, Fz ; (4.47b) º(P3/2 ) f2 (r) | L 1, J 3/2, F 3/2, Fz g2 (r) | L 3, J 3/2, F 3/2, Fz ; (4.47c) º(P5/2 ) f3 (r) | L 1, J 3/2, F 5/2, Fz g3 (r) | L 3, J 3/2, F 5/2, Fz . (4.47d) Except for º(P1/2 ), substituting these wave functions into (4.46) produces two coupled differential equations for the radial functions fi and gi . These differential equations can be solved only approximately by numerical methods. However, the energy of the 2P1/2 state can be calculated exactly because its radial wave equation is similar to that of the p state in the hydrogen atom. Its eigenvalue can be shown to be equal to [4(1 Ì)]1 . Noting that the effective mass of the light hole is given by (1 Ì)1 (Problem 4.4), we see that the energy of the 2P1/2 state is equal to that of the n 2 level of a hydrogenic acceptor with the light hole mass. The energies of the other three states have been calculated by Baldereschi and Lipari [4.14] using variational techniques and the values of the Kohn– Luttinger parameters listed in Table 4.3. Their results are shown in Table 4.4. Note that the values of some of the Kohn–Luttinger parameters have since been revised. The theoretical acceptor energy levels are compared with the experimental values available at the time of the calculation. The agreement between the experimental and theoretical ground state energies of acceptors is quite good for most diamond- and zinc-blende-type semiconductors. The notable exceptions are Si, GaP, InP, and some II–VI semiconductors. As pointed out earlier, the spherical model is not expected to work well for Si because it has a relatively large cubic term (‰/Ì ≈ 0.5, see Table 4.3). The experimental acceptor value quoted by Baldereschi and Lipari [4.14] Table 4.4. Comparison between the values of the lowest-energy bound states of acceptors for various semiconductors with the diamond or zinc-blende structures calculated by Baldereschi and Lipari [4.14, 16, 17] using (4.47) with available experimental values (values in italics represent measurements after 1973). All energies are in meV Experiment Si Ge GaP GaAs GaSb InP InAs InSb ZnS ZnSe ZnTe CdTe 45, 68.9 10.8 57–64 31 13–15 31, 56.3 10–20 ≈10 114 ≈30 ≈30 1S3/2 2S3/2 2P 1/2 2P 3/2 2P 5/2 31.6 9.8 47.5 25.6 12.5 35.2 16.6 8.6 175.6 110.1 77.7 87.4 8.6 2.9 13.7 7.6 3.8 10.5 5.1 2.7 52 33 23 26.5 4.2 0.6 4.2 1.6 0.65 2 0.4 0.2 11.7 6.1 5.1 3.7 11.2 4.2 19.1 11.1 5.6 15.5 7.9 4.2 75.1 48.6 33.4 39.9 7.6 2.5 11.7 6.5 3.2 8.9 4.4 2.3 44.1 28 19.6 22.6 4.2 Shallow or Hydrogenic Impurities was for AlSi . The more recent experimental value for BSi , 45 meV, is in better agreement with the theoretical predictions. In the case of GaP and InP the experimental values quoted were for ZnGa and CdIn , respectively. More recent values for the binding energies of MgGa and BeGa in GaP are 56.6 and 59.9 meV, respectively. The corresponding energies for MgIn and BeIn in InP are both 31 meV. These latest experimental values are in much better agreement with theory. The acceptors in ZnTe and CdTe, for which binding energies have become available recently, correspond to Li substituting for the cations. The understanding of impurities in these II–VI semiconductors is still relatively poor, in part due to inaccuracies in our knowledge of the Luttinger parameters. Lately, there has been much interest in shallow impurities in the larger bandgap II–VI semiconductors because of their use in blue and green lasers [4.18, 19]. This should lead to more precise determinations of acceptor binding energies. c) Including the Cubic Term When the cubic term is included, the wave functions have to be classified according to the irreducible representations of Td . For example, an acceptor wave function formed from a J 3/2 valence band with °8 symmetry (double group notation) and an envelope function with S symmetry in the spherical model (or °1 symmetry in Td ) has °8 symmetry (the direct product of °8 and °1 ). Similarly, if the envelope function has P symmetry (or °4 ), the symmetries of the acceptor wave functions will belong to the representations °8 ⊗ °4 °6 ⊕ °7 ⊕ 2°8 . It is easily shown that the doubly degenerate P1/2 state will become the °6 state while the four-fold degenerate P3/2 state becomes °8 in the case of Si and Ge. The six-fold degenerate P5/2 state is reducible into a doubly degenerate °7 level plus a four-fold degenerate °8 level. From these symmetry considerations one concludes that the cubic term can • • only shift the energies of the S3/2 , P1/2 , and P3/2 levels and split the degeneracy of the P5/2 level. Thus the S3/2 , P1/2 , and P3/2 levels are not affected by the cubic term to first order in ‰. When higher order terms in ‰ are included, the selection rules for the cubic term are ¢Fz 0 and ±4 (the result of multiplying two secondorder spherical tensors in the cubic term is a tensor of fourth order; see Problem 4.3). These selection rules greatly restrict the levels which can be coupled via the cubic term. As a result, the 1S3/2 , 2S3/2 , and 2P1/2 levels are basically unchanged by the cubic term. In summary, the “spherical model” in which the cubic term is neglected should be as good an approximation as models including the cubic term for calculating the lower energy levels of acceptors in tetrahedrally coordinated semiconductors. The cubic term shifts the P3/2 levels mainly by coupling them with the nearby P5/2 levels. The corresponding shift in energy is typically less than 10 %. For example, in Si, where the largest shift is expected to occur, the cubic term changes the 2P3/2 level energy from 11.2 meV to 12.13 meV. The values 179 180 4. Electronic Properties of Defects of the 2P5/2 (°7 ) and 2P5/2 (°8 ) levels calculated numerically by Baldereschi and Lipari [4.15] by including the cubic term are listed in Table 4.5. The measured excited-state energies of some common acceptors in Si and Ge are compared with the values calculated by Baldereschi and Lipari in Fig. 4.4. The agreement between theory and experiment is excellent for Ge but only fair for Si. The agreement is especially poor for the 1°8 ground state in Si. The calculated binding energy in Si is 44.4 meV while the experimental values vary from 45 meV for boron to 160 meV for indium. These discrepancies can be attributed, at least in part, to central cell corrections which become more important in Si. However, the calculation based on a 4 × 4 Luttinger Hamiltonian should break down when the calculated binding energy is larger than ¢0 . In this case, the full 6 × 6 Hamiltonian, including the °7 bands splitoff by ¢0 , must be solved [4.20]. It turns out that the spin–orbit splitting of the ground state of the acceptor levels can be much smaller than ¢ [4.20, 21]. Table 4.5. Comparison between the theoretical values of the 2P5/2 bound states of acceptors calculated with and without the cubic term for various semiconductors with diamond and zinc-blende structures by Baldereschi and Lipari [4.14, 15]. All energies are in meV “Spherical model” Si Ge GaP GaAs GaSb InP InAs InSb ZnS ZnSe ZnTe CdTe “Including cubic term” 2P 5/2 2P 5/2 (°8 , 7.6 2.5 11.7 6.5 3.2 8.9 4.4 2.3 44.1 28 19.6 22.6 8.51 2.71 13.04 7.2 3.59 9.98 4.76 2.54 49.56 31.47 22.32 25.85 °8 ) 2P 5/2 (°7 , °7) 5.86 2.04 9.42 5.33 2.61 7.32 3.63 1.91 35.57 22.68 15.36 17.68 4.3 Deep Centers We have shown in the last section that one characteristic of shallow impurity levels is that their electron wave functions typically extend over many primitive unit cells. As a result, those wave functions can be constructed from one Bloch function indexed by a single wave vector equal to that of the nearest band extremum, see (4.32). Deep centers, on the other hand, have localized wave functions which involve Bloch functions from several bands and over a large region of k-space. Thus, defects with highly localized potentials are expected to form deep centers. Such localized potentials can be caused by broken bonds, strain associated 4.3 Deep Centers 16 1Γ 8– 14 Ge Si 12 2Γ 8– 10 1Γ 8– 4 8 3Γ 8– 3 2 1 1Γ 7– 1Γ 6– 4Γ 8– 5Γ 8– 2Γ 6– 6Γ 8– 2Γ 8– 1Γ 7– 3Γ 8– 4Γ 8–– 5Γ 8 Theory B Al Valence band Ga In Eb [meV] Eb [meV] 5 6 4 2 Theory B Al Ga In Valence band Fig. 4.4. Theoretical values of shallow acceptor energies in Si and Ge calculated with the Baldereschi and Lipari Hamiltonian [4.14] compared with experimental values. (From [4.22]) with displacement of atoms, and difference in electronegativity or core potentials between the impurity and host atoms. The localized nature of deep center potentials suggests that a tight-binding molecular orbital approach should be a better starting point for studying their electronic energies. Since a defect is imbedded in a semiconductor, it is necessary to consider also the interaction between the localized defect electrons and the Bloch electrons of the host. For example, when a deep center energy level (or deep level for short) overlaps with band states of the host, it becomes a resonant state. To calculate the energies of deep levels one needs to know the defect potential and then find a way to solve the corresponding Schrödinger equation. It is very difficult to deduce the defect potential for deep centers because displacements of atoms (or lattice relaxation) can occur. Both the impurity atom and atoms surrounding it can be involved in the relaxation. The reason why lattice displacements are important in deep centers can be qualitatively seen from the following examples. Suppose an impurity atom in a semiconductor has a choice of becoming either a shallow donor on a substitutional site or a deep level via a lattice distortion. Let us assume that, as a deep level, it is located deep in the bandgap at an energy E0 (known as its thermal ionization energy) below the conduction band. On the other hand, as a shallow donor its energy will be near the conduction band edge. Thus the impurity atom can lower its electronic energy (by about E0 ) by becoming a deep center. However, it may require a lattice relaxation energy Ed to produce the lattice distortion. If E0 is larger than Ed it is energetically favorable for the impurity atom to distort spontaneously and become a deep center. It is 181 182 4. Electronic Properties of Defects necessary to know both E0 and Ed in order to predict whether this impurity will be deep or shallow. Lattice displacements are responsible for the shallow-to-deep instability which converts shallow donors in GaAs to the DX center in AlGaAs alloy [4.7, 8]. In the case of the DX centers, E0 is on the order of 0.4 eV for Si in an AlGaAs [4.23]. Actually, the electronic energy gained by DX centers via their lattice displacements is equal to 2E0 because of their peculiar property known as negative U. For further details on the DX center and on their negative properties, see the following Web Page: http://Pauline.berkeley.edu/textbook/DXCenter.pdf. Here U stands for the on-site repulsive Coulomb interaction between two electrons in the so-called Hubbard model [4.24]. For a deep center with a negative U, a second electron will actually be attracted to it even though it is occupied by one electron already as a result of lattice distortions. The resultant negatively charged state will be more stable than the neutral state. This negative U property makes it energetically even more favorable for a defect to undergo lattice relaxation and become a deep center. It has been known for some time that some large bandgap II–VI semiconductors, such as ZnS and ZnSe, cannot be doped p-type easily while others, such as ZnTe, cannot be doped n-type. This phenomenon is known as self-compensation [Ref. 4.4, p. 238]. While it is still not completely understood, recently it has been suggested that DX center formation by substitutional donors can explain why ZnTe cannot be doped n-type by common group III dopants like Al and Ga [4.25]. As another example of lattice relaxation in deep centers we consider a vacancy in a group-IV semiconductor. The removal of an atom results in a loss of four electrons in this case. This is equivalent to adding four positive charges to the otherwise neutral semiconductor. Obviously the electrons inside the semiconductor will respond by screening these positive charges. The response of the semiconductor is best understood in terms of a tight-binding model. A vacancy in a covalent semiconductor produces four unpaired dangling bonds as shown schematically in Fig. 4.5a. The four dangling bonds can (a) (b) Dangling bonds Vacancy Fig. 4.5. Schematic diagram of a covalent semiconductor with (a) an unrelaxed vacancy involving four dangling bonds and (b) a relaxed vacancy with no dangling bonds 4.3 Deep Centers be “healed” by forming two pairs of bonds among neighboring dangling bonds. Since originally the distances between atoms with dangling bonds are larger than the bond lengths in the perfect crystal, atoms with dangling bonds have to move closer to each other in order to form new bonds, as shown in Fig. 4.5b. This displacement of neighboring atoms involves an elastic energy, which is compensated for by the lowering of the energy of the four electrons originally in the dangling bonds. Since each new bond can accommodate two electrons in the bonding state, the decrease in the energy of each electron in the dangling bond is of the order of the overlap parameters (Vss , Vpp , and Vsp ) discussed in Sect. 2.7.1. We will consider in more detail the electronic energy of a vacancy in diamond- and zinc-blende-type semiconductors in Sect. 4.3.2. 4.3.1 Green’s Function Method for Calculating Defect Energy Levels In this book we will avoid the difficult problem of determining deep center potentials. Instead we will study one method to solve for the deep center energies if the potential is known. There are now first-principles techniques for calculating deep center energies including lattice relaxation [4.7, 8], but these techniques are beyond the scope of this book. The method we will consider here is the Green’s function approach to calculating the electronic structure of deep centers. Many books have been written on Green’s functions. Discussions of their applications to the defect problem can be found in those by Economou [4.26] and Lannoo and Bourgoin [4.27]. We will apply this technique to study the systematics of defects, especially isoelectronic centers, in diamond- and zinc-blende-type semiconductors. To understand the motivation for using Green’s functions to study defects we will first introduce the concept of density of states (to be abbreviated as DOS). The DOS of a system is defined as the number of allowed states per unit energy lying in the energy range between E and E ‰E. Suppose a particular system under study is described by a Hamiltonian H and its energy levels are denoted by Ek . These energy levels can be discrete or continuous. The particles in the system may be arranged periodically in space like atoms in a crystal, or be completely random as in an amorphous solid. The DOS of this system, n(E), is equal to n(E) ‰(E Ek ) (4.48) k where ‰(x) represents the Dirac delta function, [4.28] and k labels all possible states. n(E) is an important quantity because it can be calculated theoretically and can also be measured experimentally. Next we will define the resolvent or Green’s function operator G as G Lim (E H iË)1 . Ë→0 (4.49) 183 184 4. Electronic Properties of Defects To understand the reason for defining G this way, we note that the expectation value of G for an eigenstate | k of H is given by k | G | k Lim (E Ek iË)1 . (4.50) Ë→0 Using a well-known property of the delta function, the right hand side of (4.50) can be rewritten as Lim (E Ek iË)1 (E Ek )1 i‰(E Ek ), (4.51) Ë→0 where [E Ek ]1 , known as the Cauchy principal value of [E Ek ]1 , is defined by ∞ ∞ f (E ) 1 f (E )[E E ] dE dE E E ∞ ∞⎛ ⎞ EÂ ∞ f (E ) f (E ) Lim⎝ dE dE⎠. (4.52a) Â→0 E E E E ∞ EÂ 1 In some sense we can regard the function [x] 0 when x 0, 1 [x] x1 when x 0. as having the property From (4.48) and (4.51) we obtain 1 1 n(E) Im k | G | k Im TrG , (4.52b) (4.53) k where Im{A} stands for the imaginary component of a complex quantity A, and Tr{G} respresents the trace of the matrix k | G | k . Thus (4.53) establishes the relation between the operator G and n(E). We should note that the matrix element of G defined in (4.50) is a complex function of E. Its real part is always related to its imaginary part in a particular way. For example, let us denote k | G | k by g(E Ek ) [see (4.50)] and define ∞ F(E) g(E E ) f (E )dE, (4.54) ∞ where f (x) is any given function. Substituting (4.50) into (4.54) we obtain ⎛ ∞ ⎞ f (E ) dE⎠ if (E). (4.55) F(E) ⎝ E E ∞ Noting that Im{F } f (E) in (4.55), the real part of F(E) can be rewritten as ∞ Re{F(E)} 1 ∞ Im{F(E )} dE . E E (4.56) 4.3 Deep Centers This equation expressing the real part of the function F(E) in terms of its imaginary part is one of two equations known as the Kramers–Kronig relations or the dispersion relations. It is also called a Hilbert transform. In Chap. 6 we will utilize these important relations extensively in studying the linear optical response function (which will be defined in Chap. 6). Obviously the function g(E Ek ) satisfies the Kramers–Kronig relations. Another expression for n(E) which is useful for defect problems is n(E) 1 d Im log det G dE (4.57) where det G represents the determinant of the matrix k | G | k . Let us express the Schrödinger equation for the defect electron as: (H0 V)º Eº, (4.58) where H0 is the Hamiltonian of the perfect crystal, V is the defect potential, and E is the defect energy. As mention before, we will assume that V is known. Furthermore, we will assume that the wave functions º0 and eigenvalues E0 of the “unperturbed” equation (E0 H0 )º0 0. (4.59) are known. Equation (4.58) can be rewritten as º [E H0 ]1 Vº. (4.60) We will now define the “unperturbed” Green’s Function operator G0 using (4.49): G0 Lim [E H0 iË]1 , Ë→0 (4.61) so that º can be expressed as º G0 Vº (4.62) One should remember that G0 is a function of the defect energy E. There are two possible types of solutions for (4.58). a) Bound State Solutions If the defect electron energy E does not overlap with the eigenvalues E0 of the unperturbed wave equation, that the eigenstate º of the defect electron has to be a bound state. Since E does not overlap with E0 no extended state can exist at this energy. The defect electron wave function has to be localized around the defect. To determine E we can expand in terms of an orthonormal set of basis functions „j : 185 186 4. Electronic Properties of Defects º aj „ j . (4.63) j Substituting this expression into (4.62) we obtain a system of homogeneous linear equations in the unknown aj ’s: (4.64) (I G0 V)ij aj 0, i 1, 2, . . . , j where I is the unit matrix; (4.64) has nonvanishing solutions only if its determinant is zero. The defect energies E can thus be obtained, in principle, by solving the equation det[I G0 V] | I (E H0 )1 V | 0. (4.65) For a general potential V (4.65) is very complicated and difficult to solve. For point defects the potential V is localized and (4.65) can be simplified by choosing a suitable set of localized basis functions „j such that there will be only a small number of nonzero matrix elements Vij . Applications of this approach will be studied in Sect. 4.3.2. b) Resonant State Solutions In the second case, the defect energy overlaps with the eigenvalues of the unperturbed states and a resonant state is formed. For E E0 the general solution º can be expressed as: º º0 G0 Vº (4.66) The defect will modify the DOS n0 (E) of the unperturbed state. Our goal will be to calculate ‰n(E), the modification in n(E) caused by the defect. For a highly localized defect potential it will be useful to define a local density of states since we expect ‰(E) to be significant only in the vicinity of the defect. We will first introduce a matrix element of the operator G0 defined by r | k k | r (E Ek iË)1 . (4.67) G0 (r, r , E) r | G0 | r Lim Ë→0 k Using (4.51) we can show that r | k2 ‰(E Ek ). Im G0 (r, r, E) (4.68) k Now | r | k |2 equals the probability of finding an electron with wavevector k at the point r while ‰(E Ek ) is the DOS in the absence of defects [i.e., n0 (E)]. When these two terms are multiplied together, the resultant term r | k2 ‰(E Ek ) n0 (r, E) (4.69) k 4.3 Deep Centers has the meaning of an unperturbed local DOS. With the use of (4.68) n0 (r, E) can be related to G0 by n0 (r, E) (1/)Im{G0 (r, r, E)}. The total density of unperturbed states n0 (E) is given by 1 1 n0 (r, E) Im G0 (r, r, E) Im Tr G0 . n0 (E) r r (4.70) (4.71) The local density of states n(r, E) in the presence of a defect can similarly be defined as 1 n(r, E) Im G(r, r, E) , (4.72) r where G(r, r , E) is given by r | k k | r (E H0 V iË)1 . G(r, r , E) Lim Ë→0 (4.73) k For computational purposes it is more convenient to use (4.57) to define n0 (r, E) and n(r, E) so that the change in the local DOS induced by a defect can be expressed as ‰n(r, E) n(r, E) n0 (r, E) det G(r, r, E) 1 d Im log . dE det G0 (r, r, E) (4.74) Equation (4.74) can be simplified by expressing G in terms of G0 : G Lim(E H0 V iË)1 Lim(E H0 iË)1 1 V(E H0 V iË)1 G0 G0 VG. (4.75) In the above equations it is understood that Lim stands for the limit Ë → 0. Equation (4.75) is known as the Dyson equation. Using this equation G can be expressed as G (1 G0 V)1 G0 and det G as det G det (I G0 V)1 det G0 . (4.76) Substituting (4.76) for det[G] into (4.74) we obtain an expression for ‰n(r, E) in terms of G0 and V only: ! 1 d Im log(det[I G0 (r, r, E)V]) . (4.77) ‰n(r, E) dE Thus, for both bound state and resonant state solutions, the change in the electron density of states induced by a defect potential V is determined by det[I G0 V]. 187 188 4. Electronic Properties of Defects 4.3.2 An Application of the Green’s Function Method: Linear Combination of Atomic Orbitals We shall now apply the Green’s function method to calculate the bound state energies of a deep center. Linear combinations of atomic orbitals will be used as the basis functions „j . They are assumed to be given by the Löwdin orbitals ˇms (r rjs ) introduced in Sect. 2.7.2. In diamond- and zinc-blende-type semiconductors they can be further restricted to include only the four sp3 orbitals. For illustration purposes we shall consider only one type of orbital (say an s-symmetry orbital) from each atom at the lattice vectors rjs . The atoms are divided into two groups A and B such that the subspace B contains the location of all the atoms for which the defect potential V has zero matrix elements. In this simple case the defect wave function º in (4.63) can be expressed in terms of the two sets of basis functions {„A } and {„B } indexed by A and B: º aA „A aB „B . (4.78) The summation in (4.78) is over the subspaces A and B and the coefficients {aA } and {aB } are arrays. The matrices G0 and V can be represented as G0AA G0AB VAA 0 and V , (4.79) G0 0 0 G0BA G0BB where G0AA , G0AB , VAA , etc. represent matrices of G0 and V calculated for the two subspaces. Substituting (4.78) into (4.64) and (4.65) we obtain {aA } G0AA VAA {aA }, (4.80a) {aB } G0BA VAA {aA }, (4.80b) and det I G0AA VAA G0BA VAA 0 I det(I G0AA VAA ) 0. (4.81) In addition º has to satisfy the normalization condition º |º 1. (4.82) For a very localized deep center, the subspace A, representing the spatial extent of the defect, is very small. Hence the determinant in (4.81) and the matrix equations in (4.80) can be solved easily even with a personal computer. In particular, the defect energy E can be determined from (4.81) since the matrix element G0AA is a function of E. We will show later how to evaluate G0AA from the density of states of the perfect crystal. Equation (4.82) ensures that the total probability of finding the electron in subspaces A plus B is unity. A more convenient form for (4.80a) can be obtained by writing G 0 G0 formally as 2 G 0 G0 [E H0 ] dG0 , dE (4.83) 4.3 Deep Centers where G 0 is the adjoint of G0 defined as 1 G 0 Lim (E H0 iË) Ë→0 (4.84) Substituting (4.83) and (4.59) into the normalization condition º |º º | V G 0 G0 V |º 1 an equation containing only aA is obtained: dG0AA V VAA aA 1. a A AA dE (4.85) (4.86) Since (4.86) involves only a closed subspace A, it can be solved numerically provided A is kept small. This will be the case for a localized deep center. Once aA is known, aB can be determined from (4.80b). We shall now consider the extreme case where A contains only the defect site and four sp3 orbitals. These orbitals are the same sp3 orbitals as discussed already in Sect. 2.6 and denoted by S, X, Y, and Z. This approximation is reasonable for a deep substitutional impurity or a vacancy in the diamondand zinc-blende-type semiconductors. From symmetry considerations, it is not difficult to see that S transforms according to the irreducible representation A1 (°1 ) of the Td group while X, Y, and Z belong to the triply degenerate T2 (°4 ) representation. Using these four basis functions the determinants of G0 and V can be written in the simplified form G0A VA 0 0 0 0 0 0 0 0 VT 0 G0T 0 0 0 0 0 G0T 0 VT 0 0 0 0 0 0 G0T 0 0 0 VT where the matrix elements G0A and VA represent the matrix elements S | G0 | S and S | V | S, respectively. G0T and VT are defined similarly using the T2 triplet. Substituting these determinants into (4.81) we obtain two implicit equations G0A (EA )VA 1 G0T (ET )VT 1, and (4.87) from which the defect energies EA and ET (for the deep levels with symmetries A1 and T2 respectively) can be determined. Hjalmarson et al. [4.29] have studied the dependence of the deep level energies on the defect potential V in a large number of tetrahedrally bonded semiconductors. To understand their results, we shall consider G0A as a function of E. According to the definition in (4.50), G0A is equal to G0A S | G0A | S Lim [E ES (k) iË]1 , (4.88) k Ë→0 where ES (k) and k denote, respectively, the energy and wave vector of electrons in the bands which contain atomic orbitals with s-symmetry. Since we have assumed that the deep level with A1 symmetry is a bound state, there 189 190 4. Electronic Properties of Defects are no energies ES (k) for which E ES (k). As a result, (4.88) can be rewritten as G0A (E) [E ES (k)]1 (4.89) k Nd (ES ) dES . E ES (4.90) In (4.90) we have transformed the summation over the electron wave vector k into an integration over electron energy by introducing a density of states Nd (ES ). Notice that Nd (ES ) is the DOS for electrons with s-symmetry only. This is sometimes referred to as a partial or projected density of states. Equation (4.90) can also be derived from the Kramers–Kronig relations by regarding G0A (E) as a complex function of E. In general Re{G0A (E)} is related to the integral of Im{G0A (E)} over all E via (4.56). Im{G0A (E)} turns out to be equal to Nd (ES ) [see (4.51)]. To visualize the function G0A (E) we first make a crude approximation to the partial DOS of the s-symmetry valence (bonding) and conduction (antibonding) bands in a typical zinc-blendetype semiconductor such as GaAs. This is shown schematically in Fig. 4.6a. From this partial DOS we can calculate G0A (E) using (4.90). We can also (a) Nd(Es) Esv 0 (b) Ec Esc Es Ec Esc E G0A(E) Esv 0 Fig. 4.6. Schematic plots of (a) the density of states for the valence band (centered at energy Esv ) and conduction band (centered at energy Esc ) derived from the s-symmetry atomic orbitals in a zinc-blende-type semiconductor and (b) the function G0A (E) obtained from the density of states in (a) using (4.89). The energy at the middle of the gap has been chosen as the zero in the energy scale. Ec denotes the bottom of the conduction band 4.3 Deep Centers “guess” the shape of G0A (E) by noticing that there are “correlations” between the shapes of the real and imaginary parts of a complex function satisfying the Kramers–Kronig relations. Such “correlations” are illustrated with an example in Problem 4.5. The G0A (E) “guesstimated” by using such correlations is sketched in Fig. 4.6b. For E lying within the energy gap (0 E Ec ) G0A (E) is approximately a linear function of E (note that the origin of energies is assumed to be in the middle of the gap). As a result of this linear relation the solution of (4.81) produces an almost hyperbolic dependence of the trap energy EA on VA : EA ∝ (1/VA ). (4.91) Figure 4.7 shows the energies of the A1 -symmetry deep impurity levels in several diamond- and zinc-blende-type semiconductors obtained by Hjalmarson et al. [4.29]. These authors first fitted the known band structures of various semiconductors with a nearest-neighbor tight-binding model. The overlap parameters obtained from this fitting procedure were used to determine the partial DOS of s-symmetry. The defect potential VA was taken to be equal to the difference between the s atomic orbital energies of the impurity and the host atom it replaces. The deep level energies for various substitutional impurities were calculated with (4.87). The relevant impurities are listed in Fig. 4.7 above the upper horizontal axis in the order of their defect potentials VA . Notice the nearly hyperbolic dependence of the deep level energy EA on VA as predicted by (4.91). The intercepts of the quasi-hyperbolas with F E [eV] 0 N Cl Br O Se C At S B Ga Tl Sb Si Al Po Bi Zn Sn In Cd As Ge Pb Hg GaAs AlP –1 P Te I GaP AlAs Ge Si Band Edge Anion site –2 E [eV] 0 –1 GaSb InP ZnTe Band Edge GaAs –2 GaP ZnSe Cation site AlP AlAs –3 –30 –20 –10 S-Orbital Energy [eV] 0 Fig. 4.7. Energies of the A1 -symmetry deep impurity levels in various diamond- and zincblende-type semiconductors calculated by Hjalmarson et al. [4.29]. The relevant impurities are listed above the upper horizontal axis in the order of their defect potentials 191 192 4. Electronic Properties of Defects the band edges (the E 0 axis being one of them) determine the thresholds for either an attractive or repulsive potential. For some semiconductors, such as Si and Ge, the quasi-hyperbolas terminate at the point where E equals the bandgap. Beyond that point, a resonant state rather than a bound state will be formed. For quasi-hyperbolas which do not terminate at the band edges, they asymptotically approach the energies EA (±∞) when VA approaches ±∞. At these energies, unless dG0AA /dE in (4.86) vanishes also, aA 0, i.e., no electron or hole can be trapped at these energies. Thus the asymptotes of EA are the dangling-bond or ideal vacancy energies. These energies are determined by the host semiconductor. From the above discussion we can draw some qualitative conclusions about deep level energies. In general, the defect energy is not very sensitive to V when V is large. The reason is that E is given by the solution of G0 (E) 1/V, which varies slowly with V when V is much larger than zero. This explains why impurities whose atomic energies differ by more than 10 eV often give rise to deep levels with defect energies differing by less than 1 eV. For infinitely large values of V, the defect energy approaches that of an ideal vacancy. Thus the energy of a vacancy can be considered as the lower bound for a deep level energy. Based on these considerations a substitutional deep center can be regarded as a vacancy in the lowest order of approximation. A deep center wave function is predominantly determined by the host crystal rather than by the impurity. One serious limitation of this model is its neglect of lattice relaxations. Since most deep centers usually induce some lattice distortion, this model cannot predict deep center energies quantitatively. However, its use lies in predicting their chemical trends. For example, from Fig. 4.7 we can predict that As on Ga sites and O on As sites both form deep donors in GaAs, in agreement with experiment. Another application of this model is the calculation of the variation of deep center energies with changes in the host band structure. Such changes can be induced by alloying or by hydrostatic pressure. The next section is devoted to one such application in order to understand substitutional nitrogen in GaAsP alloys. The model has been recently used to estimate the spin–orbit splitting of acceptor ground states, which is much smaller than ¢0 for diamond and silicon [4.20, 21]. 4.3.3 Another Application of the Green’s Function Method: Nitrogen in GaP and GaAsP Alloys Nitrogen substituting for P in GaP is an example of an isoelectronic or isovalent center because N has the same valence as P. In this case the isoelectronic centers produce localized defect levels because of the strength of V. In many other cases, isoelectronic impurities such as phosphorus replacing As or aluminum replacing Ga in GaAs do not produce localized states. Instead they generate resonant states which overlap with the band structure and hybridize with the Bloch states. When present in sufficient concentration they can be considered as forming a random alloy such as Gax Al1x As. The band structure of these alloys can be calculated by assuming the crystal to be perfect except 4.3 Deep Centers for having an average effective or virtual crystal potential. Not surprisingly this approach is known as the virtual crystal approximation. For NP in GaP, N can attract an electron because N is much more electronegative than P. (These electrons can be introduced by n-type doping or by optical excitation.) The electronegativity of N and P, as defined by Phillips, are respectively 3.0 and 1.64 [4.30]. Once N has bound an electron and become negatively charged (to be denoted by N ), it attracts a hole just like an acceptor. As a result, N in GaP is known as an isoelectronic acceptor. Similarly Bi (whose electronegativity of 1.24 is less than that of P) is an isoelectronic donor in GaP. Isoelectronic impurities appear electrically neutral except within the immediate vicinity of the impurity. Their potentials are therefore always short-ranged. The highly localized nature of isoelectronic impurity potentials causes them to behave as deep centers in spite of the fact that they may have very small binding energies. For example, the binding energy of an electron to NP in GaP is only about 9 meV [4.31]. The very short-ranged potential of N in GaP is responsible for its application in the fabrication of light-emitting diodes (LEDs). Once N has capXN GaAs 1-x Px 2.2 Xc N N data 2.0 O 1.8 1.6 Γc O data Energy [eV] 1.4 1.2 1.0 O data 0.8 0.6 Ga Dangling Bond 0.4 0.2 0.0 GaP 0.8 0.4 x 0.6 0.2 GaAs Fig. 4.8. The energy of an A1 -symmetry deep level for N substituting an anion (labeled “N data”) in GaAs1x P alloy as a function of the alloy composition x. The open circles are experimentally measured energies of an exciton bound to an isolated N center while the line labeled “N” represents the theoretical values. The point XN represents an exciton bound to a neutral nitrogen. The lines labeled “O data” and “Ga dangling bond” are not relevant to this chapter. (From [4.29]). °c and Xc denote, respectively, conduction band minima at the ° and X points of the Brillouin zone 193 194 4. Electronic Properties of Defects tured an electron, its Coulomb potential dominates over the short-range potential. This Coulomb potential is screened by the dielectric function of the semiconductor as usual and hence N behaves like a hydrogenic acceptor with a binding energy of 11 meV [4.32]. An alternative way of looking at a hole bound to form N is to regard it as an electron–hole pair bound to a neutral N (denoted by the point XN in Fig. 4.8). An electron–hole pair is also known as an exciton. An exciton bound to an impurity like N in GaP via an attractive potential is known as a bound exciton. Excitons and bound excitons are very important in determining the optical properties of semiconductors and will be studied in more detail in Chaps. 6 and 7. At this point we simply note that normally GaP is not an efficient light emitter because it has an indirect bandgap. In order to conserve the wave vector during optical transitions, radiative recombination of an exciton in an indirect-bandgap semiconductor requires the cooperation of phonons (Sect. 6.2.6). As a result, indirect-bandgap semiconductors have smaller light emission probabilities than direct-bandgap semiconductors. However, excitons bound to N in GaP have a relatively high probability of radiative recombination because the localized N centers break the translational invariance of the crystal and thereby relax the wave vector conservation requirement in optical transitions. As a result, GaP becomes a more efficient light emitter with the introduction of N. The optical properties of impurities in GaP will be studied in more detail in Chap. 7 when we discuss luminescence. We now calculate the binding energy of an electron to N in GaP using the Green’s function method. First we have to determine the impurity potential V. Since V has a very short range we will simply assume V to be a delta function in real space. More precisely, we assume the matrix element of V to be n, R | V | n, R U0 ‰n,n ‰R,R ‰n,0 ‰R,O , (4.92) where n and n are band indices (with the lowest conduction band numbered arbitrarily as 0); R and R are lattice vectors (with NP assumed to be the origin); and | n, R denotes the Wannier function anR defined in (4.4a). When defined in this way V is called the Slater–Koster interaction potential. Experimentally it is known that N in GaP forms only one bound state inside the energy gap. Using the result of Sect. 4.3.1 the energy E of this bound state can be obtained by solving (4.65). Substituting V into (4.65) we obtain 1 U0 0, 0 | (E H0 )1 | 0, 0 0. (4.93) There are two ways to solve (4.93). One approach is to use a simple tightbinding model with the minimum number of parameters, as discussed in the last section. Another method is to use a more exact band structure obtained by methods such as the empirical pseudopotentials method (Sect. 2.5). We shall briefly describe the results of both approaches for comparison. a) Tight-Binding Method Using this method Hjalmarson et al. [4.29] have calculated the energy of an electron bound to N in GaAs1x Px alloys as a function of the alloy composition x. Their results are shown in Fig. 4.8. According to their calculation N 4.3 Deep Centers forms a resonant state above the bottom of the conduction band in GaAs. As the concentration of P in the alloy is increased, this resonant level gradually moves into the bandgap and becomes a bound state. The important thing to note is that the location of the lowest conduction minimum in the reciprocal space changes from the zone center to the X point at x ≈ 0.5. As a result, the slope of the lowest conduction band minimum versus x in Fig. 4.8 changes abruptly at x ≈ 0.5. On the other hand, the deep level energy varies smoothly with x. This is consistent with what we expect for a deep level. The energy of a highly localized center should be determined by the entire band and not by the lowest band minimum only, as in case of the shallow centers. The experimentally measured energies of an electron to N in the GaAsP alloys are shown as open circles in Fig. 4.8. While the calculated energies of the N deep level are lower than the experimental values, the measured dependence of the deep level on alloy concentration is in very good agreement with theory. In addition, the resonant nature of the N level in GaAs has been verified by Wolford et al. [4.33]. Instead of varying the concentration of P, Wolford et al. applied hydrostatic pressure to lower the conduction band minimum at X below the band minimum at °. At pressures above 30 kbar (or 3 GPa), the N deep level moved into the bandgap as in the case of increasing P concentration. Using this method, excitons bound to N in GaAs have been studied in great detail by photoluminescence experiments, see Fig. 4.9. b) Empirical “Energy Moment” Approach In this approach, we change the basis function in (4.93) from the Wannier functions back to Bloch functions |n, k. The resultant secular equation becomes U0 0, k | (E0, k E)1 | 0, k 0, (4.94) 1 N k where n 0 denotes the lowest conduction band. Equation (4.94) can be solved numerically. In particular, we recognize that the expression 0, 0 | (E H0 )1 | 0, 0 in (4.93) is related to the local DOS by the Kramers–Kronig relations. So E can be computed from the DOS of the host semiconductor in a relatively straightforward manner. Alternatively, we can obtain an analytic expression for E by introducing approximations such as expanding (E0,k E)1 into a series: E 1 1 (E0, k E)1 E0, E k 0, k E0, k E 2 (4.95) E E E 1 E0, k 1 1 ··· . E0, k E0, k E0, k Substituting (4.95) into (4.94) we obtain U0 1 U0 2 0 1 E0, k E E0, k N N U0 3 E2 E0, k ... . N (4.96) 195 4. Electronic Properties of Defects 2.0 X 1.9 L DΓ Energy [eV] 196 NX LO 1.8 2LO 3LO nce na eso R 1.7 GaAs: N 5°K 1.6 1.5 0 10 20 40 30 50 60 70 Pressure [kbar] Fig. 4.9. The energy of excitons bound to isoelectronic substitutional N deep centers (denoted as NX and indicated by large open squares) in GaAs as a function of hydrostatic pressure. The data points (indicated by small open squares) labeled LO, 2LO, etc., denote the LO phonon replicas of the main NX peaks. The open circles labeled D° denote the energy of an exciton bound to a neutral shallow donor as a function of pressure. The solid lines labeled L and X denote the higher conduction band minima at the L and X points of the Brillouin zone. (From [4.33]) Equation (4.96) can be expressed in a more compact form by defining “moments” of the band n 0: 1 E01 E0, N, (4.97a) k E02 2 E0, k N, (4.97b) and so on. These moments can be calculated from the band structure. With this notation (4.96) becomes 0 1 (U0 E01 ) E(U0 E02 ) E2 (U0 E03 ) . . . . (4.98) In the case of N in GaP it is known that E satisfies the condition EE01 1, hence we can neglect the term in (4.98) that depends on E2 and higher terms. 4.3 Deep Centers This gives the approximate solution for E as E ≈ 1 (U0 E01 ) U0 E02 . (4.99) Since we have assumed that the potential V of N in GaP is attractive, U0 is negative. Without loss of generality we can choose the energy of the bottom of the conduction band as zero. Since E02 is positive, in order that E be a solution of (4.99) lying in the gap, E has to be negative. Hence 1 (U0 E01 ) has to be negative also. This imposes the condition on U0 that | U0 E01 | ≥ 1. Faulkner [4.31] used the conduction band structure of GaP and the experimental value of the binding energy of an electron to N to derive a value for U0 based on the above model. Unfortunately, the value of U0 obtained does not explain the other experimental results such as the binding energy of an exciton to pairs of nitrogen atoms [4.34] and the properties of bound excitons in GaAsP alloys. Furthermore, the Slater–Koster potential allows the existence of only one bound state and therefore cannot explain the presence of excited states. Some of these shortcomings can be traced to the fact that the expansion in (4.95) is a good approximation only when the defect energy E is quite different from the band energies. In other words, the binding energy of the deep center has to be large. This condition is not satisfied by N in GaP. In spite of these shortcomings, this very simple model does provide a framework for understanding qualitatively some of the properties of isoelectronic impurities in semiconductors. It has become the starting point for later models proposed to overcome some of its shortcomings. In one model proposed by Hsu et al. [4.35], a long-range potential due to strain was added to the Slater-Koster potential. The energies of excited states of excitons bound to N and of excitons bound to nitrogen pairs were satisfactorily explained by choosing this longrange potential appropriately. 4.3.4 Final Note on Deep Centers Our quantitative discussion of deep centers so far has neglected lattice distortions (i.e., relaxation). This effect is known to play an important role in deep defect centers such as the EL2 [4.36] and the DX centers [4.23]. These deep centers have significant impact on semiconductor devices based on III–V and perhaps even II–VI semiconductors. Given their importance and the greater understanding we have now of their interesting properties, such as metastability and lattice relaxation, we have devoted an appendix (see A4.1 in Appendix C) to the DX centers. EL2 [4.36] and DX centers [4.23], have been found to play important roles in semiconductor devices based on III–V and perhaps even II–VI compound semiconductors. These defects exhibit interesting properties such as metastability, persistent photoconductivity, and negative U. Often these properties of deep centers can be understood only when lattice relaxations are included. Readers interested in these topics should refer to one of the review articles listed in the references, e. g. [4.23, 36] and to the Appendix C on the DX Centers to be found under Section A4.1. 197 198 4. Electronic Properties of Defects PROBLEMS 4.1 Symmetrization of the Conduction Band Wave Functions in Si for Donor Binding Energy Calculations a) There are six conduction band minima in Si. They occur along the six equivalent [100] directions inside the Brillouin zone. Use the notation X, Y, and Z to represent the wave function for the minima occurring in the [100], [010], and [001] directions, respectively, (X, Y, and Z for those along [100], [010], [001]). Apply the symmetry operations of the point group Td to these six wave functions. Show that the characters of the corresponding representation are {E } 6 {3C2 } {6S4 } {6Û} {8C3 } 2 0 2 0 b) Using Table 2.3, show that these six wave functions form a reducible representation which can be reduced to A1 ⊕ E ⊕ T2 . c) By examining the basis functions in Table 2.3, show that the six wave functions when written as the following linear combinations correspond to the irreducible representations: √ A1 : (X X Y Y Z Z)/ 6; √ E: (X X √Y Y)/2, (2Z X Y Y)/ 12; √ 2Z X √ T2 : (X X)/ 2, (Y Y)/ 2, (Z Z)/ 2. 4.2 Full Rotation Group and Spherical Tensors Consider a particle moving in a spherically symmetric potential. A rotation about an axis in the three-dimensional space is clearly a symmetry operation. The set of all rotations can be shown to form an infinite group known as the full rotation group (see for example books on group theory listed for Chap. 2). All rotations through the same angle (irrespective of the axis of rotation) can be shown to belong to the same class. Rotations by different angles belong to different classes: there are an infinite number of classes. Hence there are also an infinite number of irreducible representations. In quantum mechanics we learn that the angular momentum l is a good quantum number for particles moving in spherically symmetric potentials. Their eigenfunctions are the spherical harmonic functions {Ylm } where m l, l 1, . . . , 1, 0, 1, . . . , l. For integral values of l, these functions turn out to be the basis functions for the irreducible representations of the full rotation group. Hence an irreducible representation with {Ylm } as basis functions has dimension 2l 1. Suppose we choose a polar coordinate system (r, £, ˇ) with the z axis as the polar axis. a) Show that the effect of a clockwise rotation of the coordinate axes by an angle · about the z axis on Ylm (£, ˇ) is given by P· Ylm (£, ˇ) exp(im·) Ylm (£, ˇ). Problems b) Show that the representation matrix of such a rotation is a diagonal matrix with diagonal elements exp(im·), where m l, l 1, . . . , 0, . . . , l 1, l. Hence show that the character for such a rotation is given by " # sin l 12 · ¯l (P· ) . sin(·/2) The functions {Ylm } form a spherical tensor of order l and dimension 2l 1. For the purpose of this chapter, we need to know only {Ylm } for l 0, 1, and 2. For l 0, {Ylm } is a scalar or any function that is invariant under all rotations. The {Y1m } for l 1 are three functions defined by 1/2 3 z Y10 ; 4 1/2r 3 x ± iy Y1±1 . 8 r The spherical harmonic functions for l 2 are 1/2 2 5 3z r2 ; Y20 16 r2 1/2 15 (x ± iy)z ; Y2±1 ± 8 r2 1/2 2 15 x y2 ± 2ixy . Y2±2 32 r2 c) Suppose {Tij }, where i and j stand for x, y, and z, is now a second-rank Cartesian tensor containing nine elements. These nine elements form a reducible representation of the full rotation group. Show that the second-rank Cartesian tensor {Tij } can be reduced to the (0) (1) (2) following three spherical tensors T (0) {T0 }, T (1) {Tq }, T (2) {Tq } of order 0, 1, and 2, respectively: (0) T0 T11 T22 T33 (1) T0 (1) T± (2) T0 (2) T±1 (2) T±2 T12 T21 √ ∓(1/ 2) T23 T32 ± i(T31 T13 ) (3/2)1/2 T33 ∓(T13 ± iT23 ) (1/2) (T11 T22 ± 2iT12 ). 4.3 Luttinger Hamiltonian in Terms of Spherical Tensors Two spherical tensors can be multiplied together to generate another tensor as with Cartesian tensors. For example, the scalar product of two spherical (k) (k) tensors T (k) {Tq }, and U (k) {Uq } both of order k, can be defined as (k) (k) T · U (k) (1)q Tq(k) Uq . q 199 200 4. Electronic Properties of Defects (c) The tensor product [T (a) × U (b) ]d of two spherical tensors of orders a and b, respectively, are spherical tensors of order c defined by a b c (a) (b) (a) (b) (c) abd 1/2 T ×U (1) (2c 1) Ti Uj , d i j d i, j a b c is the 3 j symbol used in the addition of two angular where i j d momenta in quantum mechanics (see, for example, Appendix C in [4.37]). Using these definitions the terms (∇ · J)2 and (∇2x Jx2 c.p.) inside the Luttinger Hamiltonian HL in (2.70) can be expressed in terms of two spherical tensors of second rank: (2) and J (2) which can be constructed using the results of Problem 4.2 from the corresponding linear and total angular momentum operators and J via the second rank Cartesian tensors defined by: ij i j (i/xi )(i/xj ) and Jlm Jl Jm show that 1 2 (2) (2) 2 J 2 ·J 3 45 (2) (4) 1 × J (2) 4 18 (2) (70)1/2 (2) (2) (4) (2) (4) ×J 0 ×J 4 , 5 {x y }{Jx Jy } cyclic permutations (2) (4) 1 (2) (2) 1 ·J × J (2) 4 30 36 (2) (70)1/2 (2) (4) (2) (2) (4) ×J 0 ×J 4 . 5 2x Jx2 2y Jy2 2z Jz2 4.4 Average Light and Heavy Hole Masses In Sect. 2.6.2 we have already attempted to approximate the warped heavy and light hole bands with spherical bands by defining averaged effective masses with (2.69a) and (2.69b): 1 1 | C |2 2 2A 2B 1 (2.69a) m∗hh 10B2 1 | C |2 1 2 2A 2B 1 . (2.69b) ∗ mlh 10B2 In this chapter we have presented a different approach. Using the method of Baldereschi and Lipari [4.14] we can express the Luttinger Hamiltonian in terms of irreducible representations of the full rotational group: (4) p2 Ì HBL 2 2 (2) · J (2) ‰ (2) × J (2) 4 √ 9 (4) (4) ! 70 (2) × J (2) 0 (2) × J (2) 4 . 5 Problems The hole bands can be “sphericalized” by setting the cubic term, proportional to ‰ in HBL , equal to zero. Show that, in this spherical approximation, the energy dispersions of the heavy- and light-hole bands are given by E(±) 2 Á1 (1 ± Ì)k2 2m0 and that the “sphericalized” heavy- and light-hole masses are given by ⎧ ⎡ 1/2 ⎤⎫ ⎨ ⎬ 2 1 4 ⎣ 3 4| C | 1 ⎦ B 2A 1 1 ⎭ m∗hh 2 ⎩ 5 2 9B2 ⎧ ⎡ 1/2 ⎤⎫ ⎬ 1 ⎨ 4 ⎣ 3 4| C |2 1 ⎦ . 2A 1 1 B ⎭ m∗lh 2 ⎩ 5 2 9B2 Notice that in the limit C 0 the above masses become identical to those in (2.69a) and (2.69b). 4.5 Kramers–Kronig Relations Given that the imaginary part of a function F(E) is a Lorentzian: Im F(E) 1 , (E E )2 ° 2 use the Kramers-Kronig relation in (4.56) to show that the real part of F(E) is given by 1 E E Re F(E) . ° (E E )2 ° 2 An alternative, easier way to solve this problem “by inspection” is to note that if F(E) is equal to the analytic function 1 1 F(E) ° (E E ) i° then the imaginary part of F(E) is equal to the given Lorentzian. and Figure 4.10a,b shows schematically the functions Re F(E) Im F(E)}. These plots illustrate the “correlations” between functions which are related to each other by the Kramers–Kronig relations: • • If Im F(E) is symmetric with respect to the vertical axis y E0 , then is antisymmetric with respect to y E0 . Re F(E) If Im F(E) is always positive andlarge over only a limited range of values of E; E1 E E2 , then Re F(E) will be negative for E well below E1 but positive for E much larger than E2 . 201 202 4. Electronic Properties of Defects (a) Re{F(E)} E (b) E –Im{F(E)} E E Fig. 4.10. Schematic plots of the functions (a) Re{F(E)} and (b) Im{F(E)} defined in Problem 4.5 SUMMARY This chapter dealt with the study of the electronic properties of defects in semiconductors because electrically active defects play an important role in the operation of many semiconductor devices. Since defects come in many different forms we restricted our discussions to point defects only. These are separated into donors and acceptors and further divided into shallow or hydrogenic centers and deep centers. For shallow centers we introduced the effective mass approximation for calculating their energies and wave functions. Properties of shallow centers were shown to be very similar to those of the hydrogen atom except for effective mass anisotropy and other corrections arising from the host crystal lattice. Hence energy levels of shallow centers are sometimes referred to as hydrogenic levels. Many defect centers cannot be understood within this approximation and they are referred to as deep centers. Properties of deep centers are often determined by potentials, localized within one unit cell, known as central cell corrections. These localized potentials are difficult to handle. We have, therefore, presented only a rather rudimentary Green’s functions approach to calculating deep center energies. This approach was applied to explain the chemical trends of deep levels in tetrahedrally bonded semiconductors and to the special case of isovalent (substitutional nitrogen) impurities in GaAsP alloys. A very serious limitation of our approach is the neglect of lattice relaxations, which are often associated with deep centers. 5. Electrical Transport CONTENTS 5.1 Quasi-Classical Approach . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Carrier Mobility for a Nondegenerate Electron Gas . . . . . . . . . . . . . 5.3 Modulation Doping . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 High-Field Transport and Hot Carrier Effects . . . . . . . . . . . . . . . . . . . . 5.5 Magneto-Transport and the Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 203 206 223 225 232 237 241 In Chap. 4 we studied electrons and holes located around defects. Since these electrons and holes are immobile they are known as bound electrons and holes, respectively. In contrast, electrons in the conduction band and holes in the valence band of a semiconductor can carry electrical current. Hence they are referred to as free carriers. In this chapter we will study the effect of an external electric field on free carriers in a semiconductor. The response of these carriers to an electric field depends on the field strength. We will first consider the case of weak electric fields, where the behavior of carriers can be described by Ohm’s law. Under high electric fields, carriers in a semiconductor can acquire so much energy that their average kinetic energy becomes higher than that of the lattice. Such energetic electrons are known as hot electrons. It is very difficult to calculate their properties analytically, therefore our discussions of hot electrons will be qualitative. 5.1 Quasi-Classical Approach Let F represent a weak external static electric field applied to a semiconductor. We can assume without loss of generality, that this semiconductor contains only free electrons (i. e., it is an n-type semiconductor). For simplicity, we will assume that the concentration of free electrons is low enough that we can neglect their interactions with each other (such as collision and screening effects). We will also neglect local field effects due to ionic charges, i. e. the field experienced by every free electron is assumed to be equal to the external applied field. Now let º be the electric potential associated with the applied P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed., DOI 10.1007/978-3-642-00710-1_5 , © Springer-Verlag Berlin Heidelberg 2010 204 5. Electrical Transport field. The wave equation for the time evolution of an electron in a semiconductor under the influence of º is given by (H0 eº)„(r, t) i „ , t (5.1) where H0 is the one-electron Hamiltonian (in the absence of external perturbations) that we have already studied in Sect. 2.1, e is the magnitude of the electronic charge and „(r, t) is the electron wave function in the presence of the external field. As long as º is small and does not vary rapidly in space, we can use the effective mass approximation (Sect. 4.2.1) to solve (5.1). The approach is very similar to the way we handled the donor electron problem in Sect. 4.2. The difference is that, in the present case, we are interested in the nonstationary solutions, which produce a current in response to the applied field. This requires the expectation value of ev to be evaluated where v is the electron velocity operator. The current density operator j is then defined as j nev, (5.2) where n is the electron density. As we saw in Sect. 4.2, solving the Schrödinger equation within the effective mass approximation is quite an involved process. Instead of the fully quantum mechanical approach, we will adopt here a quasiclassical approach [5.1]. We shall derive a classical equation of motion for our electron in the external field based on the effective mass approximation. As we discussed in detail in Sect. 4.2.1, a wave equation for Bloch waves such as (5.1) can be replaced by an effective wave equation for the envelope functions C(R, t). For simplicity we shall assume that our electron is in an isotropic and nondegenerate conduction band with an energy minimum at the zone center (k 0) and a dispersion given by Ec (k) Ec (0) 2 k2 , 2m∗ (5.3) where m∗ is the effective mass. These assumptions are valid for electrons in direct bandgap semiconductors such as GaAs and InP but not for Si and Ge. Within the effective mass approximation the wave equation for the envelope functions can be written as [see (4.22)] 2 (5.4) Ec (0) eº(R) C(R, t) ≈ i C(R, t). ∗ 2 2m R t Instead of solving (5.4), we argue that the net effect of the crystal potential on the motion of this electron inside the semiconductor is to cause its mass to change from the value in free space to m∗ . This suggests that, as a simple approximation, we can describe the motion of this electron in an external electric field by a classical equation of motion (see, for example, [5.1]) 5.1 Quasi-Classical Approach m∗ m 2 dt Ù ∗d 2 r dr eF, dt (5.5) where r is the position of the electron and Ù is a phenomenological scattering time introduced to account for the scattering of the electron by impurities and phonons. Equation (5.5) is considered quasi-classical because the concept of an effective mass for the electron motion has been derived quantum mechanically. Once we have established (5.5), the motion of any charge q can be derived via classical mechanics. For example, under the influence of F a stationary charge will accelerate. As its velocity increases, the retardation term (m∗ /Ù) (dr/dt) will also increase. Eventually the retardation term will cancel the term due to F and a steady state in which the charge has no acceleration is attained. The steady-state velocity of the charge is known as its drift velocity vd . It is obtained from (5.5) by setting the acceleration term m∗ (d2 r/dt2 ) to zero and denoting by q the electronic charge e: vd qFÙ/m∗ . (5.6) The current density J at steady state is related to vd by J nqvd . (5.7) Combining (5.6 and 7) we obtain an expression for the current density: J nq2 FÙ/m∗ . (5.8) The second-rank conductivity tensor Û is defined in general by J Û · F. (5.9) For the case of an isotropic conduction band Û is a diagonal tensor with all diagonal elements given by Û nq2 Ù/m∗ . (5.10) 2 Since Û depends on q , the contributions to the conductivity of a semiconductor from electrons and holes always add. Semiconductors differ from metals in that their carrier densities can be varied widely by changing the temperature or the dopant concentration. It is therefore convenient to factor out the dependence of Û on n. This can be accomplished by defining a carrier mobility Ì as vd ÌF. (5.11) Combining (5.6 and 11) we obtain Ì qÙ/m∗ . (5.12) In a semiconductor containing both free electrons and free holes Û is given by Û e(ne Ìe nh Ìh ), where the subscripts e and h refer to electrons and holes, respectively. (5.13) 205 206 5. Electrical Transport 5.2 Carrier Mobility for a Nondegenerate Electron Gas The expressions we derived in the previous section are valid when all the carriers have the same scattering time. We will now generalize these expressions to the case where the carriers are distributed in a band according to the Boltzmann distribution [to be defined later in (5.22)] and the scattering time depends on the carrier energy. 5.2.1 Relaxation Time Approximation We define the distribution function fk (r) of a carrier as the probability that a band state with energy Ek will be occupied by this carrier at a carrier temperature T. We assume that in the absence of an external field the carriers are at thermal equilibrium, so that fk is equal to the Fermi–Dirac distribution function: fk0 1 , exp[(Ek ÌF )/(kB T)] 1 (5.14) where Ì F is the chemical potential (also called Fermi energy when T ≈ 0) and kB the Boltzmann constant. The equation governing the variation of fk in the presence of an external perturbation is known as the Boltzmann equation: dfk fk fk fk . (5.15) dt t field t diff t scatt Equation (5.15) includes the effects on fk due to the applied field, the diffusion of carriers, and the scattering of carriers by phonons, impurities, etc. For simplicity, we shall assume that the diffusion term is negligible and the applied field F is small enough that we can expand fk about fk0 as a function of F: fk fk0 gk (F). With this approximation we can write (fk /t)field as fk0 dEk fk0 fk ≈ qvk · F, t field Ek dt Ek (5.16) (5.17) where vk is the velocity of carriers with wave vector k. Within the relaxation time approximation, we assume that the net effect of the scattering processes is to cause gk to relax with a time constant Ùk , so that g fk ≈ k. (5.18) t scatt Ùk After substituting (5.17) and (5.18) into (5.15) we obtain fk0 gk qÙk vk · F. Ek (5.19) 5.2 Carrier Mobility for a Nondegenerate Electron Gas The corresponding generalized expression for the current density is now given by (5.20) j qfk vk dk qgk vk dk fk0 2 (vk · F)dk, (5.21) q Ùk vk Ek since qfk0 vk dk 0. Using (5.21) the corresponding expressions for Û and Ì can be easily obtained. 5.2.2 Nondegenerate Electron Gas in a Parabolic Band As an example of how to apply (5.21) we will consider the simple case of a nondegenerate electron gas in a parabolic band with an isotropic effective mass m∗ in a cubic crystal. In such crystal j and vk are parallel to F, at least in the region where Ohm’s law holds. The distribution function (5.14) for a nondegenerate electron gas can be approximated by the Boltzmann distribution: fk0 ∝ exp Ek /(kB T) (5.22) so that fk0 1 Ek ∝ . exp Ek kB T kB T (5.23) The integration over k-space in (5.21) can be replaced by an integration over the energy Ek using the density of states (DOS) introduced in Sect. 4.3.1. For a parabolic band in three dimensions, the DOS D(E) is given by (including spin degeneracy): ∗3/2 1 dk 2m 1 D(E) 2 k2 E1/2 . (5.24) dE 22 2 Substituting these results into (5.21) we can calculate j and hence Û: 3/2 ∞ q2 2m∗ Û Ù(E)E3/2 exp E/(kB T) dE. 2 ∗ 3 m kB T 0 (5.25) In analogy with (5.10) we can define an average scattering time Ù by ∞ 1 Û ∗ D(E)q2 ÙdE. (5.26) m 0 Comparing (5.25) and (5.26) we obtain ∞ 3/2 exp E/(kB T) dE 2 0 Ù(E)E . Ù ∞ 1/2 3kB T exp E/(kB T) dE 0 E (5.27) Using Ù we can express the mobility for a nondegenerate electron gas as Ì qÙ/m∗ . (5.28) 207 208 5. Electrical Transport From the expression for Ù we notice that the mobility depends on the electron temperature T. In order to calculate this temperature dependence, it is necessary to know the dependence of the scattering mechanisms on electron energy. 5.2.3 Dependence of Scattering and Relaxation Times on Electron Energy Carriers in a semiconductor are scattered by their interaction with the following excitations [Ref. 5.2, pp. 82–183]: • • • • • phonons: both acoustic and optical, ionized impurities, neutral defects, surfaces and interfaces, other carriers (e. g., scattering between electrons and holes). In order to calculate the relaxation time Ùk to be used in (5.18), we have to first consider the effect of scattering on fk . Let us define P(k, k ) as the probability per unit time that an electron with wave vector k will be scattered into another state k . Once this scattering rate is known the rate of change of fk caused by scattering can be calculated with the equation fk P(k , k)fk (1 fk ) P(k, k )fk (1 fk ) . (5.29) t scatt k k The first term inside the square brackets represents the rate at which an electron at k will be scattered into the state at k, while the second term is the rate for scattering out of the state k into k . The summation is over all processes which conserve both energy and wave vector. If we assume as before that the electron gas is nondegenerate, then fk and fk are small and can be neglected compared with unity. Applying the principle of detailed balance, P(k , k)fk0 P(k, k )fk0 , see [5.3], (5.29) simplifies to fk P(k, k ) fk (fk fk0 fk0 ) . (5.30) t scatt k k In general, (fk /t)scatt cannot be expressed as (fk fk0 )/Ùk as assumed in the relaxation time approximation. Only with more assumptions do we obtain an expression of the form (Problem 5.2) ⎛ ⎞ fk (fk fk0 ) ⎝ P(k, k )⎠ , (5.31) t scatt k k from which a scattering time Ùs can be defined as (1/Ùs ) P(k, k ), k k (5.32) 5.2 Carrier Mobility for a Nondegenerate Electron Gas where the summation is over all the final states k that satisfy both energy and momentum conservation. However, Ùs represents the residence time of the electron in state k before being scattered and is not the same as Ùk , which is equal to the time it takes a perturbed distribution to return to equilibrium. In order for thermal equilibrium to be achieved, carriers have to be scattered in and out of a state many times. When P(k, k ) is known, it is possible to calculate Ùk numerically by following the time evolution of the distribution function of an electron gas using a Monte Carlo simulation technique [5.4, 5]. 5.2.4 Momentum Relaxation Times We shall now obtain analytical expressions for Ùk by making some approximations. One approach is to equate Ùk to a momentum relaxation time Ùm . We can argue that the most important effect of scattering on electron transport is the randomization of the electron velocity. The relevant quantity is a momentum relaxation rate defined by dk/dt k(Ùm )1 (k k)P(k, k ). (5.33) k k The scattering rate P(k, k ) can be calculated using Fermi’s Golden Rule P(k, k ) (2/)|k | Hscatt | k |2 Úf , (5.34) where Hscatt is the Hamiltonian for the scattering processes which conserve both energy and wave vector, and Úf is the density of final states k per unit volume of crystal. Of the scattering processes listed earlier, the ones most effective in randomizing the electron momentum are those with impurities and with phonons. Scattering by the static potential of impurities is elastic. Scattering by acoustic phonons is nearly elastic (quasi-elastic) because of the small energy transfers involved; the average scattering angles are large. As we saw in Chap. 3, optical phonons in semiconductors have energies in the range of tens of meV, therefore scattering between electrons and optical phonons is inelastic. We will now calculate the individual rates for these scattering processes. Afterwards these rates can be added together to calculate the total scattering rate whose inverse is a measure of the relaxation time. a) Intraband Scattering by Acoustic Phonons We will assume that an electron with initial energy Ek and wave vector k is scattered to another state with energy Ek and wave vector k via the emission of an acoustic phonon with energy Ep and wave vector q. Since the total energy and wave vector of the electron and phonon have to be conserved in the scattering in a periodic lattice, the initial and final electron energies and wave vectors are related by the equations (for the case of phonon emission) Ek Ek Ep and k k q. (5.35) 209 210 5. Electrical Transport For an acoustic phonon with a small q, Ep is related to q by Ep vs q, (5.36) where vs is the phonon velocity. For simplicity we shall assume vs to be isotropic. We shall further assume that the electron is in a parabolic band with effective mass m∗ and it is scattered by acoustic phonons within the same band (this is known as intraband scattering). Since the scattering process conserves energy and wave vector, the allowed values of q are obtained by combining (5.35) and (5.36) into (2 /2m∗ ) (k2 | k q |2 ) vs q (5.37) and solving for q. The final electronic states, after emission of an acoustic phonon, are shown schematically in Fig. 5.1a. From this picture it is clear that the allowed values of q lie between a minimum (qmin ) and a maximum (qmax ). For k mvs /, qmin is zero while qmax is reached when k is diagonally opposite to k, i. e., when the electron is scattered by 180◦ (backscattering). From (5.37) qmax can easily be calculated to be qmax 2k (2mvs /). (5.38) The energy lost by the electron in emitting this phonon is Ek Ek vs qmax 2vs k 2mv2s . (5.39) To estimate the order of magnitude of these quantities, we will assume the following values of the parameters involved: m∗ 0.1m0 (m0 is the free electron mass), vs 106 cm/s, and Ek 25 meV (roughly corresponding to room temperature times kB ). For this electron k 2.6 × 106 cm1 , qmax 5 × 106 cm1 ≈ 2k, k 2.4 × 106 cm1 (k ≈ k) and Ek Ek 3.3 meV. In emitting an acoustic phonon with wave vector qmax , the electron completely (a) (b) Ek Ek Acoustic phonon q Optical phonon q2max q2min ELO k k Fig. 5.1. Schematic diagrams for the scattering of an electron in a parabolic band by emission of (a) an acoustic phonon and (b) a longitudinal optical (LO) phonon showing the final electronic states and also the range of phonon wave vectors allowed by wave vector conservation 5.2 Carrier Mobility for a Nondegenerate Electron Gas reverses its direction but its energy changes by only about 13 %. Thus scattering between electrons and acoustic phonons is nearly elastic (or quasi-elastic) and the main effect of these collisions is the relaxation of electron momentum. Using (5.34) we shall now calculate the probability PLA (k, q) that an electron in a parabolic and nondegenerate band will emit a LA phonon of wave vector q. First we shall consider only the deformation potential mechanism and use the electron LA–phonon interaction Hamiltonian HeLA defined in (3.21 and 22). The scattering matrix element in (5.34) will now be written as |k, Nq | HeLA | k , Nq |2 , where | k, Nq represents the initial state with the electron in state k and the occupation number (for a definition see Sect. 3.3.1, p. 126) of LA phonons with wave vector q equal to Nq . Similarly, | k , Nq is the final state, where the phonon occupation number is changed to Nq and the electron is scattered to state k . We will be interested in one-phonon scattering only, i. e., Nq differs from Nq by ±1. Since our goal here is to calculate the temperature dependence of the electron mobility with (5.27), we are concerned only with the dependence of PLA on electron energy and temperature. As discussed already in Sect. 3.3.1, we can express |k, Nq | HeLA | k , Nq |2 as |k, Nq | HeLA | k , Nq |2 ∝ q Nq 12 ± 12 , (5.40) where the () sign in (5.40) corresponds to emission (absorption) of a phonon by the electron. As also shown in Sect. 3.3.1, Nq at room temperature can be approximated by kB T/(vs q) 1, so that |k, Nq | HeLA | k , Nq |2 is proportional to Nq 1 for both phonon emission and absorption. As a result, we can deduce the following dependence of PLA on T and Ek PLA (k) PLA (k, q) ∝ qNq ‰[Ek Ek vs q]dq. (5.41) q Using polar coordinates, (5.41) can be expressed as qmax 3 PLA (k) ∝ q (T/q)dq ‰ 2 q/(2m) (2k cos £q)vs q d(cos £) (5.42a) 0 ≈ Tq2max /k, 0 (5.42b) where £ is the angle between k and q. Since qmax is approximately equal to 2k, PLA is roughly proportional to kT. Thus the PLA produced by the deformation potential mechanism depends on the electron energy Ek and temperature as (see Problem 5.3) PLA ∝ T(Ek )1/2 . (5.43) In noncentrosymmetric crystals, carriers can be scattered by both LA and TA phonons via the piezoelectric interaction (Sect. 3.3.3). Again we are interested mainly in the energy dependence of the corresponding scattering matrix element: |k, Nq | Hpe | k , Nq |2 . From (3.30) and (3.22) we obtain |k, Nq | Hpe | k , Nq |2 ∝ (1/q) Nq 12 ± 12 . (5.44) 211 212 5. Electrical Transport Unlike |k, Nq | HeLA | k , Nq |2 , the constant of proportionality in (5.44) depends, in general, on the direction of q, so we cannot simply substitute (5.44) into (5.41) to calculate the electron–phonon scattering rate due to the piezoelectric interaction. However, by comparing the dependence on q in (5.44 and 40) it is clear that the piezoelectric interaction is more important for small-q phonons. Since phonons with small q are less effective in relaxing carrier momentum, we may argue that the piezoelectric interaction is less important than the deformation potential interaction in momentum relaxation. This is only true if the electromechanical constants are small, such as for semiconductors with low ionicity. In more ionic crystals, such as II–VI compound semiconductors, the piezoelectric interaction tends to dominate over the deformation potential interaction [5.6]. If we can assume the constant of proportionality in (5.44) to be independent of the direction of q, then it is straightforward to show (Problem 5.4) that the piezoelectric electron–acoustic-phonon scattering rate Ppe is proportional to Ppe ∝ T(Ek )1/2 . (5.45) This expression is obviously not valid for very low energy electrons. When Ek is small, the wave vector q of the acoustic phonons involved in the scattering will be small also. Usually, in the case under consideration, corresponding to (5.45), free carriers are also present in the semiconductor, and therefore the macroscopic piezoelectric field associated with these long-wavelength phonons will be screened by the free carriers. For a nondengenerate electron gas this screening effect can be included by introducing a screening wave vector q0 , which is defined as the reciprocal of the Debye screening length ÏD , see [Refs. 5.1, p. 151; 5.2, p. 179; 6.10, p. 497] q20 1 4Ne2 , 2 4Â0 Âs kB T ÏD (5.46) where Âs is the static dielectric constant. The result is that the matrix element |k, Nq | Hpe | k , Nq |2 in (5.44) should be replaced by q3 2 |k, Nq | Hpe | k , Nq | ∝ (Nq 12 ± 12 ). (5.47) (q2 q20 )2 Notice that (5.44) is recovered if q0 0. When the screening effect is included in (5.47), i. e., q0 0, |k, Nq | Hpe | k , Nq |2 approaches zero as q → 0. Similarly Ppe goes to zero, rather than diverging like in (5.45), as the electron energy decreases to zero. Figure 5.2 shows qualitatively the dependence of Ppe on electron energy. From (5.41) we see that carriers are more likely to be scattered by LA phonons with large q via the deformation potential interaction. Since these phonons are more effective in randomizing the carrier momentum, acoustic phonon scattering (via the deformation potential interaction) is the dominant mechanism for momentum relaxation of carriers at room or lower temperatures in most semiconductors except for the very ionic ones. The acoustic 5.2 Carrier Mobility for a Nondegenerate Electron Gas Fig. 5.2. Sketch of the dependence on the energy of an electron of the rate of scattering (Ppe ) by acoustic phonons via the piezoelectric electron–phonon interaction [Ref. 5.2, Fig. 3.20] Ppe 0 h2q02 8m* E phonon scattering time for conduction electrons in GaAs (via deformation potential interaction only) has been calculated by Conwell and Vassel [5.8]. Their results are shown in Fig. 5.3. Notice that this scattering time is of the order of several picoseconds (one picosecond is equal to 1012 s and abbreviated as ps) in GaAs (Problem 5.3), and notice also how it decreases with increasing electron energy as predicted by (5.43). 10–11 GaAs τac Relaxation time [s] Acoustic Phonon τ1→2(1×108 eV/cm) 10–12 LO Phonon τpo τ1→2(5×108 eV/cm) 10–13 Γ→X Intervalley Scattering 10–14 0 0 0.18 5 0.36 10 0.54 15 0.72 20 ε in eV ε /(hω LO) Fig. 5.3. Momentum relaxation times of a conduction electron in the ° valley of GaAs as a function of electron energy. Scattering by: small wave vector LA phonons (Ùac ) via the deformation potential interaction; small wave vector optical phonons (Ùpo ) via the Fröhlich interaction and via zone-edge phonons from ° to the X valleys (Ù1→2 ) calculated by Conwell and Vassel [5.8]. Notice that the deformation potential for the ° to X intervalley scattering has been assumed to be either 1 × 108 or 5 × 108 eV/cm. These values are smaller than the now accepted value of 109 eV/cm [5.9] 213 214 5. Electrical Transport b) Intraband Scattering by Polar Optical Phonons Optical phonons in semiconductors typically have energies of the order of tens of meV (Chap. 3). Hence at low temperatures (T 100 K) most electrons do not have sufficient energy to emit optical phonons. In addition, the thermal occupation number Nq of optical phonons is very low, and consequently the probability of an electron absorbing an optical phonon is small also. Thus, optical phonon scattering processes are negligible at low temperatures. On the other hand, at room temperature, where there are sufficient high-energy electrons to emit optical phonons, they tend to dominate over acoustic phonon scattering. This is particularly true in polar semiconductors, where the Fröhlich electron–phonon interaction (Sect. 3.3.5 and Fig. 5.3) can be very strong. The distribution of final electronic states after optical phonon scattering is shown schematically in Fig. 5.1b. While scattering by acoustic phonons relaxes mainly the electron momentum, scattering by optical phonons contributes to both momentum and energy relaxation. The LO phonon scattering probability (PLO ) corresponding to PLA (k) in (5.42) can be shown to be [Ref. 5.2, p. 115, 5.10] ∞ q2 2 PLO ∝ q dq d(cos £) NLO ‰[Ek (Ek ELO )] 2 2 2 (q q0 ) 0 0 (NLO 1)‰[Ek (Ek ELO )] , (5.48) where NLO and ELO are, respectively, the LO phonon occupation number and energy. For simplicity we have assumed that the LO phonon is dispersionless, which is usually a good approximation since only phonons with q ∼ q0 contribute significantly to (5.48). The term inside the first set of parentheses comes from the Fröhlich matrix element, including screening. The terms proportional to NLO and NLO 1 are identified with phonon absorption and emission, respectively. As a result of wavevector conservation in (5.35), (5.48) can be expressed as ∞ q4 2 q PLO ∝ dq NLO ‰ (k cos £ q) ELO 2m (q2 q20 )2 0 0 2 q (NLO 1)‰ (k cos £ q) ELO d(cos £). 2m Integrating over £ results in the following expression for PLO : q1 max q2 max q3 q3 dq (NLO 1) dq, PLO ∝ NLO (q2 q20 )2 (q2 q20 )2 q1 min (5.49) (5.50) q2 min where qi max and qi min are, respectively, the maximum and minumum values of the LO phonon wave vector for phonon absorption (i 1) and phonon emission (i 2) (Problem 5.5). From Fig. 5.1b one can easily identify the 5.2 Carrier Mobility for a Nondegenerate Electron Gas electron final states corresponding to the minumum and maximum values of q. Since qi min is nonzero for optical phonons, the screening wave vector in (5.50) is not as important as for piezoelectric acoustic phonons, except in the case of highly doped semiconductors. If we neglect q0 in (5.50), PLO decreases as 1/q and scattering by small-q LO phonons is more likely than by large-q LO phonons. In contrast to the case of acoustic phonon scattering, scattering between electrons and LO phonons tends to relax the electron energy rather than its momentum. The momentum relaxation time of an electron due to LO phonon scattering can be deduced from (5.50) using (5.33). The result is [Ref. 5.2, p. 118] 1/2 1/2 1 Ek ELO Ek ELO ∝ NLO (NLO 1) Ùm Ek Ek 1/2 ELO E k NLO sinh1 Ek ELO 1/2 1 Ek ELO (NLO 1) sinh . (5.51) ELO A plot of the relaxation time for electrons in GaAs due to LO phonon scattering (via the Fröhlich interaction) is shown in Fig. 5.3 under the label Ùpo . Typically the relaxation time due to scattering by LO phonons is less than 1 ps. c) Intervalley Scattering The role of intervalley scattering in electron relaxation is different in direct and indirect bandgap semiconductors. In direct bandgap semiconductors, such as GaAs and InP, intervalley scattering is important only for electrons with sufficient energy to scatter into the higher conduction band valleys. Since these valleys are several tenths of an eV above the conduction band minimum at zone center, in these semiconductors intervalley scattering is important only for their hot electron transport properties. This will be discussed in more detail in Sect. 5.4. The situation is quite different in indirect bandgap semiconductors, such as Si and Ge. In these materials the electrons are located in conduction band minima which are not at zone center and are degenerate. In addition to intraband scattering by phonons, electrons can be scattered from one degenerate valley to another via intervalley scattering. In both materials the latter scattering processes turn out to be more important than the intraband processes in relaxing the momentum and energy of conduction electrons. In this section we shall consider only intervalley scattering of electrons in indirect bandgap semiconductors. As an example, we discuss the case of Si, where the conduction band minima occur along the six equivalent [100] directions (¢1 ) at about 0.83 of the distance from zone center to the zone edge. Electrons in one of the minima (say in the [100] direction) can be scattered either into the valley along the [100] direction or into one of the four equivalent [0,±1,0] and [0,0,±1] valleys (Fig. 5.4a). The former process is known as a g-process and the phonon involved is known as a g-phonon while the latter processes are called 215 216 5. Electrical Transport (b) (a) [001] [001] g Û f = Ûmax K111 11 [010] f [100] ο Ûg [001] = 1.2 ∆K f ∼ [110] K 001 = 1.7 ∆ Kg ∼ Fig. 5.4a,b. Schematic diagram of the intervalley scattering processes for electrons in the conduction band minimum of Si showing the phonon wave vectors involved in the g- and f-processes [Refs. 5.2 (Fig. 3.16), 5.11]. ¢K is given in units of (2/a0 ). f-processes. For both processes the electron valley after scattering can lie in the same Brillouin zone or in an adjacent one (Fig. 5.4b). The former process is known as a normal process, the latter as an umklapp process [Ref. 5.7, p. 146]. As shown in Fig. 5.4b, the wave vector ¢Kg (note that, in order to show both the g- and f-phonons in this figure, the g-phonon is now chosen along the [001] direction) of the phonon mediating the normal g-process is about 1.7 times the Brillouin zone length along the X axis. On the other hand, the phonon wave vector (Û Ûg ) of the umklapp g-process is only ≈ 0.34 of the Brillouin zone edge (measured from the zone center) in the [001] direction. The reciprocal lattice vector involved in the g umklapp process, denoted by K001 , is also along the X direction. The f-phonon ¢Kf is approximately equal to 1.2 times (2/a0 )(1, ±1, 0), a0 being the size of the unit cube in Si. The wave vector lies outside the first Brillouin zone. Hence both g- and f-processes require phonons with wave vectors outside the first Brillouin zone. Thus in the reduced zone scheme only umklapp processes are allowed. Combined with a reciprocal lattice vector K111 (2/a0 )(1, 1, 1), the resultant umklapp wave vector Û f is about 11◦ off the [001] direction (™1 symmetry) with length almost exactly equal to that of the zone-boundary value along that direction (Fig. 5.4b). The symmetries and energies of intervalley phonon modes allowed by group theory in Si are (see Fig. 3.1 and [5.2], p. 110) g-process: ¢2 (LO), 63 meV f-processes: ™1 (LA, TO; 45 and 57 meV; an average of 54 eV was used in [5.2], p. 110). The corresponding selection rules for intervalley scattering in III–V compounds have been derived by Birman et al. [5.12]. In order to fit the temperature dependence of the mobility of Si it was found necessary to include a contribution to intervalley scattering from a phonon of 16 meV energy [5.11]. According to the phonon dispersion curves 5.2 Carrier Mobility for a Nondegenerate Electron Gas of Si, this 16 meV phonon (Fig. 3.1; 16 meV ⇔ 130 cm1 ⇔ 3.9 THz) can be attributed to an LA mode with wave vector about 0.3 times the zone boundary, corresponding to the g umklap process of Fig. 5.4. This process is strictly speaking forbidden since the corresponding matrix element has ¢1 ⊗ ¢1 ⊗ ¢2 ¢2 symmetry and therefore vanishes. The presence of such processes, required by the first of the resistivity vs T curve has been explained by expanding the electron–phonon interaction as a function of phonon wave vector beyond the lowest (zeroth) order term [5.13]. Except for the higher order electron–phonon interactions, the calculation of the intervalley scattering rates is similar, in principle, to that for acoustic phonons in direct bandgap semiconductors. In practice the calculation is complicated by the anisotropy in the electron mass in Si. Assuming for the sake of simplicity an isotropic mass, we find that the intervalley scattering rate due to the zeroth-order electron– phonon interaction is given by (1/Ùiv ) ∝ Nq (Ek Ep )1/2 (Nq 1)(Ek Ep )1/2 U(Ek Ep ), where Ep is the phonon energy and U(x) is the step function: 0 for x 0, U(x) 1 for x ≥ 0. (5.52a) (5.52b) Readers interested in the contribution to the scattering rate from the first-order electron–phonon interaction should consult either [5.13] or [Ref. 5.2, p. 110]. d) Scattering by Impurities Typically a semiconductor contains defects such as impurities and dislocations. Carriers are scattered elastically by these defects, the details of the scattering mechanism depending on the defect involved. Here we will concern ourselves with scattering by the most common kind of defects, namely, charged impurities. Free carriers are produced in semiconductors by ionization of shallow impurities (except in the intrinsic case where they are produced by thermal ionization across the gap). As a result, free carriers will, in principle, always be scattered by the ionized impurities they leave behind. A way to avoid this will be presented in the next section. Our approach to calculating impurity scattering rates will be different from the approach for phonon scattering. Phonons are quantized lattice waves with well-defined wave vectors and therefore they scatter electrons from one Bloch state to another. Impurity potentials are localized in space. Hence they do not scatter electrons into well-defined Bloch states. This problem can be treated quantum mechanically using scattering theory and what is referred to as the Brooks–Herring approach [Refs. 5.2, p. 143; 5.14]. In this approach the impurity potential is approximated by a screened Coulomb potential. The screening can be either Debye [with the screening length of (5.46)] or Thomas–Fermi [Ref. 5.7, p. 266]. The scattering cross section is calculated within the Born approximation. The quantum mechanical results obtained by Brooks [5.14] are not too different from the classical results obtained earlier by Conwell and Weisskopf [5.15] so we shall first consider the Conwell–Weisskopf approach. 217 218 5. Electrical Transport Fig. 5.5. Coulomb scattering of an electron by a positively charged ion. The impact parameter b and the length K are discussed in the text. [Ref. 5.2, Fig. 4.1] e- b Ze K + Θ Conwell–Weisskopf Approach. In this approach an electron is assumed to be scattered classically via Coulomb interaction by an impurity ion with charge Ze. The corresponding scattering cross section is calculated in exactly the same way as for the Rutherford scattering of · particles [5.16]. The scattering geometry of this problem is shown schematically in Fig. 5.5. The scattering cross section Û as a function of the scattering angle £ is given by Û(£)dø 2b d | b | (5.53) where dø is an element of solid angle, b is known as the impact parameter. and d | b | is the change in | b | required to cover the solid angle dø. The impact parameter and the solid angle dø are related to the scattering angle by b K cot(£/2); dø 2 sin £d£ where K is a characteristic distance defined by Ze2 K mv2k (5.54) (5.55) and vk is the velocity of an electron with energy Ek mv2k /2. If dø and d | b | are expressed in terms of d£, (5.53) can be simplified to 2 K . (5.56) Û(£) 2 sin2 (£/2) The well-known dependence of Û on the electron velocity to the power of 4 in Rutherford scattering is contained in the term K2 . The scattering rate R (per unit time) of particles traveling with velocity v by N scattering centers per unit volume, each with scattering cross section Û, is given by R NÛv. (5.57) Since scattering by impurities relaxes the momenta of carriers, but not their energy, we can define a momentum relaxation time Ùi due to impurity scattering by (5.58) 1/Ùi Ni vk Û(£)(1 cos £)2 sin £ d£, where Ni is the concentration of ionized impurities. Within the integrand, the term (1 cos £) is the fractional change in the electron momentum due to scattering event and the term 2 sin £ d£ represents integration of the solid 5.2 Carrier Mobility for a Nondegenerate Electron Gas angle ø. In principle, £ has to be integrated from 0 to . The divergence of (5.56) at £ 0 makes the integral in (5.58) diverge. This problem can be avoided by arguing that b cannot be larger than a maximum value bmax equal to half of the average separation between the ionized impurities: bmax 12 Ni1/3 . (5.59) As a result the minimum value of £ allowable in (5.58) is £m 2 cot1 (bmax /K). (5.60) Integrating (5.58) with the condition (5.60) we obtain the following expression for 1/Ùi : 1/Ùi 4Ni vk K2 ln[sin(£m /2)] or, in terms of the electron energy Ek , 1/2 2 ⎡ 2 ⎤ 2Ek Ze2 E 1 k ⎦. 2Ni ln⎣1 Ùi m 2Ek Ni1/3 Ze2 (5.61) (5.62) The scattering rate of electrons by ionized impurities is independent of temperature and depends on the electron energy approximately like Ek3/2 due to the dependence of the scattering cross section on the particle velocity in (5.56). As a result, ionized impurity scattering tends to become dominant at low temperature where the electron energies are small and, moreover, phonon scattering freezes out. Brooks–Herring Approach. As mentioned earlier, in the Brooks–Herring approach the scattering rate of electrons by ionized impurities is calculated quantum mechanically. If the effect of screening of the impurity potentials by free carriers is taken care of by introducing a screening wave vector q0 [which is the reciprocal of the Debye screening length] defined in (5.46), then (5.56) must be replaced by ⎡ ⎤2 ⎢ Û(£) ⎣ K ⎥ (5.63) q 2 ⎦ . £ 0 2 sin2 2 2k In this way the divergence in Û(£) at £ 0 in (5.56) is automatically avoided without introducing, in a somewhat artificial way, the maximum impact parameter bmax . The electron mobility (assuming that the only scattering process is by ionized impurities) calculated by the Brooks–Herring approach (BH for short) is compared with that calculated by the Conwell-Weisskopf approach (curves labeled CW) in Fig. 5.6 as a function of carrier density for a hypothetical uncompensated semiconductor. Except for high carrier concentrations the two results are almost identical. However, for very high carrier concentrations even the Brooks–Herring approach breaks down. The question of screening at high carrier concentrations has been studied by many researchers and a detailed account can be found in [Ref. 5.2, pp. 145–152]. 219 220 5. Electrical Transport CW 10 7 BH CW cm ____2 Vs 10 BH µ 6 300 K 10 5 77 K n=NI 13 10 14 10 BH CW 1015 1016 Concentration [cm–3] 17 10 1018 Fig. 5.6. Mobility of electrons calculated by considering only ionized impurity scattering as a function of impurity concentration. The curves labeled CW have been calculated classically by Conwell and Weisskopf [5.15]. The curves labeled BH have been calculated quantum mechanically using the Brooks–Herring approach [5.14] 5.2.5 Temperature Dependence of Mobilities We are now in a position to discuss the temperature dependence of carrier mobilities in a nondegenerate semiconductor with parabolic bands. From the scattering rates of an electron in a band we first calculate the electron lifetime Ù(Ek ) by taking the reciprocal of the total scattering rate. Next we substitute Ù(Ek ) into (5.27) to obtain Ù. Since the different scattering mechanisms have different dependences on electron energy and temperature, they result in different temperature dependences of the mobility. By comparing the measured temperature dependence of the mobility with theory one can determine the contributions from the different scattering mechanisms. To facilitate this comparison we note that if Ù(Ek ) can be expressed as a function of Ek and T as being proportional to Ekn and T m then E3/2 exp(E/kB T)Ù(E)dE ∝ T mn5/2 (5.64) and Ù ∝ T mn . (5.65) Using the energy and temperature dependence of the scattering rate obtained in the previous section we can conclude that • • • Ì ∝ T 3/2 for acoustic phonon (deformation potential) scattering; Ì ∝ T 1/2 for acoustic phonon (piezoelectric) scattering; Ì ∝ T 3/2 for ionized impurity scattering. 5.2 Carrier Mobility for a Nondegenerate Electron Gas 10 5 10 5 (b) 10 Mobility [cm2/V s] Mobility [cm2 /V s] (a) 4 A 10 190 K 4 630 K 10 3 10 100 200 50 Temperature [K] 500 3 50 100 200 Temperature [K] 500 Fig. 5.7a,b. Temperature dependence of mobility in n-type Si. The solid curve in (a) represents the experimental results. The curves in (b) are the relative contributions to the mobility from scattering by different kinds of phonons. Curve A represents the contribution from intravalley acoustic phonon scattering while the other two curves represent contributions from intervalley scattering by phonons whose energies correspond to temperatures of 190 K (or 16 meV) and 630 K (54 meV). The filled circles in (a) display a fit to the experimental curve using the theoretical curves in (b) [5.13] Figure 5.7 shows the temperature dependence of the mobility in intrinsic n-type Si. The experimental results [solid curve in (a)] can be explained by a combination of intravalley scattering by acoustic phonons and intervalley scattering by two phonons of energies 16 meV (129 cm1 , TA) and 54 meV (436 cm1 , LO). The electron–phonon interaction for the LO intervalley scattering is symmetry allowed for phonons along ¢ while that for the TA phonon is forbidden. Ferry [5.13] attributed the nonvanishing value of the latter to contributions from phonons close to but not exactly along ¢. Figure 5.8 shows the mobility in n-type Si for various donor concentrations. The shape of the experimental curves at high donor concentrations can be explained by the dominance of ionized impurity scattering at low temperatures, as sketched in the inset. The experimental temperature dependence of mobility in n-type GaAs is compared with theory in Fig. 5.9. Again the experimental results can be understood in terms of ionized impurity scattering at low temperatures and phonon scattering at higher temperatures. At room temperature, the scattering of electrons in GaAs is dominated by the polar LO phonon processes. 221 5. Electrical Transport 10 4 LOG µn ND=1014cm–3 µn [cm2/(Vs)] 10 10 (T)3/2 (T)–3/2 Impurity Lattice scattering scattering 16 3 10 17 1018 10 1019 2 50 100 200 T [K] 500 1000 Fig. 5.8. Temperature dependence of mobilities in n-type Si for a series of samples with different electron concentrations. The inset sketches the temperature dependence due to lattice and impurity scattering [5.17] Neutral impurity 108 Hall mobility [cm2V–1s–1] 222 Ionized impurity 107 106 Piezoelectric 105 Deformation potential 104 Polar 103 1 10 102 T [K] 103 104 Fig. 5.9. Temperature dependence of mobility in n-type GaAs determined by Hall measurements (points) by Stillman et al. [5.18]. The dashed curves are the corresponding contributions from various scattering mechanisms calculated by Fletcher and Butcher [5.19] (from [5.19]) 5.3 Modulation Doping 5.3 Modulation Doping From the temperature dependence of mobilities in Si and GaAs we conclude that scattering by ionized impurities ultimately limits the carrier mobility at low temperatures. This limitation can be circumvented by using the method of modulation doping proposed by Störmer et al. [5.20]. The idea behind modulation doping is illustrated in Fig. 5.10. Two materials with almost identical lattice constants but different bandgaps are grown on top of each other to form a heterojunction (see Chap. 9). One example of a well-behaved heterojunction used commonly in the fabrication of semiconductor laser diodes is GaAs/Alx Ga1x As (other examples will be discussed in Chap. 9). The lattice constants of these two semiconductors differ by less than 1 %. The bandgap of AlGaAs with less than 40 % of Al is direct and larger than that of GaAs. The difference between their bandgaps is divided in an approximately 60/40 split between the conduction and valence bands (for further discussions see Chap. 9). The results are very abrupt discontinuities, known as band offsets, in their energy bands at the interface, as shown schematically in Fig. 5.10. If the material with the larger bandgap (AlGaAs) is then doped with shallow donors, the Fermi level is shifted from the middle of the bandgap of AlGaAs to the donor level. In order to maintain a constant chemical potential throughout the two materials, electrons will flow from AlGaAs to GaAs. This causes the band edges to bend at the interface as shown in Fig. 5.10, a phenomenon known as band bending. We shall show in Sect. 8.3.3 that band bending also occurs near the surface of semiconductors as a result of the existence of surface states. Due to band bending the electrons in GaAs are now confined by an approximately triangular potential near the interface and form a two-dimensional (2D) electron gas. These 2D electrons are physically separated from the ion- n-AlGaAs non-doped GaAs 2-DEG 1.2 eV Gate 1.8 eV Semi-insulating GaAs substrate Ionized Donors 2-DEG Ec EF 2-DEG = Two-dimensional electron gas Metal AlGaAs GaAs Fig. 5.10. The structure and band diagram of a modulation-doped heterojunction between GaAs and n-AlGaAs. Ec and EF represent, respectively, the conduction band edge and the Fermi energy 223 5. Electrical Transport ized impurities in AlGaAs, hence they are only weakly scattered by the charged impurities. This method constitutes the modulation doping technique mentioned above [5.20]. If scattering by interface defects can be avoided, the mobility of the 2D electron gas in a modulation-doped sample can approach the theoretical limit set by phonon scattering in the absence of impurity scattering. Using this method carrier mobilities exceeding 106 cm2 /(Vs) have been achieved in GaAs. Figure 5.11 shows the temperature dependence of the mobility of a 2D electron gas at a GaAs/Al0.3 Ga0.7 As heterojunction. Notice that unlike the mobility depicted in Fig. 5.9, the mobility in Fig. 5.11 does not decrease when the temperature is lowered towards zero, as would be expected if scattering by ionized impurities were present. However, some residual scattering by the potential of the impurities located inside the Al0.3 Ga0.7 As is still present; it is labeled “remote impurities” in Fig. 5.11. It approaches a small constant value at low temperatures so that modulation doping improves the carrier mobility when phonon scattering is frozen. Since electron scattering in these samples is dominated by phonons (except at very low temperatures), it is possible to determine the absolute volume deformation potentials of LA Background impurity Deformation potential + piezoelectric Optical phonon Remote impurity Inherent limit 6 10 Total Mobility µe [cm2/(Vs)] 224 Absolute limit 10 5 Ga0.7Al0.3As-GaAs o d = 200 A 10 4 1 10 Temperature [K] 100 Fig. 5.11. Mobility of a two-dimensional electron gas in a modulation-doped GaAs/ Ga0.7 Al0.3 As heterojunction as a function of temperature. The closed circles indicate the experimental results. The various broken curves represent calculated contributions to the mobility from different scattering mechanisms. The solid curve represents the sum of all those contributions [5.21] 5.4 High-Field Transport and Hot Carrier Effects phonons quite accurately from the temperature dependence of the electron mobility [5.21]. Modulation doping is now utilized in the fabrication of field-effect transistors with very high mobility. These transistors are known either as MODFETs (which stands for modulation-doped field-effect transistors) or HEMTs (high electron mobility transistors) [Ref. 5.22, p. 698]. 5.4 High-Field Transport and Hot Carrier Effects The formalism developed in Sect. 5.1 for calculating the carrier drift velocity leads to Ohm’s law and is valid only at low electric fields. In most semiconductors we find that Ohm’s law breaks down at electric fields exceeding 104 V/cm. In this section we shall study the effect of high electric fields on carrier distributions and also other transport phenomena which can occur under high electric fields. As we pointed out in the introduction, these high-field effects can only be calculated numerically [5.4, 5.23] and therefore our discussions will necessarily be qualitative. The main difficulty in these calculations results from the very fast rates at which carriers gain energy under the high electric field. When these rates are larger than those for energy loss to the lattice, the carriers are no longer at thermal equilibrium with the lattice. There are two possible scenarios for these nonequilibrium situations. In one case, carriers are in thermal equilbrium among themselves but not with the phonons. In this situation carriers can be said to be in quasi thermal equilibrium. Their distribution can still be characterized by a Fermi–Dirac distribution, albeit with a temperature different from the sample temperature (defined as that of the phonons which are in equilibrium with the thermal sink to which the sample is attached). Usually these carriers have higher temperatures than the lattice, hence they are known as hot carriers. In the second scenario, the carriers cannot be described by an equilibrium distribution and therefore do not have a well-defined temperature. In the literature one may also find that these nonthermal equilibrium carriers are loosely referred to as hot carriers. More precisely these carriers should be called nonequilibrium carriers. Hot-carrier effects are important in the operation of many semiconductors devices such as laser diodes, Gunn oscillators, and short-channel field-effect transistors [Ref. 5.22, pp. 698–720]. The hot carriers in these devices are generated electrically by a high field or by injection through a barrier. Hot carriers can also be produced optically by high intensity photon beams such as in laser annealing [5.24]. What conditions determine whether a carrier distribution is an equilibrium one or not? The answer depends on the magnitude of the various time scales which characterize the interaction among the carriers and their interaction with the lattice relative to the carrier lifetime. Let us define the time it takes a nonequilibrium carrier distribution to relax to equilibrium as the thermal- 225 5. Electrical Transport ization time. Processes contributing to thermalization are carrier–carrier and carrier–phonon interactions. As shown in Fig. 5.3, carrier–phonon interaction times can range from 0.1 ps (for polar optical phonons and for phonons in intervalley scattering) to tens of picoseconds (for acoustic phonons). Carrier– carrier interaction times depend strongly on carrier density. This has been measured optically in GaAs. At high densities (1018 cm3 ) carriers thermalize in times as short as femtoseconds (equal to 1015 s and abbreviated as fs) [5.25]. Thus the thermalization time is determined by carrier–carrier interaction at high carrier densities. At low densities, it is of the order of the shortest carrier–phonon interaction time. Often carriers have a finite lifetime because they can be trapped by defects. If both electrons and holes are present, the carrier lifetime is limited by recombination (Chap. 7). In samples with a very high density of defects (such as amorphous semiconductors) carrier lifetimes can be picoseconds or less. Since the carrier lifetime determines the amount of time carriers have to thermalize, a distribution is a nonequilibrium one when the carrier lifetime is shorter than the thermalization time. A transient nonequilibrium situation can also be created by perturbing a carrier distribution with a disturbance which lasts for less than the thermalization time. The properties of hot carriers can be different from those of equilibrium carriers. One example of this difference is the dependence of the drift velocity on electric field. Figure 5.12 shows the drift velocity in Si and GaAs as a function of electric field. At fields below 103 V/cm, the carriers obey Ohm’s law, namely, the drift velocity increases linearly with the electric field. At higher fields the carrier velocity increases sublinearly with field and saturates at a velocity of about 107 cm/s. This leveling off of the carrier drift velocity at high field is known as velocity saturation. n-Type GaAs shows a more complicated behavior in that its velocity has a maximum above the saturation velocity. This phenomenon is known as velocity overshoot (Fig. 5.12) and is found usually only in a few n-type semiconductors such as GaAs, InP, and InGaAs. For 10 8 Drift velocity [cm/s] 226 GaAs (Electrons) 10 Si (Electrons) 7 Si (Holes) 106 GaAs (Holes) T=300K 10 5 10 2 10 3 10 4 Electric field [V/cm] 10 5 10 6 Fig. 5.12. Dependence of drift velocity on electric field for electrons and holes in Si and GaAs [5.17]. Notice the velocity overshoot for electrons in GaAs 5.4 High-Field Transport and Hot Carrier Effects electric fields between 3 × 103 V/cm and 2 × 105 V/cm, the velocity of electrons in GaAs decreases with increasing electric field. This phenomenon is known as negative differential resistivity. We shall consider these high field behaviors of carriers separately. 5.4.1 Velocity Saturation The Boltzmann equation (5.15) is difficult to solve under high-field conditions, for which the carrier distribution can be a nonequilibrium one. One simplifying approach is to expand the carrier distribution as a function of carrier velocity in a Taylor series. This leads to a field-dependent mobility of the form Ì(F) Ì(0) ‚F 2 . . . . (5.66) Carriers are sometimes referred to as warm carriers when only the terms up to ‚F 2 are important [Ref. 5.26, p. 102]. As mentioned in Sect. 5.1, hot carrier properties are usually calculated numerically using a Monte Carlo simulation method; a discussion of these calculations is beyond the scope of this book [5.27]. Instead, we will present a highly simplified explanation of why the drift velocity in most semiconductors saturates at more or less the same value of 107 cm/s. Within the quasi-classical approach that we adopted in Sect. 5.1, carriers in a semiconductor are regarded as free particles with effective mass m∗ . Their average energy E can be defined as E m∗ v2d /2, where vd is their drift velocity. The saturation in vd under a high electric field therefore implies that the average energy of the carriers no longer increases with electric field at high field strengths. This can be understood if there is an energy loss mechanism that becomes dominant at large E. Scattering with optical phonons is the most obvious candidate. A simple-minded picture of what happens is as follows. At low fields, carriers are scattered elastically by acoustic phonons and these processes lead to momentum relaxation of the carriers. The carrier distribution is essentially a “drifted” equilibrium distribution (Problem 5.2). At intermediate fields, E becomes large enough for some of the carriers in the high-energy tail of the distribution to start to scatter inelastically with optical phonons. This distorts the carrier distribution and causes E to increase sublinearly with the field. At still higher fields, more of the carriers are scattered inelastically, until energy relaxation processes dominate. When the rate at which carriers gain energy from the field is balanced exactly by the rate of energy loss via optical phonon emission, E (and also vd ) becomes independent of electric field. The saturation velocity vs can thus be deduced from the energy-loss rate equation Eop dE , (5.67) eFvs dt Ùe where Eop is the optical phonon energy and Ùe is the energy relaxation time. A corresponding rate equation for momentum relaxation is 227 228 5. Electrical Transport m∗ vs d(m∗ vs ) eF , (5.68) dt Ùm where Ùm is the momentum relaxation time. Assuming that scattering by optical phonons is the dominant process at high fields, both Ùe and Ùm are equal to the optical phonon scattering time Ùop . In the steady state, dE/dt 0 and d(m∗ vs )/dt 0. Therefore the solution for vs from (5.67) and (5.68) is simply vs (Eop /m∗ )1/2 . (5.69) Notice that Ùop is absent in the expression for vs . For most tetrahedrally bonded semiconductors, the optical phonon energy is of the order of 40 meV and the carrier effective mass m∗ is of the order of 0.1m0 . Substituting these values into (5.69) we obtain vs ≈ 2 × 107 cm/s. This explains both the constancy and order of magnitude of the experimental saturation velocities in many semiconductors. 5.4.2 Negative Differential Resistance Electrical resistance is normally associated with dissipation of electrical energy in the form of heat in a conductor. Thus a negative electrical resistance suggests that electrical energy can be “created” in such a medium. However, it should be noted that a negative differential resistance (often abbreviated as NDR) is only a negative AC resistance. This means that NDR can be used in designing an AC amplifier only. When we study electronics we learn that an amplifier coupled with a properly designed positive feedback circuit can be made into an oscillator. Thus one important application of materials exhibiting NDR is in the construction of high-frequency (typically microwave frequencies) oscillators. The Esaki tunnel diode1 is an example of a device exhibiting NDR [Ref. 5.22, pp. 641–643]. More recently resonant tunneling diodes (see Chap. 9 for further discussions) have also been shown to exhibit NDR [5.28]. The principles behind the NDR in these devices are different from those of n-type GaAs under a high electric field. To understand the NDR in GaAs we have to refer to the conduction band structure shown in Fig. 2.14. While the lowest conduction band minimum in GaAs occurs at the Brillouin zone center, there are also conduction band minima at the L points, which lie about 0.3 eV higher in energy. The effective mass of electrons in these L valleys is not isotropic. For motion along the axis of the valleys, the longitudinal mass is 1.9m0 while the transverse mass is 0.075m0 [5.29]. These masses are much larger than the effective mass (to be denoted by m∗° ) of 0.067m0 for electrons in the ° valley. On the basis of (5.12) we expect the mobility of electrons in the ° valley (to be denoted by Ì° ) to be larger than that of electrons in the L valleys (denoted by ÌL ). At low electric fields all the electrons are in the ° valley and the electron mobility is high 1 Leo Esaki shared the 1973 Nobel Prize in Physics for his discovery of the phenomenon of electron tunneling in the diodes named after him. 5.4 High-Field Transport and Hot Carrier Effects because of the small m∗° . As the field is increased, electrons gain energy until some of them have sufficient energy to transfer via intervalley scattering to the L valleys. This intervalley scattering now competes with intravalley relaxation via scattering by optical phonons. In GaAs the time it takes an electron to emit a LO phonon via the Fröhlich interaction (Fig. 5.3) is about 200 fs. The corresponding ° to L intervalley scattering time at room temperature is less than 100 fs [5.30, 31]. However, the time it takes the electron to return to the ° valley is of the order of picoseconds because the density of states of the ° valley is much smaller than that of L valleys. As a result, for high enough electrics fields, we expect that a significant fraction of the electrons will be excited into the L valleys and the electron conductivity will become Û e(N° Ì° NL ÌL ), (5.70) where N° and NL are, respectively, the number of electrons in the ° and L valleys. Since ÌL is smaller than Ì° , the conductivity decreases with increasing field, leading to a negative differential resistance. The field dependence of the electron drift velocity in GaAs deduced from the above picture is shown in Fig. 5.13. At even higher fields (E Eb in Fig. 5.13) there will be more electrons in the L valleys than in the ° valley because the former have larger density of states and the intervalley transfer of electron stops. Now the electrons in the L valleys are accelerated by the external field and their velocities increase linearly with field again as shown schematically in Fig. 5.13. The threshold field Ec at which the drift velocity begins to decrease is commonly referred to as the critical field. It should be noted that at one time it was thought that the NDR in GaAs was caused by transfer of electrons to the X valleys. After it was demonstrated that the L valleys were lower in energy than the X valleys [5.32], transfer to the L valleys became accepted as the mechanism responsible for NDR in GaAs. Velocity µΓE µLE 0 Ea Ec Eb Electric field Fig. 5.13. Sketch of the dependence of the drift velocity of electrons in GaAs on electric field based on the qualitative model in Sect. 5.4.2 229 230 5. Electrical Transport In order to observe NDR it is necessary to satisfy the following conditions. There must be higher energy valleys to which carriers can be excited under high electric field. The mobility of carriers in these higher energy valleys should be much smaller than in the lower energy valleys. The separation of the higher energy valleys from the lower energy valleys should be much larger than kB T, where T is the device operation temperature, in order that the higher valleys are not populated thermally. However, this separation should not be larger than the bandgap. Otherwise, before the carriers have acquired enough energy from the field to transfer to the higher valleys they can already excite carriers from the valence band into the conduction band via impact ionization [Ref. 5.22, pp. 322–384]. These conditions are satisfied by the conduction bands of GaAs, InP [5.26], and the ternary alloy Inx Ga1x As (x 0.5). 5.4.3 Gunn Effect In 1963 J. B. Gunn [5.33, 34] discovered that when a thin sample (thickness of the order 10 Ìm) of n-type GaAs is subjected to a high voltage (such that the electric field exceeds the critical field Ec in GaAs), the current through the sample spontaneously breaks up into oscillations at microwave frequencies as shown in Fig. 5.14. The frequency of oscillation is inversely proportional to the length of the sample across which the field is applied. As will be shown below, the frequency of oscillation turns out to be equal to the saturation velocity vs divided by the sample length. For sample lengths of the order of 10 Ìm and Fig. 5.14. Oscilloscope traces of Gunn oscillations in a thin piece of GaAs under a high electric field. Current waveform produced by the application of a voltage pulse of 16 V amplitude and 10 ns duration to a specimen of n-type GaAs 2.5 × 103 cm in length. The frequency of the oscillating component is 4.5 GHz. Lower trace: 2 ns/cm horizontally, 0.23 A/cm vertically. Upper trace: expanded view of lower trace [5.33] 5.4 High-Field Transport and Hot Carrier Effects vs equal to 107 cm/s, the oscillation frequency is of the order of 1010 Hz, i. e. 10 gigahertz2 . Electromagnetic waves of such high frequencies are known as microwaves. Hence the obvious application of the Gunn effect is the fabrication of microwave generators known as Gunn diodes. The Gunn effect is one example of how NDR can lead to high-frequency oscillations. To understand this effect qualitatively [5.35], we will assume that the field dependence of the drift velocity in n-type GaAs has the simple form shown schematically in Fig. 5.15a. Suppose a constant high voltage is applied to the sample so that carriers drift from the left to right as shown schematically in Fig. 5.15b. We assume that the electric field is maintained at a value slightly below the threshold field Ec . Due to fluctuations in the electric field at finite temperatures, a small region labeled D in Fig. 5.15b has a field slightly above Ec at time t 0. The carriers on both sides of D have now higher drift velocities than carriers inside D. As a result, carriers will pile up on the left hand side in D while the carrier density will drop on its right hand side. This charge pile-up in D at t 0 leads to an increase in electric field inside D and a decreasing field outside, as shown in Fig. 5.15b. Because of the NDR for (a) (b) υd E D Domain Carrier drift Ec υs t=0 t >> 0 0 Ec E 0 d (c) Carrier density Fig. 5.15. (a) A highly simplified field dependence of the drift velocity in GaAs. (b) Spatial dependence of the electric field in a GaAs sample biased near the critical field Ec showing the build-up of a domain D inside the sample as a function of time. (c) Charge density variation across the GaAs sample showing the charge pile-up and depletion in the vicinity of the domain D Charge pile-up Charge depletion D 0 2 d The unit of frequency is hertz (Hz), named after Heinrich Hertz who produced and detected radio waves in 1888. One hertz is equal to one cycle per second. 231 232 5. Electrical Transport fields larger than Ec , the increase in the field inside D leads to further slowing down of electrons inside D and hence more charge pile-up. This process, once started, will continue until most of the applied field is across D, as shown in the dotted curve in Fig. 5.15b for t 0. Figure 5.15c displays the charge distribution along the length of the sample. The region D where the electric field is high is known as a domain. Only one domain can exist inside the sample at one time since most of the applied voltage will be across this domain. The most likely place for domains to be formed is the cathode, since the field fluctuations tend to be largest there. Under the influence of the applied voltage this domain will drift across the sample with the saturation velocity until it reaches the anode, thus giving rise to a periodic oscillation in current. The frequency of this oscillation is equal to vs divided by the length of the sample. As a result of this oscillatory current, electromagnetic waves are radiated from the sample. From this simple description it is clear that Gunn oscillators are very efficient, yet miniature, microwave generators. 5.5 Magneto-Transport and the Hall Effect We conclude this chapter by discussing the electric current induced in a sample in the presence of both electric and magnetic fields. As we pointed out in Sect. 5.1, in a cubic crystal the second-rank conductivity tensor Û can usually be represented by a diagonal matrix. This is not true when a magnetic field is present. In this case the conductivity tensor contains off-diagonal elements that are linearly dependent on the magnetic field. In this section we will derive this magneto-conductivity tensor and use the result to study an important phenomenon known as the Hall effect. Our approach in this section will be classical, leaving a quantum mechanical treatment to Chap. 9, where we shall consider the quantum Hall effect in two-dimensional electron gases. 5.5.1 Magneto-Conductivity Tensor We shall first assume that the sample is an infinite, cubic and nonmagnetic crystal. Without loss of generality we can suppose that a magnetic field Bz is applied to the sample along the z axis, while an electric field F is applied along any arbitrary direction. To calculate the resultant current we use the quasi-classical approach adopted in Sect. 5.1. In the presence of both electric and magnetic fields, the equation of motion for the electrons (5.4) is replaced by the Lorentz equation:∗ m∗ ∗ m∗ dr d2 r (e) F (v × B/c) , 2 dt Ù dt (5.71) The equations in this section are transformed into SI units by deleting the velocity of light c. 5.5 Magneto-Transport and the Hall Effect where c is the speed of light in vacuum. In (5.71) we have assumed that m∗ and Ù are isotropic. For generalizations see [5.36, 37]. Under steady-state conditions, dv/dt d2 r/dt2 0, we obtain (5.72) (m∗ /Ù)vd (e) F (vd × B/c) for the electron drift velocity vd . In terms of its components along the x, y, and z axes, the three components of this equation can be written as (5.73a) (m∗ /Ù)vd,x (e) Fx (vd,y Bz /c) , (5.73b) (m∗ /Ù)vd,y (e) Fy (vd,x Bz /c) , (m∗ /Ù)vd,z (e)Fz . (5.73c) By multiplying each of the above equations by the electron density n and charge (e) we obtain the corresponding equations for the current density j n(e)vd : jx (ne2 Ù/m∗ )Fx (eBz /m∗ c)Ù jy , (5.74a) jy (ne2 Ù/m∗ )Fy (eBz /m∗ c)Ù jx , (5.74b) jz (ne2 Ù/m∗ )Fz . (5.74c) It is convenient at this point to introduce the definitions Û0 ne2 Ù/m∗ , (5.75) which can be recognized as the zero-field conductivity, and ˆc eBz /(m∗ c), (5.76) which is the classical cyclotron frequency of the electron in the presence of the magnetic field Bz . Using these definitions, (5.74) can be simplified to jx Û0 Fx ˆc Ù jy , (5.77a) jy Û0 Fy ˆc Ù jx , (5.77b) jz Û0 Fz . (5.77c) Solving (5.77), we obtain the three components of the current density: 1 jx Û0 (Fx ˆc ÙFy ), (5.78a) 1 (ˆc Ù)2 1 Û0 (Fy ˆc ÙFx ), (5.78b) jy 1 (ˆc Ù)2 jz Û0 Fz . (5.78c) Based on (5.78) we can define a generalized magneto-conductivity tensor Û (B) for the electrons as ⎛ ⎞ 1 ˆc Ù 0 Û0 ⎝ˆc Ù ⎠. Û (5.79) 1 0 1 (ˆc Ù)2 2 0 0 1 (ˆc Ù) 233 234 5. Electrical Transport Notice that (5.79) contains the sum of a diagonal and an antisymmetric tensor. The sign of the off-diagonal elements depends on the sign of the charge. From (5.79) we conclude that the effects of the magnetic field on the charge transport are twofold. (1) The conductivity perpendicular to the magnetic field is decreased by the factor [1(ˆc Ù)2 ]1 . The corresponding increase in the sample resistance induced by a magnetic field is known as magnetoresistance (for small values of B it is proportional to B2 ). (2) The magnetic field also generates a current transverse to the applied electric field, resulting in off-diagonal elements in the conductivity tensor. These are linearly proportional to the magnetic field whereas the diagonal elements are quadratic in the magnetic field. The off-diagonal elements give rise to the Hall effect to be discussed in the next section. 5.5.2 Hall Effect Let us consider a sample in the form of a rectangular bar oriented with its longest axis along the x axis, as shown in Fig. 5.16a. The electric field F is now applied along the x axis while the magnetic field B is still along the z axis. According to Lorentz’s law, when electrons start to drift along the x axis under the influence of the electric field, they also experience a force in the y direction. This results in a current in the y direction although there is no applied electric field along that direction. One typical experimental configuration involves a closed current loop in the x direction while leaving an open circuit in (b) B 1 3 2 4 I d (a) B x V 2 3 4 1 5 z y Hall Voltage Hall Voltage 1 3 V V' Resistivity I 4 2 Current Source Fig. 5.16a, b. Sample geometries for performing Hall measurements: (a) sample in the form of a bar and (b) sample in the form of a thin film which is used in the van der Pauw method [5.39]. B denotes the magnetic field. I stands for the current source while V represents the meter for measuring the Hall voltage 5.5 Magneto-Transport and the Hall Effect the y direction, as shown in Fig. 5.16a. As a result of this open circuit the current density jy must be zero. From (5.78b) we see that an electric field Fy is induced by the presence of the B field. This phenomenon is known as the Hall effect [5.38] after E.H. Hall (1855–1938), who discovered it at Johns Hopkins University in 1879 and then became a professor at Harvard [from 1881 to 1921]. A simple physical picture of what happens is as follows. The magnetic field causes the charges to drift in the y direction. As a result, charges pile up on the two opposite sample surfaces perpendicular to the y axis and create an electric field Fy , which cancels the effect of the Lorentz force. Under the steady-state condition jy 0, the induced field Fy is equal to (5.80a) Fy ˆc Ù jx /Û0 while the current measured in the x direction is given by jx Û0 Fx . (5.80b) The measured quantity in this experiment is Fy while the externally controlled parameters are jx and B. Therefore one defines the Hall coefficient RH as the ratio (5.81) RH Fy /(jx Bz ). Combining (5.80a) and (5.80b), we find that RH is equal to3 RH ˆc Ù 1 . Û0 Bz nec (5.82) Notice that the sign of RH depends on the sign of the charge. While the Hall coefficient in (5.82) is negative (since we have assumed the charges are electrons), it can be easily shown that RH becomes positive for holes. Thus we see that the Hall effect is an important technique for determining both the concentration and the sign of charged carriers in a sample. This technique is not limited to semiconductors only but is also used extensively in the study of metals. In compensated semiconductor samples, where both electrons and holes are present, RH can be shown to be given by (Problem 5.6) Np b2 Nn , (5.83) RH ec(bNn Np )2 where Nn and Np are the concentrations of the negative and positive charges, respectively, and b is the ratio of their mobilities: Ìn /Ìp . Corrections to (5.82) for the case of anisotropic masses and Ù have been given by Herring and Vogt [5.37]. 5.5.3 Hall Coefficient for Thin Film Samples (van der Pauw Method) One limitation of the Hall effect measurement described in the previous section is the requirement that the sample be in the shape of a rectangular bar. As discussed in Sect. 1.2, samples are often grown in the form of thin epitaxial 3 To convert to SI units delete c. 235 236 5. Electrical Transport films on some insulating substrate. The extension of the Hall technique to such thin films was developed by van der Pauw [5.39]. Two common geometries for the van der Pauw method of measuring the Hall coefficient and resistivity in a thin sample are shown in Fig. 5.16b. This method is particularly convenient for a disk of irregular shape. The current is fed through the contacts 3 and 4 while the Hall voltage is measured across the contacts 1 and 2. The “clover” shape in Fig. 5.16b has the advantage of keeping the current flow away from the Hall voltage contacts. To minimize the error in the measurement of the Hall voltage due to the fact that the current flow may not be perpendicular to the line joining the contacts 1 and 2, one usually measures the voltage both with the magnetic field V12 (±B) and without the field V12 (0). Van der Pauw showed that the Hall coefficient is given by [V12 (B) V12 (0)]d [V12 (B) V12 (B)]d , (5.84) I34 B 2I34 B where d is the thickness of the film, B is the magnetic field, and I34 is the current flowing from contact 3 to contact 4. The sample resistivity Ú can also be measured with the van der Pauw method. In this case two adjacent contacts such as 2 and 3 (I23 ) are used as current contacts while the two remaining contacts are used for measuring the voltage drop (V41 ). The resultant resistance is defined as R41,23 : (5.85) R41,23 |V41 | I23 . RH Another measurement is then made in which current is instead sent through the contacts 1 and 3 and the voltage is measured across the contacts 2 and 4. From the resulting resistance R24,13 , together with R41,23 , Ú can be calculated with the expression d(R24,13 R41,23 )f (5.86) 2 ln 2 where f is a factor that depends on the ratio R24,13 /R41,23 ; f is equal to 1 when this ratio is exactly 1 [Ref. 5.26, p. 63]. When this ratio is equal to 10, f decreases to 0.7. Usually a large value for this ratio is undesirable and suggests that either the contacts are bad or that the sample is inhomogeneously doped. Ú 5.5.4 Hall Effect for a Distribution of Electron Energies So far we have assumed that all the charged carriers have the same properties. We shall now consider a collection of electrons with a range of energies E and a distribution function f (E). We denote the average of any electron property a(E) by a: a a(E)f (E)dE f (E)dE. (5.87) Using this definition, (5.78) can be rewritten as jx ·Fx ÁBz Fy (5.88a) Problems jy ·Fy ÁBz Fx jz Û0 Fx , where∗ $ Ù 1 (ˆc Ù)2 % & ne3 Ù2 Á ∗2 m c 1 (ˆc Ù)2 ne2 · ∗ m (5.88b) (5.88c) # (5.89a) (5.89b) In the limit of a weak magnetic field or, when (ˆc Ù)2 1, we can approximate 1 (ˆc Ù)2 by one and thus write: ne2 ne3 Ù2 Ù and Á (5.90) ∗ m m∗2 c Within this approximation the Hall coefficient for a distribution of electrons can be expressed as4 · RH rH Ù2 (nec)Ù2 nec (5.91) The factor rH Ù2 /Ù2 is called the Hall factor. Its magnitude depends on the scattering mechanisms that contribute to Ù and is usually of the order of 1 [Ref. 5.26, p. 57]. In the limit of strong magnetic fields, or for very pure samples, when (ˆc Ù)2 1, (5.91) remains valid with rH 1 (Problem 5.7). In principle we can determine the carrier mobility by measuring RH and Û0 and using (5.75 and 82) to obtain Ì R H Û0 , (5.92) but in practice the carriers usually have a distribution of energies, so that the mobility calculated from (5.92) is not the same as the mobility Ì defined by (5.12). Instead the mobility defined by (5.92) is referred to as the Hall mobility ÌH and is related to Ì by ÌH rH Ì. (5.93) PROBLEMS 5.1 Drifted Carrier Distributions Using (5.19) show that, within the relaxation time approximation, the carrier distribution in the presence of the field F can be approximated by fk fk0 (Ek qÙk vk · F). for a small external field. This means that the effect of the electric field is to shift the entire distribution (without distortion) by the energy qÙk vk · F. This is just the energy gained by a charge q with velocity vk in the field F during a time Ùk . 4 remove c to convert to SI units. 237 238 5. Electrical Transport 5.2 a) Drifted Maxwell–Boltzmann Distributions Suppose the thermal equilibrium electron distribution fk0 in (5.14) is approximated by a Boltzmann distribution function fk0 A exp Ek /(kB T) . For free carriers located in a spherical band with effective mass m∗ the electron energy is given by Ek (1/2)m∗ v2k . The resultant fk0 is known as a Maxwell–Boltzmann distribution. Using the result of Problem 5.1, show that the carrier distribution in the presence of a weak external electric field F can be approximated by m∗ (vk vd )2 fk ≈ A exp , 2kB T where vd is the drift velocity defined in (5.6). The interpretation of this result is that the external field causes the carrier velocities to increase uniformly by an amount equal to vd while leaving the distribution function unchanged. Consequently the resultant distribution is known as a drifted Maxwell–Boltzmann distribution. b) Relaxation Time Approximation The purpose of this problem is to show how the relaxation time approximation (5.18) can be obtained starting from (5.30). We will make the following assumptions: 1) The electronic band is isotropic, with effective mass m∗ . 2) Scattering is completely elastic (so that Ek Ek and fk0 fk0 ). 3) The applied field is weak so that (5.19) is valid. a) With these assumptions, show that fk fk (fk fk0 ) 1 (vk · F) (vk · F) . Substitute this result into (5.30) and show that P(k, k ) 1 (vk · F)/(vk · F) . Ùk1 k b) To simplify the above expression we choose (without loss of generality) coordinate axes such that k is parallel to the z-axis and F lies in the yz-plane. Let ı and ı be, respectively, the angles between k and F and between k and F. Let the polar coordinates of k in this system be (k , ·, ‚). Show that (vk · F) (vk · F) tan ı sin · sin ‚ cos ·. c) Assume that the elastic scattering probability P(k, k ) depends on · but not on ‚. Show that Ùk1 P(k, k )(1 cos ·). k The physical interpretation of this result is that the relaxation time in elastic scattering is dominated by large angle scattering (i. e., processes with · ). Problems 5.3 Intravalley Scattering by LA Phonons a) Using (5.42) show that the contribution of deformation potential interaction to the intravalley LA phonon scattering time (Ùac ) of an electron in a nondegenerate band with isotropic effective mass m∗ and energy E is given by √ 1 2(ac )2 (m∗ )3/2 kB T(E)1/2 , Ùac 4 Úv2s where ac is the volume deformation potential for the electron, T is the temperature, kB is the Boltzmann constant, Ú is the crystal density, and vs is the LA phonon velocity. b) Assume that the parameters in (a) have the following values, appropriate to GaAs: m∗ 0.067; E 0.36 meV; ac 6 eV; Ú 5.31 g/cm3 , and vs 5.22 × 105 cm/s. Show that Ùac 7 × 1012 s (7 ps) at T 300 K. 5.4 Piezoelectric Acoustic Phonon Scattering Rate Assume that the constant of proportionality in (5.44) is independent of angle. Substitute the result into (5.41) and perform the integration corresponding to that in (5.42). Show that instead of a scattering probability proportional to T(Ek )1/2 as in (5.43), the probability for piezoelectric scattering is proportional to T(Ek )1/2 . See p. 202 for discussions on how to remove the divergence in the scattering probability when Ek → 0. 5.5 Rate of Scattering by LO Phonons for Electrons in a Parabolic Band a) Consider a polar semiconductor with a dispersionless LO phonon energy ˆLO . The Fröhlich electron–LO-phonon interaction Hamiltonian is given by (3.36). For an electron in a nondegenerate conduction band with isotropic effective mass m∗ , the electron wave vector and energy above the band minimum are denoted by k and Ek , respectively. Show that for Ek ˆLO the minimum and maximum phonon wave vectors, q2 min and q2 max , of the phonon emitted by the electron are given by q2 min k[1 f (Ek )] and q2 max k[1 f (Ek )] where 1/2 f (Ek ) 1 (ˆLO /Ek ) . b) Show that the corresponding q1 min and q1 max for absorption of one LO phonon are given by q1 min k[f (Ek ) 1] and q1 max k[f (Ek ) 1] 239 240 5. Electrical Transport where 1/2 f (Ek ) 1 (ˆLO /Ek ) . In the special case that k 0, q1 min q1 max [2m∗ ˆLO /]1/2 . c) Substituting the above results into (5.50), show that the momentum relaxation rate by LO phonon scattering is given by (5.51) in the limit q0 0. d) Assume that a conduction band electron in GaAs has Ek /(ˆLO ) 4. Use the Fröhlich interaction in (3.36) to calculate the scattering rate of this electron by LO phonons. Some materials parameters for GaAs are: density Ú 5.31 g/cm3 ; m∗ 0.067m0 ; Â0 12.5; Â∞ 10.9; and ˆLO 36 meV. 5.6 Hall Coefficient for Samples Containing both Electrons and Holes a) Show that, for a sample containing Nn electrons and Np holes per unit volume with the corresponding mobilities Ìn and Ìp , the equations for the current density in the presence of applied electric field F and magnetic field Bz are jx (·n ·p )Fx (‚n ‚p )Bz Fy , jy (·n ·p )Fy (‚n ‚p )Bz Fx , jz Û0 Fx , where ·i Ni eÌi and ‚i ·i Ìi /c (delete c for SI units) for i n and p. b) Assume that jy 0, as in a conventional Hall effect measurement, and derive Fy . Calculate the Hall coefficient RH Fy /(jx Bz ). 5.7 Hall Factor in the Limit of Strong and Weak Magnetic Fields Show that the Hall coefficient for electrons with a distribution of energies and scattering times Ù is given by: 1 Á2 B2z Á RH 2 1 · ·2 where · and Á are defined in (5.89a,b). Summary SUMMARY In this chapter we have discussed the transport of charges in semiconductors under the influence of external fields. We have used the effective mass approximation to treat the free carriers as having classical charge and renormalized masses. We first considered the case of weak fields in which the field does not distort the carrier distribution but causes the entire distribution to move with a drift velocity. The drift velocity is determined by the length of time, known as the scattering time, over which the carriers can accelerate in the field before they are scattered. We also defined mobility as the constant of proportionality between drift velocity and electric field. We calculated the scattering rates for carriers scattered by acoustic phonons, optical phonons, and ionized impurities. Using these scattering rates we deduced the temperature dependence of the carrier mobilities. Based on this temperature dependence we introduced modulation doping as a way to minimize scattering by ionized impurities at low temperatures. We discussed qualitatively the behavior of carriers under high electric fields. We showed that these hot carriers do not obey Ohm’s law. Instead, their drift velocities at high fields saturate at a constant value known as the saturation velocity. We showed that the saturation velocity is about 107 cm/s in most semiconductors as a result of energy and momentum relaxation of carriers by scattering with optical phonons. In a few n-type semiconductors, such as GaAs, the drift velocity can overshoot the saturation velocity and exhibit negative differential resistance. This is the result of these semiconductors having secondary conduction band valleys whose energies are of the order of 0.1 eV above the lowest conduction band minimum. The existence of negative differential resistance leads to spontaneous current oscillations at microwave frequencies when thin samples are subjected to high electric fields, a phenomenon known as the Gunn effect. Under the combined influence of an electric and magnetic field, the transport of carriers in a semiconductor is described by an antisymmetric second rank magneto-conductivity tensor. One important application of this tensor is in explaining the Hall effect. The Hall coefficient provides the most direct way to determine the sign and concentration of charged carriers in a sample. 241 6. Optical Properties I CONTENTS 6.1 Macroscopic Electrodynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 The Dielectric Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 Excitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Phonon-Polaritons and Lattice Absorption . . . . . . . . . . . . . . . . . . . . . . . 6.5 Absorption Associated with Extrinsic Electrons . . . . . . . . . . . . . . . . . 6.6 Modulation Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.7 Addendum (Third Edition): Dielectric Function . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 244 253 276 292 305 315 333 334 343 The fundamental energy gaps of most semiconductors span the energy range from zero to about 6 eV. Photons of sufficient energy can excite electrons from the filled valence bands to the empty conduction bands. As a result, the optical spectra of semiconductors provide a rich source of information on their electronic properties. In many semiconductors, photons can also interact with lattice vibrations and with electrons localized on defects, thus making optical techniques also useful for studying these excitations. Their optical properties are the basis of many important applications of semiconductors, such as lasers, light emitting diodes, and photodetectors. Figure 6.1 shows schematically some of the optical processes which can occur when a medium is illuminated by light. At the surface of the medium, MEDIUM Reflected Transmitted (Absorbed) Scattered (Raman, Brillouin...) Incident Luminescence Fig. 6.1. Schematic diagram showing the linear optical processes that occur at the surface and in the interior of a medium. The incident beam is assumed to arrive at the surface of the medium from vacuum (or air) P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed., DOI 10.1007/978-3-642-00710-1_6, © Springer-Verlag Berlin Heidelberg 2010 244 6. Optical Properties I a fraction of the incident light is reflected and the rest transmitted. Inside the medium some of the radiation may be absorbed or scattered while the remainder passes through the sample. Some of the absorbed electromagnetic waves may be dissipated as heat or reemitted at a different frequency. The latter process is known as photoluminescence. Electromagnetic waves are scattered by inhomogeneities inside the medium. These inhomogeneities may be static or dynamic. An example of a dynamic fluctuation is the density fluctuation associated with an acoustic wave. Scattering of light by acoustic waves is usually referred to as Brillouin scattering [6.1a]. (This phenomenon was independently discovered by Mandelstam [6.1b].) Scattering of light by other elementary excitations, such as optical phonons or plasmons, is known as Raman scattering. (Sir C.V. Raman received the Nobel Prize in Physics in 1930 for discovering, in 1928 in Calcutta, the effect named after him.) In general, the strongest optical processes are reflection and absorption because they involve the lowest order of interaction between electromagnetic waves and elementary excitations inside the medium. Light scattering involves two such interactions (since there is incident radiation and scattered radiation) hence it tends to be weaker. In this book we shall not consider nonlinear optical processes (such as sum and difference frequency generations), which involve higher-order optical interactions. Readers interested in these topics should consult [6.2–4]. Because there are many different ways that photons can interact with excitations inside semiconductors, we shall divide the discussion on the optical properties of semiconductors into two chapters. In this chapter, the fundamental optical properties of semiconductors will be presented. Chapter 7 will discuss the more specialized topics such as photoluminescence and light scattering. 6.1 Macroscopic Electrodynamics In a dielectric medium an external sinusoidal electromagnetic wave with electric field vector E(r, t) E(q, ˆ) sin(q · r ˆt), where q is the wavevector and ˆ is the frequency, will induce a polarization vector P, which is related to the applied field via a second-rank tensor: Pi (r , t ) ¯ij (r, r , t, t )Ej (r, t)dr dt. (6.1) ¯ij is known as the electric susceptibility tensor. To simplify the notation, summation over the repeated index j in (6.1) is automatically implied. Time is, of course, homogeneous in the absence of time-dependent perturbations. It is often assumed that space is also homogeneous to avoid complications such as local field corrections (avoided by averaging all microscopic quantities over a unit cell).1 With this assumption, (6.1) can be simplified to 1 In recent years there has been considerable interest in the propagation of electromagnetic waves through periodic structures composed of macro- or microscopic elements such as semiconductor spheres. These samples are called photonic crystals [6.5]. 6.1 Macroscopic Electrodynamics Pi (r , t ) Â0 ¯ij (|r r |, |t t |)Ej (r, t)dr dt. (6.2) From the convolution theorem, (6.2) can be expressed in terms of the Fourier transforms of P, ¯, and E (see Sect. 4.2.1 for a definition of Fourier transforms): Pi (q, ˆ) Â0 ¯ij (q, ˆ)Ej (q, ˆ). (6.3) In principle, all the linear optical properties of the medium are determined by the complex electric susceptibility tensor ¯ij (q, ˆ). Note that while P(r , t ), ¯ij (r, r , t, t ), and E(r, t) are all real, their Fourier transforms can be complex. The fact that ¯ij (r, r , t, t ) is real imples that ¯ij (q, ˆ) ¯∗ij (q, ˆ). For comparison with experiments it is often more convenient to define another complex, second-rank tensor, known as the dielectric tensor. This tensor Âij (q, ˆ) is defined by Di (q, ˆ) Â0 Âij (q, ˆ)Ej (q, ˆ) (6.4) where D(q, ˆ) is the Fourier transform of the electric displacement vector D(r, t) defined by D(r, t) E(r, t) 4P(r, t). It follows from their definitions that ¯ij (q, ˆ) and Â(q, ˆ) are related by Âij (q, ˆ) 1 4¯ij (q, ˆ) 1 ¯ij (q, ˆ) in SI units. (6.5) The real and imaginary parts of the dielectric tensor will be denoted by Âr (q, ˆ) and Âi (q, ˆ), respectively. We will now state, without proof, some of the properties of Â(q, ˆ) [6.6]: Â(q, ˆ) Â ∗ (q, ˆ), Âij (q, ˆ) Âji (q, ˆ). (6.6) (6.7) Equation (6.6) follows from the fact that Â(r, t) has to be a real function of space and time. Equation (6.7) is one example of a general property of all socalled kinetic coefficients known as the Onsager relations. In most of the cases that we shall study, the wavelength of light is much larger than the lattice constants or other relevant dimensions (such as the exciton radius to be discussed in Sect. 6.3) of the semiconductor crystals. As a result, the magnitude of the photon wavevector q can be assumed to be zero. Unless noted otherwise, we shall therefore assume that to be the case and abbreviate the dielectric tensor as Â(ˆ). If we assume that Â(q, ˆ) is independent of q whatever the value of q (although in fact this is only true for small q’s) and calculate its Fourier transform (see also Sect. 4.2.1), we find that Â(r, ˆ) is proportional to (the Dirac ‰-function) ‰(r). This means that the response to E(r) is local, i.e., D(r) depends only on the field applied at the point r. On the other hand, if Â is taken to depend on q, its Fourier transform depends on r r and the response is nonlocal. The variation of Â with q is called spatial 245 246 6. Optical Properties I dispersion. In most cases of interest in semiconductor optics this variation is rather small [ 105 times the values of Âii (0, ˆ)]. Nevertheless it has been observed in semiconductors such as Ge and GaAs [6.7, 8]. Readers interested in this topic should consult the book by Agranovich and Ginzburg [6.9]. The rest of our discussions on the optical properties of semiconductors will be concerned mostly with the calculation of the dielectric tensor and its properties. In either isotropic media or cubic crystals the dielectric tensor Â(ˆ) has only three identical diagonal elements. In cases where the tensor nature of Â(ˆ) is not important we shall replace Âij (ˆ) by a scalar function Â(ˆ) known as the dielectric function. This will be assumed to be true for the rest of our discussions unless stated otherwise. Among the semiconductors we have studied so far, only the II–VI compounds with the wurtzite structure, e.g., CdS and ZnO (Problem 3.7), are not cubic. These crystals are said to be uniaxial since they contain a special axis known as the optical axis (which coincides with the c-axis in the wurtzite structure). When plane electromagnetic waves propagate along this axis they have the same velocity independent of their polarization direction. Along other crystallographic axes, the light velocity varies with the polarization, giving rise to the phenomenon known as birefringence. Crystals with tetragonal or hexagonal symmetry (e.g. wurtzite or chalcopyrite structures) are uniaxial. Those with lower symmetries have two directions along which plane electromagnetic waves travel with the same velocity regardless of their polarization. They are said to be biaxial (e.g. orthorhombic GeS, GeSe). The macroscopic optical properties of an isotropic medium can also be characterized by a complex refractive index ñ. The real part n of ñ is usually also referred to as the refractive index. The imaginary part Î is known as the extinction index or coefficient. The normal-incidence reflection coefficient or reflectance of a semi-infinite isotropic medium in vacuum is given by [6.10] |(ñ 1)/(ñ 1)|2 . (6.8) When light is absorbed in passing through a medium from a point r1 to another point r2 , the absorption coefficient · of the medium is defined by I(r2 ) I(r1 ) exp(·|r 2 r1 |), (6.9) where I(r) denotes the intensity at r. The absorption coefficient is related to Î by · 4Î/Ï0 , (6.10) where Ï0 is the wavelength of the light in vacuum. The complex refractive index ñ is related to Â(ˆ) by Â(ˆ) (ñ)2 . (6.11) 6.1 Macroscopic Electrodynamics 6.1.1 Digression: Units for the Frequency of Electromagnetic Waves At this point it is important to make a digression to present the various units of frequency of electromagnetic waves found in the literature. In principle the frequency of light (to be denoted by Ó) is given in Hertz (Hz), i.e., cycles per second. The angular frequency ˆ is related to Ó by ˆ 2Ó (radians per second). In light scattering spectroscopy and infrared spectroscopy one often encounters another unit, known as wavenumber, which is defined as the reciprocal of the wavelength Ï. A wavenumber of 1 cm1 corresponds to a wavelength of 1 cm or a frequency of 3×1010 Hz (i.e., 30 GHz). When we study quantum processes involving electromagnetic waves, we quantize the energy of electromagnetic waves into photons. The energy of a photon is equal to ˆ, where is Planck’s constant. Photon energies are often expressed in electron volts (or eV) or sometimes in units of an equivalent temperature T (in Kelvin). The photon energy is then equal to kB T, where kB is Boltzmann’s constant. The conversion factors between eV and the various units of frequency are 1 eV ↔ 8065.5 cm1 ↔ 2.418×1014 Hz ↔ Ï 1.2398 Ìm ↔ 11600 K or 1 cm1 ↔ 0.12398 meV. 6.1.2 Experimental Determination of Optical Functions There are several ways to determine the optical functions of a semiconductor as a function of photon energy. The appropriate method depends on whether the photon energy is above or below the bandgap [6.11]. If the photon energy is below the electronic bandgap and well above any phonon energies, the sample absorption coefficient is either zero or very small. The relevant optical function is then the refractive index (which is real). This can be measured by several different methods. One very accurate method is to fabricate the material into a prism and to measure the angle of minimum deviation of a beam of light passing through this prism. Another method is to polish the sample into a thin slab with parallel surfaces and to measure the interference fringes in the sample transmission or reflection spectra. When the photon energy is increased from below to above the bandgap, typically the semiconductor absorption coefficient increases rapidly to values as large as or larger than 104 cm1 . As a result the sample becomes opaque for photon energies higher than the bandgap unless its thickness is very small. Since the intensity of light transmitted through a sample decreases exponentially with thickness according to (6.9), it is necessary to thin the sample down to about ·1 in order to detect easily the transmitted radiation. The quantity ·1 is therefore known as the optical penetration depth. Since · tends to increase rapidly as a function of photon energy above the bandgap, a series of progressively thinner samples is necessary in order to measure · over a wide photon energy range. An alternative and more popular method for determining the complex dielectric function of strongly absorbing samples is to use reflection measure- 247 6. Optical Properties I ments. The major drawback of these measurements is their sensitivity to the sample surface quality. As pointed out above, the penetration depth of light into a sample is equal to ·1 and for semiconductors · is typically of the order of 104 –106 cm1 above the absorption edge. For such large absorption coefficients, light will probe only a thin layer, about 1 Ìm or less thick, at the top of the sample. As a result, the reflectance will be very sensitive to the presence of surface contaminants such as oxides or even air pollutants. Unless great care is taken to achieve an atomically clean surface in an ultra-high vacuum (see Chap. 8 for a definition of ultra-high vacuum and discussions on surface properties of semiconductors), the measured reflectance is that of a “composite”, consisting of a surface contaminant layer and the bulk sample. Some authors have labeled the dielectric functions deduced from the reflectance of such contaminated samples as “pseudodielectric functions” [6.12]. As an example of the sensitivity of the dielectric function to sample surface quality, we compare in Fig. 6.2 the “pseudodielectric function” of an oxidized GaAs surface (oxide thickness 10 Å) with that of GaAs with an abrupt and clean surface. Notice that the largest difference in Â between these surfaces occurs around 4.8 eV photon energy. In this energy range the value of Î is about 4 [6.12], with a corresponding penetration depth of about 50 Å. Obviously, even an oxide layer of only 10 Å will make a difference in the reflectivity. E2 E1 20 εr 10 εi <ε > 248 0 GaAs Abrupt Oxidized, d = 10Å –10 2 3 4 Energy [eV] 5 6 Fig. 6.2. The real and imaginary parts of the dielectric function of GaAs measured by ellipsometry. The solid curve, labeled “abrupt”, was obtained for an atomically clean surface, the broken one for a surface covered by an oxide layer. [6.12] Except for this surface sensitivity, determining the dielectric function from reflection measurements is quite straightforward. It involves irradiating the sample at either normal or oblique incidence. In oblique incidence techniques, the reflectance s and p of the s- and p-polarized components of the incident light are measured (components of the incident radiation perpendicular and parallel to the plane of incidence are labeled, respectively, as s- and ppolarized). These reflectances are related to the complex refractive index by the Fresnel formulae [6.10] 6.1 Macroscopic Electrodynamics cos ˇ (ñ2 sin2 ˇ)1/2 2 s |r s | cos ˇ (ñ2 sin2 ˇ)1/2 2 (6.12a) and ñ2 cos ˇ (ñ2 sin2 ˇ)1/2 2 p |r p |2 , ñ2 cos ˇ (ñ2 sin2 ˇ)1/2 (6.12b) where rs and rp are the complex reflectivity for s- and p-polarized light, respectively, and ˇ is the angle of incidence. The complex refractive index can be deduced by measuring both s and p at a fixed ˇ. An oblique angle of incidence technique which has become very popular in the past decade is ellipsometry. This name derives from the fact that when linearly polarized light that is neither s- nor p-polarized is incident on a medium at an oblique angle, the reflected light is elliptically polarized (Fig. 6.3). The ratio (Û) of the complex reflectivities rp /rs can be determined by measuring the orientation and the ratio of the axes of the polarization ellipse corresponding to the reflected light. The complex dielectric function can be determined from Û and ˇ using the expression (Problem 6.1) 2 1Û 2 2 2 Â sin ˇ sin ˇ tan ˇ . (6.13) 1Û Figure 6.3 shows schematically the principal components of an ellipsometer [6.13]. The light source can be either a laser or a broad-band source such as a xenon gas discharge or a quartz-halogen lamp. In the case of a broad-band on Light source tor tec De M oc hro ma or sat tor n pe m Co Signal Analyzer S E Polarizer S S Sample E P Polarization before sample P Electronics & Computer E(t) P Polarization after sample Fig. 6.3. Schematic diagram of an ellipsometer [6.13]. P and S denote polarizations parallel or perpendicular to the plane of incidence, respectively 249 250 6. Optical Properties I source the light is passed through a monochromator to select a narrow band of frequencies. Ellipsometry performed over a wide range of photon frequencies is known as spectroscopic ellipsometry. The light leaving the monochromator is passed through a linear polarizer. After reflection from the sample surface the light experiences a relative phase shift ı between its s and p components and becomes elliptically polarized. There are several variations in the method to detect the ellipticity of the reflected light. In Fig. 6.3 a compensator introduces another relative phase shift ı which exactly cancels the ellipticity induced by the reflection and the light becomes linearly polarized again. This null condition can be easily detected by passing the light through an analyzer, which consists of another linear polarizer oriented to block out the light after the compensator. Despite the increasing popularity of ellipsometers, perhaps the most common and also the simplest technique for determining the optical constants is to measure the normal-incidence reflectance. Figure 6.4 shows the construction of the apparatus used by Philipp and Ehrenreich [6.14] to measure the normal-incidence reflectance of semiconductors from about 1 eV to 20 eV. Modern versions of this setup are basically the same except for improvements in the light source, gratings and detectors. Instead of gas-discharge lamps synchrotron radiation [6.15, 16] is preferred nowadays as the source of high intensity and broad-band radiation extending from the infrared to the X-ray region. Holographic gratings have mostly replaced mechanically ruled gratings since much more uniform and closely spaced grooves can be generated by interference effects. In the area of detectors, the biggest improvement has been the appearance of multichannel detectors such as CCDs (which stands for chargecoupled devices). These are solid-state detectors that are sensitive from the near infrared (wavelengths of about 1 Ìm) to the ultraviolet. They can also be used in the vacuum ultraviolet and soft-x-ray region together with a scintillator and image-intensifiers. They allow the entire optical spectrum, covering a wide range of wavelengths, to be recorded electronically in one exposure. Finally, the electronic signal from these detectors can be processed by desktop computers to display the optical constants in real time with time resolution of milliseconds. In principle, it is necessary to measure both the normal-incidence reflectance and the absorption coefficient · in order to determine the complex refractive index and hence the dielectric function Â(ˆ). In practice it is sufficient to simply measure over a wide range of photon frequencies and then deduce the absorption coefficients using the Kramers–Kronig relations (KKRs) or dispersion relations, which were introduced in Sect. 4.3.1. 6.1.3 Kramers–Kronig Relations If we assume that the field strength of the incident radiation is weak enough that the induced polarization is linearly dependent on the electric field, both ¯(ˆ) and Â(ˆ) describe the linear responses of a medium to an external field. 6.1 Macroscopic Electrodynamics It can be shown that linear response functions such as Â or ¯ satisfies the KKRs Âr (ˆ) 1 ∞ 2 0 ˆ Âi (ˆ )dˆ ˆ2 ˆ2 (6.14) and 2ˆ Âi (ˆ) ∞ 0 (a) Âr (ˆ )dˆ , ˆ2 ˆ2 (6.15) Vacuum grating monochromator L B C D A S P2 P1 (b) Hydrogen Argon Gas inlet A – Concave grating – off-axis pivot B – Slit-to-grating distance adjustment C – Slit width adjustment D – Filter holder P1 P2 – Photomultiplier detectors L – Lamp S – Sample holder { { 2000 Microns 140 Volts 1 Ampere Continuum 3.5 to 7.5 eV Line spectrum 7.5 to 15 eV 150 Microns 75 Volts 3 Amperes Line spectrum 13 to 28 eV Barium aluminate cathode Glass-tokovar seal Anode (grounded) Entrance slit Ring seal 1cm × 0.3cm Capillary (quartz) “O”-Ring seal Fig. 6.4. (a) The vacuum reflectometer used by Philipp and Ehrenreich [6.14] to measure the normal incidence reflectance of semiconductors from about 1 to 20 eV. (b) Detailed construction of the gas discharge lamp they used 251 252 6. Optical Properties I where means the principal value of the integral. The proof of this relation (see, for example, [6.10] and Problem 6.2) is based on the principle of causality (i. e., a response to an applied field such as the polarization cannot precede the applied field). Although the refractive index is not a response function, we can derive a KKR for ñ based on the fact that it has the same analytic properties as Â. For example, ñ approaches unity as ˆ approaches infinity and, if relativistic causality holds (i. e., the response cannot propagate faster than the speed of light), ñ is analytic in the upper half plane of the complex variable ˆ. As a result, a set of KKRs for ñ can be obtained from (6.14 and 15) by replacing Âr and Âi by n and Î, respectively. Since it is easier to measure the normal-incidence reflectance than either Â or n of a bulk sample in most experiments, it is desirable to derive a KKR for the reflectance. Such a relation can be obtained by constructing a complex function, known as complex reflectivity, with analytic properties similar to Â. Let us define such a function r̃ as (ñ 1) Ú exp(iı). (6.16) r̃ (ñ 1) Consider a contour integral of the function 1 ˆ ˆ f (ˆ ) ln r̃(ˆ ) (ˆ ˆ) 2 1ˆ (6.17) over the contour C shown in Fig. 6.5. The function f is constructed so that, in contrast to ln r̃, it approaches zero as ˆ approaches infinity. Furthermore, the only poles of f (ˆ ) are i and ˆ and the residue of f at ˆ gives ln r̃(ˆ). From the Cauchy theorem the contour integral of f is given by the sum of the residues at i and ˆ. The result can be written as 1 f (ˆ )dˆ 2i ln r̃(ˆ) ln r̃(i) . (6.18) 2 C Taking the real part of both sides of (6.18) we obtain (note that the principal part of the integral in (6.19) is equal to the contour integral in (6.18) minus half of the residue at ˆ ˆ, see Fig. 6.5): ∞ ∞ (1 ˆ ˆ) ln Ú(ˆ )dˆ ı (1 ˆ2 )(ˆ ˆ) (6.19) [the fact that ln r̃(i) is real, needed for this derivation, can be surmised from (6.48 and 49) below]. By simplifying this equation further, we can express ı in terms of an integral of ln Ú(ˆ): 2ˆ ı ∞ 0 ln Ú(ˆ )dˆ . (ˆ2 ˆ2 ) (6.20) Using (6.20), the complex reflectivity, refractive index, and dielectric function can all be deduced from measurement of the reflectance over a wide frequency range. Since it is difficult to measure the reflectance from zero to infinite fre- 6.2 The Dielectric Function Fig. 6.5. Contour C for integrating the function f in (6.17) to obtain the KKR for the reflectivity C ι ω quency, it becomes necessary to use extrapolations to both low and high frequencies. At low frequency in an undoped sample can be approximated by a constant. At high enough frequencies the semiconductor can be approximated by a free electron gas with the dielectric constant Â 1 (ˆp /ˆ)2 , (6.21) where the plasma frequency ˆp (see Problem 6.3 for its definition and derivation) is determined by the density of valence electrons only. The core electrons are so tightly bound that their contributions to the dielectric function can usually be neglected. 6.2 The Dielectric Function 6.2.1 Experimental Results Some typical reflectance spectra of group IV and III–V semiconductors measured by Philipp and Ehrenreich [6.14] are shown in Figs. 6.6a–8a. The corresponding real and imaginary parts of the dielectric function and the imaginary part of the so-called energy loss function (1/Â) deduced from the reflectance spectra using the KKRs are shown in Figs. 6.6b–8b. The dielectric function of GaAs displayed in Fig. 6.8b compares well with that measured by ellipsometry over a smaller photon energy range, shown in Fig. 6.2. Notice that both the reflectance spectra and the dielectric functions in Si, Ge, and GaAs show considerable structure in the form of peaks and shoulders. These structures arise from optical transitions from the filled valence bands to the empty conduction bands. That such structures occur in the optical transitions between valence bands and conduction bands in crystalline semiconductors should not be surprising (they are, however, smoothed out by disorder in amorphous semiconductors). In Sect. 2.3.4 we studied the selection rules for 253 254 6. Optical Properties I 80 (a) Si 60 R × 10 R 40 R [%] 20 0 60 2.0 (b) –Im{ε –1} 40 1.5 εi 1.0 –Im{ε –1} 20 εi , εr 0 0.5 εr –20 0 5 10 15 Energy [eV] 20 25 0 Fig. 6.6. (a) Reflectance curve of Si measured at room temperature. (b) The real (Âr ) and imaginary (Âi ) parts of the dielectric function and the imaginary part of (1/Â) (known as the energy loss function) of Si deduced from the reflectivity curve in (a) using the Kramers–Kronig relation [6.14]. Notice that the peak of Im{1/Â}, occurs at the plasma energy of the valence electrons (Problem 6.3) the matrix elements of the electric dipole operator between two given electron wavefunctions in zinc-blende-type crystals. In the following sections we will discuss the relation between the band structure of a semiconductor and its optical spectra based on a microscopic theory of the dielectric function. 6.2.2 Microscopic Theory of the Dielectric Function We will use a semi-classical approach to derive the Hamiltonian describing the interaction between an external electromagnetic field and Bloch electrons inside a semiconductor. In this approach the electromagnetic field is treated classically while the electrons are described by quantum mechanical (Bloch) 6.2 The Dielectric Function 60 (a) 40 Ge R R [%] R × 10 20 0 25 1.2 (b) εi –Im{ε –1} 15 0.8 –Im{ε –1} 5 ε r, ε i 0 0.4 εr –5 0 5 15 10 Energy [eV] 20 25 0 Fig. 6.7a,b. Curves for Ge similar to those for Si in Fig. 6.6 wave functions. Although this approach may not be regarded as being as rigorous as a fully quantum mechanical treatment in which the electromagnetic waves are quantized into photons (e. g., [6.17]), it has the advantage of being simpler and easier to understand. This approach generates the same results as the quantum mechanical treatment, including even spontaneous emission (to be discussed in Chap. 7). We start with the unperturbed one-electron Hamiltonian introduced already in (2.4): 0 p2 /2m V(r). (6.22) To describe the electromagnetic fields we introduce a vector potential A(r, t) and a scalar potential º(r, t). Because of gauge invariance, the choice of these potentials is not unique. For simplicity, we will choose the Coulomb gauge [6.10], in which º 0 and ∇ · A 0. (6.23) 255 256 6. Optical Properties I 60 (a) GaAs 40 R R [%] R × 10 20 0 25 (b) –Im{ε –1} 0.8 εi 15 εr, ε i –Im{ε –1} 0.4 5 0 εr –5 0 5 10 15 Energy [eV] 20 25 Fig. 6.8a,b. Curves for GaAs similar to those for Si in Fig. 6.6 In this gauge the electric and magnetic fields (E, B) are given by2 1 A and B ∇ × A, E (6.24) c t where c is the velocity of light. The classical Hamiltonian of a charge Q in the presence of an external magnetic field can be obtained from the free-particle Hamiltonian by replacing the momentum P by P(QA/c), where P is the momentum conjugate to the position vector [6.10, p. 409]. Correspondingly, we obtain the quantum mechanical Hamiltonian describing the motion of a charge e in an external electromagnetic field by replacing the electron momentum operator p in (6.22) by p (eA/c): 1 [p (eA/c)]2 V(r). 2m (6.25) The term [p (eA/c)]2 /2m can be expanded [keeping in mind that p is an operator which does not commute with A(r)] as 2 1 eA p2 e e2 A2 e p . (6.26) A·p p·A 2m c 2m 2mc 2mc 2mc2 2 In (6.24, 25, 26, 28, 29, 31) delete c for SI units. 6.2 The Dielectric Function Using the definition of p as the operator (/i)∇ we can express the term p · A as (p · A)f (r) A · ∇f ∇ · A f. (6.27) i i From (6.23), ∇ · A 0, and therefore [e/(2mc)]p · A [e/(2mc)]A · p. For the purpose of calculating linear optical properties we can also neglect the term e2 A2 /(2mc2 ), which depends quadratically on the field. Under this assumption we can approximate by e 0 A · p. (6.28) mc Compared with the unperturbed Hamiltonian 0 , the extra term [e/(mc)]A · p describes the interaction between the radiation and a Bloch electron. As a result, this term will be referred to as the electron–radiation interaction Hamiltonian eR : eR e A · p. mc (6.29) Note that the form of eR depends on the gauge we choose. Another form of eR commonly found in the literature is eR (e)r · E. (6.30) Equation (6.30) can be shown to be equivalent to (6.29) in the limit that the wavevector q of the electromagnetic wave is small [(6.30) corresponds to the electric dipole approximation; (6.29) is more general]. Both forms of eR neglect the term quadratic in the field. In the case of (6.30), the interaction between the electrons and the electromagnetic field via the Lorentz force has been neglected. Since this force depends on v × B and since the velocity v varies with E, this term has a quadratic dependence on the applied field. The advantage of using (6.29) for semiconductors is that the matrix elements of the electron momentum enter directly into the k · p method of band structure calculation. For example, the matrix element between the lowest °1c conduction band and the top °4 valence band in tetrahedrally bonded semiconductors can be determined from the conduction band effective mass using (2.44). Other matrix elements are related to the dispersion of the valence bands as shown in (2.63–65). There are several ways to calculate the dielectric function of a semiconductor from eR . Again, we will take the simplest approach. We first assume that A is weak enough that we can apply time-dependent perturbation theory (in the form of the Fermi Golden Rule) to calculate the transition probability per unit volume R for an electron in the valence band state |v (with energy Ev and wavevector kv ) to the conduction band |c (with corresponding energy Ec and wavevector kc ). To do this we need to evaluate the matrix element |c|eR |v|2 : |c|eR |v|2 (e/mc)2 |c|A · p|v|2 . (6.31) We will now write the vector potential A as Aê, where ê is a unit vector parallel to A. In terms of the amplitude of the incident electric field E(q, ˆ), the amplitude of A can be written as 257 258 6. Optical Properties I E (6.32) {exp[i(q · r ˆt)] c.c.} , 2q where c.c. stands for complex conjugate. The calculation of the matrix element c|A · p|v involves integration over space. The integration over time of the term exp[i(ˆt)] in (6.32) and the corresponding factors in the electron Bloch functions leads formally to exp(iEc t/) exp[i(ˆt)] exp(iEv t/)dt ∝ ‰(Ec (kc ) Ev (kv ) ˆ), (6.33) A i. e., the delta function found in the Fermi Golden Rule. This result means that the electron in the valence band absorbs the photon energy and is then excited into the conduction band. Hence this term in (6.32) describes an absorption process. Similarly, the matrix element of the complex conjugate: c| exp(iˆt)|v, gives rise to ‰(Ec (kc ) Ev (kv ) ˆ). This term is nonzero when an electron which is initially in the conduction band emits a photon and ends up in the valence band. Since this emission process occurs now in the presence of an external field, this term describes a stimulated emission process. In other words, the two terms in (6.32) describe, respectively, absorption and emission of photons by electrons in a semiconductor under the influence of an external electromagnetic field. Notice that the magnitudes of the matrix elements describing both processes are equal. The stimulated emission term, represented as c.c. in (6.33), will be discussed in more detail in Chap. 7 but will be neglected in this chapter. Writing the Bloch functions [see (2.6)] for the electrons in the conduction and valence bands, respectively, as |c uc, kc (r) exp[i(kc · r)] (6.34a) |v uv, kv (r) exp[i(kv · r)] (6.34b) and and using the expression for A in (6.32), we obtain |c|A · p|v|2 2 |E|2 ∗ . u exp[i(q k ) · r](ê · p)u exp(ik · r)dr c v v,kv c, kc 2 4q (6.35) Operating with p on uv, kv exp(ikv · r) yields two terms: puv, kv exp(ikv · r) exp(ikv · r)puv, kv kv uv, kv exp(ikv · r). (6.36) u∗c,kc , The integral of the second term in (6.36) multiplied by vanishes because uc, kc and uv, kv are orthogonal. We can split the corresponding integral of the first term u∗c, kc exp[i(q kc kv ) · r]puv, kv dr into two parts by writing r Rj r , where r lies within one unit cell and Rj is a lattice vector. Because of the periodicity of the functions uc, kc and uv, kv , we find 6.2 The Dielectric Function u∗c, kc exp[i(q kc kv ) · r]puv, kv dr ⎛ ⎞ ⎝ exp[i(q kc kv ) · Rj ]⎠ u∗c,kc exp[i(q kc kv ) · r ]puv,kv dr . j (6.37) unit cell The summation of exp[i(qkc kv ) · Ri ] over all the lattice vectors Rj results in a delta function ‰(q kc kv ). This term ensures that wavevector is conserved in the absorption process: q kv kc . (6.38) Equation (6.38) is a consequence of the translation symmetry of the crystal and therefore must be satisfied for all processes in a perfect crystal. It is, however, relaxed in amorphous semiconductors (see Appendix by J. Tauc on p. 566). Using (6.38), the integral over the unit cell in (6.37) simplifies to u∗c, kc exp[i(q kc kv ) · r]puv, kv dr u∗c, kv q puv, kv dr . (6.39) unit cell unit cell This expression can be further simplified if we assume that q is much smaller than the size of the Brillouin zone, a condition usually satisfied by visible photons, whose wavelengths are of the order of 500 nm. For small q the wavefunction uc,kv q can be expanded into a Taylor series in q: uc,kv q uc,kv q · ∇ k uc, kv . . . . (6.40) When q is small enough that all the q-dependent terms in (6.40) can be neglected, the matrix element |c|ê · p|v|2 is given by ⎛ ⎞2 ⎜ ⎟ ∗ ⎟ |c|ê · p|v|2 ⎜ (6.41a) ⎝ uc, k (ê · p)uv, k dr ⎠ . unit cell This approximation is known as the electric dipole approximation [it can be shown to be equivalent to using (6.30)] and the corresponding matrix element in (6.41a) as the electric dipole transition matrix element. Notice that the electric dipole approximation is equivalent to expanding the term exp(iq · r) in (6.32) into a Taylor series: 1 i(q · r) . . . and neglecting all the q-dependent terms. In this case we have kv kc , and the transitions are said to be vertical or direct. If the electric dipole matrix element is zero, the optical transition is determined by the q · ∇ k ukv term in (6.41). The matrix element ⎛ ⎞2 ⎜ ⎟ ∗ ⎟ |c|ê · p|v|2 ⎜ (6.41b) ⎝ q · (∇ k uc, k )(ê · p)uv, k dr ⎠ unit cell 259 260 6. Optical Properties I gives rise to electric quadrupole and magnetic dipole transitions. These higher order optical transitions can also be considered as arising from the i(q · r) term in the Taylor expansion of exp(iq · r). Compared to the electric dipole transitions they are reduced in strength by a factor of (lattice constant/wavelength of light)2 [6.7]. From now on we shall restrict ourselves to electric dipole transitions unless stated otherwise. To simplify the notation we drop the subscript v or c in the electron wavevectors kv and kc , since they are the same. In most cases the momentum matrix element in (6.41a) is not strongly dependent on k [6.18] so we shall replace it by the constant |Pcv |2 . Equation (6.31) can then be simplified to read |c|eR |v|2 (e/mc)2 |A|2 |Pcv |2 . (6.42) In using (6.42) one must remember that we have defined A in (6.32) as a sum of exp[i(q · r ˆt)] and its complex conjugate exp[i(q · r ˆt)] in order that A be a real function of space and time. However, of these two terms only the one containing exp(iˆt) yields the absorption process. Its complex conjugate, which gives rise to stimulated emission, has been completely disregarded in the present discussion. The electric dipole transition probability R for photon absorption per unit time obtained by substituting (6.42) and (6.32) into the Fermi Golden Rule: R (2/) |c|eR |v|2 ‰(Ec (kc ) Ev (kv ) ˆ) (6.43a) kc ,kv is thus given by R 2 2 e 2 E(ˆ) |Pcv |2 ‰(Ec (k) Ev (k) ˆ). mˆ 2 (6.43b) k If we restrict the summation to those k’s allowed per unit volume of crystal then (6.43b) gives the absorption transition rate per unit volume of the crystal. The power lost by the field due to absorption in unit volume of the medium is simply the transition probability per unit volume multiplied by the energy in each photon: Power loss Rˆ. (6.44) This power loss from the field can also be expressed in terms of either · or Âi of the medium by noting that the rate of decrease in the energy of the incident beam per unit volume is given by dI/dt, where I is the intensity of the incident beam: c dI dI dx (6.45) ·I dt dx dt n Âi ˆI (6.46) 2 . n The energy density I can be related to the field amplitude by 6.2 The Dielectric Function n2 |E(ˆ)|2 . (6.47) 8 Equating dI/dt with the expression for the power loss per unit volume of the field in (6.44) we obtain I Âi (ˆ) 2 1 2e |Pcv |2 ‰(Ec (k) Ev (k) ˆ). 4Â0 mˆ (6.48) k By using the KKRs we can then obtain the expression for Âr : ⎡ ⎤ |Pcv |2 ⎦ 4e2 ⎣ 2 Âr (ˆ) 1 4Â0 m mˆcv ˆ2cv ˆ2 (6.49) k where ˆcv Ec (k) Ev (k). We have purposely written (6.49) in a form similar to the dielectric function for a collection of classical, charged, harmonic oscillators with frequencies ˆi (Problem 6.4): 4e2 Ni , (6.50) Âr (ˆ) 1 4Â0 m ˆ2i ˆ2 i where Ni is the number of oscillators per unit volume with frequencies ˆi . Comparing the two expressions for Âr in (6.49) and (6.50), we see that the dimensionless quantity 2|Pcv |2 (6.51) mˆcv is essentially the “number” of oscillators with frequency ˆcv . Therefore fcv is known as the oscillator strength of the optical transition.3 fcv 6.2.3 Joint Density of States and Van Hove Singularities Note that in (6.48) most of the dispersion in Âi comes from the summation over the delta function ‰(Ec (k) Ev (k) ˆ). This summation can be converted into an integration over energy by defining a joint density of states for the (doubly degenerate) conduction and valence bands (see Sect. 4.3.1 for the definition of density of states): 1 dSk Dj (Ecv ) , (6.52) 43 |∇ ∇k (Ecv )| where Ecv is the abbreviation for Ec Ev , and Sk is the constant energy surface defined by Ecv (k) const. We have assumed that both the conduction and valence bands are doubly degenerate (as a result of spin), which is strictly 3 The summation in (6.49) is performed over the k vectors allowed per unit volume of crystal. 261 262 6. Optical Properties I valid for centrosymmetric crystals but not for zinc-blende-type crystals [6.19]. Since eR does not involve electron spin, the spin state of the electron does not change in an optical transition (provided there is no spin–orbit coupling). With (6.52) we can make the following replacement in (6.4 and 49): → Dj (Ecv )dEcv (6.53) k It has been pointed out by Van Hove [6.20] that the density of states of ∇k (E)| electron and phonon bands possesses singularities at points where |∇ vanishes [see (6.52)]. These points are known as critical points and the corresponding singularities in the density of states are known as Van Hove singularities. Assuming that k 0 is a critical point in three-dimensional space, E(k) can be expanded as a function of k about the critical point: E(k) E(0) ·1 k21 ·2 k22 ·3 k23 . . . (6.54) Van Hove singularities are classified according to the number of negative coefficients ·i in (6.54). In three-dimensional space there are four kinds of Van Hove singularities, labeled M0 , M1 , M2 , and M3 critical points. For example, a M0 critical point has no negative ·i ’s and therefore represents a minimum in the band separation Ecv . M1 and M2 are known as saddle points, since the plots of their energies versus wavevector resemble a saddle. An M3 critical point represents a maximum in the interband separation. It has been shown extensively in the literature (see for example [6.11]) that the density of states in the vicinity of an M0 critical point of doubly degenerate valence and conduction bands is (22 ·3/2 )1 (E E0 )1/2 , E E0 ; ·3 ·1 ·2 ·3 (6.55) Dj 0, E E0 The dependences on E of the densities of states in the vicinity of Van Hove singularities are listed in Table 6.1 for one-dimensional to three-dimensional kspace. The corresponding Van Hove singularities in Âi are sketched in Fig. 6.9. 6.2.4 Van Hove Singularities in Âi The real and imaginary parts of the dielectric function can be calculated readily from the band structure of a semiconductor using (6.49) and (6.48), respectively. A detailed comparison of the theoretical and experimental curves is one of the most stringent tests of the accuracy of a band structure calculation. From such a comparison it is possible to identify the optical transitions in reciprocal space which give rise to the structures in the experimental dielectric functions. In Figs. 6.10 and 11 we show comparisons of the theoretical and experimental dielectric function curves for Si and GaAs. The theoretical curves have been calculated from the band structures obtained by the empirical pseudopotential method. Figure 6.12 shows a similar comparison for the imaginary part of the dielectric function in Ge [6.25] except that the band structure was 6.2 The Dielectric Function Table 6.1. Van Hove singularities in one, two, and three dimensions and the corresponding density of states Dj . C stands for an energy-independent constant Type Dj E E0 E E0 Three dimensions M0 M1 M2 M3 0 C (E0 E)1/2 C (E0 E)1/2 (E E0 )1/2 C C (E E0 )1/2 0 Two dimensions M0 M1 M2 0 ln(E0 E) C C ln(E E0 ) 0 One dimension M0 M1 0 (E0 E)1/2 (E E0 )1/2 0 M1 ωg M3 Minimum ωg Saddle point Maximum ωg εi ωg Minimum ωg ωg ωg εi 2 Dimensions ωg 1 Dimensions M2 εi 3 Dimensions M0 Maximum ωg Fig. 6.9. Schematic dependence of the imaginary part of the dielectric constant (Âi ) on frequency near Van Hove singularities (i.e., interband critical points) in one, two, and three dimensions 263 264 6. Optical Properties I 50 Si (a) 40 Theory Experiment 30 εr 20 10 0 –10 –20 0 1 2 3 4 5 6 7 Photon energy [eV] (b) 40 Fig. 6.10a,b. A comparison between the experimental and calculated dielectric function of Si: (a) real part and (b) imaginary part. In (b) the results of two theoretical calculations, one including and the other excluding local-field corrections, are presented [6.21]. For more recent theoretical results see [6.22, 23]. The local field corrections are due to changes in the higher Fourier components of the crystal (pseudo)-potential induced by the electromagnetic field. Note that, according to (b), their effect is small; they do not improve agreement with experimental data. The sharp peak observed at 3.3 eV has been attributed to excitonic effects (see Sect. 6.3.3 and [6.24]) Experiment With local-field corrections Without local-field corrections 30 εi 20 ×3 10 0 0 2 4 6 8 10 12 Photon energy [eV] calculated with the k · p method. The agreement between theory and experiment is quite good in all three cases because some of the input parameters for the band calculations were actually determined by fitting structures observed in the experimental curves. This limitation of the empirical methods of band structure calculations has been overcome in more recent ab initio pseudopotential calculations as discussed in Sect. 2.5.2. There are many similarities in the overall shape of the imaginary part of the dielectric functions in Figs. 6.10–12. This is true not only for the three semiconductors shown here, but also for most of the tetrahedrally bonded semiconductors in the group IV, III–V and II–VI families. The main difference between their dielectric functions lies in the energies of the transitions. A close examination of the Âi of these semiconductors shows that they all possess the following features: 6.2 The Dielectric Function Fig. 6.11a,b. Results for GaAs similar to those presented in Fig. 6.10 for Si (the theoretical results do not include local field corrections) [2.8] p. 105 30 25 GaAs (a) Theory Experiment 20 εr 15 10 5 0 –5 –10 –15 0 1 2 3 4 5 6 7 8 6 7 8 Photon energy [eV] 30 (b) 25 εi 20 15 10 5 0 0 1 2 3 4 5 Photon energy [eV] • An onset due to transitions between the absolute valence band maximum and the conduction band minimum. This is known as the fundamental absorption edge. The strength of this absorption edge depends on whether the valence band maximum and the conduction band minimum occur at the same point in the Brillouin zone. Since transitions between bands with the same wavevector are labeled as direct, semiconductors whose fundamental absorption edge involves a direct transition are said to have a direct absorption edge. Otherwise the absorption edge is said to be indirect. Diamond, Si, SiC, Ge, AlAs, AlSb, and GaP have indirect absorption edges, while GaN, GaAs, GaSb, InP, InAs, InSb and all the II–VI semiconductors have direct absorption edges. Within the scheme presented so far, optical transitions across an indirect bandgap are not allowed by the wavevector conservation condition. As we shall show in the next section, optical transitions between two bands with different wavevectors (knows as indirect transitions) are possible with the involvement of phonons, although they are orders of magnitude weaker than direct transitions. Hence they can be observed only when their energy is below that of all the direct transitions. Âi becomes appreciable usually at the onset of the lowest-energy direct 265 266 6. Optical Properties I E2 E1(Λ3 – Λ1) 25 E1(L3 – L3) 20 εi E0(Γ25 – Γ15 ) 15 Calc. Exp. > 10 Ge 5 L3 – L 1 0 2 3 4 Photon energy [eV] 5 6 Fig. 6.12. A comparison between the experimental and calculated imaginary part of the dielectric function in Ge. The theoretical curve was calculated from a band structure obtained by the k · p method without spin-orbit interaction [6.25] • • transition. In the diamond and zinc-blende-type semiconductors this transition usually occurs at the center of the Brillouin zone between the °4v valence band and the °1c conduction band and is usually referred to in the literature as the E0 transition. Whenever the valence band has a sizable spin–orbit interaction, for example in semiconductors containing heavy elements such as In, As, and Sb, this transition is split by spin–orbit coupling into two transitions. The higher energy °7v –°6c transition involving the split-off valence band is labeled the E0 ¢0 transition. Above the fundamental absorption edge, Âi typically rises to an asymmetric peak related to transitions occurring along the eight equivalent [111] directions of the Brillouin zone (a direction and all equivalent ones are represented as 111). If the spin–orbit coupling is small (such as in Si and GaP), only one peak is observed and the transition is known as the E1 transition. Band structures suggest that these transitions involve M1 -type critical points in their joint density of states. [Since the negative longitudinal mass of these transitions (i.e., (1/·1 ), with ·1 defined in (6.54)) is very large, the E1 critical points are often modeled by a two-dimensional M0 critical point.] When the spin–orbit interaction in the valence bands is large, the E1 transitions are split into the E1 and E1 ¢1 transitions. Using the k · p method, the spin–orbit splitting in the valence band along the 111 directions ¢1 can be shown to be approximately 2/3 of the spin– orbit splitting ¢0 at zone center [6.11]. This “two-thirds rule” provides a consistency check on the identification of the E1 transitions. Table 6.2 lists ¢0 , ¢1 and the ratio ¢0 /¢1 in a number of tetrahedrally coordinated semiconductors. Except for InP and GaN, this rule is well obeyed by all the semiconductors in the list (see Problem 6.20). Âi reaches a strong absolute maximum known as the E2 peak. This peak contains contributions from transitions occurring over a large region of the 6.2 The Dielectric Function Table 6.2. The valence band spin–orbit splitting at zone center (¢0 ) and in the 111 directions (¢1 ) and their ratio in several tetrahedrally coordinated semiconductors (list compiled from [6.19]). GaN values were calculated with the LCAO-LDA method in [6.26]. The experimental value of ¢0 for GaN is 17 ± 1 meV [6.26] • Semiconductor ¢0 [eV] ¢1 [eV] ¢0 /¢1 Si Ge GaN GaAs InP InAs InSb ZnSe CdTe 0.044 0.296 0.019 0.341 0.108 0.38 0.803 0.432 0.949 0.03 0.187 0.032 0.220 0.133 0.267 0.495 0.27 0.62 1.47 1.58 0.59 1.55 0.81 1.42 1.62 1.59 1.53 Brillouin zone close to the edges in the 100 and 110 directions [6.21]. Some of these transitions are associated with M2 critical points. Superimposed on these features are weaker structures labeled E0 and E1 transitions. These involve transitions between the valence bands and higher conduction bands at the zone center and along the 111 directions, respectively. The above system for labeling the interband optical transitions was proposed by Cardona [6.11]. Transitions occurring at the zone center, along the 111 directions and along the 100 directions are denoted by subscripts 0, 1, and 2, respectively. As an illustration, these optical transitions are indicated by arrows in the band structure of Ge in Fig. 6.13. This band structure has been calculated by a “full-zone k · p method”, which is an extension of the k · p method discussed in Sect. 2.6 in which the electron wavevector k is no longer restricted to be near a critical point but can extend all the way to the zone edge [6.18]. The overall agreement between theory and experiment in Figs. 6.10–12 supports the identifications of the structures in the optical spectra in terms of critical points in the density of states. It should be pointed out that many of the remaining disagreements between theory and experiment in Figs. 6.10–12 have since been removed in more recent calculations. The present “state of the art” is represented by ab initio calculations which include Coulomb interaction between the excited electron and the hole left behind. This interaction enhances the E1 transitions while weakening E1 , thus correcting deficiencies of Figs. 6.10, 11 [6.22, 23]. Table 6.3 lists the experimental energies of structures in the optical spectra measured at low temperatures for a number of semiconductors. In principle, by comparing these energies with critical point energies in the calculated joint density of states, the types of Van Hove singularities responsible for these structures can be deduced. In practice, the higher energy transitions are often found to contain contributions from several critical points of different types. Only the E0 and E1 transitions can be attributed definitively to three-dimensional critical points with M0 and M1 (or two-dimensional M0 ) types of Van Hove singularities. 267 6. Optical Properties I Λ4 , Λ5 Λ6 4 E1 Γ6– E1+∆ 1 E1 Λ4 , Λ5 – Γ7 E E 0 + ∆ 0 0 + Γ8 E0> ∆6 Λ6 X5 E2 > – L 4,L–5 L–6 2 > Λ6 L+6 ∆7 Γ8– >> L+4,L+5 L+6 > > ∆7 Γ7 + ∆6 –2 > 268 eV π k= a (111) X5 2π k= a (100) k=(000) Fig. 6.13. The band structure of Ge showing the various direct transitions responsible for the structures in the imaginary part of the dielectric function shown in Fig. 6.12. The transitions giving rise to the various structures in the dielectric function are identified Table 6.3. The measured energies [eV] of the prominent structures in the optical spectra of some diamond and zinc-blende-type semiconductors. All energies are low temperature values except that of the E0 transition in Si, which was measured at room temperature. Compiled from data listed in [6.27], [6.28] and [6.29]. a Transition Si Ge GaAs InP GaP GaN E0 E0 ¢0 E1 E1 ¢1 E0 E0 ¢0 E2 E1 4.185 4.229 3.45 — 3.378 — 4.330 5.50 0.898 1.184 2.222 2.41 3.206 3.39 4.49 5.65 1.5192 1.859 3.017 3.245 4.488 4.659 5.110 6.63 1.4236 1.532 3.287 3.423 4.70 5.17 5.05 2.869 2.949 3.780 3.835 4.72 4.88 5.22 6.8 3.302a 3.319a 7.03 7.63 Grown on MgO. 6.2.5 Direct Absorption Edges We shall now consider in more detail the optical transitions at the fundamental absorption edge, since many semiconductor optoelectronic devices, such as lasers and photodetectors, involve these transitions. As pointed out in the preceding section, there are direct and indirect absorption edges. In the case of 6.2 The Dielectric Function a direct absorption edge, Âi can be calculated from (6.48). Let mc and m˘ denote, respectively, the effective masses of the conduction and valence bands (assumed to be spherical for simplicity) and Eg the direct energy gap. The energy difference Ecv in the vicinity of the energy gap can be expanded as Ecv Eg (2 /2Ì)k2 , (6.56) 1 where Ì is the effective mass defined by Ì1 m1 c mv . Using (6.52) the joint density of states Dj can be calculated to be 1/2 3/2 2 3 [2 Ì /( )](Ecv Eg )1/2 for Ecv Eg , (6.57) Dj 0 for Ecv Eg . Substituting this result into (6.48) we obtain Âi near Eg as Âi (ˆ) Ax –2 (x 1)1/2 0 for x 1, for x 1, (6.58a) where A 2e2 (2Ì)3/2 |Pcv |2 Eg3/2 m2 and x ˆ/Eg . (6.58b) Using the KKRs, Âr near Eg can be shown to have the form (Problem 6.2). Âr (ˆ) const Ax2 [2 (1 x)1/2 ] for x 1, const Ax2 [2 (1 x)1/2 (1 x)1/2 ] for x 1, (6.59) where the constant term is determined by contributions from transitions above the fundamental absorption edge. According to (6.58) a plot of Â2i , or the square of the absorption coefficient, as a function of the photon energy should be a straight line. The energy gap is given by the intercept of the line with the x axis and either Ì or |Pcv |2 can be determined from its slope. An example of such a plot is given in Fig. 6.14 for PbS. An equivalent semilogarithmic plot for InSb is given in Fig. 6.15. A fit to the experimental values of Âr (ˆ) in PbS with the expression (6.59) is shown in Fig. 6.14 (b). 6.2.6 Indirect Absorption Edges If the lowest energy gap is indirect, a photon can excite an electron from the valence band to the conduction band with the assistance of a phonon. The wavevector difference between the electrons in the two bands is supplied by the phonon. If the phonon energy and wavevector are denoted by Ep and Q, the energy- and wavevector-conservation conditions in the optical process are represented by 269 6. Optical Properties I Absorption coefficient squared [108 cm–2] 2.5 PbS 2.0 (a) 22 1.5 (b) 77 K 20 1.0 εr 373 K 18 0.5 Experiment 16 0.35 0.45 0.55 0.2 0.65 0.3 0.4 0.5 Photon energy [eV] Photon energy [eV] Fig. 6.14. (a) Plot of the square of the absorption coefficient of PbS as a function of photon energy showing the linear behavior discussed in the text. The intercept with the x-axis defines the direct energy gap. Reproduced from [6.30]. (b) Fits (curves) to the experimental values of the real part of the dielectric function of PbS (data points) measured at 77 and 373 K with the expression in (6.59). Reproduced from [6.144]. InSb 10 4 αhω [cm–1eV] 270 10 3 Experiments αhν=A(hω–Eg)1/2 Corrected for variation of matrix element 10 2 10 0 0.2 0.4 0.6 0.8 Photon energy hν [eV] Fig. 6.15. Semilogarithmic plot of the absorption coefficient of InSb at 5 K as a function of photon energy. The filled circles represent experimental results from [6.31]. The curves have been calculated using various models. The intercept with the x-axis gives the direct bandgap of InSb [6.32] 6.2 The Dielectric Function > > E > > | Γ15 > HeR-mediated transition H ep-mediated transition 1 > > X1 ∆1 1 Fig. 6.16. Schematic band structure of Si as an indirect-bandgap semiconductor showing the phonon-assisted transitions (labeled 1 and 2) which contribute to the indirect absorption edge. |°15 and |¢5 represent intermediate states 2 Γ25 >k 2 > | ∆ 5> X4 ˆ Ecv ± Ep and kc kv ∓Q, (6.60) where and correspond, respectively, to emission and absorption of a phonon. Processes involving several phonons are in principle also possible but usually with much smaller probabilities. As a specific example of an indirect absorption edge we will consider Si. The band structure of Si in the vicinity of the indirect gap ¢1 °25 is shown schematically in Fig. 6.16. The absorption processes near this energy gap now consist of two steps. One of these steps involves the electron–photon interaction eR while the other step involves the electron–phonon interaction ep . Both interactions will be assumed to be weak enough for perturbation theory to be valid. The calculation of the optical transition probability can therefore be performed by using second order perturbation theory. A systematic way to calculate this probability makes use of Feynman diagrams. We shall defer the discussion of this technique until Chap. 7, when we apply it to study Raman scattering. Using Feynman diagrams to calculate the transition probability at an indirect absorption edge is left for Problem 7.7. In this chapter we shall point out, without proof, several possible processes which contribute to the indirect absorption edge. In one of them an electron is first excited via a virtual transition (i. e., a transition which does not conserve energy – although such transitions have to conserve wavevector as a result of the translation symmetry of the crystal) from the valence band to an intermediate state |i by absorbing the incident photon. A second virtual transition takes the electron from |i to the ¢1 conduction band state via absorption or emission of a phonon. In the final state there is an electron in the ¢1 conduction band, a hole in the °25 valence band state and a phonon has been either created or annihilated. This process is shown schematically for Si in Fig. 6.16 by arrows labeled 1. A second possible phonon-assisted indirect optical transition is also shown in the same figure by arrows labeled 2. These processes are similar except that for process 2 the intermediate states occur at ¢. 271 272 6. Optical Properties I There are other possible processes which contribute to absorption at an indirect bandgap. In principle these terms have to be combined with the contributions from the above two in calculating the transition probability. To understand why the above two terms have been singled out, we shall examine their contribution to the transition probability Rind using an extension of Fermi’s Golden Rule to second order perturbation (see Sect. 7.2.4 for further details): 2 2 f|ep |ii|eR |0 Rind ‰(Ec (kc ) Ev (kv ) ˆ ± Ep ); Ei0 ˆ i kc ,kv (6.61) |0 represents the initial state of the system with a filled valence band and an empty conduction band and phonon occupation number Np . In the final state |f an electron has been excited into the ¢1 conduction band, a hole has been created at the °25 valence band, and Np has changed by one. For the two processes in Fig. 6.16, the intermediate state |i involves either an electron excited into the ¢1 conduction band (shown by arrow 2) or a hole created at the °25 valence band (shown by arrow 1). In principle, it is necessary to permute the time order in which eR and ep occur and also to sum over all possible intermediate states |i in calculating Rind . However, processes in which the phonons excite an electron across the gap make a negligible contribution because of the energy denominator in (6.61). Similarly, intermediate states for which Ei0 ˆ are unimportant. As a result, the two processes shown in Fig. 6.16 are usually the most important ones. In many semiconductors, the matrix elements which appear in (6.61) can be assumed to be constant in the vicinity of the indirect bandgap. Therefore the photon energy dependence of Rind can be obtained by summing over the delta function in (6.61). By converting the summations over kc and kv to integrations over the conduction and valence band energies Ec and Ev , respectively, via their density of states Dv (Ev ) and Dc (Ec ) we obtain Rind ∝ Dv (Ev )Dc (Ec )‰(Ec Ev ˆ ± Ep )dEc dEv . (6.62) Assuming that the bands are parabolic and three-dimensional, we find (Ev )1/2 for Ev 0, (6.63) Dv ∝ 0 for Ev 0, and Dc ∝ (Ec Eig )1/2 0 for Ec Eig , for Ec Eig . (6.64) The zero of the energy scale has been taken at the top of the valence band and Eig is the indirect energy gap. Substituting Dv and Dc into (6.62) and integrating over Ev one obtains ˆ∓E p Eig Rind ∝ (Ec Eig )1/2 (ˆ ∓ Ep Ec )1/2 dEc . Eig (6.65) 6.2 The Dielectric Function By changing the variable to x Ec Eig , ˆ ± Ep Eig (6.65) can be expressed as 1 Rind ∝ (ˆ ∓ Ep Eig ) x1/2 (1 x)1/2 dx. 2 (6.66) 0 On performing the integral in (6.66) we can conclude that, in the vicinity of an indirect bandgap, Âi depends on the photon energy as Âi (ˆ) ∝ (ˆ ∓ Ep Eig )2 0 for ˆ ≥ Eig ± Ep , otherwise. (6.67) Thus an indirect energy gap can, in principle, be distinguished from a direct one by the different dependence of their absorption coefficients on photon energy. In addition, every indirect energy gap gives rise to two absorption edges, at Eig Ep and Eig Ep , for each phonon Ep that can mediate the indirect transition. The edge at Eig Ep corresponds to phonon absorption. The electron–phonon matrix element |f|ep |i|2 in (6.61) is proportional to Np , where Np is the phonon occupation number (Sect. 3.3.1). This absorption edge is therefore present only at high temperatures and disappears at temperatures too low for such phonons to be thermally excited. On the other hand, the higher energy edge at Eig Ep involves phonon emission and hence is proportional to (1 Np ). It is present at both high and low temperatures. Identification of these two edges by their different temperature dependence enables not only Eig but also Ep to be determined. Figures 6.17–19 show the absorption edges of three indirect bandgap semiconductor: Si, Ge, and GaP. In these materials several phonons can participate in indirect transitions, giving rise to a number of absorption thresholds. The temperature dependence of these edges in Ge and GaP is shown in Figs. 6.18 and 19. Notice that at low temperature the shape of these indirect absorption edges deviates from the proportionality to the square of the photon energy predicted by (6.67). Instead, their shape resembles more the square root dependence given in (6.58) for direct gaps. The explanation for this deviation is that exciton effects modify the shape of these indirect absorption edges at low temperatures. These effects will be discussed in Sect. 6.3. 6.2.7 “Forbidden” Direct Absorption Edges The last case we shall consider involves a direct-bandgap semiconductor where an electric dipole transition between the top valence band and the lowest conduction minimum is forbidden by a selection rule. One example of a semicon- 273 6. Optical Properties I K 290 249 K K 195 K 10 333 9 Si α1/2 [cm –1/2] 8 7 6 5 4 3 2 1 0 1.0 1.1 1.2 1.3 1.4 Photon energy [eV] Fig. 6.17. Plots of the square root of the absorption coefficients of Si versus photon energy at several temperatures. The two segments of a straight line drawn through the experimental points represent the two contributions due to phonon absorption and emission [6.33] 6 Ge 2.3 291 K 5 195 K 90 K 2.2 249 K 4 < 0.709 3 0.708 77 K 0.707 Square root of absorption coefficient [cm–1/2] 274 4.2 K & 20 K 2 0.9 1 0.7 0.769 0.771 0 0.62 0.64 0.66 0.68 0.70 0.72 0.74 0.76 0.78 0.80 0.82 0.84 0.86 Photon energy [eV] Fig. 6.18. Plots of the square root of the absorption coefficients of Ge versus photon energy at several temperatures. The two insets compare the exciton-induced abruptness of the absorption edge due to phonon emission at high and low temperatures [6.34] ductor with such a “forbidden” direct absorption edge is Cu2 O, whose crystal structure and zone-center phonon properties were studied in Problem 3.1. This crystal is centrosymmetric. Both the conduction and valence band extrema oc- 6.2 The Dielectric Function 6 78 K GaP 5 19 K LO+TA2 TO+TA1 3 LO TO 2 > > > TA 2 > > 1 > α1/2[cm –1/2] 4 LA Fig. 6.19. Plots of the square root of the absorption coefficients of GaP versus photon energy at two different temperatures. The labels denote the exciton-enhanced absorption thresholds associated with the emission of various phonon modes. Note the square-root singularities at the onset of the various phonon-aided processes. These square-roots are typical of indirect excitonic absorption (e.g. without k conservation) [6.35] > > 0 2.30 2.34 2.38 2.42 Photon Energy [eV] cur at the zone center and have even parity [6.36]. The electron momentum operator p in eR has odd parity under inversion. As a result of the matrixelement theorem discussed in Sect. 2.3.3, electric dipole transitions are allowed only between states of different parity. Hence they are forbidden by the parity selection rule at the absorption edge of Cu2 O. In the case of optical transitions involving isolated atoms or molecules, the electronic density of states has discrete peaks. When the electric dipole matrix element vanishes one may have to consider higher order optical transitions (such as quadrupole transitions). For interband transitions the density of states is a continuum. When |Pvc |2 is zero at an M0 critical point, this does not imply that there will be no electric dipole absorption edge; the density of states is zero anyway at an M0 critical point. The vanishing of |Pvc |2 exactly at the critical point just means that one has to consider the possibility that |Pvc |2 does not vanish for electron wavevectors k slightly off the critical point. In general, one finds |Pvc |2 to have a nonzero k-dependent component. For example, in the case of Cu2 O one can use the k · p expansion in (2.37) to express either the conduction or valence band wavefunctions as a function of k. This expansion introduces some mixture of odd-parity wavefunctions, giving rise to parity-allowed electric-dipole transition matrix elements. Phenomenologically one can expand |Pvc |2 as a Taylor series in k. Assuming that the critical point occurs at k 0 and |Pvc (0)|2 0, we find |Pvc (k)|2 |dPvc /dk|2 k2 0(k4 ). (6.68) When we substitute (6.68) into (6.48) the optical transition matrix element introduces a term proportional to k2 . Since the joint density of states at a direct gap is proportional to k in three dimensions (6.57), Âi (ˆ) becomes proportional to k3 . Hence for a direct and “forbidden” bandgap semiconductor Âi (ˆ) depends on photon energy as 275 276 6. Optical Properties I Âi (ˆ) ∝ (ˆ Eg )3/2 0 for ˆ Eg for ˆ Eg . (6.69) Compared to direct but “allowed” absorption edges, a “forbidden” edge increases more slowly with energy in the vicinity of the bandgap. As a result, “forbidden” absorption edges are difficult to identify except when there are strong exciton effects which change the smooth absorption edges into sharp peaks. These effects will be studied in the next section. 6.3 Excitons The approach we have adopted so far to view optical absorption processes is that an incident radiation field excites an electron–hole pair inside the semiconductor. The properties of the electron and the hole are both described by the band structure within the one-electron approximation. In this section we shall go beyond this approximation and consider the effects of electron– electron interaction on the absorption spectra. To simplify the calculation we shall make the following assumptions. We shall include only the Coulombic part of the electron–electron interaction neglecting both exchange and correlation terms. Furthermore, the interaction between the excited electron in the conduction band and those left behind in the now almost filled valence band will be replaced by an electron–hole interaction. Attraction between the electron and the hole causes their motion to be correlated and the resultant electron–hole pair is known as an exciton. Typically excitons have been studied in two limiting cases. For strong electron– hole attraction, as in ionic crystals, the electron and the hole are tightly bound to each other within the same or nearest-neighbor unit cells. These excitons are known as Frenkel excitons. In most semiconductors, the Coulomb interaction is strongly screened by the valence electrons via the large dielectric constant. As a result, electrons and holes are only weakly bound. Such excitons are known as Wannier–Mott excitons [6.37, 38] or simply as Wannier excitons. In this book we shall be concerned with Wannier excitons only [6.39–41]. The properties of Wannier excitons can be calculated with the effective mass approximation introduced in Sect. 4.2. Within this approximation, the electron and the hole are considered as two particles moving with the effective masses of the conduction and valence bands, respectively. Donors and acceptors studied in Chap. 4 can be regarded as “excitons” in which one of the particles has an infinite effective mass. Since the difference in effective mass between the electron and the hole in a semiconductor is not as large as that between the electron and the proton, excitons are more analogous to positro- 6.3 Excitons nium, an electron–positron pair. As a result of the Coulomb interaction between the electron and hole, the potential acting on an electron (or a hole) in a crystal is not translationally invariant. As in any two-particle system, the exciton motion can be decomposed into two parts: a center-of-mass (CM) motion and a relative motion of the two particles about the CM. With this decomposition, the potential acting on the exciton CM still has translational invariance since the Coulomb interaction depends only on the relative coordinate of the electron and hole. Within the effective mass approximation, the exciton CM behaves like a free particle with mass M me mh (where me and mh are, respectively, the electron and hole effective masses). The relative motion of the electron and the hole in the exciton is similar to that of the electron and the proton inside the hydrogen atom. There are bound states and continuum states. The bound states are quantized with principal quantum numbers n 1, 2, 3, etc., and orbital angular momentum l 0, , 2, etc. In the continuum states, excitons can be considered to be ionized into free electrons and free holes but their wavefunctions are still modified by their Coulomb attraction. In the literature, one often finds schematic diagrams in which the exciton energy levels are shown superimposed on a one-electron energy band structure. Strictly speaking this is incorrect. Since the exciton is a two-particle state, its energy levels cannot be represented by one electron energy levels. To clarify this point further, we compare the energies of an electron–hole pair in a one-electron energy band diagram and in a two-particle energy diagram in Fig. 6.20. In the one-electron picture the ground state of the semiconductor is represented by a filled valence band and an empty conduction band. Since there are no electron–hole pairs in the ground state, this state is represented by the origin in the two-particle picture. In the one-particle picture, the excited state is represented by an electron in the conduction band (with wavevector ke ) and a hole in the valence band (wavevector kh kv ). This excited state corresponds to an exciton in the two-particle state. We note that optical excitation is not the only mechanism for creating such excited states. An energetic electron, for example, can also create an exciton. In the two-particle picture, the exciton wavevector K is given by ke kh . As pointed out earlier, the potential for the exciton CM motion is translationally invariant even when the electron is attracted to the hole. K is therefore a good quantum number. The kinetic energy Eke of the exciton is related to K by the free-particle expression [to be derived later, see (6.78)] Eke 2 K 2 . 2M (6.70) Thus exciton levels can be represented by parabolas in the two-particle energy diagram in Fig. 6.20b. We shall show later that the exciton state wavefunction with CM wavevector K is a linear combination of many electron–hole pair wavefunctions with wavevectors ke and kh satisfying the condition K ke kh . Thus the one-particle picture in Fig. 6.20a is not correct even for the exciton continuum states. 277 278 6. Optical Properties I (a) One-electron picture (b) Two-particle picture Eeh E Empty Ground state k K Filled 0> Eeh E ke Ee + E h Excited state –kh k K=ke + kh K 0> Eeh • Cannot be represented in one-electron picture Correlated e – h pair (exciton) n=1 2 2 E1 + h K 2M E1 K 0> Eeh E Optical absorption • n=1 Photon k Photon K 0> Fig. 6.20. Comparison between the energy levels of the ground state and excited states of a semiconductor in a one-electron band picture (a) and in a two-particle picture (b). Also, schematic diagrams showing processes in which a photon is absorbed while producing an electron-hole pair Figure 6.20b shows schematically an optical transition in the two-particle energy diagram. Since the CM motion is translationally invariant, wavevector conservation applies only to the exciton wavevector and not to those of the 6.3 Excitons individual electrons or holes. To conserve both energy and wavevector during absorption, this process can occur only at the intersection between the radiation (or photon) and the exciton dispersion curves, as shown in Fig. 6.20b. At this point the electron–radiation (or more precisely the photon–exciton) interaction couples the exciton and radiation to form a mixed mechanical-electromagnetic wave known as an exciton-polariton [6.42, 43]. These will be studied after we have considered excitonic effects at different kinds of critical points. 6.3.1 Exciton Effect at M0 Critical Points We now consider quantitatively the effect of Coulomb attraction on the motion of electrons and holes in the vicinity of an M0 critical point of a direct bandgap semiconductor in three dimensions. We shall assume the conduction band to be spherical with energy 2 k2e , (6.71) 2me where Eg is the bandgap, and the corresponding hole energy to be given by Ee (ke ) Eg 2 k2h . (6.72) 2mh Let the Bloch functions for the electron and the hole be represented by „kc (re ) and „kh (rh ), respectively. As in Sect. 4.2 we assume that the Coulomb interaction between electron and hole is weak due to screening by the valence electrons, so that the effective mass approximation is valid. We write the exciton wavefunction æ as a linear combination of the electron and hole wavefunctions: æ(re , rh ) C(ke , kh )„ke (re )„kh (rh ). (6.73) Eh (kh ) ke ,kh Similar to the case of the donor electron in Sect. 4.2, the electron and hole in an exciton are localized relative to their CM, so it is more convenient to express their wavefunctions in terms of Wannier functions rather than Bloch functions. In terms of the Wannier functions aRe (re ) and aRh (rh ) for electron and hole, respectively, the exciton wavefunction can be written as æ(re , rh ) N 1/2 º(Re , Rh )aRe (re )aRh (rh ), (6.74) Re ,Rh where º(Re , Rh ) is the exciton envelope wavefunction. The wave equation for º(Re , Rh ) analogous to (4.22) is [6.44] e2 2 2 2 2 ∇ Re ∇ Rh º(Re , Rh ) 2me 2mh 4Â0 Â0 |Re Rh | (6.75) Eº(Re , Rh ), where Â0 is the zero-frequency dielectric constant of the semiconductor. Equation (6.75) can be solved in the same way as in the case of the hydrogen atom. 279 280 6. Optical Properties I One expresses Re and Rh in terms of two new coordinates: a center-of-mass coordinate R and a relative coordinate r defined by R me Re mh Rh and r Re Rh . me mh (6.76) The equation of motion for the CM is now decoupled from that for the relative motion because the Coulomb interaction term does not involve R. The two resultant equations are 2 ∇2R „(R) ER „(R), (6.77a) 2M 2 e2 ∇2r 2Ì 4Â0 Â0 r ˇ(r) Er ˇ(r), (6.77b) where Ì, the reduced mass of the exciton, is defined by 1 1 1 . Ì me mh (6.77c) The total energy of the exciton E is simply the sum of ER and Er . The solutions of (6.77a and b) can be obtained readily. Equation (6.77a) describes a free particle whose eigenfunction and energy are given by „K (R) (N)1/2 exp(iK · R) and ER 2 K2 . 2M (6.78) ER represents the kinetic energy of the CM motion and is therefore the same as Eke in (6.70). Equation (6.77b) is similar to the equation describing the motion of the donor electron discussed in Sect. 4.2.2. As in the hydrogen atom, its wavefunctions and energies can be indexed by three quantum numbers: a principal quantum number n, the angular momentum quantum number l and the magnetic quantum number m. The wavefunction ˇ can be expressed in polar coordinates (r, ı, ˇ) as: ˇnlm (r) Rnl (r)Ylm (ı, ˇ), (6.79) where Rnl (r) can be expressed in terms of the associated Laguerre polynomials and Ylm (ı, ˇ) are the spherical harmonic functions. These functions are tabulated in many quantum mechanics textbooks and therefore will not be reproduced here. For isotropic effective masses Er depends on n only and is given by Er (n) Er (∞) R∗ , n2 (6.80) where Er (∞) is the minimum energy of the continuum states, i. e., the energy gap Eg in (6.69), and R∗ is the Rydberg constant for the exciton defined as 6.3 Excitons Ìe4 R∗ 2 2 (4Â0)2 Â20 Ì mÂ20 × 13.6 eV. (6.81) If the hole mass is much heavier than the electron mass, as in the case of most tetrahedrally bonded direct gap semiconductors, the reduced mass Ì is close to the electron effective mass and hence the exciton Rydberg constant should be comparable to the donor binding energy. Furthermore, the exciton Bohr radius is also comparable to the donor electron Bohr radius. Combining the above results for the relative motion and CM motion of the exciton, we obtain the following envelope wavefunctions and energies for the exciton: √ ºnlm (R, r) (1/ N) exp(iK · R)Rnl (r)Ylm (ı, ˇ), (6.82) 2 K 2 R∗ (6.83) 2. 2M n The energy spectrum of a Wannier exciton is shown schematically in Fig. 6.20b and in greater detail in Fig. 6.21. The above model of excitons based on electrons and holes with spherically symmetric parabolic dispersion is useful for understanding qualitatively exciton effects on optical spectra. However, it is not accurate enough for quantitative interpretation of experimental spectra in diamond- and zinc-blende-type semiconductors. As we discussed in Chap. 2, the valence band structure in these families of materials is complicated by degeneracies and warping. Of the various attempts to calculate excitonic effects based on realistic band structures, we shall mention the one by Baldereschi and Lipari [6.46]. They calculated the exciton binding energies by using a “spherical effective hamiltonian” Enlm Eg E ∞ 2 R* n=1 E∞ = Eg 0> K Fig. 6.21. The energy states of a Wannier exciton showing both its bound states n 1 to 3 and the continuum states. Eg is the bandgap and R∗ the exciton binding energy 281 282 6. Optical Properties I Table 6.4. Exciton binding energy (R∗ ) and Bohr radius (a0 ) in some direct bandgap semiconductors. The three semiconductors labeled (W) have the wurtzite crystal structure while the others have the zinc-blende structure. Experimental values of R∗ for GaAs and InP are from [6.48, p. 155] and for CdTe, ZnTe, ZnSe and ZnS are from [6.49]. The corresponding values for a0 are calculated from (4.25) by substituting the experimental values of the reduced mass (rather than the effective mass m∗ ) and the static dielectric constant. The theoretical values of R∗ are from [6.46] Semiconductor GaNa GaAs InP CdTe ZnTe ZnSe ZnS ZnO (W) CdSe (W) CdS (W) a R∗ [meV] R∗ (theory) [meV] 27 4.9 5.1 11 13 19.9 29 59 15 27 32 4.4 5.14 10.71 11.21 22.87 38.02 a0 [Å ] 24 112 113 70 56 45 28 for the A-exciton of wurtzite GaN, see [6.45] to treat the holes similar to the one they proposed for hydrogenic acceptors (Sect. 4.2.4) [6.47]. Table 6.4 lists the experimentally determined exciton binding energies and Bohr radii in a number of direct bandgap semiconductors. The binding energies are compared with the theoretical values obtained in [6.46]. While the agreement between theory and experiment is quite good for R∗ in the smaller-bandgap semiconductors, there are significant discrepancies for the more ionic materials. We mention that Altarelli and Lipari [6.50] have calculated the exciton dispersion in semiconductors with degenerate valence bands and showed that there are striking deviations from the parabolic dependence of (6.83). However, a detailed discussion of this calculation is beyond the scope of this book. 6.3.2 Absorption Spectra of Excitons In principle, the absorption spectra of excitons can be calculated from the exciton energies and wavefunctions in (6.83 and 82) with the introduction of an interaction Hamiltonian between excitons and photons. Conceptually, however, optical absorption by excitons is different from optical absorption in the one-electron picture. In the two-particle picture, optical absorption is the conversion of a photon into an exciton; conservation of energy and wavevector requires that this process must occur at the point where the photon dispersion curve (broken line in Fig. 6.22b) intersects the exciton dispersion curves. At these intersections the photon and exciton are degenerate. When an exciton– photon interaction (even a very weak one) is introduced, the resultant eigen- 6.3 Excitons 20620 Fig. 6.22. Dispersion curves of a “bare” photon, a “bare” exciton (dashed curves) and an exciton-polariton (solid curves labeled I and II) for the A exciton in CdS. The curves labeled I and II are usually referred to as the “upper” and “lower” branches of the polariton [6.51] I Photon Frequency [cm–1] ωL II 20600 Exciton ωT 20580 –3 –2 –1 0 1 2 3 Wave vector [106 cm–1] states are linear combinations of the photon and exciton wavefunctions. Such a “coupled state” of an exciton with a photon is known as an exciton-polariton. Its dispersion relations (solid curves labeled I and II) are different from those of the uncoupled or “bare” photon and exciton as shown in Fig. 6.22 (drawn for the so-called A exciton in CdS). In general, “polariton” is the name given to any coupled electromagnetic and polarization wave traveling inside a medium. The polarization wave in the present case is associated with the electric dipole moments of the excitons (assumed to be nonzero). As excitons travel in the medium they radiate electromagnetic waves. In turn, the electromagnetic waves can excite excitons. In principle, there is no way to separate the exciton wave from the electromagnetic wave. Thus introducing an exciton–photon interaction does not necessarily mean that energy will be lost by photons inside the medium. In this polariton picture energy is converted from photons to excitons and vice versa. Suppose the sample is a thin slab and light is incident on the sample from the left. Outside the sample there is only an electromagnetic field associated with the photons. As it enters the sample the electromagnetic wave is converted into a polariton wave (Fig. 6.23). Unless there are other interactions that can scatter the polaritons inside the sample, they will travel unattenuated to the sample surface on the right. On exiting the slab from the right surface, the polaritons are reconverted into photons with no loss except for those polaritons reflected back at the surface. Thus no optical absorption has occurred inside the medium. In order for absorption to occur (that is, for energy to be dissipated from the photon field that enters the sample) polaritons have to be scattered inelastically, e. g., by phonons. After inelastic scattering some po- 283 6. Optical Properties I Sample Incident photon > > Reflected photon Transmitted polariton > > 284 Transmitted Photon > Reflected polariton Fig. 6.23. A schematic diagram showing the transmission of photons through a semiconductor slab via propagation of polaritons inside the sample laritons will eventually exit the sample and appear in the form of emission (or luminescence, see Chap. 7 for further details) at a different photon energy. The relative probability of re-emission and relaxation via phonons depends on the polariton branch. High energy polaritons from branch I in Fig. 6.22 have large photon components in their wavefunction (and therefore are said to be photon-like); they have little interaction with phonons and are more likely to escape from the medium. However, once they are scattered elastically by defects into branch II, with a large exciton component in their wavefunctions (or exciton-like), they lose their energy efficiently via scattering with phonons or by nonradiative recombination. It is predominantly through the latter that energy in polaritons becomes dissipated inside a medium, resulting in optical absorption [6.52]. It is rather complicated to calculate the optical absorption using the above exciton-polariton picture since it is necessary to introduce energy dissipation processes for polaritons via phonon scattering. One way to avoid this difficulty is to assume that, as a result of scattering between excitons and phonons, the exciton damping constant is larger than the exciton–photon interaction. In this approximation one can replace polaritons by the “bare” photons and excitons. Whenever a photon is converted into an exciton it will lose its energy completely inside the medium via exciton damping processes. As a result, the rate of dissipation of energy from the photon field is completely determined by the rate of conversion of photons into excitons. Within this approximation we can use Fermi’s Golden Rule to calculate the optical transition probability per unit volume for converting a photon into an exciton. Similar to (6.43) we obtain R (2/) |f|xR |0|2 ‰(Ef (K) E0 ˆ), (6.84) f where |0 is the initial (ground) state with no excitons, |f the final state, where an exciton with energy Ef and wavevector K has been excited optically, and HxR the exciton–photon interaction. Because of wavevector conservation, K 6.3 Excitons should be equal to the photon wavevector, which is negligible, i. e., K ke kv ≈ 0. From now on we will therefore denote both kv and ke by k. The contributions to the imaginary part of the dielectric function (Âi ) due to exciton absorption consists of two parts: one arising from the bound states and the other from the continuum. For the discrete bound states, we can express the exciton wavefunction in terms of the envelope wavefunctions given in (6.82). The optical matrix element can be shown to be ([6.44] and Problem 6.7): √ f|xR |0 (1/ N)eik·r ˇnlm (r)„k (re )„k (rh )|xR |0 (6.85a) r,k √ (1/ N)eik·r ˇnlm (r)„ck |ceR |„vk . (6.85b) r,k If we assume that the matrix element „ck |ceR |„vk is independent of k, the summation of exp(ik · r) over k in (6.85) results in the delta function ‰(r). Hence the summation over r can be easily performed, giving |f|xR |0|2 N |ˇnlm (0)|2 |„ck |eR |„vk |2 . (6.86) When r 0, we have Re Rh and therefore |ˇnlm (0)| represents the probability of finding the electron and hole within the same primitive cell. The physical interpretation of (6.86) is that the probability of exciting an exciton optically is proportional to the overlap of the electron and hole wavefunctions. Since |ˇnlm (0)|2 is nonzero only for l 0, only excitons with s symmetry can be optically excited. Using the hydrogen atom wavefunctions one can show that Âi for the bound states is equal to (in atomic units with m0 e 1) 2 Âi (ˆ) ∞ 8 |P|2 Ì3 1 ‰(ˆ ˆn ), n3 ˆ2 (4Â0)3Â30 (6.87) 1 where |P|2 |„ck |ê · p|„vk |2 , see (6.41), and a factor of 2 has been included to take into account spin degeneracy. Thus the oscillator strength of the bound states with quantum number n decreases as n3 while their binding energy decreases as n2 . In the limit n → ∞ the discrete peaks of the bound states merge into a quasi continuum with density of states given by [6.44] n3 (4Â0 )2 Â20 dn . (6.88) dˆ Ì Substituting (6.88) into (6.87) we find that, as ˆ approaches the bandgap, Âi (ˆ) approaches Âi (ˆ) 8 |P|2 Ì2 . ˆ2g 4Â0 Â0 (6.89) For the continuum states the exciton wavefunctions can be expressed in terms of confluent hypergeometric functions [6.44, 53]. The corresponding contribution of exciton absorption to the imaginary part of the dielectric constant is given by ([6.44] and Problem 6.7) 285 6. Optical Properties I Âi 2 |P|2 (2Ì)3/2 (ˆ ˆg )1/2 ÙeÙ , ˆ2 sinh Ù (6.90) where Ù is defined (in atomic units) as. R∗ 1/2 Ù ˆ ˆg (6.91) > In the limit ˆ → ˆg one finds (Problem 6.7) that Âi approaches (6.89), and therefore it varies smoothly from the discrete bound states to the continuum, a physically rather appealing result. Figure 6.24 shows schematically the exciton absorption coefficient, including contributions from both the bound and continuum states. The broken curve displays the corresponding absorption coefficient when the exciton effect is neglected. We note that the exciton effect enhances the absorption coefficient both above and below the bandgap. Instead of decreasing to zero at the bandgap, the absorption coefficient approaches a constant as in the case of an M0 critical point in two dimensions. For a comparison of Elliott’s theory with experimental results, we show in Fig. 6.25 the absorption spectra of GaAs near the bandgap at different temperatures. Since the binding energy of the exciton in GaAs is about 5 meV (Table 6.4), only a broadened n 1 bound state is observed at 21 K. Notice that excitons in GaAs should become thermally ionized at room temperature; however, the GaAs absorption edge is still modified by excitonic effects. Excitonic effects also modify the shape of the absorption edge in indirect bandgap semiconductors such as Ge and GaP at low temperatures, as we pointed out in Sect. 6.2.6. Instead of rederiving the absorption coefficient in this case, we present the following argument. As shown in Fig. 6.21, the exciton energy levels consist of series of parabolas centered at K 0 in direct Absorption coefficient 286 n=1 Fig. 6.24. Comparison between the absorption spectra in the vicinity of the bandgap of a direct-gap semiconductor with (solid lines) and without (broken curve) exciton effects n=2 Eg Energy > absorption coefficient [104 cm–1] 6.3 Excitons GaAs 1.1 21 K 0.9 90 K 0.0 186 K 294 K 0.7 ~ ~ 1.42 1.44 1.46 1.48 1.50 1.52 1.54 Photon energy [eV] Fig. 6.25. Excitonic absorption spectra of GaAs near its bandgap for several sample temperatures. The gray lines drawn through the 21, 90 and 294 K data points represent fits with (6.90) [6.54] bandgap semiconductors. In an indirect bandgap semiconductor, such as Ge, the conduction band minima are at L and the valence band maximum is at the zone center. We therefore expect an exciton created from these band extrema to form parabolas centered at the wavevectors k0 kL , where kL is the wavevector of the electron at L at Ge. In the direct gap materials, excitons can be excited directly by photons only at the point where the photon and exciton dispersion curves intersect (Fig. 6.22). This wavevector conservation condition is relaxed in indirect gap materials by the participation of phonons. As a result, photons can excite excitons at any point on the parabolas with nearly the same probability. Thus the absorption coefficient is proportional to the density of final states, which has the same shape as the absorption edge at direct bandgap semiconductors for uncorrelated electron–hole pairs (i. e., without excitonic effects). Hence the absorption edge in indirect bandgap semiconductors including excitonic effects has the same dependence on energy as in a direct bandgap semiconductor without excitonic effects [represented by (6.58a)]. So far the best example of an excitonic Rydberg series has been found in the semiconductor Cu2 O. As pointed out in Sect. 6.2.6, the conduction and valence band extrema in Cu2 O have the same parity under inversion. Optical transitions between these two bands are electric-dipole forbidden but possible as magnetic-dipole or electric-quadrupole transitions. Their optical transition probability is thus proportional to the k-dependent term in the matrix element |c, k|k · p|v, k|2 . Using (6.68) one can show that this transition probability depends on the derivative |dºnlm (0)/dr|2 of the excitonic envelope function evaluated at r 0 [6.44]. This leads to the conclusion that exciton bound states with p symmetry are weakly electric-dipole active at a “forbidden” direct bandgap. The absorption coefficient is proportional to 287 6. Optical Properties I 2 dºnlm (0) 2 ∝ n 1 dr n5 (6.92) and is identically zero for the n 1 level (since this is the only level without a p state). Figure 6.26 shows the weakly allowed excitonic absorption peaks in Cu2 O involving the so-called yellow exciton series 2p, 3p, 4p, etc., measured by Baumeister [6.55]. The observed peaks are fitted very well with the Rydberg series: En (2.166 0.097/n2 ) eV (n 2, 3, . . .). (6.93) Separately, a very sharp and weak exciton peak associated with the 1s exciton has been observed in Cu2 O at 2.033 eV. It is excited via magnetic-dipole and electric-quadrupole transitions [6.56]. From the continuum threshold energy of 2.166 eV in (6.93) one obtains a binding energy of 0.133 eV for the 1s state, while the higher exciton states in the same series can be fitted with the smaller Rydberg energy of 0.097 eV. The reason for this difference is the central cell correction discussed already in Sect. 4.2.2 in connection with hydrogenic impurities. A discussion of central cell effects in excitons is beyond the scope of this book. 6.3.3 Exciton Effect at M1 Critical Points or Hyperbolic Excitons In Table 6.1 we showed that the Van Hove singularity in the density of states at an M1 critical point has a shape described by C (E0 E)1/2 (where C is a constant and E0 is the energy of the critical point) for E E0 and is equal to C for E E0 . The corresponding shape of Âi in the vicinity of such a critical Photon energy [eV] 2.12 ln(transmission) –3 –2 < 288 –1 2.13 2.14 Cu2O 2.15 2.16 n=5 n=3 n=4 n=2 0 17 100 Fig. 6.26. The low-temperature absorption spectrum of Cu2 O showing the excitonic p series associated with its “dipole-forbidden” band edge [6.55] 17 200 17 300 Photon energy [cm –1] 17 400 6.3 Excitons point in the joint density of states is sketched in Fig. 6.9. The characteristic feature of Âi is that it rises sharply as E approaches E0 from below and decreases slowly for E above E0 . In Sect. 6.2.4 we mentioned that the E1 and E1 ¢1 transitions in the optical spectra of diamond- and zinc-blende-type semiconductors are attributed to M1 -type critical points based on band structure calculations. However, experimentally it was found that the shape of the E1 transitions deviates significantly from that expected for M1 critical points. Figure 6.27 shows the imaginary part of the dielectric constant (Âi ) in the region of the E1 transitions in two II–VI semiconductors: CdTe and ZnTe. The dashed curve was calculated from the pseudopotential band structures by Walter et al. [6.58] without exciton effects. It shows the asymmetric shape expected for the three-dimensional M1 -type critical points. However, the experimental curves 10 (a) CdTe 8 Kane εi 6 4 2 nonexcitonic 0 3.30 3.50 3.40 (b) ZnTe 10 8 εi 3.60 Kane 6 4 A&N 2 0 3.45 3.55 3.75 3.65 Photon energies [eV] 3.85 Fig. 6.27a, b. Imaginary part of the dielectric constant (Âi ) in the region of the E1 transitions for (a) CdTe and (b) ZnTe. The red solid curves represent the experimental results of Petroff and Balkanski [6.57]. The dashed curve labeled “nonexcitonic” is calculated from the band structure obtained by Walter et al. [6.58] without excitonic effects. Dotted curves labeled Kane and A&N have been calculated, respectively, by Kane [6.59] and Antoci and Nardelli [6.60], both including excitonic effects 289 290 6. Optical Properties I measured by Petroff and Balkanski [6.57] show asymmetries in the opposite direction, i. e., the peaks are sharper above the critical point rather than below. In addition, a weaker structure appears at energies higher than the main strong peak in both spectra. These discrepancies between the experiment and the theory based on a one-electron band calculation have been explained by excitonic effects at M1 critical points. Such excitons occurring at saddle points are known as hyperbolic excitons (since the constant energy surfaces near M1 critical points are hyperboloids). Kane [6.59] calculated the lineshape of Âi near an M1 saddle point ˆ1 by solving the wave equation for the relative motion of the electron and hole: P12 P22 P32 e2 º(r) Eº(r), (6.94) 2Ì1 2Ì2 2Ì3 4Â0 Â0 r where Ì1 , Ì2 0 and Ì3 0. In the extreme case when |Ì3 | → ∞ (6.94) reduces to the exciton equation of motion for an M0 critical point in two dimensions. Analytic solutions in this case are known [6.61]. Quasi-two-dimensional excitons are known to exist in layered-type semiconductor such as GaSe (Sect. 7.2.7). More recently they have been found to be important for the optical properties of quantum wells (Chap. 9). Their bound state energies (indexed by the quantum number n) E2D are given by the series E2D (n) E2D (∞) R∗ /(n 12 )2 for n 0, 1, 2, . . . , (6.95) where the effective Rydberg R∗ is the same one as defined in (6.81) for threedimensional excitons. The corresponding oscillator strengths, analogous to those in (6.87) but for the two-dimensional case, are proportional to (n 12 )3 . The ratio f0 /f1 of the oscillator strengths of the n 0 peak to the n 1 peaks is given by (1/2)3 /[(3/2)3 ] 27. The important feature of the twodimensional M0 exciton is the dominance of the n 0 peak. For finite |Ì3 | but |Ì3 | Ì1 , Ì2 , Kane solved (6.94) using the adiabatic approximation for the heavier mass direction. The numerical solutions show that the effects of a finite |Ì3 | are to decrease the binding energy and to broaden asymmetrically the n 0 peak in the corresponding two-dimensional exciton. His results for the cases of m3 Ì3 /Ì1 320, 40, and 5 are shown in Fig. 6.28. Phillips [6.62] has interpreted this asymmetric broadening in terms of a Fano interference [6.63] between a discrete state and a continuum. When Ì3 is negative, there is a continuum of allowed states with energy below the M1 critical point. The n 0 state in the “two-dimensional” exciton can decay into these continuum states and becomes a resonant state (Sect. 4.3). The lineshape of the n 0 state is similar to the so-called auto-ionizing states found in atomic spectra. Kane’s theory explained quantitatively the absorption spectra in CdTe. (Fig. 6.27a) but not in ZnTe [6.57] where the theoretical peak position is lower in energy than the experimental one although their lineshapes agree qualitatively. Later Antoci and Nardelli [6.60] showed that the theoretical peak position in ZnTe can be made to agree better with experiment by slightly modifying the energy bands along the 111 directions. Their results are also compared with experiment in Fig. 6.27b. 6.3 Excitons 10 m3 = – 40 Stot (hω) 8 6 4 m3 = –320 2 m3 = –5 0 –2 –4.0 –3.5 –3.0 –2.5 –2.0 –1.5 –1.0 –0.5 Energy in [light mass atomic units] 0 0.5 1.0 Fig. 6.28. Contribution to the imaginary part of the dielectric constant (Âi ) in the vicinity of an M1 critical point (with energy chosen at the origin) calculated numerically by Kane [6.59] for the cases m3 Ì3 /Ì1 320, 40, and 5. The m3 40 and 5 curves have been multiplied by factors of 5 and 20, respectively, in order to be displayed on the same vertical scale as the m3 320 curve. The light mass atomic unit of energy is 2Ì1 /Â0 Ry In recent years more elaborate many-body calculations of exciton effects on the whole dielectric function have largely corrected the discrepancies between theory and experiment shown in Figs. 6.10–12 [6.64, 65]. For an example of such calculations and a comparison with the measured UV spectrum of GaN see Sect. 6.7. 6.3.4 Exciton Effect at M3 Critical Points We have found so far that excitonic effects tend to enhance the oscillator strength at M0 and M1 critical points. Since the total oscillator strength is proportional to the total number of valence electrons (see the sum rule in Problem 6.5) it should be “conserved” in some way. In other words, the gain in oscillator strength at M0 and M1 critical points induced by the excitonic interaction must be compensated by losses elsewhere. Optical transitions are suppressed at M2 and M3 critical points [6.66]. The equation for the relative motion [i. e., the analog of (6.77b)] for electron–hole pairs at M3 critical points is almost identical to that for M0 critical points except that the reduced mass is negative. This is equivalent to keeping the reduced mass positive but changing the sign of the Coulomb attraction term in (6.77b). This means that at an M3 critical point the electron and hole can be regarded as having normal positive masses but repelling rather than attracting each other via the Coulomb interaction. The result is that no bound states are formed. The repulsion keeps them apart and therefore the optical transition probability is suppressed. The solutions of the wave equation can be shown to be similar to the continuum solutions of (6.77b). Now Âi (ˆ ˆ3 ), where ˆ3 is the frequency of the M3 critical point, is given (in atomic units, e m0 1) by [6.66] 291 6. Optical Properties I Fig. 6.29. Comparison between the lineshapes of the imaginary part of the dielectric constant in the vicinity of an M3 critical point calculated with and without exciton effects [6.66]. The energy units are exciton Rydbergs e – h interaction band approximation εi [arbitrary units] 292 –10 –20 0 E–E3 [ R* ] Âi 2 |P|2 (2Ì)3/2 (ˆ3 ˆ)1/2 Ù eÙ , ˆ2 sinh Ù where Ù is defined as R∗ 1/2 . Ù ˆ3 ˆ (6.96a) (6.96b) The resultant shape of Âi is shown in Fig. 6.29. The strong suppression of the singularity in the optical transition strength is presumably the reason why no M3 critical points have been positively identified in optical spectra. 6.4 Phonon-Polaritons and Lattice Absorption In Chap. 3 we discussed how phonons in crystals containing more than one atom per primitive cell are classified into acoustic and optical phonons. As their names imply, optical phonons can interact with electromagnetic radiation. We shall study this interaction in this section. Since phonons are quantized simple harmonic oscillators, we shall begin by reviewing the response of a collection of identical and charged simple harmonic oscillators (SHO) to a radiation field in the form of the plane wave E(r, t) E0 exp i(k · r ˆt). (6.97) We shall assume that these SHO are isotropic and uniformly distributed in the entire space (in order to avoid problems related to the presence of surfaces). The mass and charge of the SHOs are M and Q, respectively. The natural vibrational frequency of each SHO is ˆT . In response to the applied field the 6.4 Phonon-Polaritons and Lattice Absorption SHO are displaced from their equilibrium positions by the vector u. The equation of motion of the SHOs is M(d2 u/dt2 ) Mˆ2T u QE. (6.98) In the steady state the solutions to (6.98) can be expressed as u u0 exp[i(k · r ˆt)]. (6.99) Substituting this into (6.98) we obtain the solution for u0 : u0 QE0 . M(ˆ2T ˆ2 ) (6.100) Since these SHOs are charged and they are all displaced by the same amount u, they produce a macroscopic polarization P oscillating also at frequency ˆ: P NQu, (6.101) where N is the density of the SHOs. The electric displacement vector D of the medium is given by D E 4P ÂE, D Â0 E P Â0 ÂE (SI units) (6.102) where Â is the dielectric function of the isotropic medium. Substituting (6.100 and 101) into (6.102) we obtain Â: Â1 NQ2 4NQ2 1 (SI units) M(ˆ2T ˆ2 ) Â0M (ˆ2T ˆ2 ) (6.103) When (6.103) is generalized to a collection of SHOs with different resonance frequencies ˆi we obtain (6.50). Equation (6.103) can also be expressed in terms of the refractive index n of the medium: 4Ni Q2 Ni Q2 1 (6.104) (SI units). n2 1 M(ˆ2i ˆ2 ) Â0 M(ˆ2i ˆ2 ) i i Equation (6.104) has been used to explain the anomalous dispersion in the refractive indices of gases in the vicinity of absorption lines and is known as Sellmeier’s equation [6.67]. Before proceeding further with (6.103) we shall include also the contribution of the valence electrons to the total dielectric function Â of the medium. To distinguish the valence electron contribution from that of SHOs, we shall denote one by Âe and the other by Âl (e and l stand, respectively, for electrons and lattice). We shall assume that the bandgap Eg ˆ, so that the radiation field appears to be static to the electrons and Âe (ˆ) can be approximated by Âe (0). On the other hand if ˆ ˆT the SHOs cannot follow the electric field and they no longer contribute to the total dielectric function and therefore Âl → 1 in (6.103). Thus for (Eg /) ˆ ˆT we have the total Â ≈ Âe (0). It is usual to designate Âe (0) as Â∞ and call it the high frequency dielectric 293 294 6. Optical Properties I constant since it is the dielectric constant at a frequency much higher that the vibrational frequencies but below electronic excitation energies. When Â∞ is included in (6.103), Â Âl Âe becomes Â(ˆ) Â∞ 4NQ2 NQ2 Â (SI units) ∞ M(ˆ2T ˆ2 ) Â0 M(ˆ2T ˆ2 ) (6.105) provided ˆ (Eg /). As there are no excess charges in the medium, the electric displacement D satisfies the Gauss equation div D 0 (6.106) or equivalently Â(k · E0 ) 0. (6.107) This equation is fulfilled when either Â 0 or (k · E0 ) 0. We shall consider these two cases separately. Case 1 (Transverse Field): (k · E0 ) = 0 If E0 is also zero we obtain the trivial situation u P D 0. If E0 is nonzero then (k · E0 ) 0 implies that E0 is perpendicular to the propagation direction. In other words, the electric field has to be transverse. For such transverse fields the response of the SHOs is described by the dielectric function in (6.105). In particular, Â diverges when ˆ approaches ˆT . As a result, ˆT represents the resonance frequency of the medium when a transverse vibration is excited (the transverse resonance frequency in short). Case 2 (Longitudinal Field): E0 k and Â = 0 When the electric field is longitudinal (so that E0 · k 0), Â has to vanish in order that (6.107) be satisfied. From (6.105) we see that this can occur at frequencies ˆL defined by Â(ˆL ) 0. Solving (6.105) we obtain ˆ2L ˆ2T 4NQ2 NQ2 ˆ2T (SI units). MÂ∞ Â0 Â∞ M (6.108) To understand what happens at ˆL , we note that (6.102) can be written as E (1/Â)D. When Â 0, E is not necessary zero even for D 0. In fact the longitudinal electric field at ˆL , to be denoted as EL , is given by EL (4/Â∞ )P (4/Â∞ )NQu (1/Â0 Â∞ )NQu (SI units) (6.109) (when D 0). This implies that no external charges are required to generate an electric field when the SHOs are oscillating at ˆL . Instead, the longitudinal electric field EL is produced by the polarization induced by the oscillations. From (6.109) we see that EL is a macroscopic field (since P is a macroscopic quantity). Furthermore, this field points in the opposite direction to the polarization and therefore it contributes an additional restoring force to the longitudinal oscillation. This explains why ˆL , the longitudinal resonance frequency, 6.4 Phonon-Polaritons and Lattice Absorption in (6.108) is always larger than the transverse frequency ˆT . It should be emphasized that EL should not be confused with the macroscopic electric field in the parallel-plate capacitor shown in Fig. 3.3. While the planes of positive and negative charges in a solid appear to resemble parallel-plate capacitors, the fields they produce are microscopic. At equilibrium, in the absence of an LO phonon, these microscopic fields when summed over many unit cells will produce a zero macroscopic field. Otherwise a macroscopic polarization would exist even without an external field as in ferroelectric materials. When an LO phonon is excited in the medium, the relative displacements of the charges result in many induced dipole moments. They sum to a macroscopic polarization, which gives rise to the longitudinal field EL . The charge Q and mass M of the SHOs are microscopic properties that are sometimes difficult to measure. On the other hand quantitities such as ˆT , ˆL , and Â∞ can be determined experimentally. Often it is convenient to introduce another quantity Â0 Â(0), the low frequency dielectric constant, so that the dielectric function can be expressed in terms of measurable quantities (Problem 6.4): ˆ2L ˆ2T ˆ2 ˆ2 Â(ˆ) Â∞ 1 2 Â∞ L2 (6.110a) 2 ˆT ˆ ˆT ˆ2 or Â(ˆ) Â∞ Â0 Â∞ . 1 (ˆ2 /ˆ2T ) (6.110b) From these results one can derive the Lyddane–Sachs–Teller (LST) relation (Problem 6.4): ˆ2 Â0 L2 . Â∞ ˆT (6.111) 6.4.1 Phonon-Polaritons The above discussion of the interaction between electromagnetic fields and charged harmonic oscillators neglects the radiation produced by the oscillating macroscopic polarization P. As a result, the above theory predicts that transverse and longitudinal resonance occur at ˆT and ˆL , respectively, even for zero wavevector. Since whether a wave is transverse of longitudinal depends on the direction of its displacement relative to its wavevector, one expects however, that the transverse and longitudinal vibrations should become degenerate in the limit that the wavevector approaches zero. After all, there is no way to distinguish between the two when the wavevector is zero. This shortcoming is rectified by taking retardation effects into consideration [6.68]. 295 296 6. Optical Properties I A complete description of the interaction between electromagnetic waves and charges must invoke Maxwell’s equations. Equation (6.106) is only one of them. The remaining three equations (in the absence of any current in the medium) are div B 0, (6.112a) curl H (1/c)(D/t), (6.112b) curl E (1/c)(B/t), (6.112c) (set c 1 for SI units) where B and H are, respectively, the magnetic induction and the magnetic field. Since we have limited ourselves to considering only nonmagnetic semiconductors in this book, we can use the approximation B H (for SI units B Ì0 H, where Ì0 is the permeability of vacuum). It is well known, of course, that Maxwell’s equations can be combined to generate two wave equations (one for E and one for H) that describe the propagation of electromagnetic fields [6.10]. Since electromagnetic waves are transverse (in an infinite medium) they couple to transverse excitations such as TO phonons but not to LO phonons. We can therefore limit our considerations from now on to Case 1 only. Equation (6.112a) implies that the H field is also perpendicular to k. As in the case of E, we shall assume that H is represented by a plane wave: H(r, t) H0 exp[i(k · r ˆt)]. (6.113) By substituting E and H from (6.97 and 113) into (6.112b and c), respectively, we obtain two linear homogeneous equations in E0 and H0 . In order that these two equations have nontrivial solutions we require that the characteristic determinant be zero. This condition can be expressed as k2 (ˆ2 /c2 )Â, (6.114a) which we recognize as the dispersion of a transverse electromagnetic wave inside a nonmagnetic medium with dielectric constant Â. Substituting into (6.114a) the expression for Â in (6.111) we obtain the dispersion relation 2 ˆ Â Â 0 ∞ k2 2 Â∞ . (6.114b) c 1 (ˆ2 /ˆ2T ) Figure 6.30 (solid curves) shows a plot of the solutions of (6.114b). If we rewrite (6.114b) as a quadratic equation in ˆ2 , we see that for every value of k there are two solutions for ˆ2 , in other words there are two “branches” to the dispersion curve, similar to the exciton-polariton dispersion sketched in Fig. 6.22. It is easy to show that as k → 0, one solution of (6.114b) approaches ˆ2 c2 k2 /Â0 (known as the “lower branch”) while the other one (“upper branch”) approaches the constant value ˆL . Thus the frequency of the transverse oscillations in the limit of zero wavevector (for the upper branch) becomes degenerate with the longitudinal oscillation frequency, as expected because of the cubic symmetry. On the other hand, when k → ∞ the dispersion of the upper branch is given by ˆ2 c2 k2 /Â∞ while the lower branch 6.4 Phonon-Polaritons and Lattice Absorption Fig. 6.30. Schematic diagram of the dispersion curves of an uncoupled light wave and lattice vibrations and of their coupled optical wave (called a phonon-polariton) in a polar crystal [6.68]. a: light in vacuo; b: photon-phonon coupled mode (upper polariton); b1 : photon dispersion in the medium but without coupling to the phonons; c, d: longitudinal and transverse uncoupled lattice vibrations, respectively; f : transverse phonons coupled to the photons (lower polaritons) 5 a b 4 ω/ω T b1 3 2 Perfect reflection 1 c d f 0 2 4 6 kc/ω T 8 approaches ˆT . Since the longitudinal oscillations cannot couple to the transverse electromagnetic wave, they have no dispersion, a fact which is represented in Fig. 6.30 by the horizontal straight line passing through ˆL . Although the above results have been derived for SHOs distributed uniformly in space, they can be shown [6.68] to be valid also for an ionic (or partly ionic) crystal containing two atoms per unit cell provided we make the following substitutions. The displacement of the SHO is replaced by the relative displacement of the two ions in the primitive unit cell or Mu → Ì(u u ), (6.115) where u and u are, the displacements of the positive and the negative ions and Ì is the reduced mass of the two ions A and B with masses mA and mB , 1 respectively (Ì1 m1 A mB ). The charge Q should be replaced by an ef∗ fective ionic charge e on the ions (one positive and the other negative). The meaning of e∗ will be discussed in 6.4.4. The transverse and longitudinal oscillation frequencies are now identified with the frequencies of the TO and LO phonons, respectively. The resultant transverse wave whose dispersion is described by (6.114b) in crystals is known as a phonon-polariton. Its dispersion curve can be understood in terms of coupled vibrations. In the absence of the TO phonons the dispersion of the electromagnetic oscillation in Fig. 6.30 is given by the straight line ˆ ck/Â1/2 ∞ . If the TO phonon (which is assumed to be dispersionless) does not couple to radiation it will be represented in the same figure by a horizontal straight line passing through ˆT . At the wavevector where these two lines intersect (i. e., the modes are degenerate) they can couple to each other. The reason is that electromagnetic waves can excite the TO phonons while the oscillating charges can radiate electromagnetic waves. The two kinds of waves cannot be separated. As a result of this coupling the frequencies of the two modes are altered: one is raised while the other is low- 297 298 6. Optical Properties I ered. In other words, the two modes seem to “repel” each other. This is sometimes also referred to as level anticrossing. Notice that for ˆ ˆT the TO phonon also contributes to the dielectric function. As a result, the polariton dispersion for small ˆ is given by (ck/ˆ) Â1/2 0 . In Chap. 7 we shall describe in further detail the measurement of the TO and LO phonon frequencies in semiconductors near k 0 and of the phonon-polariton dispersion in GaP using light scattering techniques (Fig. 7.26). 6.4.2 Lattice Absorption and Reflection Once the contribution to the dielectric constant from lattice vibrations is known, it is straightforward to calculate the corresponding optical properties of the sample, such as absorption coefficients, refractive index and reflectance, using the KKRs and (6.10, 11, and 8). For example, the imaginary part of the dielectric function is obtained from (6.105) with the KKR (Problem 6.4). The resultant expression consists of a delta function centered at the TO phonon frequency. This is therefore also the lineshape of the absorption spectrum of an infrared-active optical phonon. Equation (6.110) shows that Â is negative between the TO and LO phonon frequencies and the complex refractive index pure imaginary. The reflectance of the sample from (6.8) is therefore 1 between ˆL and ˆT . This means that no incident light can penetrate the sample. As we shall see later, the reflectivity at ˆT is reduced from 100 % when damping of the TO phonon is included in the calculation. Still, the reflectivity remains highest at ˆT . As a result the frequency of the TO phonon is known as the reststrahlen (after a German word meaning residual rays) frequency. For better agreement with experiment it is necessary to introduce a damping constant Á for the TO phonons [6.70]. The result is that the equation of motion (6.98) becomes M(d2 u/dt2 ) MÁ(du/dt) Mˆ2T u QE and the corresponding dielectric constant in (6.103) is complex: 4NQ2 (SI units). Â(ˆ) Â∞ 4Â0 M(ˆ2T ˆ2 iˆÁ) (6.116) (6.117a) Â(ˆ) can also be expressed in terms of Â∞ and Â0 as in (6.110b): Â(ˆ) Â∞ Â0 Â∞ . [1 (ˆ2 /ˆ2T )] i(ˆÁ/ˆ2T ) (6.117b) A plot of the real and imaginary parts of Â(ˆ) for Á/ˆ 0.05 is shown in Fig. 6.31a. The reflectivity coefficients calculated from (6.117b) are displayed for several values of Á/ˆ in Fig. 6.31b. Figure 6.32 exhibits the measured lattice reflection spectra in several zinc-blende-type semiconductors. They can all be fitted reasonably well by curves calculated from (6.117b) with (6.8) using the phonon frequency and the damping constant as the only adjustable parame- 6.4 Phonon-Polaritons and Lattice Absorption 75 (a) n2 – k2, 2nk 50 γ /ω T = 0.05 n2 – k2 25 2nk 0 –25 0.75 1.00 1.25 Reduced frequency [ω /ω T] 1.50 LO TO 100 ε0=15, ε∞=12 Reflectivity [%] (b) 75 γ ω T = 0.0040 γ = ω T 0.020 γ ω T = 0.050 50 25 0 0.75 1.00 1.25 Reduced frequency [ω /ωT] 1.50 Fig. 6.31. Plot of (a) the real and imaginary parts of the complex dielectric constant and (b) the reflectivity coefficients calculated from (6.117b). The vertical arrows indicate the frequencies of the TO and LO phonons. Note the deep minimum in the reflectivity which corresponds to Âr ≈ 1 [6.69] ters. The parameters obtained in this way are listed in Table 6.5. The phonon frequencies can be measured independently by other techniques such as Raman scattering (Chap. 7), while Á can be deduced from time-resolved Raman scattering since it is the inverse of the phonon lifetime [6.70, 73]. For calculations of phonon linewidths based on the electronic band structure see [6.70]. These widths can be considered as the imaginary part of an anharmonic correction to the energy (self-energy). Its real part is an anharmonic correction to the phonon frequency [6.71]. 6.4.3 Multiphonon Lattice Absorption Although the optical phonons in covalent semiconductors, such as Si and Ge, are not infrared active (Sect. 2.3.4) these semiconductors also absorb infrared 299 6. Optical Properties I 80 60 40 Reflectivity [%] 300 InAs GaAs AlSb 20 0 80 60 40 InSb GaSb 20 InP 0 180 200 220 240 260 280 300 250 350 450 Wave number [cm–1] Fig. 6.32. Comparison between experimental (solid curves) lattice reflection spectra in several zinc-blende-type semiconductors with those calculated from (6.117b) using (6.8) (broken curves). The TO and LO phonon frequencies and the corresponding damping constants were adjusted to fit the experimental spectra. The spectra on the left-hand side were measured at liquid helium temperature; those on the right are room temperature spectra [6.69] Table 6.5. The TO (ˆT ) and LO phonon (ˆL ) frequencies and the ratio of the damping constant (Á) to ˆT determined from lattice reflection spectra in several zinc-blende-type semiconductors [6.69] and from Raman scattering [6.72] Semiconductor InSb InAs InP GaSb GaAs GaP GaN AlSb CdTe ZnSe Temperature [K] ˆ T [cm1 ] ˆ L [cm1 ] Á/ˆ T 4.2 300 4.2 300 4.2 4.2 296 300 300 300 1.2 80 184.7 179.1 218.9 307.2 230.5 273.3 268.2 366.3 555 318.8 145 211 197.2 190.4 243.3 347.5 240.3 297.3 291.5 401.9 740 339.6 170 257 0.01 0.016 0.01 0.01 0.01 0.01 0.007 0.003 – 0.0059 – 0.01 radiation. Figure 6.33a shows their infrared absorption spectra measured by Collins and Fan [6.74]. The corresponding spectra in Si measured as a function of temperature by Johnson [6.75] are shown in Fig. 6.33b. A mechanism 6.4 Phonon-Polaritons and Lattice Absorption Wavenumber (Si) [cm–1] 800 600 450 1200 1000 1400 TO+TA 8.4 (a) Si TO+LA TO+LO 2TO 20 Absorption coefficient (Ge) 4.0 LO+LA 2.0 1.0 0.8 10 5 0.4 3 0.2 Ge 0.1 1.0 0.8 0.4 0.3 Absorption coefficient (Si) LO+TA 30 300 400 500 600 700 Wavenumber (Ge) [cm–1] 1.3 TO+TA 1.2 1.1 1.0 (b) Lattice absorption bands of vacuum grown silicon 1 2 3 4 0.8 0.7 0.6 365 K 290 K 77 K 20 K Fig. 6.33. (a) Lattice absorption in Si and in Ge measured by Collins and Fan [6.74]. (b) Lattice absorption in Si measured at lower frequencies at several different temperatures by Johnson [6.75] 0.5 LO+TA 0.4 LO+LA TO+LA TO+LO 1 0.3 > 2 > Absorption coefficient [mm–1] 0.9 0.2 2TO 3 0.1 4 TO+2LO 0 30 40 50 60 70 80 90 100 110 120 130 140 Wavenumber [mm–1] 150 160 170 301 302 6. Optical Properties I for these absorption processes has been proposed by Lax and Burstein [6.76]. In general, we can regard the polarization P in a medium as a function of the TO phonon displacements u. When we expand P as a function of u in zinc-blende-type semiconductors we find the lowest order nonzero term to be proportional to u as in (6.101) (crystals containing a constant term independent of u are known as ferroelectrics). In crystals with the diamond structure this first-order term vanishes because of the parity selection rule (the optical phonons are even, hence they cannot produce on odd parity polarization vector). As a result one has to include the second-order terms. Nonzero secondorder terms in phonon displacements give rise to the infrared absorption in Si and Ge. According to Lax and Burstein [6.76], these terms can be visualized as the joint effect of two vibrations. The first one breaks the inversion symmetry and induces charges on the two atoms in the primitive cell. The second vibration causes these charges to oscillate and generate an electric-dipole moment which couples to the electromagnetic wave. The combinations of two-phonon modes contributing to the electric-dipole moment in the diamond structure can be determined by using group theory [6.77]. Many of these two-phonon modes involve one optical phonon plus an acoustic one, both at zone edges. When two phonons participate in the lattice absorption, conservation of energy and wavevector requires that q1 q2 k ≈ 0, (6.118a) where q1 and q2 are the wavevectors of the two phonons and k is the photon wavevector, and ˆ1 ˆ2 ˆ, (6.118b) where ˆ1 , ˆ2 , and ˆ are the corresponding phonon and photon frequencies. Unlike the one-phonon absorption process, the phonon wavevectors are thus no longer restricted to the zone center. This means that the two-phonon absorption spectra can be a broad continuum determined by the two-phonon density of states (DOS). Thus one can try to identify the structures in the twophonon spectra in Fig. 6.33 with critical points in the phonon DOS. The energies of the critical points deduced in this way can be compared with phonon dispersion curves determined by neutron scattering. Table 6.6 shows the identifications of the peaks in the infra-red absorption spectra of Si based on the assumption that these peaks involve sums and differences of four zone-edge phonon frequencies in the TA, LA, TO and LO phonon branches: ˆTA 127.4 cm1 ; ˆLA 333.9 cm1 ; ˆTO 482.3 cm1 ; and ˆLO 413.8 cm1 . Notice that here the TO and LO phonons are not degenerate since these are zone-edge phonons rather than zone-center ones. These multiphonon absorption peaks in Si have also been correlated with critical points in the phonon DOS (at points L, X, W and ™ in the Brillouin zone) [6.79]. Multiphonon absorption spectra have been observed in zinc-blende-type semiconductors. Be- 6.4 Phonon-Polaritons and Lattice Absorption Table 6.6. List of the peak frequencies in the multiphonon absorption spectra of Si and their identification in terms of combinations of four zone-edge phonons [6.78] Observed peak frequency [cm1 ] Identification Calculated peak frequency [cm1 ] TOTA LOTA TOTA LOLA TOLA TOLO 2TO TO2LO 354.9 541.2 607.9 747.7 816.2 896.1 964.6 1309.9 371.8 566.2 609.8 739.7 818.7 896.1 963.9 1301.9 sides the Lax–Burstein mechanism, an additional mechanism is present in this case. Since one-phonon absorption is allowed, the incident photon can virtually excite the zone-center TO phonon. This TO phonon then decays via anharmonic interactions into two phonons. These results have been reviewed by Spitzer [6.78] and will not be repeated here. Amorphous Ge and Si, in which the translational symmetry is lifted, exhibit rather strong infrared absorption [6.80]. 6.4.4 Dynamic Effective Ionic Charges in Heteropolar Semiconductors Using (6.108) and (6.111) we can express e∗ in terms of experimentally measurable quantities: 1/2 Ì(Â0 Â∞ ) e∗ 4Â0 ˆT . 4N (6.119) Since this effective charge is associated with the absorption induced by TO phonons it is referred to as the transverse or Born effective charge. Using (6.119) we obtain an expression for the macroscopic longitudinal electric field EL generated by LO phonons: EL [4ÌNˆ2T (Â0 Â∞ )/4Â0 Â2∞ ]1/2 (u u ), (6.120a) which can also be written as 1 1 1/2 EL [4ÌNˆ2L (Â1 ∞ Â0 )(4Â0 ) ] (u u ). (6.120b) Equation (6.120b) has already been introduced in (3.32). Sometimes it is convenient to express (6.120b) as EL 4Ne∗L (u u ) (6.121) 303 304 6. Optical Properties I by introducing another effective ionic charge e∗L , which is known as the longitudinal or Callan effective charge. Both e∗ and e∗L are examples of effective charges determined from lattice vibrations. They are referred to as dynamic effective charges, as distinct from the static effective charges which result from the static transfer of electrons from the cation to the anion when an ionic crystal is formed. The static effective charge is related to the ionicity or polarity of the crystal [6.81, 82]. However, since ionicity is a somewhat qualitative concept, several functional relationships have been proposed in the literature to relate the ionicity to static and dynamic charges. We reproduce here the one proposed by Harrison [6.82] for the transverse charge: e∗H Z 4 (·P /3)(20 8·2P ), (6.122) where Z is the cation core charge (three and two for III–V and II–VI compounds, respectively) and ·P is the polarity defined by Harrison [6.82]. The latter can be calculated within the LCAO scheme. If the bonding is assumed to be dominated by the p orbitals, then ·P is defined by ·P Epc Epa 2 ]1/2 [(Epc Epa )2 4Vxx (6.123) where Epc , Epa , and Vxx are, respectively, the atomic p electron energies of the cation and anion and their overlap parameter defined in (2.80c) (Sect. 2.7.2). Notice that ·P 0 when the cation and anion are identical (such as in a homopolar crystal). In Table 6.7 we display the experimental values of e∗ and e∗L together with those of ·P and the corresponding values of e∗H obtained with (6.122). Note the nonmonotonic dependence of e∗ and e∗H on ·P (compare, for example InSb with CdTe). The transverse effective charge can also be estimated from pseudopotential form factors such as those in Table 2.21. This determination, however, requires a knowledge of the wavefunctions and an integration over the entire Brillouin zone, similar to that needed for the calculation of the dielectric function. The corresponding expressions have been given by Vogl [6.86] and by Sanjurjo et al. [6.85]. The latter group of researchers have shown that the rather forbidding complete expression for the effective charge e∗PS in terms of pseudopotential form factors can be reduced to the following simple form: e∗PS Z 4 8Pi 1 Pi2 (6.124) where Z is the cation core charge as in (6.122) and Pi va3 /vs3 with vs3 and va3 being the symmetric and antisymmetric pseudopotential form factors defined in Sect. 2.5.1. Table 6.7 shows some of the values of e∗PS in zinc-blende-type semiconductors obtained with (6.124) by Sanjurjo et al. [6.85] and also values calculated by de Gironcoli et al. [6.84] using the ab initio pseudopotential method. Using the same method the latter group and also King-Smith and Vanderbilt [6.87] have calculated, in addition, the piezoelectric constants (see also Sect. 3.3.3), which are also related to ·P . Equation (6.124) yields a poor 6.5 Absorption Associated with Extrinsic Electrons Table 6.7. Experimental values of the transverse (e∗ ) and longitudinal (e∗L ) effective charges in zinc-blende-type semiconductors [6.69, 83]. Provided for comparison with these experimental values are theoretical transverse charges e∗H estimated from the values of ·P using (6.122) (both values obtained from [6.82]) and e∗PS deduced from the semiempirical pseudopotential form factors. All effective charges are in units of the electronic charge a b c Semiconductor e∗ e∗L ·P e∗H e∗PS InSb InAs InP GaSb GaAs GaP GaN AlSb AlAs AlP AlN ZnSe ZnTe CdTe 2.5 2.6 2.5 1.8 2.2 2.0 2.7c 1.9 2.3 2.28 2.75 2.03 2.00 2.35 0.16 0.22 0.26 0.13 0.2 0.24 0.52c 0.19 0.26 0.31 0.59 0.34 0.27 0.32 0.53 0.55 0.58 0.45 0.48 0.51 0.60 0.45 0.48 0.51 0.58 0.75 0.74 0.78 2.11 2.24 2.35 1.74 1.92 2.43 2.43 1.78 1.91 2.03 2.36 1.88 1.86 1.94 2.0a 2.3a 2.4a 1.6a 2.0a 2.0a 2.9b 1.8a 2.1a 2.2a 2.9b 2.8b 2.5b 1.6b From [6.84]. Calculated with (6.124) using the pseudopotential form factors from [6.85]. Obtained from available parameters with (6.119) approximation in cases where Pi 1. For the II–VI compounds and largebandgap III–V compounds (such as GaN and AlN) it gives reasonable results. However, together with (6.122), it has proven to be useful for estimating the effect of external perturbations (such as hydrostatic and uniaxial stress) on the effective charge [6.88]. 6.5 Absorption Associated with Extrinsic Electrons In Chap. 4 we studied the electronic properties of impurities in semiconductors. The corresponding extrinsic electrons can also interact with electromagnetic waves. In fact, infrared absorption and related optical spectroscopies are the main techniques for determining the impurity energy levels discussed in Chap. 4. In this section we shall concentrate on absorption associated with donors and acceptors in diamond- and zinc-blende-type semiconductors only. The optical properties of these impurity electrons depend on the sample temperature. At low temperatures carriers are trapped on the bound states of the impurities. At sufficiently high temperature the impurities are ionized and their carriers become free, as in metals. Free-carrier absorption is particularly important in small-bandgap semiconductors such InSb, lead chalco- 305 306 6. Optical Properties I genides (such as PbTe) and some II–VI compounds (e. g. HgCdTe) since their impurity levels are so shallow that they are completely ionized at relatively low temperatures. We shall consider the optical properties of extrinsic electrons in these two regimes separately. 6.5.1 Free-Carrier Absorption in Doped Semiconductors The electrical and optical properties of free carriers in simple metals, such as the alkali metals, have been covered extensively in many textbooks on solidstate physics (e. g. [6.89, 90]) on the basis of the Drude model. We shall use this model also, since free carriers introduced into semiconductors by doping behave in many ways like those in simple metals. One important difference between the two is that the carrier concentration in a semiconductor can be changed. Since the dopant concentration is typically less than 1020 cm3 (except in very special cases) the plasma frequencies of carriers in semiconductors (Problem 6.3) are usually in the infrared range whereas they are in the visible or ultraviolet for metals. To obtain the free-carrier contribution to the dielectric function of a semiconductor within the Drude model, we start with the corresponding expression (6.117a) for the TO phonon. In the same spirit as in Problem 6.4 we can obtain the “Drude free-carrier expression” by setting the phonon frequency ˆT in (6.117a) to zero: Â(ˆ) Â∞ 4Nc e2 (SI units). 4Â0 m∗ (ˆ2 iˆÁc) (6.125) In (6.125), Nc , e, and m∗ are, respectively, the density, charge and effective mass of the free carriers. Á1 now represents their scattering time and is rec lated to the phenomenological scattering time Ù introduced in Sect. 5.1. We can decompose (6.125) into a real and an imaginary part: ˆ2p Âr (ˆ) Â∞ 1 2 , (6.126a) ˆ Á2c Â∞ ˆ2p Ác Âi (ˆ) , (6.126b) ˆ(ˆ2 Á2c ) where ˆ2p 4Nc e2 /(4Â0 m∗ Â∞ ) (6.126c) and ˆp is the plasma frequency of the free carriers screened by the dielectric constant Â∞ . Notice that Âi (ˆ), the imaginary part of the dielectric function is proportional to Ác , and hence the absorption coefficient is too. The reason for this is well known in metal optics. A free-carrier absorption process is the annihilation of a photon with the excitation of a carrier from a filled state below the Fermi energy EF to an empty state above it.This is shown schematically in Fig. 6.34. As in the case of excitons (Sect. 6.4), both energy and wavevector 6.5 Absorption Associated with Extrinsic Electrons have to be conserved in this process. Equivalently, this process can occur only at the point where the photon dispersion curve in Fig. 6.34 (with its origin at 1) intersects the free carrier dispersion. As seen from Fig. 6.34, this does not happen, because of the large slope of the photon curve. Wavevector can be conserved if the transition is accompanied by scattering with a phonon or an impurity (represented by the horizontal arrow in Fig. 6.34). By using the definition of the absorption coefficient in (6.10) and the expression in (6.126b) we obtain the free-carrier absorption coefficient ·c : ·c (ˆ) Â∞ ˆ2p Ác nr c(ˆ2 Á2c ) , (6.127) where nr is the real part of the refractive index and c the speed of light. At low frequencies. (i. e. ˆ Ác ) ·c can be written as ·c 4Nc e2 . 4Â0 nr cm∗ Ác (6.128) Comparing ·c with the corresponding expression for the electrical conductivity Û in (5.10) we can rewrite (6.128) as ·c 4Û nr c (6.129) provided we can equate (Ác )1 to the scattering time Ù. As we saw in Chap. 5, the conductivity for a sample at nonzero temperatures is determined by the > > hω < < E 2 Photon < < EF > 2 1 >k 1 Free carrier 0 > K Fig. 6.34. Schematic diagram of a free-carrier absorption process near the Fermi level EF . The thin red straight line labeled “photon” represents the light dispersion. During absorption a carrier from state 1 below EF is excited to an empty state 2 above EF . Scattering with a phonon or impurity, represented by the horizontal arrow, is needed to conserve energy and wavevector in this process 307 6. Optical Properties I average scattering time Ù defined by (5.27), whereas the scattering processes which determine Ùc involve a band of carriers around EF with width equal to ˆ or kB T, whichever is smaller. Due to the dependence of the scattering probabilities on carrier energy (Sect. 5.2.3) Ác (Ù)1 and (6.129) is only an approximation. However, the various scattering processes which contribute to Ác are similar to those for Ù, such as scattering with acoustic phonons, optical phonons, and ionized impurities. We shall not repeat these calculations here but instead refer interested readers to the review article by Fan [6.91] for details. Thus, in conjunction with electrical transport measurements, free-carrier absorption is a very useful technique for studying the scattering mechanisms of carriers in semiconductors. Figure 6.35 shows a log–log plot of the free-carrier absorption coefficient in n-type InAs at room temperature for electron concentrations varying between 2.8 × 1016 and 3.9 × 1018 cm3 [6.92]. The straight line drawn through the data points suggests that ·c can be fitted with the simple expression ·c ∝ Ïp , (6.130) where Ï is the wavelength of the infrared radiation. The exponent p is equal to 3 in InAs. Other zinc-blende-type semiconductors have also been found to obey (6.130), except that the value of p varies between 2 and 3 [6.91]. Equation (6.130) can be understood if we assume that ˆ Ác in (6.126b) and the refractive index nr is approximately independent of ˆ (e. g., if the valence electron contribution Â∞ to nr is much larger than the free-carrier contribution). With these assumption ·c can be written as 100 F E D αc cm–1 308 C 10 B A 5 1 Fig. 6.35. Free-carrier absorption in n-type InAs at room temperature for six different carrier concentrations (in units of 1017 cm3 : A: 0.28; B: 0.85; C: 1.4; D: 2.5; E: 7.8; and F: 39 [6.92] 3 5 10 λ microns 15 6.5 Absorption Associated with Extrinsic Electrons Âi ˆ ∝ (ˆ2 Á2c )1 ∝ Ï2 . (6.131) nr c Deviations of p from 2 can be explained by the dependence of Ác on ˆ. The fact that the scattering mechanisms which make the dominant contribution to Ác vary with the semiconductor can be invoked to explain the variation in p for different materials [6.91]. In the optical transition depicted in Fig. 6.34 the initial and final states of the electron lie within the same band. The resultant free-carrier absorption is therefore called intraband. Interband free-carrier absorption can occur if the band containing the carriers is separated from another empty band by an amount smaller than the bandgap. The inset of Fig. 6.36 shows schematically two such transitions between the spin–orbit-split (so) hole band and the heavy ·c 400 hh band GaAs (Zn doped) p = 2.7×1017/cm3 lh band 200 Absorption coefficient [cm–1] lh → hh 100 so band 80 60 84 K 197 K 295 K 40 370 K so → lh 20 so → hh 10 0.1 0.2 0.3 0.4 0.5 0.6 Photon energy [eV] Fig. 6.36. The infrared absorption spectra of p-type GaAs (hole concentration: 2.7×1017 cm3 ) at four different temperatures. The peaks at 0.15, 0.31 and 0.42 eV are identified, respectively, with the transitions lh→hh, so→lh, and so→hh (hh, lh and so stand for the heavy hole, light hole, and spin–orbit split hole bands, respectively). The inset shows schematically transitions between the spin–orbit split (so) hole band and the heavy hole (hh) and light hole (lh) bands and also between the latter two [6.93] 309 6. Optical Properties I hole (hh) and light hole (lh) bands in p-doped diamond- and zinc-blende-type semiconductors. The corresponding infrared absorption spectra due to intervalence transitions in p-type GaAs are shown in Fig. 6.36 as a function of temperature [6.93]. Three broad peaks at 0.15, 0.31 and 0.42 eV can be identified and have been attributed to the lh→hh, so→lh and so→hh transitions, respectively. From such intervalence band absorption measurements, the spin–orbit coupling and the ratios of effective masses of the top valence bands in semiconductors such as InSb, InAs, GaAs, and GaSb have been determined [6.91]. According to the Drude model the reflectivity of metals drops very steeply in the range 0 Âr 1, i. e. at the frequency slightly above the plasma frequency [6.89]. If Âi ≡ 0 the reflectivity drops to zero when Âr 1. This decrease in reflectivity is known as the plasma edge or Drude edge. In most real metals the reflectivity does not vanish when Âr 1 because the plasma frequency is usually high enough for some interband transitions to contribute to Âi . In doped semiconductors the plasma frequency is often below the bandgap so that the only contribution to Âi comes from scattering of the free carriers and is given by (6.126b). As a result, doped semiconductors can exhibit very sharp plasma edges in their reflectivity curves. An excellent example of these edges is shown in Fig. 6.37 for n-type InSb [6.94]. The solid curves are fits to the experimental points with the effective mass m∗ as the adjustable parameter. Spitzer and Fan [6.94] found that m∗ in InSb increases from 0.023m0 (free electron mass) at low carrier concentration to 0.041m0 at high concentrations. This behavior can be explained by the large nonparabolicity of the conduction band of InSb, which is a consequence of its small bandgap (see Problem 6.15). 100 N [cm–3] 3.5×1017 6.2×1017 1.2×1018 80 2.8×1018 4.0×1018 InSb: N-Type Reflectivity [%] 310 60 40 20 0 5 10 15 20 25 Wavelength [µm] 30 35 Fig. 6.37. Plasma edges observed in the room temperature reflectivity spectra of n-type InSb with carrier concentration N varying between 3.5×1017 cm3 and 4.0×1018 cm3 [6.94]. The solid curves are fits to the experimental points using the reflectivity calculated with (6.8) and (6.126a,b) 6.5 Absorption Associated with Extrinsic Electrons 6.5.2 Absorption by Carriers Bound to Shallow Donors and Acceptors In Chap. 4 we showed that shallow donors and acceptors in diamond- and zinc-blende-type semiconductors behave somewhat like “hydrogen atoms embedded in a solid”. It is well known that a hydrogen atom can absorb electromagnetic radiation via electronic transitions between its quantized levels. These transitions give rise to series of sharp absorption lines known as the Lyman, Balmer, Paschen, etc., series in the spectra of atomic hydrogen [6.95]. By analogy with the hydrogen atom we expect that the electron in a donor atom or the hole on an acceptor can also be excited optically from one bound state to another. In addition, we expect these transitions to obey selection rules similar to those in the hydrogen atom, e. g., electric-dipole transitions are allowed between states with s and p symmetries (i. e., when the difference in the angular momentum quantum number ¢l equals one) but forbidden between states of the same symmetry. Figure 6.38a shows the absorption spectrum of phosphorus donors in Si at liquid helium temperature measured by Jagannath et al. [6.96]. The concentration of donors is around 1.2 × 1014 cm3 . Notice that the absorption peaks are very sharp because of the discrete nature of the energy levels involved. These peaks are assigned to transitions originating from the 1s(A1 ) ground state (Sect. 4.2.3) of the P donors in Si to their excited levels labeled 2p0 , 2p± , etc. As pointed out in Sect. 4.2.3, the degeneracy of the three p levels with magnetic quantum numbers m 0, ±1 in a hydrogen atom are split in the donor atoms in Si because of the anisotropic effective mass tensor associated with the lowest conduction band. In addition to the 1s(A1 ) ground state, donors in Si have two other slightly higher energy states with symmetries 1s(E) and 1s(T2 ) as a result of the valley–orbit coupling (Fig. 4.3). These states are not occupied at liquid helium temperature. They become thermally populated and contribute to infrared absorption at higher temperatures. Transitions from these higher energy 1s states have been observed in Si:P by Aggarwal and Ramdas [6.97] as shown in Fig. 6.38b. The energies of the bound states in shallow donors in Si, determined with great precision from such infrared absorption spectra, have already been compared with theoretical calculations in Fig. 4.3. In spite of its sensitivity and resolution, infrared absorption spectroscopy of shallow impurities has its limitations. The oscillator strength of a transition decreases as the quantum number n of the final state increases and hence higher energy bound states are more difficult to observe. There is another technique which is even more sensitive than infrared absorption in measuring shallow impurity energy levels in semiconductors. This remarkable technique, known as photothermal ionization spectroscopy (PTIS), can detect impurity concentrations as low as 108 cm3 ! It was first reported by Lifshits and Nad [6.98]. The basic process in this technique can be described as phonon-assisted photoconductivity. Photoconductivity is the name for electric conductivity induced by shining light on a sample [6.99]. For example, an intrinsic semiconductor at low temperature may have a very low conductivity because there are 311 6. Optical Properties I 2p 8 + 2p o (a) Si:P 2p 0 α [cm–1] Absorption coefficient [cm–1] 8 4 3p + 0 34.13 34.03 Energy [meV] 4 4p + 5p + 3p 0 4p 0 44 1s(A1) → 2po 1s(T2) → 4p + 1s(E) → 3p + 1s(T2) → 3p + 1s(T2) → 3p o c: 1s(T2) → 2po d: 1s(E) → 2po 40 T=30 K > T=80 K 25 > 20 > T=59 K > b: 1s(E) → 2p + (b) 20 10 36 Photon energy [meV] 32 a: 1s(T2) → 2p + 0 Absorption coefficient [cm–1] 312 30 35 Photon energy [meV] Fig. 6.38a,b. Absorption spectrum of phosphorus donors in Si. (a) Sample at liquid helium temperature containing around 1.2×1014 cm3 of P. The inset shows the 2p0 line on an expanded horizontal scale [6.96]. (b) Between 30 and 80 K in a sample containing 5.2×1015 cm3 of P [6.97] very few thermally, excited carriers. When it is illuminated by light with photon energy larger than its bandgap, free carriers (both electrons and holes) are excited. The resultant increase in conductivity is known as intrinsic photoconductivity. In a doped semiconductor at low temperature (when all the carriers are frozen on the shallow impurities) extrinsic photoconductivity can occur when the photon energy of the incident light is sufficient to ionize the 6.5 Absorption Associated with Extrinsic Electrons impurities. Thus impurity ionization energies can be measured with photoconductivity. This technique does not work for the excited bound states of the impurities unless they are occupied. However, these states may be so close to the continuum that once carriers from the ground state have been excited optically into them they can be ionized by absorbing a phonon. The phonons required can be thermally created by maintaining the sample at a temperature T such that kB T is slightly larger than the ionization energy of the excited state to be studied. A schematic diagram of the photothermal ionization process is shown in the inset of Fig. 6.39. The PTIS spectrum of ∼ 2 × 1014 cm3 P donors in Si is shown in the same figure. A comparison between Figs. 6.38a and 39 shows that the strengths of the transitions to the higher excited states (n 3 to 6) in PTIS are enhanced relative to the n 2 and 3 levels. A PTIS spectrum in ultra-pure p-type Ge measured by Haller and Hansen [6.100] at 8 K is shown in Fig. 6.40. This sample contains a net acceptor concentration of only 1010 cm3 ! The predominant group III acceptor is Al. The concentrations of B and Ga are about 20 times lower. The observed peaks have been identified by comparing them with the theoretical acceptor levels calculated by Baldereschi and Lipari [6.47] (Sect. 4.2.4). Table 6.8 summarizes the binding energies for various excited states of group III shallow acceptors in Ge as determined by PTIS. For comparison the corresponding energies calculated within the model of Baldereschi and Lipari [6.47] are shown under the column labeled “Theory”. The group theoretical notations in parentheses are based on the cubic point group of the crystal. Since PTIS can mea- Phonon > 4p + 2p0 > Photoresponse [arbitrary units] 3p+ ∞ Photon 5p + 1s 5f 0 2p + 5f + 4f + 6p+ > 4f 0 > 4p0 3p0 2p 0 34 38 42 Photon energy [meV] 46 Fig. 6.39. Photothermal ionization spectrum of phosphorus-doped Si measured by Jagannath et al. [6.96]. The inset shows schematically the photothermal ionization process for a donor atom 313 6. Optical Properties I Al (C) p-type Ge Photothermal response [arbitrary units] → 314 Al (D) B(D) Al (G) ×4 L2 L1 Ga (D) B(C) Al (B) Al (A) Al (I) 0 * * 100 50 0 0 5 Photon energy 10 [cm–1] 15 [meV] Fig. 6.40. Photothermal ionization spectrum of ultra-pure p-type Ge measured at 8 K [6.100]. For the meaning of the labels A, B, C, etc. in parentheses see Table 6.8. The peaks labeled L1 , L2 , and ∗ are artifacts (“ghosts”) produced by the Fourier transform infrared spectrometer Table 6.8. Binding energies [meV] of group III acceptors in Ge as determined by PTIS. To convert the transition energies measured by PTIS into binding energies the energy of the 2°8 state (peak D) has been assumed to be equal to the theoretical value [6.47] of 2.88 meV [6.101] Binding energy [meV] Peak B Al Ga In Tl G E D C 4.61 3.27 2.88 2.14 4.65 2.88 2.13 4.58 3.3 2.88 2.13 4.57 3.54 2.88 2.10 4.52 3.57 2.88 2.13 a B 1.76 1.49 1.48 1.48 1.76 1.48 1.78 1.5 A∗ 1.16 1.13 1.15 1.15 1.14 A 1.03 1.00 1.01 1.00 1.01 Theory 4.58 (1°8 ) 2.88 (2°8 ) 2.13 (1°7 ) 2.11 (3°8 ) 1.48 1.22 1.14 1.13 (4°8 ) (5°8 ) (2°7 ) (6°8 ) 6.6 Modulation Spectroscopy sure only the energy difference between an excited state and the ground level, the binding energies in Table 6.8 have been obtained by assuming that the 2°8 level (peak D) has the calculated binding energy of 2.88 meV. From this table we see that the energy separations of shallow acceptor levels in Ge are in very good agreement with theory. Also, the chemical shifts between different acceptors due to central cell corrections are largest for the 1°8 level. 6.6 Modulation Spectroscopy The spectra of the dielectric function of semiconductors above the fundamental absorption edge are rather broad (Figs. 6.11 and 12). They could be described as broad bands with some superimposed Van Hove singularities (i. e., interband critical points). The reason for this can be found in the rather weak nature of Van Hove singularities, especially those of the three-dimensional variety. According to Table 6.1 they are of the form (E Ei )1/2 , i. e., the optical functions remain finite for E Ei although their derivatives with respect to either E or Ei diverge. This suggests measuring directly one of these derivatives instead of the dielectric function: the background should largely disappear and sharp peaks should appear at the interband critical points (CPs). This is accomplished with any of the many modulation spectroscopy techniques to be described in this section. Most of our precise knowledge of CP energies stems from reflectance modulation measurements. We note that the extreme accuracy with which Â(ˆ) can be measured with present day ellipsometric methods enables one to numerically obtain derivatives of Â(ˆ) (up to third order). This fact produced a certain shift of emphasis from modulation spectroscopy to spectral ellipsometry in the decade 1975–1985. Since 1985, however, there has been a revival in the use of modulation spectroscopy techniques in connection with semiconductor superlattices and quantum wells ([6.102], see also Chap. 9). The use of modulation techniques for studying interband CPs can probably be traced to Frova and Handler [6.103] and Seraphin and Hess [6.104], who measured so-called electrotransmission and electroreflectance spectra, where the modulation was produced by an applied ac electric field. Essential for the development of these techniques was the commercial availability of lock-in amplifiers, which are devices that select a small ac signal synchronous with the modulation (acting as reference) while any other signal, including noise, is rejected. The measured signal is normalized to the average intensity of the transmitted or the reflected beam and to the amplitude of the modulating agent. In this manner the logarithmic derivative of the transmittance or reflectance with respect to the modulation agent is obtained while the intensity I0 of the incident light, including its fluctuation, is eliminated. Typical modulation amplitudes are of the order of 104 –105 of the incident beam intensity; noise 315 6. Optical Properties I levels can be kept below 106 . For reviews of modulation spectroscopy see [6.11, 105, 106]. The power of reflectance modulation techniques is illustrated in Fig. 6.41 for GaAs. Note the sharp structures at the E0 , E0 ¢0 , E1 , E1 ¢1 , E0 and E2 critical points which appear in the photon energy (i. e., frequency) derivative. These structures are well-reproduced in the theoretical spectra (broken curve in Fig. 6.41c) calculated from the band structure using the pseudopotential method [6.21]. Notice that the experimental E1 and E1 ¢1 peaks are much sharper than the corresponding theoretical ones because of excitonic effects discussed in Sect. 6.3.3. A transmittance modulation spectrum yields directly the corresponding derivative of the absorption coefficient · (except for minor reflection corrections). The relationship between the reflectance mod- 0.6 GaAs R (300K) 0.5 E2 E1 E1 + ∆1 R (a) E0 0.4 E0 0.3 ~ E0 + ∆0 1 dR [eV –1] R dE 1~ E0 E1 E0 E1 + ∆1 E2 ~ ~ Fig. 6.41. Reflectance and frequency modulated reflectance spectra of GaAs. (a) Room temperature reflectance spectrum of GaAs measured by Philipp and Ehrenreich [6.14], the same as that in Fig. 6.8 (b) (1/R)(dR/dE) spectrum calculated by Sell and Stokowski [6.107] by taking the derivative with respect to photon energy E of a 2 K reflectance curve. (c) The solid curve is the (1/R)(dR/dE) spectrum measured by Zucca and Shen [6.108] with a wavelength modulation spectrometer. The broken curve is a theoretical curve calculated from a pseudopotential band structure. The spectra in (a) and (b) are adapted from [6.105]. The spectra in (c) are adapted from [6.21] 0 x10 –1 (b) –2 1 dR (2K) R dE E2 (c) 1 dR [eV –1] R dE 316 E0 E0 0 E0 + ∆0 1 dR (4K) R dE E1 + ∆1 E1 –2 0 4 2 Photon energy [eV] 6 6.6 Modulation Spectroscopy ulation and the corresponding modulation of real and imaginary parts of the dielectric function is more complex. Since the modulation amplitude is small, we can always linearize this relation by introducing the so-called Seraphin coefficients ‚r and ‚i : ¢ ‚r ¢Âr ‚i ¢Âi (6.132a) with ‚r ln ln and ‚i . Âr Âi (6.132b) The coefficients ‚r and ‚i can be obtained by differentiation of (6.8) using (6.11) (Problem 6.16). The spectral dependence of ‚r and ‚i on frequency is sketched in Fig. 6.42 for germanium [6.109]. Note that around the fundamental edge only ‚r is significant. Therefore in this region the shape of the reflectance modulation spectra corresponds to the modulation of Âr . Around E1 and E1 ¢1 both ¢Âr and ¢Âi contribute equally to the spectrum. Around E0 , however, ¢Âi dominates, while at higher frequencies (E2 , E1 ), ¢Âr dominates again with a sign reversal (note that ‚r is negative above 3.5 eV). Obviously ¢Âr and ¢Âi can be separated by using the Kramers–Kronig relations. In this case, extrapolations beyond the spectral range are not important (Problem 6.16c). Conceptually, the simplest modulation spectra are those in which the light frequency is modulated. They just yield the derivative of Âr and Âi with respect to E, i. e., for a critical point (E Ei )1/2 we obtain a spectrum looking like (E Ei )1/2 . Other types of modulation spectra (with so-called external modulation) are obtained by sinusoidally modulating an external agent which affects Ei , such as the temperature, an applied stress, or an electric field. In 0.03 βi βr βr, βi 0.01 –0.01 –0.03 Fig. 6.42. Spectral dependence of the Seraphin coefficients ‚r and ‚i calculated for Ge at room temperature [6.109] 1 2 3 Photon Energy [eV] 4 317 318 6. Optical Properties I many cases such spectra are easier to obtain than their frequency-modulated counterparts. Moreover, they may lead to additional information on the coupling of the external perturbation to the electronic system. These agents not only change Ei but also modify the prefactor of (E Ei )1/2 by changing the oscillator strength and the reduced masses (6.51 and 56). Moreover, it becomes imperative to consider the lifetime broadening of the critical points produced by interaction with phonons and other scatterers. Here we shall represent such broadening by the energy ° and write, for instance in the case of a threedimensional M0 CP, the density of states above Ei as D(E) ∝ Re{(E Ei i°)1/2 } (6.133) (The corresponding expressions for Âr (E) and Âi (E) near M0 , and also other types of CPs including broadening are given in [6.11].) An external perturbation will, in general, modulate not only Ei but also ° (the latter effect is particularly strong in the case of temperature modulation). Among the various external perturbation agents we must also distinguish between those which preserve translational invariance (e. g., temperature, strain) and those which destroy it along one or more directions (electric field, magnetic field). Only in the former cases can we assume that the modulated signal is proportional to the derivative of (6.133) with respect to Ei or °. Since (6.133) is the consequence of translational symmetry in all three directions, the application of a uniform electric field , which destroys the translational invariance along its direction z (because the perturbation Hamiltonian is proportional to ez) makes (6.133) meaningless. This case will be treated in Sect. 6.6.3. Using dimensionless energy units W E E0 , ° (6.133) can be rewritten as D(W) ∝ ° 1/2 Re{(W i)1/2 } ° 1/2 (6.134a) 1 W (W 2 1)1/2 . 2 2 (6.134b) By means of (6.134a, b, 48, and 49) we obtain dÂr 1 dÂr ∝ ° 1/2 F(W), dE dE0 2 dÂi 1 dÂi ∝ ° 1/2 F(W), dE dE0 2 where the function F(W), shown in Fig. 6.43, is given by 1/2 F(W) (W 2 1)1/2 (W 2 1)1/2 W . (6.135a) (6.135b) Likewise we can calculate the derivatives of Âr and Âi with respect to the broadening energy °. We find at a three-dimensional (3D) M0 CP 6.6 Modulation Spectroscopy Fig. 6.43. Universal function F(W) used to represent the derivatives of Âr and Âi with respect to E, E0 and ° at threedimensional critical points > F(W) 1.0 0.5 –10 –5 0 ω−ω g W= Γ 5 10 > 1 dÂr ∝ ° 1/2 F(W), d° 2 (6.135c) dÂi 1 ∝ ° 1/2 F(W). d° 2 (6.135d) The expressions equivalent to (6.135) for other types of CPs can be easily derived by the reader (Problem 6.17). We conclude this introduction by mentioning that phonons in semiconductors also modulate their dielectric function at the corresponding vibrational frequency. This modulation is responsible for the phenomenon of Raman scattering [to be discussed in Sect. 7.2, see (7.36)]. 6.6.1 Frequency Modulated Reflectance and Thermoreflectance A frequency modulation spectrometer is constructed by allowing the frequency of the light coming out of the exit slit of the monochromator to have a small modulation sinusoidally dependent on time. The corresponding change in the reflected light, synchronous with the frequency modulation, is detected with a lock-in amplifier. Thermoreflectance is measured by subjecting the sample to a periodic variation in temperature produced by an alternating current or a periodically chopped laser beam. An increase in temperature preserves the average symmetry of a crystal. However, in principle, both the Ei and ° of a critical point are changed. At E0 and E1 the gaps decrease with increasing temperature at a rate of about 4.5 · 104 eV K1 in most zinc-blende-type semiconductors. ° increases at a rate of about 1.5 · 104 eV K1 [6.110], see Fig. 6.44. Thus the thermoreflectance spectra are expected to be dominated by the shift in the gap, i. e., by (6.135a) for M0 3D CPs or their equivalents in the case of other types of CPs. The frequency-modulated spectra of GaAs are shown in Fig. 6.41. They have 319 6. Optical Properties I been obtained by two different methods: the spectrum in Fig. 6.41b was computed from a reflectance spectrum of GaAs measured at 2 K, those in Fig. 6.41c were measured directly with a wavelength-modulated spectrometer. The two different approaches give very similar results. The corresponding thermoreflectance spectra at 80 K and 300 K are shown in Fig. 6.45. The frequency modulated spectrum of the E1 and E1 ¢1 CPs is nearly the same as the thermo-reflectance spectrum at 80 K shown in Fig. 6.45. This confirms the fact E0 [eV] 0.9 Ge Direct gap 0.8 0.7 Fig. 6.44. Temperature dependence of the direct gap (E0 ) of germanium [6.111] 0 200 T [K] 400 600 8 GaAs Scale 4 0 4 –4 300 K E0 0 ∆R/R [10–4] 80 K ∆R/R [10–4] 320 E0 + ∆0 –8 E'0 Scale –4 E1 1 2 E1 + ∆1 3 4 Photon energy [eV] E2 5 6 Fig. 6.45. Thermoreflectance spectrum of GaAs at 80 and 300 K as reported by Matatagui et al. [6.112]. Note the structures at the critical points E0 , E0 ¢0 , E1 , E1 ¢1 , E0 , and E2 6.6 Modulation Spectroscopy that, at least for these CPs, the thermoreflectance spectrum is mainly produced by the gap shift and not by the increase of ° with increasing temperature. This conclusion, however, should not be regarded as general. 6.6.2 Piezoreflectance Piezoreflectance spectra are usually obtained by applying a periodically modulated uniaxial stress to the sample. This can be accomplished in a number of ways, for example by coupling the cone of a loudspeaker to the sample with a pushrod. In another method, more common these days, the sample is mounted on a piezoelectric transducer in the manner shown in Fig. 6.46 or in another similar way. Results obtained for the E0 gap of CdTe samples oriented along either [100] or [111] are shown in Fig. 6.47. These spectra are determined mainly by the derivative of the E0 exciton energy with respect to the strain. The strongly anisotropic nature of these spectra (note the difference in sign between ê ¯ and ê ⊥ ¯, ¯ represents here the strain direction) is due to the fact that the strain splits the energies of the hole in the exciton, as discussed in Sect. 3.3.2, with a splitting linear in the magnitude of the strain ¯ and proportional to the deformation potentials of the top of the valence band, b for [100] strain and d for [111] strain. At the same time the strain has a hydrostatic component which leads to the uniform shift of both split components by an amount pro- Liquid nitrogen Z Vacuum grease Sample (2 × 15 × 0.1 mm) Y X Ki Kr Fig. 6.46. Details of the piezoelectric transducer modulator arrangement used by Gavini and Cardona [6.113] for piezoreflectance measurements. The blackshaded parallellopided represents a lead zirconate-titanate (PZT) transducer. The ends of a thin (100 Ìm) sample (shaded red) are glued to the transducer with vacuum grease (shaded black) which freezes at low temperatures, thus giving a strong bond to the transducer 321 6. Optical Properties I CdTe χ || [100] 4 χ || [111] 4 e⊥χ e || χ 2 0 0 –2 –2 –4 –4 1.57 1.58 1.59 1.60 1.57 1.58 1.59 103 ∆R R 2 ∆R R 103 322 1.60 Photon energy [eV] Fig. 6.47. Piezoreflectance spectra of CdTe [6.113] at 80 K for two directions of the applied stress ¯, taken with polarizations ê parallel and perpendicular to ¯ portional to a, where a is the volume deformation potential defined in (3.20). Using the wavefunctions shown in (3.20) we can see that the ( 32 , 32 ) split exciton couples only to the ê ⊥ ¯ polarization while the ( 32 , 12 ) exciton couples mainly to ê ¯. This is the reason for the opposite signs of the modulated signal exhibited for these two polarizations in Fig. 6.47. From the ratios of strengths of these two signals one can obtain the corresponding ratio of uniaxial to hydrostatic deformation potentials (b/a and d/a) (Problem 6.18). In cases in which a is known (as it was for CdTe when the work of Fig. 6.47 was performed) one can determine both b and d from the anisotropy of the signals in Fig. 6.47. One thus finds for CdTe [6.113] b 1.1 eV and d 5.45 eV, in rather good agreement with other measurements and calculations [6.29]. 6.6.3 Electroreflectance (Franz–Keldysh Effect) As mentioned above, even a uniform electric field of magnitude (the notation is used here for electric field to distinguish it from energy E) lifts the translational symmetry along its direction. We discuss next the theory of the dielectric function of a semiconductor around an M0 critical point under the presence of . We assume, for simplicity, that the CP is isotropic (a restriction which can be easily lifted, the reader is encouraged to do it as an exercise), with reduced mass Ì. The applied uniform field along z can be represented by a contribution to the Hamiltonian ez which, obviously, is not translationally invariant along z. The effect of on an electron–hole pair, however, depends only on the relative separation of electron and hole, r, and not on the 6.6 Modulation Spectroscopy center-of-mass coordinate R [Sect. 6.3.1; (6.76)]. As in the case of excitons, the center-of-mass motion is not affected by the uniform electric field, leading to an equation equivalent to (6.77a). The solutions of this equation are plane waves and only those with K 0 contribute to the optical absorption. Hence we can neglect the center-of-mass motion in the calculation of Â(ˆ, ). The equation for the relative motion, equivalent to (6.77b), becomes 2 2 ∇ r ez Er ˇ(r) 0, (6.136a) 2Ì where e is the (negative) charge of the electron. Equation (6.136a) can be separated into an equation for the components of r perpendicular to , not involving , and another for the z component 2 d2 ez Ez ˇ(z) 0. (6.136b) 2Ì dz2 The solution ˇ(z) of (6.136b) must be multiplied by the plane-wave solution of the corresponding x, y equation 1 ˇ(x, y) √ exp[i(kx x ky y)], (6.136c) N where N is the appropriate normalization constant and the energy Ez must be added to the kinetic energy in the x, y plane in order to obtain the total “relative coordinate” energy Er : 2 (k2x k2y ) Ez . 2Ì Equation (6.136b) can be written in the simple form Er E0 d2 ˇ(Í) Íˇ(Í) dÍ2 by introducing the dimensionless reduced variable 1/3 Ì|e| Ez z 2 2 , Í £ (6.136d) (6.137a) (6.137b) where the so-called electrooptical energy £ is given by £ e2 2 2 2Ì 1/3 . (6.137c) The solutions of (6.137a) which fulfill the appropriate regularity conditions for z → ±∞ can be written in terms of the Airy function Ai(Í) [6.114] as (|e|)1/2 Ai(Í), (6.138) £ where the prefactor (|e|)1/2 /£ guarantees orthonormality with respect to the continuous variable Ez . ˇEz (Í) 323 324 6. Optical Properties I The dipole matrix element needed for the calculation of Âi (ˆ, ) with (6.48) is given by the equivalent of (6.86) |Pvc |2Ez NP2 |ˇEz (0)|2 . (6.139) Equation (6.48) must be integrated over Ez and summed over all possible values of kx and ky . The latter is accomplished by introducing the density of states, which, instead of the three-dimensional (6.55), for two dimensions and at an M0 CP is (including the spin degeneracy) Ì for Ex,y E0 , D(Ex,y E0 ) 2 (6.140) 0 for Ex,y E0 The corresponding Âi (ˆ, ) thus becomes ∞ 2e2 (2Ì)3/2 P2 £1/2 Âi (ˆ, ) Ai2 (Í)dÍ m2 E2 (6.141) Í0 with E0 E and E ˆ. £ The integral in (6.141) can be easily performed by using a standard integral representation for Ai(Í) [Ref. 6.11; App. I]. We find ∞ Ai2 (Í)dÍ ÍAi2 (Í) Ai2 (Í) (6.142) Í0 Í0 Actually, the quantity of interest in a modulation spectroscopy experiment is not Âi (ˆ, ) but rather the change introduced in Âi by . This can be written as ¢Âi (ˆ, ) Âi (ˆ, ) Âi (ˆ, 0) 2e2 (2Ì)3/2 P2 £1/2 F m2 E2 E0 E £ (6.143a) where F(Í) Ai2 (Í) ÍAi2 (Í) (Í)1/2 H(Í) (6.143b) and H represents the Heaviside step function (which is zero [one] for negative [positive] argument). The real part of ¢Â(ˆ, ) can be obtained by replacing F(Í) in (6.143) by its Kramers–Kronig transform: G(Í) Ai (Í)Bi (Í) ÍAi(Í)Bi(Í) Í1/2 H(Í), (6.143c) 6.6 Modulation Spectroscopy where Bi(Í) is the modified Airy function, which diverges for Í → ∞. For details of the derivation above see [6.11] and the original derivation of Âi (E, ) by Thamarlingham [6.115]. The functions F(Í) and G(Í) are plotted in Fig. 6.48. The inset shows a schematic plot of the imaginary part of the dielectric function Âi in the vicinity of a 3D M0 CP, both with and without a field . The effect of an electric field on an optical absorption edge was first discussed independently by Franz [6.117] and Keldysh [6.118] and hence it is known as the Franz–Keldysh effect. The oscillations in Âi (ˆ) above the band gap are known as Franz–Keldysh oscillations. In the presence of , Âi is no longer zero below the bandgap E0 but decreases exponentially. This can be understood simply by the fact that the term ez in (6.136b) tilts the bands spatially. As a result, the bandgap vanishes. The conduction band energy can always be lowered enough to overlap with the valence band at different points of real space by making z large enough. However, the electron wishing to make a transition from the valence band to the conduction band has to tunnel through a distance dependent on . For photon energy ˆ E0 the absorption can be regarded as photon-assisted tunneling from the valence to the conduction band (see Sect. 9.5). So far we have neglected lifetime broadening of E0 . Also, very often the modulating field is produced at a surface depletion layer (8.22 and 23) and is, therefore, strongly nonuniform. Both effects can be taken care of by introducing Airy functions of a complex variable. This, and also the treatment of other G(η) 0.2 F(η), G(η) 0.1 F(η) 0 –0.1 –0.2 ε=0 εi –0.3 E0 –4 –2 η 0 2 Fig. 6.48. Three-dimensional electrooptic functions F(Ë) (solid line) and G(Ë) (dashed line) according to [6.116]. The inset shows the imaginary part of the dielectric function with (red) and without (black) applied electric field 325 6. Optical Properties I types of CPs, is beyond the scope of this book (interested readers are referred to [6.11, 119]). Equation (6.143a), in connection with Fig. 6.48 indicates that around an M0 critical point the modulation spectrum (¢/) should exhibit a sharp peak at the gap energy E0 , decay rapidly below E0 , and oscillate above E0 . It can be shown, using standard asymptotic expansions for the Airy functions [6.114] that the oscillatory behavior, in the limit of large |Í|, has the form [6.120] ¢ 2 3/2 1 ∝ |Í| cos . (6.144) Í 3 2 Labeling the maxima and minima consecutively by an index n we find from (6.144 and 137c) (En E0 )3/2 An B, (6.145) where A depends only on Ì(A ∝ Ì1/3 ) and physical constants. The larger , the more widely spaced the oscillations become. A fit of the energies En of maxima and minima with (6.145) allows Ì to be determined provided is known [6.121]. As an example of the Franz–Keldysh oscillations we show in Fig. 6.49 the spectrum obtained for a GaAs layer (100 nm thick) by modulating the field between 0.9 and 1.1 × 105 V/cm in the configuration displayed in the inset. A large number of oscillations are observed, with some evidence of a beating be- 1.5 > GaAs n+ Transparent gold electrode > 1.0 100 nm > 0.5 ∆R/R [10–4] 326 GaAs intrinsic 0.0 –0.5 –1.0 –1.5 1.2 1.4 1.6 1.8 Photon energy [eV] 2.0 2.2 Fig. 6.49. Electroreflectance signal observed for strongly uniform modulati